Neutron Scattering  JuSER  Forschungszentrum JÃ¼lich
Forschungszentrum Jülich
in der HefmhoftzGemeinschaft
Thomas Brückel, Gernot Heger, Dieter Richter
and Reiner Zorn (Eds .)
Laboratory Course
Neutron Scattering
Lectures
RWTH Aachen
University of Bonn
University of Münster
Materie und Material
Matter and Materials
Schriften des Forschungszentrums Jülich
Reihe Materie und Material / Matter and Materials Volume 15
Forschungszentrum Jülich GmbH
Institut für Festkörperforschung
Thomas Brückel, Gernot Heger, Dieter Richter
and Reiner Zorn (Editors)
Neutron Scattering
Lectures of the Laboratory course
held at the Forschungszentrum Jülich
In cooperation with
RWTH Aachen, University of Bonn and University of Münster
Schriften des Forschungszentrums Jülich
Reihe Materie und Material / Matter and Materials Volume 15
ISSN 14335506 ISBN 3893363246
Bibliographic information published by Die Deutsche Bibliothek
Die Deutsche Bibliothek lists this publication in the Deutsche
Nationalbibliografie; detailed bibliographic data is available in the
Internet at .
Publisher and
Distributor :
Forschungszentrum Jülich GmbH
Central Library
52425 Jülich
Phone +49 (0) 24 61 61 53 68 . Fax +49 (0) 24 61 61 61 03
email : zbpublikation@fzjuelich .d e
Internet : http ://wwvv.fzjuelich .de/zb
Cover Design :
Grafische Betriebe, Forschungszentrum Jülich GmbH
Printer :
Grafische Betriebe, Forschungszentrum Jülich GmbH
Copyright : Forschungszentrum Jülich 2003
Schriften des Forschungszentrums Jülich
Reihe Materie und Material / Matter and Materials, Volume 15
New revised edition from Matter and Materials Volume 9
ISSN 14335506
ISBN 3893363246
Neither this book nor any part may be reproduced or transmitted in any form or by any means,
electronic or mechanical, including photocopying, microfilming, and recording, or by any
information storage and retrieval system, without permission in writing from the publisher .
Contents
.
.
1 Neutron Sources H . Conrad
2 Properties of the Neutron, Elementary Scattering Processes D . Richter
3 Elastic Scattering from ManyBody Systems Th . Brückel
4 Polarization Analysis w Schweika
5 Correlation Functions Measured by Scattering Experiments R . Zorn
D . Richter
6 Continuum Description :
Grazing Incidence Neutron Scattering O .H . Seeck
7 Diffractometer G . Heger
8 Smallangle Scattering and Reflectometry D . Schwahn
9 Crystal Spectrometer :
Tripleaxis and Backscattering Spectrometer F . Güthoff
H . Grimm
10 Timeof Flight Spectrometers M . Monkenbusch
11 Neutron Spinecho Spectrometer, NSE M . Monkenbusch
R . Zorn
12 Structure Determination G . Heger
13 Inelastic Neutron Scattering : Phonons and Magnons M . Braden
14 Soft Matter : Structure D . Schwahn
15 Polymer Dynamics D . Richter
16 Magnetism Th . Brückel
17 Translation and Rotation M . Prager
18 Texture in Materials and Earth Sciences w Schäfer
Neutron Sources
Harald Conrad
1 . Neutron Sources
Harald Conrad
1 .1 Introductory remarks
Slow neutrons are a virtually unique probe for the investigation of structure and dynamics of
condensed matter and biomolecules . Neutrons are called slow, if their kinetic energy is below
1 keV. As the first neutrons used as microscopic probes were generated in nuclear reactors,
historic terms like thermal neutrons are also frequently used in the classification of neutrons .
In reactor physics the term thermal is used to distinguish these neutrons, which sustain the
nuclear chain reaction, from the fart fission neutrons with energies of several MeV . Thermal
neutrons, i.e . with an average kinetic energy of  25 meV, are of particular interest in the
context of this course . They are in thermal equilibrium with an adequate slowing down medium
(moderator) like graphite, light or heavy water at ambient temperature (kBT  25 meV) .
With the availability of cryogenic moderators, cold neutrons ( = 3 meV) became important
in recent decades, too . Strictly speaking, cold or so called trot neutrons ( = 200 meV) have
to bc considered as thermal, too, because these are neutron gases in thermal equilibrium with
a moderator at a particular temperature . Cold neutrons are in equilibrium with a cryogenic
moderator, e .g . liquid hydrogen at 20 K or solid methane at liquid nitrogen temperature, 77 K .
Hot neutrons are those in equilibrium with e .g . a graphite block heated to 2000 K, say .
These trot neutrons and the even more energetic, so called epithermal neutrons (E > 1 eV)
may in the future gain importance for scattering experiments, in particular with respect to
pulsed accelerator driven neutron sources (sec below). But it is important to realize that there
are no primary sources known, which directly deliver neutrons in the relevant energy range of
typically 10 3 eV < E < 1 eV . All existing sources emit primary neutrons with energies of
about 10 6 eV or above and we are left with the difficult task to reduce the neutron energy
between 6 and 9 orders of magnitude (moderation) .
1 .2 Free Neutrons
Free neutrons are unstable (half life about 12 minutes) . As a nuclear constituent they are stable,
though, and as bound particles virtually ubiquitous, except in light hydrogen. So, the only
means of generating free neutrons are nuclear reactions . There is a variety of possible reactions,
mostly forced ones, although spontaneous neutron emission is known to exist as well. A
number of neutron sources is described in the Appendix, in particular with respect to the
achievable intensities . There are, of course, other criteria (e.g . cost or technical limitations),
but for the neutron scattering experiment the highest possible signal (intensity) at the detector
is decisive . The quality of an experiment strongly depends on the counting statistics,
which in turn govems the resolution capability of a neutron diffractometer or spectrometer .
This criterion excludes most of the sources described in the Appendix for modem neutron
scattering instruments, although electron accelerators for (y,n)reactions were successfully
utilized for a certain time . For other applications like medical or in nuclear and plasma
physics those sources were and still are of importance .
In the following we will explain in greater detail the two most important sources for neutron
scattering experiments : the nuclear reactor and the spallation source .
1 .3 The nuclear reactor as a neutron source
Fission of a single 235U nucleus with one thermal neutron releases on average 2 .5 fast neutrons
with energies around 1 MeV . So, this is more than needed to sustain a chain reaction .
Therefore we can withdraw typically 1 neutron per fission for puiposes like neutron scattering
experiments without disturbing the chain reaction. The source strengths Q(n/s), i .e. neutrons
emitted per second, achievable with these surplus neutrons are limited in particular by problems
ofremoving the energy released, which is about 200 MeV per fission. Using the relation
1 eV = 1.6x10 19 Ws we get Q  3x10 16 n/s per MW reactor power to be removed . As mentioned
in the introduction the fast neutrons have to be slowed down to thermal energies to be
useful for neutron scattering .
The stochastic nature ofthe slowing down of neutrons by collisions with light nuclei ofthe
moderator medium (e .g . protons in water) leads to the notion of a neutron flux ~D as a quality
criterion for thermal neutron sources . This flux is defined as the number of (thermal) neutrons
per second isotropically penetrating a unit area . In order to calculate the flux d)(r) for a given
source distribution Q(r) (the fuel elements of a reactor core submersed in a moderator medium)
we had to solve the general transport (Boltzmann) equation . But there are no analytical
solutions possible for realistic geometries of reactor cores [1] . An estimate, however, will be
given for simple model : a point source located in the center ofa spherical moderator vessel. If
the radius of the vessel is equal to the so called slowing down length Ls [2], then 37% of the
source neutrons become thermal . Using the deflnition (Dt, = v ,l,  n (average neutron velocity
Pu,), where the stationaiy neutron density n is given by a balance equation, viz . n = q ' ti (balance
= production rate  life time) with q as the so called slowing down density, we have
d) f, = v a, , q  ti = P a,  0 .37 Q / (47c Ls 3 /3) 'T, (1 .1)
where the slowing down density q is the number of neutrons slowed down to thermal energies
(i .e . to about 25 meV) per unit volume and per second. For a point source of strength Q in the
center of a spherical moderator volume of radius r = L s we obtain what we have inserted for q
in (2 .1) . The life time (also called relaxation time) is given by [2] ti = (Yabs'vth + D'BZ)1
where Y .,b, and D are the coefficients of absorption and diffusion of neutrons, respectively,
and B2 = (Tc/L s )2 a geometrical factor, the "buckling", which is a measure for the spatial flux
distribution . Inserting numerical values, Ls = 29 cm, Eabs = 3x 10 5 cm ' and D = 2x10 5 cm2/s
for heavy water (Jülich's research reactor FRJ2 is heavy water moderated), we obtain with
the source strength Q  3x10 16 n/(s MW) a thermal neutron flux fia, = 1 .1x 10 13 n/(cm2s MW) .
Extrapolating this to 23 MW, the power of the FRJ2, we obtain a)a, = 2.5x1014 n/(cm2 s) . This
is only 25% too big, a suiprisingly good result taking into accourt the non realistic assumption
Fie. 1 . 1 Horizontal cut through the reactor block of the Jülich research reactor FR72.
(The numbers below the acronyms are the beam charnel heights above thefloor of the experimental
hall.)
ofthe reactor being a point source . In fact the core of the FRJ2 consists of 25 tubular, 60 cm
high fuel elements arranged within a lateral grid of about one meter in diameter . The core is
submersed in and cooled by heavy waten streaming through the tubes . Figure 1 .1 shows a plan
cross sectional view ofthe reactor block .
The FRJ2 is operated with highly enriched uranium 235U . With the existing relaxed fuel
element arrangement an essential neutron flux enhancement, e .g . by an order of magnitude,
were only possible with a corresponding but unwanted power increase . A different possibility
exists in compacting the core, a solution chosen for the high flux reactor at the Institut Laue
Langevin in Grenoble, France . In fact, its core consists of a single annular fuel element of
40 cm outer and 20 cm inner diameter, respectively . Operated at 57 MW, a disturbed flux at
the beam tube noses of fia, =1.2x10 15 n / (cm2 s) is obtained .
Technical limitations
We have just established a relation between neutron yield and reactor power released as heat .
Disregarding for the moment investment and operation costs, the limiting factor for achievable
neutron yields is the power or, to be more precise, the power density in the reactor core .
This technically decisive factor, the power density (1VIW/liter), was not included in the
number given in the previous section, because it depends on the details of the reactor, in
particular the core size, the uranium enrichment and the fuel density in the fuel elements . The
size of the primary neutron source (reactor core, target volume, etc.) is important for a high
flux of thermal neutrons within the moderator . In Table 1 .A .1 of the Appendix a selection of
reactions is given and related to its neutron yields and power densities .
It is now well established that power densities in reactor cores cannot substantially be increased
without unwanted and impracticable consequences, such as liquid sodium cooling . In
particular, the service time of reactor vessel components like beam tube noses or cold sources
would become intolerably short due to radiation damage . Experience with the Grenoble High
Flux Reactor shows that these service times are of the order of seven years . Ten tunes higher
fluxes would result in impracticable service times under one year .
1 .4 Pulsed contra continuons sources
Regarding these arguments, we may ask ourselves, whether high flux reactors have already
reached a fondamental lirait . This were cetainly the case, if we expected a flux increase by
another order of magnitude like the one observed in reactor development since the fifties (sec
Table 1 .1).
Period Example Flux (D [1013
195060 FRM1 München  1
196070 FRJ2 Jülich 10
197080 HFR Grenoble 100
CM2
S1 ]
198090 ? 1000 ???
Table 1 .1
Development ofthermalfuxes ofresearch reactors
A flux increase by a factor of about 6 over that ofthe Grenoble reactor had been envisaged
for a new research reactor in Oak Ridge, USA . This enhancement would have been only possible
by a power increase to 350 MW with a simultaneous increase of the average power density
by a factor of 4 compared to Grenoble . After ten years of planning, the US Department of
Energy decided not to build this so called ANS (Advanced Neutron Source).
At this point we have earnestly to ask, whether the decision was adequate to build ever
more powerful but continuously operating reactors . From a technical point of view is was
perhaps the easiest path, from the point of view of neutron scattering, on the other hand, it
was by no means necessary or economic . In order to accept this we only have to realize that
the two standard methods of neutron scattering, i .e. crystal and time of flight techniques, in
any case only use a minute fraction (102 . . . 104 ) of the source flux. Monochromatization
and/or chopping the primary beam as well as collimation and source to detector distance
(shielding!) may even reduce the source flux by factors of 108 to 1011 , depending on resolution
requirements .
Time of flight spectroscopy inefficiently utilizes the continuous reactor flux for two reasons,
because it requires both a monochromatic and a pulsed beam . Crystal spectrometers and
diffractometers use an extremely narrow energy band, too . The rest of the spectrum is literally
wasted as heat . Obviously, time of flight techniques wich pulsed operation at the same average
source power yield gain factors equal to the ratio of peak to average flux . With crystal techniques
higher order Bragg reflections can be utilized, because they become distinguishable by
their time of flight. In other words, the peak flux will be usable between pulses as well .
So, without increasing the average power density, pulsed sources can deliver much higher
peak fluxes, e.g. 50 times the HFR flux . Now, which type of pulsed source is to be preferred :
a pulsed reactor or an accelerator driven source? This question is not easy to answer. Possibly
it depends on the weights one is willing to assign to the particular arguments . Important arguments
are cost, safety, pulse structure or the potential for other uses than neutron scattering .
If we set aside the costs and ask about safety, we can assert that accelerator driven sources
(e .g . spallation sources) are inherently safc, because no critical configuration is needed for the
neutron production . A pulsed reactor, on the other hand, bas to run periodically through a
prompt super critical configuration . Therefore the external control mechanisms (absorbers) of
the continuously operating reactor will not work. The power excursion must be limited by inherent
mechanisms, e .g . by the temperature rise of the fuel . Although it may be unlikely in reality,
malfunctions of the necessarily mechanical insertion of excess reactivity (rotating parts
of fuel or reflector) may lead to substantial damage of the reactor core . No problems exist in
that respect with a spallation neutron source. Furthermore, the proton beam can be shut down
within a few milliseconds . Neutron generation by protons enables the shaping of pulse structures
(pulse duration below 1 microsecond, arbitrary pulse repetition rates) basically unfeasible
with mechanical devices .
1 .5 The Spallation Neutron Source
1 .5 .1 The spallation reaction
For kinetic energies above about 120 MeV, protons (or neutrons) cause a reaction in atomic
nuclei, which leads to a release of a large number of neutrons, protons, mesons (if the proton
energy is above 400 MeV), nuclear fragments and yradiation . This kind of nuclear disintegration
has been named spallation, because it resembles spalling ofa stone with a hammer .
The spallation reaction is a two stage process, which can be distinguished by the spatial
and spectral distribution of the emitted neutrons . This is depicted schematically in Figure 1 .2 .
l1Et1a tiu I?~i t Yittcl 1lFtl,i1
f t
f',',l' c', t
P'ntsPtfy ~ ;Si1
Fig. 1.2 The spal1crlion process
In stage 1 the primary proton knocks on a nucleon, which in turn knocks on another nucleon
of thé saine nucleus (inteanuclear cascade) or of a différent nucleus (internuclear cascade)
. With increasing energy of thé primaiy particle thé nucléons kicked out of thé nuclei
will for kinematic reasons (transformation from center of mass to laboratoiy system) be
emitted into decreasing solid angles around forward direction . The energy distribution of thé
cascade particles extends up to thé primary proton energy . Alter emission of thé cascade particles
thé nuclei are in a highly excited state, whose energy is released in stage 2 mainly by
evaporation ofneutrons, protons, deuterons, aparticles and heavier fragments as well as yradiation
. Depending on thé particular evaporation reaction course, différent radioactive nuclei
remain . These evaporation neutrons are isotropically emitted. They are thé primary source
neutrons, in which we are interested in thé prescrit context . The spectrum of thé evaporation
neutrons is very similar to that of nuclear fission and has a maximum at about 2 MeV . This is
thé veiy reason, why we cari utilize thé spallation neutrons as with a fission reactor .
The yield of evaporation neutrons increases with proton energy and depends on thé target
material . The following expression for thé yield has been found empirically
Y = f  (A + 20)  (E  b) neutrons / proton, (1 .2)
where A is thé mass number of thé target material (9
For uranium, which releases neutrons by fission as well, b = 0 .02 GeV. In Figure 1 .3 the yield
for lead and uranium is plotted and related to the energy released per neutron . The latter has
important consequences as already discussed in section 1 .3 .
1 .5 .2 Technical details
A spallation neutron source consists of three important components, the accelerator, the target
and the moderators . For reasons discussed in sections 1 .3 and 1 .4 the planned European
Spallation Source (ESS) will be pulsed .
1 .5.2.1 The accelerator
The concept of the ESS envisages a pulsed linear accelerator (linac), which will supply the
full beam power, and two subsequent storage rings for compressing the pulses from the linac .
The ESS design parameters are :
linac proton energy
1 .33 GeV,
average curr ent 3 .75 mA
average beam power 5 MW
linac peak current 0 .1 A
ring peak current 100 A
repetition rate 50 S1
linac pulse duration 1 ms
pulse duration after compression 1 ps
300 m long (superconducting cavities)
ring diameter : 52 m
It is worthwhile to point out that we need a rather complex machine to accelerate particles
from rest to kinetic energies of 1 GeV or above and extract them in pulses of only 1 ps duration
. For the case of the ESS we need five stages of acceleration and compression such as
 electrostatic acceleration to 50 keV
 radio frequency quadrupole (RFQ) acceleration from 50 keV to 5 MeV
 drift tube linac (Alvareztype) from 5 MeV to 70 MeV
 superconducting multiple cavity linac from 70 MeV to 1330 MeV
 two (!) compressor rings (space charge !) .
1 .5.2.2 The target solid or liquid?
According to relation (1 .2), heavy elements (large mass number A) are favored as target candidate
materials, in particular the refractory metals tantalum, tungsten or rhenium, but also
lead, bismuth or even uranium . Whatever material is selected, it will be subject to heavy multiple
loads . Firstly, about 60% of the 5 MW average beam power is dissipated within the tar
get as heat, the rest is transported as released radiation to the target vicinity like moderators,
reflector and shielding or is converted into nuclear binding energy . Secondly, all materials bit
by protons (and fast neutrons) will suffer from radiation damage. Finally, the extremely short
proton pulses generate shocklike pressure waves in target and structural materials, which
may substantially reduce the target seivice life. In order to both keep average target temperaturcs
low and reduce specific radiation damage and loads due to dynamic effects from shock
waves, a solid rotating target is conceivable and bas been proposed for the ESS . As any solid
target has to be cooled, it will inevitably be "diluted" by the coolant, whereby the primary
source's luminosity will be diminished . One should therefore operate the target in its liquid
state avoiding an additional cooling medium. Radiation damage would be no longer a problem
wich the target, but of course with its container . Obviously, the refractoiy metals are excluded
due to their high melting points. So we are left with elements like lead, bismuth, the
PbBi eutectic or  of course  mercury . In tact, mercury has been chosen for the ESS, because
it was also shown to exhibit favorable neutron yield conditions as presented in Figure 1 .4 .
Fig. 1 .4 Calculated axial leakage distributions offast neutronsfrom a leadnefected
mercury target compared to waten cooled tantalum and tungsten targets, respectively .
The dimensions of a target along the beam path will reasonably be chosen according to the
range of the protons of given kinetic energy . For mercury and the ESS energy of 1 .33 GeV
this is about 70 cm . Lateral target dimensions are optimized so that the moderators are not too
far from the proton beam axis (solid angle!) . A typical targetmoderatorreflector configuration
is depicted schematically in Figure 1 .5 .
neutron beann channels
Fi
1 .5 Schematic vertical and horizontal cuts through the innerpart ofthe target block.
1 .5.2.3 The moderators
We will now turn to the "heart" ofthe facility, the moderators, which were just shown in the
last figure above in their relative positions next to the target . As the upper and lower faces of
the target are equivalent for symmetry reasons with respect to the emission of fast neutrons, it
is obvious to exploit both sides with moderators . The question now is, whether we shall use
D 20 as the slowing down medium like in all modern medium and high flux reactors or possibly
H2O? As we have discussed in section 1 .4, not the highest possible average neutron flux is
the only reasonable demand, but rather the highest possible peak flux for a given (or requested)
average flux . In that respect, H2O is the preferred material due to its bigger slowing
110
down power and stronger absorption for thermal neutrons (sec below) . The reason for this
seemingly paradoxical demand for stronger absorption is that the achievable neutron peak
flux is not only proportional to the proton peak current, but also depends on the storage time T
(sec below) of thermal neutrons in the moderator . We should point out here that the slowing
down time for H2O and D 20 is small compared to the storage time T. The neutron peak flux is
given by the following expression, which is the result of a convolution of a proton pulse of
duration tp with an exponential decay of the neutron field within the moderator wich storage
(decay) time T.
_  rep tp / r
1) th = ')th ' (i  e )
tp
where 4) th , ~th are peak and average flux, respectively, and t,, is the time between pulses .
In the limit tp > 0 expression (1 .3) reduces to 4 th = _~ th  trep / z, i .e . even a 8shaped current
pulse results in a finite neutron peak flux . We see as well that in this case the peak flux is
inversely proportional to the moderator storage time . Also with finite cunrent pulses a short
storage time is important for obtaining large peak fluxes . The storage time T of a thermal neutron
is a measure of the escape probability from the moderator and is obviously determined by
both the geometry ofthe moderator vessel and the absorption cross section of the moderator
medium (sec section 1 .3) and can be written [2] :
T = ( vtn ' Yabs + 3 D n2 / L2 )  1 (1 .4)
where v t1, is the average neutron velocity, E abs the macroscopic absorption cross section, D
the diffusion constant for thermal neutrons and L is a typical moderator dimension . The absorption
cross section of H2O is about 700 times bigger than that of D20 . If it were only for
this reason, an H20moderator had to bc small (small L in (1 .4)), because we want of course
utilize the neutrons that leak from the moderator. So, a short storage time must not entirely bc
due to selfabsorption . As, on the other hand, H2O possesses the langest known slowing down
density (the number of neutrons, which become thermal per cm3 and s), an H20moderator
anyhow does not need to be big . In section 1 .3 we have already quoted that within a spherical
moderator vessel with its radius equal to the slowing down length Ls (= 18 cm for H20), 37%
of the fast neutrons emitted from a point source located in the center become thermal. In fact,
an H20moderator must not bc essentially larger, because within a sphere with r = 23 cm already
80% ofthe neutrons are lost due to absorption .
For these reasons a pulsed spallation source will have small (V  1 .5 liter) H20moderators
for thermal neutrons . The corresponding storage time of such H20moderators bas been
measured and is i = 150 ps [3], which is in good agreement with the estimate according to
(1 .4) . Small size and absorption diminish in any case the tune average neutron yield . In order
to improve this without deteriorating the peak fluxes, two tricks are used.
Firstly, a moderator
is enclosed by a socalled reflector (see Fig .
1 .5), a strongly scattering ("reflecting") but non
moderating material, i .e . a heavy element with a large scattering cross section like lead . Secondly,
the leakage probability from the moderator interior, i .e .
a region of higher flux due to
geometrical buckling (Chapter 1 .3), is enhanced by holes or grooves pointing toward the neutron
beam holes. Both measures give gain factors of 2 each, whereby the reflector gain is so to
speak "for free", because the anyway necessary lead or iron shielding bas the saine effect.
A
reflector can be imagined to effect such that it
scatters fast neutrons back, which penetrated
the moderator without being or insufficiently slowed down .
Similar considerations hold as
well for cold moderators employed with spallation sources (Fig . 1 .5) .
As a final remark let us point out that the overall appearance of a target station can hardly
be told from a reactor hall with the respective experimental equipment in place .
In both cases
neutrons are extracted from the moderators by beam channels or guide tubes and transported
to the various scattering instruments .
In the following Table 1 .2 the expected and experimentally supported flux data of ESS are
shown and compared te , those of existing sources .
High flux reactor
(HFR)
Grenoble R
Pulsed reactor
HiRH
Dubna (R
Spallation source
ISIS
Chilton
ESS
HgTarget
H2O Moderator
4 [cm ' s' ] 10 15 2  1016 4 .5 10 15 1 .4 10 17
(U[cm2S' 1 10 15 2 . 1013 7  1012 0.6 .
()15
Pulse repetition rate v [s1 1  5 50 50
Pulse duration [106 s]  250 30 165
dl0"cm 2 S 1 ] l* 1 2 .2 70
* with neutron chopper 100 s 1
Tab .
1 .2 Comparison ofthe performance of varions modern neutron sources
112
Appendix
Neutron Sources  an overview [4]
1 .A.1 Spontaneous nuclear reactions
Although every heavy nucleus is unstable against spontaneous fission, this reaction is generally
suppressed by adecays beforehand .
hand, an exotic isotope, 252Cf,
With the advent of nuclear reactors, on the other
became available in suffcient amount from reprocessing spent
nuclear fuel, where 3% of the decays are by spontaneous fission. The rest is adecay . The
data of a 252Cfsource are :
 yield: 3 .75 neutrons / fission
resp . 2.34 x 1012 neutrons / (gram s)
 half life : 2 .65 y (including adecay)
 average neutron energy : 2.14 MeV (fission spectrum)
1 .A.2 Forced nuclear reactions
In this case we can distinguish between reactions initiated by both charged and neutral particles
. In this context yquanta are regarded as neutral "particles".
1 .A .2 .1 Reactions with charged particles
Although we will restrict the discussion to light ions such as protons, deuterons and aparticles,
a wide field is covered from the historically important radiumberylliumsource to the
latest sources like plasma focus or spallation sources .
(a,n)Reactions
Reaction partners with these sources are either natural (Radium, Polonium) or artificial
(Americium, Curium) radioactive isotopes and a light element such as Beryllium as target
material .
Using a radiumberylliumsource Bothe and Becker discovered in 1930 a new
particle, which they failed to identify it as the neutron . Two years later Chadwick accomplished
this earning him the Nobel prize for this feat. Modern sources employ artificial isotopes
alloyed with Beryllium . Yields are between 10 4 and 103 neutrons per particle . The
technical parameters of a modern 241 Am/Be source are :
 yield: 0 .9 x 10 7 neutrons / s per gram
 half life : 433 y
 neutron energy : a few MeV (complex line spectrum)
241
1 1 3
(p,n) and (d n)Reactions
Bombarding targets (Be, . . . , U) with protons or deuterons ofmedium energy (Eki, < 50 MeV),
either neutrons are released foira the target nuclei in the case of protons or the neutrons are
stripped from the deuterons during the impact and thereby released. Yields are of the order of
102 n/p resp . 10 14 n/s per milliAmpere .
An interesting special case is the reaction between the two heavy hydrogen isotopes, because
it can be exploited in two différent ways. One variant is thé socalled neutron generator
utilizing thé large reaction cross section of thé DTreaction, which peaks already at vely
low deuteron energies (5 barn at 0 .1 MeV) . With this low particle energy thé emitted neutrons
are virtually monoenergetic (E = 14 MeV) and thé émission is isotropie . The target may be
gaseous or Tritium dissolved in adequate metals (Ti, Zr) . The yield for a DTneutron generator
with Ek;(d+) = 0 .1 MeV is of thé order of 10 11 neutrons/s per milliAmpere .
The second variant of exploiting thé DTreaction is thé plasma source . In this source both
gases are completely ionized by applying high pressure and temperature forming a homogeneous
plasma, which releases neutrons via thé fusion reaction. In principle, this is thé same
reaction as with thé neutron generator .
Such sources operate in a pulsed mode, because thé
plasma bas to be ignited by repeated compression . Due to thé need for this compression this
spécial kind of a plasma source is also called thé plasma focus . Up to now yields of about
3 x 10 12 neutrons / s have been obtained experimentally . Planned facilities are expected to deliver
10 16 neutrons / s .
Chapter 1 .5 bas already been dedicated in greater detail to (p,n) or (d,n)reactions at high
particle energies (> 100 MeV), which lead to spalling of thé target nuclei ("spallation") . At
this point we only want to give a typical number for thé neutron yield for comparison with thé
other reactions quoted in this Appendix:
 yield (for 1 GeV protons on lead) : 25 neutrons / proton
resp . 1 .5 x 10 1 ' neutrons / s per milliAmpere
 average neutron energy : 3 MeV (evaporation spectrum)
+ cascade neutrons (up to proton energy) .
1.A .2.2 Reactions with neutral "particles"
(yn)Reactions (photonuclear reactions)
Gamma radiation of radioactive isotopes can release so called photoneutrons, a process,
which is indeed exploited in devices analogous to (a,n)sources . A typically spherical y
source of a few centimeters in diameter is enclosed by a shell of target material . Due to the
extremely high yactivities needed, even weakest neutron sources (106 n/s) can only be hand
114
led remotely. It is rauch more convenient to turn on the source when needed by replacing y
radiation by bremsstrahlung generated by electron bombardment of a heavy metal target .
Using e.g . 35 MeV electrons, we obtain a yield of about 10 2 n/e resp . 0.8 x 10 14 n/s per mA .
Neutron induced nuclearfission (thé nuclear reacior)
Of all neutron sources realized up to now, nuclear reactors are still thé most intense ones .
We had therefore dedicated a detailed chapter for this kind of source (chapter 1.3) .
For comparison we have compiled thé yields, heat deposition, source strengths and power
densities ofthé varions reactions in thé following Table 1.A .1 .
Reaction Yield Heat deposition Source strength Source power
[MeV / n] [n/s] Density
/ Liter
Spontaneous fission 252Cf 3 .75 n/fission 100 2 x 1012 91 0.9
39 W/
9Be (d,n) (15 meV) 1 .2 x 102 n/d 1200 8 x 1013 mA1 
3H (d,n) (0 .2 MeV) 8 x 105 n/d 2500 5 x 101 ' mA"' 
Spallation 28 n/p 20 10 18 0.5 (ESS)
1.33 GeV protons on Hg
Photoproduction 1 .7 x 10 2 n/e 2000 4 x 10 14 5 (Harwell)
W e,n 35 MeV
235U frssion 1 n/fission 200 2 x 1018 1 .2*
nuclear chain reaction
(HFRGrenoble
* At thé hot spot 3 .3 MW/L. For 2 x 10 18 source neutrons per second this gives a thermal flux of 10' 5 n cm2 s
Table I.A.1
Yield, heat déposition, source strength andpower densityfor selected neutron
sources
Literature
[1] S. Glasstone, A. Sesonske, Nuclear Reactor Engineering ; van Nostrand Comp . Inc ., 1963
[2] K.H . Beckurts, K.Wirtz, Neutron Physics ; SpringerVerlag, 1964
[3] G. Bauer, H. Conrad, K. Friedrich, G. Milleret,H. Spitzer; Proceedings 5 11' International
Con£ on Advanced Neutron Sources, JülConf45, ISSN 03445789, 1981
[4] S. Cierjacks, Neutron Sources for Basic Physics and Applications ; Pergamon Press, 1983
1 1 5
Properties of the Neutron
Elementary Scattering Processes
Dieter Richter
2 . Properties of the neutron, elementarg
scattering processes
D. Richter
2 .1 A few remarks on history
In 1932 the neutron was discovered by Chadwick . The naine results from the observation that
the neutron apparently does not possess an electric charge : it is neutral . Today, one knows
that the neutron is an ensemble of one up quark and two down quarks . According to the
standard theory, the total charge therefore amounts to 2/3 é + 2 ( 1/3 e) = 0 . At prescrit this
theoretical statement is proven with a precision of 10 21 e1
Only four years later in 1936 Hahn and Meitner obselved the ferst manmade nuclear fission .
In the saine year also the frst neutron scattering experiment was performed. Its setup is
shown in Fig .2 .1 . Neutrons were taken from a radium beryllium source which was covered by
a paraffm moderator . From that moderator neutron beams were extracted such that they bit
magnesium oxide single crystals which were mounted on a cylindrical circumference under
the appropriate Bragg angle. After reflection they were guided to a detector which was
mounted opposite to the radiumbelyllium source . In order to avoid any directly penetrating
neutrons a big piece of absorber was mounted in between the detector and the source .
Magnesium ozidc singlc
crystals mountcd around
cylindrical circumfercncc
Figure 2 .1 :
Mitchell and Powers's apparatus for demonstrating the diffraction of neutrons
(alter Mitchell and Powers 1936) .
In December 1942 Ferme build his ferst nuclear reactor in Chicago  the so called Chicago
pile  which led to the frst controlled nuclear chain reaction . Only one year later the Oak
Ridge Graphite Reactor went critical . It had a power of 3.5MW and was originally used for
the production of fissionable material . Fig .2 .2 shows this reactor which by now is a national
historic landmark . At this reactor, Shull build the ferst neutron diffractometer which became
operationally at the end of 1945 . At that instrument the frst antiferromagnetic structure
(Mn02) was solved (Shull, Noble Price 1994). At the end of the 40's and the beginneng of the
50's nuclear reactors for neutron research came into operation in several countries . 1954 the
Canadian NRU Reactor in Chalk River was the most powerful neutron source wich a flux of
310 14n/cm 2s 1 . There Brockhouse developed the triple axis spectrometer which was
designed, in order to observe inelastic neutron scattering and in particular to investigate
elementary excitations in solids . For this achievement Brockhouse received the Nobel Price in
1994 . Another milestone in neutron scattering was the installation of the ferst cold source in
Harwell (Great Britain) . This cold source allowed to moderate neutrons to liquid hydrogen
temperatures with the effect that for the ferst time long wavelength neutrons became available
in large quantities .
Figure 2 .2 : View ofthe Oak Ridge Graphite Reactor .
22
In the 60's the ferst high flux reactor specially designed for beam hole experiments became
critical in Brookhaven (USA) . It provided a flux of 10 15 n/cmZs1. For research reactors this
level of flux was not significantly surpassed since then. Finally, 1972 the high flux reactor at
the Institute Laue Langevin in Grenoble (France) went into operation . This reactor since then
constitutes the most powerful neutron source worldwide .
In parallel using proton accelerators already beginning in the 60's, another path for neutron
production was developed . Pioneering work was performed at the Argonne National
Laboratory (USA) . At present the most powerful Neutron Spallation Source is situated at the
Rutherford Laboratoiy in Great Britain which bases on a proton beam of about 200KW beam
power. The future of neutron scattering will most probably go along the lines of spallation
sources . At present in the United States the construction of a 2.5MW spallation source has
commenced wich the aim to get operational in 2005 . European plans to build a Megawatt
Spallation Source are still under development and hopefully a European decision for the
European Spallation Source (ESS) will be reached in the year 2003 .
After the war, Germany was late in the development of neutron tools for research . Only in
1955 international agreements allowed a peaceful use of nuclear research. In the saine year
the frst German Research Reactor became critical in Garching . In the early 60's powerful
research reactors were build like for example the FRJ2 reactor in Jülich which provides a
flux of 2. 10 14 n/cxri Zs ' . Instrumental developments became a domain of German neutron
research. A number of important German contributions in this field are the backscattering
spectrometer, the neutron small angle scattering, the instruments for diffuse neutron scattering
and high resolution time of flight machines .
2 .2 Properties of the neutron
The neutron is a radioactive particle with a mass of m = 1.675 . 10 27kg . It decays alter a
mean lifetime of z= 889 .1 ± 1 .8s into a proton, an electron and an antineutrino (/3 decay) .
n > p+ + e + v (+ 0 .77 MeV) (2 .1)
23
For any practical application the imite lifetime of the neutron has no consequence . At neutron
velocities in the order of 1000m/s and distances in experiments up te,
are negligible .
100m lifetime effects
The neutron cames a spin of 1/2 which is accompanied by a magnetic dipole moment
Ii" = 1 .913 p,, (2 .2)
where uN is the nuclear magneton . The kinetic energy of the neutron E n = z ni,  un
may be
given in différent units as follows
1 meV = 1 .602  10 22 J =:> 8.066 cm '
since E = hv 1 meV=> 0.2418 . 10 12 Hz
since E = kBT : 1 meV=> 11 .60 K
The neutron wavelengths is obtained from the de Broglie relation
_ h h
m n Un =/( 21n E" )1i2
(2 .3)
According to the conditions for moderation, neutrons in different wavelength regimes are
separated into different categories as displayed in Fig .2 .3 . They are produced by moderation
in particular moderators which are kept at different temperatures .
hot thermal cold very cold ultra cold
AM
102
v v v
10 2 104 10 6
E [eV]
Figure 2 .3 : Relation between neutron wavelength and their corresponding kinetic energies .
24
Hot neutrons in reactors are obtained from hot sources at temperatures around 2000K .
Thermal neutrons evolve from ambient moderators while cold neutrons are obtained from
mainly liquid hydrogen or deuterium moderators . The velocity distribution of the neutrons
evolving from such a moderator are given by a Maxwell velocity distribution
o (u ) = vs exp
(2 .4)
Thereby, 0(u) du is the number of neutrons which are emitted through an unit area per
second with velocities between v and v+dv. Fig .2 .4 displays Maxwellian flux distributions
for the three types of moderators discussed above .
ulkm s  '
Figure 2 .4 :
Velocity distributions of neutrons from cold (25K), thermal (300K) and hot
(2000K) moderators .
Finally, Neutrons as well as Xrays are used for scattering experiments on materials . Table
2 .1 compares the most important properties ofboth radiations .
25
Table 2 .1 :
Comparison of Xrays and neutrons
Xrays are transversal
electromagnetic waves
neutrons are particle waves
Mass Mpho, = 0 ni, = 1 .6749286(10)  1027kg
Charge 0 0
Spin 1 1/z
Magnetic Moment 0 fi,, _  1.91304275(45),uN
Typical Energy 10keV 25meV
Wave length Â x = c% =1.24Â
,i h
"  2Em )
1/2
=1 .8Â
Velocity speed of light
2Elv2
u  =
n
C m n
2200 5/sec
2 .3 Neutron production
Neutrons are generated by nuclear reactions . For the investigation ofmatter a large luminosity
that means a high flux of neutrons 0 ofthe requested energy range is essential . Such fluxes at
prescrit cari only be obtained through nuclear fission or spallation . Both are schematically
displayed in Fig .2 .5 .
In nuclear fission a thermal neutron is absorbed by an 235U nucleus . The thereby highly
excited nucleus fissions into a number of smaller nuclei of middle heavy elements and in
addition into 25 (on average 2 .5) highly energetic fast fission neutrons . Typical energies are
in the rage of several MeV. In order to undertain a nuclear chain reaction, on the average 1 .5
moderated neutrons are necessaiy . At a balance a research reactor delivers about 1 neutron per
fission event .
The most powerful research reactor worldwide, the IIFR at the Institute Laue Langevin in
Grenoble, produces a neutron flux of
elated values for the FRJ2 reactor in Jülich for comparison are (ah,, = 2  10 14 n/cm2s at 23
MW .
sion
th ~f rI°i~f r
fL~lll[ 3fl
cI f e.
'21'.ctP_:
rlr.4t tttfa ui 1Y4r
f.=l ,;.f
1ii :td, < 1
i ius.f t r s ip 1,
Figure 2 .5 : Schematic presentation of the fission and spallation process .
In the spallation process highly energetic protons which are typically at energies of about
1GeV hit a target of heavy nuclei like tungsten or tantalum . The proton excites the heavy
nucleus strongly and in the event in the order of 2025 neutrons are evaporated from such a
nucleus . The energies of the spallation neutrons are typically in a range from several MeV up
to hundreds of MeV. Other than a research reactor, a spallation neutron source can easily be
operated in a pulsed mode, where a pulsed proton beam hits a target . At the spallation source
ISIS at the Rutherford Laboratory for example, the repetition frequency amounts to 50Hz . In
27
this way even at a comparatively low average neutron flux very high pulsed fluxes may be
obtained . In the thermal range for example, the Rutherford source is able to surpass the ILL
with respect to the peak flux significantly . Such pulsed sources can be used in particularly
well for time of flight experiments which will be discussed later in the school .
2 .4 Neutron detection
Generally the detection of neutrons is performed indirectly through particular nuelear
reactions which produce charged particles . A number of possible reactions are listed in
Table 2 .2 .
Proportionality counters operate wich a gas volume of 3He or BF 3 (enriched with' °B) . Such
counters deliver sensitivities to nearly 100% . Scintillation counters absorb neutrons within a
polymer or glass layer which is enriched by 6 Li and ZnS . Neutron absorption then leads to
fluorescence radiation which is registered via a photo multiplayer or directly wich a
photographie film. Finally, fission chambers use the n + 235U reaction and have generally only
a low counting probability . They are mainly used in order to control the beam stability and are
applied as monitors.
Table 2 .2 :
Nuclear reactions used for neutron detection .
The cross sections are given in barns (lb =10 28 m 2 ).
Reaction Cross Section for Particles Energy Total Energy
25meV neutrons generated [MeV] [MeV]
P 0.57 0 .77
n + 3He 5333 b 3 T 0 .2
6 n + Li
941 b
3T 2 .74 4 .79
4He 2 .05
4He 1.47 2 .30
n +' °B 3838 b 7 Li 0 .83
y 0.48(93%)
n + 235U 681 b fission 12
28
2 .5 Scattering amplitude and cross section, the Born approximation
We now consider the scattering event by a fixed nucleus . The geometry for such a scattering
process is sketched in Fig .2 .6 . The incoming neutrons are described by plane waves e'krr
travelling in z direction . At the target this plane wave interacts with a nucleus and is scattered
into a solid angle S2 df.
e ikr
Incident
neutrons
r = (0, 0, Z)
Figure 2.6 : Scattering geometiy for an incident plane wave scattered at a target .
The partial cross section is defmed by
_d6 _ current of scattered neutrons into (52,
A2
current of incident neutrons
dÇ2)
(2 .5)
Quantum mechanically the current is given by
2mi (Y/*V y/VvV/ *)
(2 .6)
For an incident plane wave yr= ezkr Eq.[2 .6] leads immediately to j = h~ , where V is
n
the normalization volume . The scattered spherical wave has the form 1 f(Ç2)e"" therej(~
r
29
describes the solid angle dependent scattering amplitude. Inserting this form for the scattered
wave into Eq .[2 .6] for large r
J, _ hk If( )Iz ~2
mn
dS2 2 .7)
is obtained. Finally, inserting the incoming and scattered cunents into Eq .[2 .5] we obtain for
the cross section
d6  I hk'I ml If (Ç2)12 dÇ2  I
f (sa)~z
dS2 Ihklml dn
(2 .8)
du is also called differential cross section .
We realize, that a scattering experiment delivers
information on the absolute value of the scattering amplitude, but not on f(n) itself.
Informations on the phases are lost. The total cross section is obtained by an integration over
the solid angle
(T = f d2 du
(2 .9)
12 M
Our next task is the derivation off(n) in the so called Bom approximation . We start with the
Schrödinger equation ofthe scattering problem
z
 4+V(r)
2m
yr = EV/ (2 .10)
where V(r) is the scattering potential .
We note, that for scattering on a free nucleus the mass
term in the kinetic energy has to be replaced by the reduced mass li = M mn . For large
mn +M
distances (r > oo), V= 0 and we have E = h2k2l2m,, . Inserting into Eq.[2 .10] leads to the wave
equation
2 10
(A+k2 ) yr = u(Z:) yr
V( u~r)= z " r)
The wave equation is solved by the appropriate Greenfunction
(A2+k2)GLr') = 4zd(rr')
'b ~ =' I
G(rL' ) = e Ir _ 0
(2 .12a)
(2.12b)
u (r) yr (r) = f dr' S (r  r') u(r') yr(r')
(2 .12c)
where G(r) is the Greenfunction solving the wave equation with the ofunction as
inhomogeneity . Using Eq.[2 .12c] the wave Eq.[2 .11] may be formally solved by
v/ (r) = e'=
_ 1 f dr' G (Lr') u ( L' ) V ( r' ) (2 .13)
4; 
In Eq .[2 .13] the first part is the solution of the homogenous equation and the second part the
particular solution of the inhomogeneous one . The integral Eq .[2 .13] may now be solved by
iteration. Starting with the incoming wave vP= eikr as the zero order solution, the v+ 1 order
is obtained from the order vby
e'k 
41 f G(rL') u(L') y/v(r') d 3 r' (2 .14)
In the Born approximation we consider the first order solution which describes single
scattering processes . All higher order processes are then qualified as multiple scattering
events . The Born approximation is valid for weak potentials . 6'°` 0 1 where a is the size
a z
of the scattering object . For a single nucleus this estimation gives about 107 and the Born
approximation is well fulfilled .
2 1 1
9
We note one important exception, the dynamical scattering theory, which considers the
scattering problem close to a Bragg reflection in a crystal . Then multiple beam interferences
are important and the Born approximation ceases to apply . For most practical puiposes,
however, the Born approximation is valid. Under the Born assumption the scattered wave
function becomes
1 e`k~= 'I 2m,
y/ = err   = V (I:') e 'kI dzr' (2 .15)
4z Irr~I
z
In order to arrive at a final expression, we have to expand all expressions containing r and r'
around r. Thereby, we consider that r' is a sample coordinate and small compared to r. We
have
1 '
 1 + O 1
Irr I r ( rr
)
(2 .16)
rr'
Irr'I  grad (r) = rr'
Inserting Eq.[2.16] into Eq.[2 .15] gives
1 e'~  =k=~' 2m
e d'r' V/ e'   
' =` V (r') e'~I
(2 .17)
4z r hz
k
: direction ofthe scattered wave k'
Irl
EI
Eq . [2 .17] may be written as
(k'
IVI k)
m
e (2 .18)
2Z hz r
fp)
leads to the final expression for the cross section Eq .[2 .8]
2 12
_du _
mn
\2
A2~2z r2~
I(k'
IVI
k)I2 (2 .19)
We now also allow for inelastic processes, where the sample undergoes a change of its state
from I Â) > I Â') . For the cross section we now also have to consider the changes of state as
well as different length of the wave vectors of the incoming and outgoing waves, which lead
to factors k' and k in the cuvent calculation.
(2 d6 k' ~ m n
dÇ2) (,k=, ;~)  k 2z
2
I(k',Z' IVI k,)1 2
.20)
The scattering event must fulfill energy and momentum conservation .
fmally at the double differential cross section
With that we arrive
a26
_ _k'
M aü) k (2z
M)n
h2
\ 2
Pa 1 (k', a' IVI k,a)2 s(hw + (2 .21)
The summation over Â is carried out over all possible initial states À of the system with their
appropriate probability P Â. The sum over V is the surr over all final states, the ofunction
takes care of the energy conservation, thereby hao is the energy transfer of the neutron to the
system . This double differential cross section will be discussed in detail in the lecture on
correlation functions .
2 .6 Elementary scattering processes
2 .6 .1 The Fermi pseudo potential
The interaction of the neutron with a nucleon occurs under the strong interaction on a length
scale of 1 .5  1015m. For that process, the Born criterium is not fulfilled and for the scattering
process on a single nucleus the Born series would have to be summed up . Fortunately, this is
a problem of nuclear physics and for the pulposes of neutron scattering a phenomenological
approach suffices . Considering that the wavelengths of thermal neutrons are in the order of
101°m we realize, that they are much larger than the dimension of a nucleus of about 1015m.
2 13
Therefore, for any scattering event we may perform a separation into partial waves and
consider only thé isotropie Swave scattering . These scattering processes may bc described by
one parameter thé scattering length b = bi + i  b2. Thereby bl describes scattering, while b2 is
thé absorption part. For thermal neutrons thé scattering potential of a single nucleus becomes
(Ferrai pseudo potential)
V (r) = 2z b z bS (LR) (2 .22)
Mn
The scattering lengths b have been measured as a fonction of neutron energy . For thermal and
lower energies thé réal parts of these scattering lengths are constant and depend in an nonsystematic
way on thé number ofnucléons (sec Fig .2 .7).
We realize, that there are positive as well as negative scattering lengths . Following a
convention most of thé scattering lengths are positive . In this case, we have potential
scattering with a phase shift of 180° between thé incoming and scattered wave . Negative
values result from résonance scattering where thé neutrons penetrate thé nuclei and create a
compound nucleus . The emitted neutrons do not undergo a phase shift. We also realize strong
différences in thé scattering lengths for some isotopes . In particular important is thé différence
in scattering length between hydrogen and deuterium (by, = 0 .374, bd =+0.667) . This
significant différence in scattering length is thé basis of all contrast variation experiments in
sort condensed matter research as well as in biology (sec later lectures) . We also note, that thé
scattering lengths may dépend on thé relative orientation of thé neutron spin with respect to
thé spin of thé scattering nucleus . Again a veiy prominent example is thé hydrogen. There thé
scattering length for thé triplet state, neutron and hydrogen spins are parallel, amounts to
bl,ipiet = 1 .04  10 12cm while thé scattering length for thé singlet situation, neutron and
hydrogen spins are antiparallel, is b,ingret = 0.474  1012cm .
E
ô
ô
x
z
w
0
z
_w
U
N
Figure 2 .7 : Scattering length of nuclei for thermal neutrons as a function of atomic weight .
2 .6 .2 Coherent and incoherent scattering
The scattering of neutrons depends on the isotope as well as on the relative spin orientations .
We now will look into the consequences in regarding the elastic scattering from an ensemble
of isotopes with the coordinates and scattering lengths {R, , b, } . The pseudo potential of this
ensemble has the form
V (L)  2z b z Y, b, 8(r  R ) (2 .23)
ni,
l
with Eq . [2 .l8] we may calculate the matrix element of Vbetween k and k' as
~k' IVI k) = 2z b z b f e>k'r ä (r _ R, ) e>~ d3 r (2 .24)
m
2zb 2
m
b, eiQnr Q  k_ k'
The matrix element is just a Fourier surr over the atomic positions decorated with the
appropriate scattering length bi. The scattering cross section is obtained following Eq .[2.19] .
2 15
Thereby we now also consider the spin states ofthe nuclei before and after scattering s and s' .
The initial state probabilities are given by Ps .
d6_ 
P exp (iQ (R R,, » (s' b;, b s > (2 .25)
dÇ2 SS' il'
We commence with spin independent interactions and assume that spatial coordinates and
scattering lengths are not correlated  that means different isotopes are distributed randomly .
Then Eq .[2 .25] may be evaluated to
_d6
M ,
(bâ b,)
exp (iQ (R, 2R, .»
(2 .26)
In order to evaluate Eq.[2 .26] further, we introduce two scattering lengths averages  the
mean square average and the mean scattering length .
They are given by
N
b2=1 ~b2 ; b =l ~,br
N ,
(2 .27)
With these defmitions, the average product of b, and bt' becomes
(br br~ = (1 _ Srr, ) b2 +611 , b 2
(2 .28)
Finally, introducing Eq .[2 .28] into the expression for the cross section Eq.[2 .26] we obtain
d6 1 [(1 _ Srr')
2 + srr , 2] exp iQ ( Rj  Rj' )
dÇ2
i,,
(2 .29)
2
)+ b2 b2 2.iQ~Ë exp, R I ,)
il ,
Obviously, the cross section contains two contributions .
A coherent one where we have
constructive interference of the neutron waves eminating from the different nuclei . This
2 16
scattering is observed with the average scattering length b . In addition there exists ineoherent
scattering as a result ofthe isotope disorder . It is not able of interference and isotropie .
We now consider spin dependent scattering from one isotope with the nuclear spinj. Both the
nuclear spin as well as the neutron spin are statistically distributed. There exist two compound
spin states :
(i) neutron and nuclear spin are parallel : then I=j + 1/z. This spin state has the multiplicity
of 2j + 2 . Its scattering length is b+ .
(ii) neutron and nuclear spin are antiparallel I = j  1/2 the multiplicity is 2j and the
corresponding scattering length equals b  . The a priory probabilities for the compound
spin states are given by the number of possibilities for their realization divided by the
total number.
+_ 2j+2 _ j+1
p
2j + 2 + 2j 2j + 1
p  = j
2j+1
(2 .30)
The corresponding average scattering lengths become
b = p + b+ + p b (2 .31)
b2 = p + b +2 + p  b 2
We now consider the proton as an example . Here j= 1/2, b + =1 .04 . 10 12 cm,
b = 4 .74  1012cm, p+= 1/4, p = 1/4. Inserting into Eq .[2 .31] we fmd b = 0 .375 
1012 cm
and b 2 = 6 .49 . 1024cm2 . These values lead to a coherent cross section
'7,.h = 4z . b 2 =1 .77 .1024cm2 . For the incoherent cross section, we obtain
6;,, = 4z  (b 2  b2 ) = 79 .8 .10 24 cm 2 . This value is the largest incoherent cross sections of all
isotopes and makes the hydrogen atom the prime incoherent scatterer which can be exploited
for hydrogen containing materials .
2 17
2 .7 Comparison between Xray and neutron scattering
Other than neutrons, Xrays are scattered by the electrons, which are distributed in space
around the respective nucleus . This spatial distribution leads to an atomic form factor which is
the Fourier transformed ofthe electron density distribution pi(! :). It depends in principle on the
degree of ionisation of a nucleus but not on the isotope .
fi (Q) = f pi (r) exp (iQr) dV (2 .32)
Since the atomic radii (about 10 4 times larger than the radius of a nucleus) are comparable
with the wavelength, the scattering amplitude f(Q) depends strongly on Q . Thus, with
increasing scattering angle the scattering intensity drops significantly . Furthermore, the atom
formfactor depends on the number of electrons Z and is given by
f; (Q=o)=Z
(2 .33)
Thereby, Z is the number of electrons of an atom or of an ion .
the atomic formfactor normalized to one as a function of sin B
Fig .2 .8 displays schematically
t
sin 9
Figure 2.8 :
Schematic representation of normalized Xray and magnetic neutron scattering
form factors as a function of sin BQ.
2 18
For a spherical electron distribution pj(r), f(r) depend only on the absolute value of Q. For
neutral atoms and possible ionic states they bas been calculated by HartreeFock calculations
and may be found tabulated .
Since the atomic form factors depend on the atomic number, the scattering contributions of
light atoms for Xrays are only weak . Therefore, in structure determinations the precision of
the localization of such important atoms like hydrogen, carbon or oxygen is limited in the
presence of heavy atoms . Neutrons do not suffer from this problem since the scattering length
for all atoms are about equal .
In particular important is the case of hydrogen . In the bound state the density distribution of
the only electron is typically shifted with respect to the proton position and an Xray structure
analysis in principle cannot give the precise hydrogen positions . On the other hand, bonding
effects which are important for the understanding of the chemistry, may be precisely studied
by Xray electron density distributions .
Atoms or ions with slightly different atom number like neighbouring elements in the periodic
table are difficult to distinguish in Xray experiments. Again, neutron scattering experiments
also by the use ofthe proper isotope allow a by far better contrast creation . Such effects are in
particular important for e .g . the 3delements .
The paramagnetic moment of an atom or ion fcj results form the unpaired electrons . The
density distribution of these electrons oj,n (r) is also named magnetization density or spin
density and is a partial electron density compared to the total electron density pj(r) . Because
of the magnetic dipole interaction, the amplitude of the magnetic neutron scattering is given
in analogy to Eq.[2 .32] as the Fourier transformed of the magnetization density pjM (r) . The
normalized scattering amplitude
(Q) 1
fjM
rI

J
pjM (r) exp
(iQr
dV
(2 .34)
2 19
is also named magnetic form factor . If the spin density distribution is delocalised as e .g . for
3delements, the magnetic form factor decays even more strongly than the Xray analogue .
2 .8 Conclusion : Why are neutrons interesting?
Modem materials research together with the traditional scientifc interest in the understanding
of condensed matter at the atomic scale requires a complete knowledge of the arrangement
and the dynamcs of the atours or molecules and of their magnetic properties as well. This
information can be obtained by investigating the interaction of the material in question with
varies kinds of radiation such as visible light, Xrays or synchrotron radiation, electrons, ions
and neutrons . Among them, neutrons play a unique role due to the inherent properties
discussed above
" their dynamic dipole moment allows the investigations of the magnetic properties of
materials .
" their large mass leads to a simultaneous sensitivity to the spatial and temporal scales that
are characteristic of atomic distances and motions .
" neutrons interact differently with different isotopes of the saure atomic species . This
allows the experimentator to paint selected atoms or molecules by isotopes replacement.
" neutrons can easily penetrate a thick material  an important advantage for material
testing .
" the interaction of the neutron with a nucleus bas a simple form (Born approximation)
which facilitates the direct unambiguous theoretical interpretation of experimental data .
A more thorough introduction to neutron scattering may be found in the following
books :
[1] Bacon G.E ., Neutron Diffraction, Clarendon Press, Oxford (1975)
[2] Bacon G.E. (Ed .), Fifty Years of Neutron Domaction : The advent of Neutron
Scattering, Adam Hilger, Bristol (1986)
Bée M., Quasielastic Neutron Scattering: Principles and Applications in Solid State
Chemistry, Biology and Materials Science, Adam Hilger, Bristol (1988)
[4] Lovesey S .W. and Springer T. (Eds.), Dynamics of Solids and Liquids by Neutron
Scattering, Topics in Current Physics, Vol. 3, Springer Verlag, Berlin (1977)
Lovesey S.W ., Theory ofNeutron Scatteringfrom Condensed Matter, Vol. 1 : Nuclear
Scattering, Vol . 2 : Polarization Effects and Magnetic Scattering, Clarendon Press,
Oxford (1984)
[6] Sköld K . and Price D .L . (Eds .), Methods ofExperimental Physics, Vol. 23, Part A, B,
C : Neutron Scattering, Academic Press, New York (1986)
Springer T ., Quasielastic Neutron Scatteringfor the Investigation of Diffusive Motions
in Solids and Liquids, Springer Tracts in Modern Physics, Vol . 64, Springer Verlag,
Berlin (1972)
[8] Squires G .L ., Introduction to the Theory of Thermal Neutron Scattering, Cambridge
University Press, Cambridge (1978)
[9] Williams W.G., Polarized Neutrons, Clarendon Press, Oxford (1988)
[10] Willis B .T . (Ed.), Chemical Application of Thermal Neutron Scattering, Oxford
University Press, Oxford (1973)
[1l] Windsor C.G ., PulsedNeutron Scattering, Taylor & Francis, London (1981)
Elastic Scattering from ManyBody Systems
Thomas Brückel
3 . Elastie Seattering from ManyBody Systems
Thomas Brückel, IFF, FZJülich
3 .1 Introduction
So far we have learnt about the production of neutrons and their interaction with a single
atom. In this chapter, we will discuss the scattering of thermal neutrons from a sample
containing many atoms . In the first part, we will assume that the atours are nonmagnetic and
only the scattering from the nucleus will be considered . In the second part, we will discuss the
scattering from the spin and orbital angular momentum ofthe electrons in a magnetic solid .
For simplification, we will assume in this chapter that the atours are rigidly fieed on
equilibrium positions, i . e . they are not able to absorb recoil energy. This assumption is
certainly no longer valid, if the neutrons are scattered from a gas, especially in the case of
hydrogen, where neutron and the atour have nearly the saine mass . In this case, the neutron
will change its velocity, respectively its energy, during the scattering event. This is just the
process of moderation and without this socalled inelastic scattering (i. e . scattering connected
wich a change of kinetic energy of the neutron) we would not have thermal neutrons at all .
Also when scattered from a solid (glass, polycrystalline or single crystalline material)
neutrons can change their velocity for example by creating sound waves (phonons) . However,
in the case of scattering from a solid, there are always processes in which the recoil energy is
being transfen ed to the Sample as a whole, so that the neutron energy change is negligible and
the scattering process appears to be elastic . In this chapter we will restrict ourselves to only
these scattering processes, during which the energy of the neutron is not changed. In
subsequent chapters, we will leam how large the fraction of these elastic scattering processes
is, as compared to all scattering processes .
Quantum mechanics tells us that the representation of a neutron by a particle wave field
enables us to describe interference effects during scattering . A sketch of the scattering process
in the socalled Fraunhofer approximation is given in figure 3 .1 .
Fit. 3 .1 : A sketch of the scattering process in the Fraunhofer approximation, in which it is
assumed that plane waves are incident on sample and detector due ta the fact that
the distance sourcesample and sampledetector, respectively, is signicantly
larger than the site ofthe sample.
In the Fraunhofer approximation it is assumed that the size of the sample is much smaller than
the distance between sample and source and the distance between sample and detector,
respectively . This assumption holds in most cases for neutron scattering experiments . Then
the wave field incident on the sample can bc described as plane waves . We will further
assume that the source emits neutrons of one given energy . In a real experiment, a socalled
monochromator will select a certain energy from the white reactor spectrum. Altogether, this
means that the incident wave can be completely described by a wave vector k . The saine holds
for the wave incident on the detector, which can be described by a vector k' . In the case of
elastic scattering (diffraction), we have :
k=lkl =lk'I =k'=~ (3 .1)
Let us define a socalled scattering vector by :
Q=kk'
(3 .2)
The magnitude of the scattering vector can be calculated from wave length k and scattering
angle 26 as follows :
32
Q = Q = k2 + k2  2kk' cos2B
(3 .3)
During a scattering experiment, the intensity distribution is being determined as a function of
the scattering vector :
I M (Q)
(3 .4)
The proportionality factors arise from thé detailed geometiy ofthé experiment . Our task is to
détermine thé arrangement of thé atoms in thé sample from thé knowledge of thé scattering
cross section da/dÇ2(Q) . The relationship between scattered intensity and thé structure of thé
sample is especially simple in thé approximation ofthé socalled kinematic scattering. In this
case, multiple scattering events and thé extinction ofthé primary beam due to scattering in thé
sample are being neglected . Following figure 3 .2, thé phase différence between a wave
scattered at thé origin ofthé coordinate system and at thé position r is given by :
k .rk '.r=Q .r
(3 .5)
Fit. 3 .2 : A sketch illustrating thé phase différence between a beam being scattered at thé
origin ofthé coordinate system and a beam scattered at thé position r.
The scattered amplitude at thé position r is proportional to thé scatteringpower density ps (r) .
The meaning of p, in thé case of neutron scattering will bc given later . The total scattered
amplitude is given by a coherent superposition of thé scattering from all positions r within thé
sample, i . e . by thé integral :
33
A = 1Ps (r)  e'Q 'Yd3r (3 .6)
Le. the scattered amplitude is connected with the scattering power density p s(r) by a simple
Fourier transform:
A = F( Ps ( ?") (3 .7)
A knowledge of thé scattering amplitude for all scattering vectors Q allows us to determine
via a Fourier transform thé scattering power density uniquely . This is thé complete
information on thé sample, which can bc obtained by thé scattering experiment .
Unfortunately, life is not so simple . There is thé more technical problem that one is unable to
détermine thé scattering cross section for all values of (Q . The more fundamental problem,
however, is given thé fact that normally thé amplitude of thé scattered wave is not
measurable . Instead only the scattered intensity I  JA12 can bc determined . Therefore, the
phase information is lost and thé simple reconstruction of thé scattering power density via a
Fourier transform is no longer possible . This is thé socalled phaseprobleni of scattering .
The question what we can learn about the structure of the sample from a scattering experiment
despite this problem will bc the subject of the following chapters . For the moment, we will
ask ourselves the question, which wavelength we have to choose to achieve atomic resolution.
The distance between neighbouring atoms is in the order of a few times 0 .1 nm. In the
following we will use the "natural atomic length unit" 1 A = 0 .1 nm . To obtain information on
this length scale, a phase différence of about Q  a ~ 2 x has to be achieved, compare (3 .5) .
According to (3 .3) Q~~ for typical scattering angles (2 0 ~ 60°) . Combining these two
estimations, we end up with thé requirement that thé wavelength ;, has to be in thé order of
thé interatomic distances, i . e . in thé order of 1 Â to achieve atomic resolution in a scattering
experiment . This condition is ideally fulfilled for thermal neutrons .
34
3 .2 Fundamental Scattering Theory
In this chapter, we will give a simple formulation of scattering theory . Our purpose is to
derive (3 .7) from fundamental principles . The conditions under which (3 .7) holds and the
limitations of kinematical scattering theory will thus become clearer . During a fast reading
this section can be skipped. More details can be found in [1] .
In quantum mechanics, neutrons are described as particle wave fields through the Schrödinger
equation :
(3 .8)
yr is the probability density amplitude, V the interaction potential . In the case ofpurely elastic
E
scattering E = E', the time dependence can be described by the factor exp~ iht 1
. Assuming
)
this time dependence, a wave equation for the spatial part ofthe probability density amplitude
yr can be derived from (3 .8) :
0`P +k2 (r)`Y = 0 (3 .9)
In (3 .9) we have introduced a spatially vaiying wave vector with the magnitude square:
k2
L) _ 2 (E  V~~~ (3 .10)
Solutions of (3 .8) in empty space can be guessed immediately. They are given by plane waves
IP = T0 expCiCk !: ~ with k2 = 2 E .
tJJ
2n The relations between magnitude of the wave
vector, wave length and energy ofthe neutron E can be written in practical units :
35
k[Ä1 ]z 0.695
E
meV
,,[Ä] 9.0451 VE meV (3 .11)
E[meV ~t
81.8/2[Ä]
To give an exaniple, neutrons of wavelength a,
= 2.4 A have an energy of 14 .2 meV with a
magnitude ofthe neutron wave vector ofk = 2.6 A_ 1 .
To obtain solutions of the wave equation (3 .9) in matter, we reformulate the differential
equation by explicitly separating the interaction terni :
(A+k
2m V . IP = : x
2
(3 .12)
Here k denotes the wave vector for propagation in empty space . The advantage of this
formulation is that the solution of the left hand side are already known. They are the plane
waves in empty space . Equation (3 .12) is a linear partial differential equation, i . e. the
superposition principle holds : the general solution can be obtained as a linear combination of
a complete set of solution functions . The coefficients in the series are determined by the
boundary conditions . To solve (3 .12) one can apply a method developed for inhomogeneous
linear differential equations . For the moment, we assume that the right hand side is fixed
(given as x) . We deine a "Greensfunetion" by:
(A+k''~(r,r')=8(rr')
(3 .13)
We can easily verify that a solution of (3 .l3) is given by :
G( :,
e iklrr'I
z^') = (3 .14)
4mlr r'I
36
The meaning of (3 .l4) is immediately clear : the scattering from a pointlike scatterer (8
potential) gives a emitted spherical wave .
Using the "Greensfunction" G(r,r'),
given :
a formal solution of the wave equation (3 .l2) can be
Y = 'Po + 1G ( ?", ?" , ) X (?" , )d 3r'
(3 .l5)
Here, we have taken the initial conditions of a incident plane wave yi into account. That
(3 .l5) is indeed a solution of (3 .l2) can be easily verified by substituting (3 .l5) into (3 .l2) . If
we finally substitute the defmition of x, one obtains :
Y(!:)= yf°(r) +
2 jG(r, r')v(r') (r' 3r' (3 .16)
(3 .16) has a simple interpretation : the incident plane wave yi (r) is superimposed by spherical
waves emitted from scattering at positions r' . The intensity of these spherical waves is
proportional to the interaction potential V(r') and the amplitude of the wave feld at the
position r' . To obtain the total scattering amplitude, we have to integrate over the entire
sample volume .
However, we still have not solved (3 .12) : our solution y appears again in the integral in
(3 .16). In other words, we have transformed differential equation (3 .12) into an integral
equation. The advantage is that for such an integral equation, a solution can be found by
iteration. In the zeroth approximation, we neglect the interaction V completely . This gives y
= yi . The next higher approximation for a weak interaction potential is obtained by
substituting this solution in the right hand side of (3 .16). The frst nontrivial approximation
can thus be obtained :
37
1 ik, r 2rnn fexp(iklr i"'I)
h 2 4zIrr'l
(3 .17) is nothing else but a mathematical formulation of the wellknown Huygens principle
for wave propagation.
The approximation (3 .17) assumes that the incident plane wave is only scattered once from
the potential V(r') . For a stronger potential and larger sample, multiple scattering processes
can occur . Again, this can be deduced from the integral equation (3 .16) by further iteration .
For simplification we introduce a new version of equation (3 .16) by writing the integral over
the "Greens function" as operator G :
V V/ +GVV (3 .18)
The socalled first Born approximation, which gives the kinematical scattering theory is
obtained by substituting the wave function yr on the right hand side by yi
y/ ' =V° +GVyr ° (3 .l9)
This first approximation can be represented by a simple diagram as a sum of an incident plane
wave and a wave scattered once from the potential V.
The second approximation is obtained by substituting the solution of the first approximation
(3 .19) on the right hand side of equation (3 .18) :
V2 = Vf' +GVV1
=V° +GVyi +GVGVyi (3 .20)
Or in a diagrammatic form :
38
1 . e. in the second approximation, processes are being taken into account, in which the neutron
is scattered twice by the interaction potential V . In a similar mannen, all higher order
approximations can be calculated . This gives the socalled Born series . For a weak potential
and small samples, this series converges rather fast . Often, the first approximation, the
kinematic scattering theory, holds very well. This is especially the case for neutron scattering,
where the scattering potential is rather weak, as compared to xray or electron scattering .
Due to the strong Coulomb interaction potential, the probability for multiple scattering
processes of electrons in solids is extremely high, making the inteipretation of electron
diffraction experiments very difficult . But even for neutrons, the kinematic scattering theory
can break down, for example in the case of Bragg scattering from large ideally perfect single
crystals, where the Born series does not converge . The wave equation has to bc solved exactly
under the boundary conditions given by the crystal geometry . For simple geometries,
analytical solutions can be obtained . This is then called the dynamical scattering theory . Since
for neutrons, the kinematical theory holds in most cases, or multiple scattering events can be
conected for easily, we will no longer discuss dynamical theory in what follows and refer to
[l, 2] .
Let us return to the first Born approximation (3 .17) . According to Fraunhofer, we assume in a
further approximation that the size of the sample is significantly smaller than the distance
sampledetector . The geometry to calculate the far field limit of(3 .17) is given in figure 3 .3 .
dtector
Fig. 3 .3 : Scattering geometry for the calculation ofthefar field Limit at the detector. In the
Fraunhofer approximation, we assume that IRI» Ir'I .
39
Under the assumption IRI » ~r 'I , we can deduce from figure 3.3 the following approximation
for the emitted spherical wave :
R
exp (ikIrr'I ) .
exp ik R _L' ._R _ exp ikR .eik'r'
Ir r'I R ,.,
(3 .21)
The probability density amplitude for the scattered wave field in the lirait of large distances
from the sample is thus given by :
~  eik .R + 2m e ikR iV'(R)
V(r,~ei r , d3r,
4zR
(3 .22)
This is just the sum of an incident plane wave and a spherical wave emitted from the sample
as a whole . The amplitude of the scattered wave is given according to (3 .22) :
ALQ) 2m" fV(r)eiQ * rd3r
4zh2
F[V(r)]
(3 .23)
1 . e . the amplitude of the scattered wave is proportional to the Fourier transform of the
interaction potential in the Sample . In the case of pure nuclear scattering of neutrons, this
interaction potential is the Ferraipseudopotential (See proceeding chapter) . Finally, the
measured intensity is proportional to the magnitude square ofthe scattering amplitude :
(3 .24)
3 .3 The Patterson or PairCorrelationFunction
As already mentioned in the introduction, the phase information is lost during the
measurement of the intensity according to (3 .24) . For this reason, the Fourier transform of the
scattering potential is not directly accessible in most scattering experiments (note, however
that phase information can bc obtained in certain cases) . In this section, we will discuss,
which information can bc obtained from the intensity distribution of a scattering experiment .
3 10
The saure problem will bc dealt with in a more general context in thé chapter on correlation
functions . Substituting (3 .23) into (3 .24), we obtain for thé magnitude square ofthé scattering
amplitude, a quantity directly accessible in a scattering experiment :
2/( 2% 2 iQi° 3 * ,
iQ .r ' 3 ,
AQ~ = fV~r)ed rfV ~r)e d r
4~~2 j
= ffd 3rd 3r'V(r)V * (
r')e iQ` ?"~ )
= fd 3R fd3rV(R + r)V * (r)eiQ .r
r  r' R
This shows that the scattered intensity is propoitional to the Fourier transform of a function
P(R) :
I(Q )  ALQI2
_ FR
[
P
(
E)
]
(3 .25)
However, this function is not thé interaction potential, but thé socalled Pattersonfunction :
P(R)= fd 3rV *(r)V(r+R)
(3 .26)
This function correlates thé value of thé interaction potential at position r, wich thé value at
thé position r + R, integrated over thé entire sample . If, averaged over thé Sample, no
conelation exists between thé values of thé interaction potential at position R and r + R, then
thé Patterson function P(R) vanishes . If, however, a periodic arrangement of a pair of atoms
exists in thé Sample wich a difference vector for thé positions R, then thé Patterson function
will have an extremum for this vector R. Thus, thé Patterson function reproduces all thé
vectors connecting one atour with an other atom in a periodic arrangement . In tact, thé
Patterson function is just a special case of thé pair conelation functions accessible by
scattering .
The meaning of thé Patterson function can bc illustrated by a simple example. Figure 3 .4
shows an arrangement of three atoms in thé form of a triangle. We can construct thé Patterson
function by copying this original pattern and shifting thé copy wich respect to thé original by a
différence vector R . In this case of a discrete distribution of thé interaction potential V(r) (we
also assume that V(r) is real), we can just count how mang points of thé original and thé
3 1 1
translated pattern coincide for this given différence vector R. Only if two or more atoms
coincide, will we have a nonvanishing value for P(R) according to (3 .26) for this discrete
distribution of potentials . In this manner we can construct thé Patterson function given in
figure 3 .4 .
Patterson funeti
Fit.
3.4 : Construction of thé Patterson functionfor a pattern, which consists ofthree atours at
thé corners ofa triangle.
It is this function which we would obtain by Fourier transforming thé diffraction pattern of a
periodic arrangement of our original triangular pattern . One can easily see that in thé
Patterson function all vectors connecting one atour with any other one in thé original pattern
can be obtained . In our simple case, thé original pattern can be guessed. However, thé guess is
not unique : we could also choose thé mirror image.
3 .4 Scattering from a Periodic Lattice in three Dimensions
As an example for thé application of formulas (3 .23) and (3 .24), we will now discuss thé
scattering of thermal neutrons from a single crystal. More precisely, we will restrict ourselves
to thé case of a Bravais lattice with one atour at thé origin ofthé unit cell . We further assume
that there is only one isotope with scattering length b . The single crystal is fmite with N, M
and Pperiods along thé basis vectors a, b and c . The scattering potential, which we have to
use in (3 .23) is a sum over thé Fermipseudopotentials of all atoms :
N1 M1 P1 2 ;rh2
V(r)= 1 1 1 .b .g(,:(n .a+m .b+p .ç» (3 .27)
n=0 m=0 p=0 nIn
The scattering amplitude is thé Fourier transform of thé scattering potential (compare 3 .23) :
3 12
ALQ) = Ybfe'Q'rB(r(n .a+m .b+p»ç »d 3r
n,m,p
1 inQ .IM1 iQ .b p1 ipQ .ç
=b Y e  Y, e  Y, e 
n=0 m0 p=0
geometrical series (3 .28)
Summing up the geometrical series, we obtain the scattered intensity :
sing
2 NQ  a sing 2 MQ  b sing 2 pQ . ç
I(Q )  = Ibl2
ALQI2
sin21Q 2 .  2 . b_ sin21Q 2  c
(3 .29)
As expected, the scattered intensity is proportional to the magnitude square of the scattering
length b . The dependence on the scattering vector Q is given by the socalled Lauefunction .
The latter is plotted along one lattice direction a in figure 3 .5 .
30
"Laue" function N=5 and N=10
Fil Lauefunction along the lattice
respectively .
direction a for a lattice with 5 and 10 periods,
The main maxima are found at the positions Q = n  .
a
The maximum intensity scales with
the square of the number of periods, the halfwidth is given approximately by
2z . The
Na
3 13
more periods contribute to coherent scattering, the sharper and higher are the main peaks .
Between the main peaks, there are N2 side maxima . With increasing number of periods N,
their intensity becomes rapidly negligible compared to the intensity of the main peaks. The
main peaks are of course the well known Braggreflections, which we obtain when scattering
from a crystal lattice . From the position ofthese Bragg peaks in momentum space, the metric
ofthe unit cell can be deduced (lattice constants a, b, c and unit cell angles (X, ß, y) . The width
ofthe Bragg peaks is determined by the size of the coherently scattering volume (parameters
N, M and P), among other factors . Details will be given in subsequent chapters .
3 .5 Coherent and Incoherent Scattering
In the last section, we assumed that we have the saure interaction potential for all lattice sites .
In the case of xray scattering, this can be well realised for a chemically clean sample, for
example a Ni single crystal. However, neutrons are scattered from the nuclei and for a given
atomic species, there can exist several isotopes with different scattering lengths (five different
isotopes for the case of nickel). Moreover, the scattering length depends on the orientation of
the nuclear spin relative to the neutron spin . In this section we will discuss the effects ofthese
special properties of the interaction of neutrons and nuclei for the scattering from condensed
matter .
Let us assume an arrangement of atoms wich scattering lengths bi on fixed positions R .
this case, the scattering potential writes :
For
2
y 2 t
Mn
Ybi8 ( f^Ri)
i
(3 .30)
The scattering amplitude is obtained from a Fourier transform:
ALQ) =1 bie'Q .R' (3 .31)
When we calculate thé scattering cross section, we have to take into account that thé différent
isotopes are distributed randomly over all sites . Also thé nuclear spin orientation is random,
except for very low températures in extemal magnetic fields . Therefore, we have to average
over thé random distribution of thé scattering length in thé sample :
3 14
du LQ) = ALQJ2
=
e'Q .A' .
* i
e  ~,bje
avérage over the random distribu1n
(3 .32)
In calculateng the expectation value of the product of the two scattering lengths at sites i and j,
we have to take into account that according to the above assumption, the distribution of the
scattering length on the différent sites is completely unconelated . This implies that for i :# j,
the expectation value of the product equals to the product of the expectation values .
Only for i
= j, we have a correlateon, which gives an additional term describing the mean quadratic
deviation from the average :
l 1_ ( b~ ( b )  (b)2
i :# j
\bibj/  1 2 2 /
i \b / ?\b/ \b/l V
\
(b  } =j
((b  (b~)2~ = lb2  2b(b~ + (b)2 ~ = (b2 }  (b)2 (3 .33)
Therefore, we car Write the cross section in the following form :
du (Q) (b)2 Y, eiQ.RI
i
2
" coherent"
(3 .34)
"incoherent"
The scattering cross section is as a sum of two terms.
Orly the ferst term contains the phase
factors e' 4 .x , which result from the coherent superposition of the scattering from pairs of
scatterers . This term takes into accourt interference effects and is therefore named coherent
scattering . Orly the scattering length averaged over the isotope and nuclear spin distribution
enters this term .
The second term in (3 .34) does not contain any phase information and is
proportional to the number N of atours (and not to NZ !) . This term is not due to the
interference of scattering from different atours . As we car see from (3 .33) (lire i = j), this
3 15
terni corresponds to thé scattering from single atoms, which subsequently superimpose in an
incoherent manner (adding intensities, not amplitudes!) . This is thé reason for thé intensity
being proportional to thé number N of atoms . Therefore thé second terra is called incohérent
scattering. Coherent and incoherent scattering are illustrated in figure 3 .6 .
Scattering from the
regular mean lattice
~> interfrence
Nx
Scattering from randomly
distributed defects
~> isotropic scattering
Fig. 3.6: Tivodimensional illustration ofthé scattering processfrom a lattice ofN atoms of
a given chemical species, for which tira isotopes (small dotted circles and large
hatched circles) exist. The area ofthé circle represents thé scattering cross section
of thé single isotope. The incident wave (top part of thé figure for a special
arrangement ofthé isotopes) is scattered coherently only from thé average lattice .
This gives rise to Bragg peaks in certain directions . In thé cohérent scattering only
thé average scattering length is visible. Besides these interférence phenomena, an
isotropic background is observed, which is proportional ta thé numberN ofatoms
and to thé mean quadratic déviation from thé average scattering length. This
incohérentpart of thé scattering is represented by thé louverpart ofthéfigure.
The most prominent example for isotope incohérence is elementary nickel . The scattering
lengths ofthé nickel isotopes are listed together with their natural abundance in table 3 .1 [3] .
The différences in thé scattering lengths for thé various nickel isotopes are enormous . Some
isotopes even have negative scattering lengths . This is due to resonant bound states, as
compared to thé usual potential scattering .
3 16
Tab . 3.1 : The scattering lengths of the nickel isotopes and the resulting scattering length of
natural 28Ni [3] .
Neglecting the less abundant isotopes 61Ni and 64 Ni, the average scattering length is calculated
as :
(b) ~~ [0.6814.4+0.262.8+0.04( 8 .7)1fnz ~t 10.2fm (3 .35)
which gives the total coherent cross section of
=> 6 coherent = 4;r(b~2
z 13 .1 barn (exact : 13 .3(3)bam) (3 .36)
The incoherent scattering cross section per nickel atoms is calculated from the mean quadratic
deviation :
I ooherent  4z10 .68(14 .410.2)2+0 .26(2 .810.22
+0 .04 .(8 .7 10.2 2 1 fm 2 (3 .37)
5 .1barn (exact : 5 .2(4)barn)
Values in parentheses are the exact values taking into account the isotopes 61Ni and 64Ni and
the nuclear spin incoherent scattering (sec below) .
From (3 .36) and (3 .37), we learn that the
incoherent scattering cross section in nickel amounts to more than one third of the coherent
scattering cross section.
3 17
The most prominent example for nuclear spin incoherent scattering is elementary hydrogen .
The nucleus of the hydrogen atom, the proton, bas the nuclear spin 1 = '/z. The total nuclear
spin of the system H + n can therefore adopt two values : J = 0 and J = 1 . Each state has its
own scattering length : b for the singlett state (J = 0) and b+ for the triplett state (J = 1) 
compare table 3 .2 .
Total Spin Scattering Length Abundance
J=0 b_=47.5fm _1
4
J=1 b+ =10.85 fin _3
4
_  3 .739(1) fin
Tab . 3 .2: Scattering lenghs for hydrogen [3] .
As in the case of isotope incoherence, the average scattering length can be calculated:
(b)  [1 ( 47.5) +  . (10 .85~~ fin = 3.74fin (3 .38)
This corresponds to a coherent scattering cross section of about z 1.76 barn [3] :
=> 6coherent = 4;~b~ 2 =1 .7568(10) barn (3 .39)
The nuclear spin incoherent part is
average :
again given by the mean quadratic deviation from the
07nuclearspin =4zC4(47 .5+3.742 +3 10.85+3 .74)2
J
fin 2 =80 .2 barn
incoherent
(exact: 80 .26(6) barn) (3 .40)
Comparing (3 .39) and (3 .40), it is immediately clear that hydrogen scatters mainly
incoherently . As a result, we observe a large background for all samples containing hydrogen .
3 18
We note immediately that we should avoid all organic glue for fixing our samples to a sample
stick. Finally, we note that deuterium with nuclear spin 1 = 1 bas a much more favourable
ratio between coherent and incoherent scattering :
6Dh. = 5.592(7)barn ; 6D. = 2.05(3)barn (3 .41)
The coherent scattering lengths of hydrogen (3.74 fin) and deuterium (6.67 fm) are
significantly different . This can be used for contrast variation by isotope substitution in all
samples containing hydrogen, i . e . in biological samples or soft condensed matter samples,
see conesponding chapters .
A further important element, which shows strong nuclear incoherent scattering, is vanadium .
Natural vanadium consists to 99,75 % of the isotope "V with nuclear spin 7/2 . By chance, the
ratio between the scattering lengths b+ and b of this isotope are approximately equal to the
reciprocal ratio of the abundances . Therefore, the coherent scattering cross section is
negligible and the incoherent cross section dominates [3] :
6 oh
=0.01838(12)barn ;
6vcoh = 5.08(6) barn (3 .42)
For this reason, Bragg scattering of vanadium is difficult to observe above the large
incoherent background . However, since incoherent scattering is isotropie, the scattering from
vanadium can be used to calibrate multidetector arrangements .
Here, we will not discuss scattering lengths for further elements and refer to the values
tabulated in [3] .
3 .6 Magnetic Neutron Scatering
So far, we have only discussed the scattering of neutrons by the atomic nuclei . Apart from
nuclear scattering, the next important process is the scattering of neutrons by the magnetic
moments of unpaired electrons . This socalled magnetic neutron scattering cornes about by
the magnetic dipoledipole interaction between the magnetic dipole moment of the neutron
and the magnetic field of the unpaired electrons, which has spin and orbital angular
momentum contributions (see figure 3 .7).
3 19
Fil Schematic illustration of the interaction process of a neutron with the atomic
magnetic moments via the dipole interaction .
This magnetic neutron scattering allows us to study the magnetic properties of a sample on an
atomic level, i . e . with atomic spatial and atomic energy resolution . A typical problem
studied is the determination of a magnetic structure, i . e . the magnitudes and arrangements of
the magnetic moments within the sample . Besides the wellknown and simple ferromagnets,
for which all moments are parallel, there exists a whole zoo of complicated ferai and
antifenomagnetic structures, such as helical structures, spin density waves, etc . (compare
figure 3 .8) .
Fil Schematic illustration of the magnetic structures of the hexagonal rare earth
metals. Within the hexagonal basal plane, all moments are parallel. The figure
shows the sequence of moments in successive planes along the hexagonal caxis .
Besides simple ferromagnetic phases ( , helical (e), conical (d) and caxismodulated
structures (b) etc. are observed.
320
These magnetic structures can be understood on the basis of magnetic interactions, which
again can be determined by neutron scattering from measurements of the magnetic excitation
spectra. Magnetic structures are only stable in a certain range of theromdynamic parameters,
such as temperature, pressure or magnetic field . As we approach the limits of a stability
region, magnetic phase transitions into a différent magnetic phase occur. An example is thé
transition from a longrange magnetic order at low temperatures to a paramagnetic high
temperature phase . By means of neutron scattering, thé spectra of magnetisation fluctuations
close to a magnetic phase transition can be determined . Such measurements provide thé
experimental foundation of thé famous renormalisation group theory ofphase transitions .
In what follows, we will give an introduction into the formalism of magnetic neutron
scattering . Again, we will restrict ourselves to the case of elastic magnetic scattering .
Examples for magnetic scattering will we given in a later chapter.
To derive thé magnetic scattering cross section ofthermal neutrons, we consider thé situation
shown in figure 3 .9 : a neutron with thé nuclear moment gN is at position R with respect to an
electron with spin S, moving with a velocity _ve.
Fit. 3 .9 : Geometryfor thé dérivation ofthé interaction between neutron and electron .
Due to its
electron according to :
magnetic dipole moment, the neutron interacts with the magnetic field of the
(3 .43)
32 1
Here, the magnetic moment ofthe neutron is given by :
IU n =YnuN'6
(3 .44)
a denotes the spin operator, gN the nuclear magneton and yN = 1 .913 the gyromagnetic factor
ofthe neutron . The magnetic field B of an electron is due to a spin and orbital part B = Bs +
BI, The dipole field of the spin moment is given by :
As =0x R 3
> 'ue = 2jUB 'S (3 .45)
The field due to the movement ofthe electron is given according to BiotSavart :
e v e x R
B L
=
c R3
(3 .46)
The magnetic scattering cross section for a process, where the neutron changes its wave
vector from k to k' and the projection of its spin moment to a quantisation axis z from az to az
can be expressed within the first Born approximation :
du(_
2
mn I/k~6 _
) ,IVmIk6_)I2
2zh 2
(3 .47)
As mentioned, we only consider the single differential cross section for elastic scattering .
Introducing the interaction potential from (3 .43) to (3 .46) in (3 .47), we obtain aller a lot of
algebra [4, 5] :
_d6 _ ( )2  1
YnrO 6_ , 6
dS2
~ 2

f~B (
(3 .48)
The prefactor ynro has the value ynro = 0.539  1012 cm = 5 .39 fin . Here, M 1(Q) denotes the
component of the Fourier transform of the sample magnetisation, which is peipendicular to
the scattering vector Q :
322
M1LQ)=QMQ)xQ
M(Q)= IM (r)e i Q " d 3 r
(3 .49)
(3 .50)
The total magnetisation is given as a sum of the spin and orbitalangular momentum part
according to :
M~r)=MS~?"~+ML~r)
MS (L)= 2PB'S (?" ) = 2PBYd(i"Yi).Si
i
(3 .51)
(3 .48) tells us that with magnetic neutron scattering, we are able to determine the
magnetisation M(r) in microscopie atomic spatial coordinates r . This gives a lot more
information as a simple macroscopic measurement, where we obtain the ensemble average of
the magnetisation over the entire sample . We also see from (3 .48) that the orientation of the
nuclear spin momentum of the neutron (represented by az) plays an important role in
magnetic scattering . This is not surprising, since magnetism is a vector property of the sample
and obviously there should be an interaction with the vector property of the neutron, its
nuclear magnetic moment . Therefore, the analysis of the change of the direction of the
neutron nuclear moment in the scattering process should give us valuable additional
information as compared to a determination of the change of energy and momentum direction
of the neutron alone . These socalled polarisation analysis experiments are discussed in the
following chapter. For our present purposes, we will completely neglect these dependencies .
Finally, to obtain an idea of the size ofmagnetic scattering relative to nuclear scattering, we
can replace the matrix element in (3 .48) for a spin 1/2 particle by the value 1 qB . This gives us
an "equivalent" scattering length for magnetic scattering of 2.696 fm for a spin '/z paiticle .
This value corresponds quite well to the scattering length of cobalt, which means that
magnetic scattering is comparable in magnitude to nuclear scattering.
In contrast to nuclear scattering, we obtain for magnetic scattering a directional term : neutrons
only "see" the component of the magnetisation peipendicular to the scattering vector (see
figure 3 .10) .
323
Fig. 3.10 : For magnetic neutron scattering, only the component M of the magnetisation
perpendicular to the scattering vector Q is ofrelevance.
That only M gives rise to magnetic neutron scattering, can be understood from the notion
that neutrons are scattered from the dipolar field of the electrons . This is depicted for two
différent geometries in figure 3 .11 . For thé case that thé magnetisation is parallel to thé
scattering vector, thé planes for equal phase factor cut though thé dipolar field in such a way
that due to symmetry reasons, thé field averaged over these planes vanishes . This is no longer
thé case, ifthé magnetisation is perpendicular to thé scattering vector. This special directional
dependence allows it to determine thé orientation of magnetic moments relative to thé lattice .
M il
Q
Fie. 3.11 : Illustration ofthe directional dependencefor the scattering froin a dipolarfzeld: in
the case where M I I Q the dipolar fzeld averaged over planes with equal phase
factors is zero, so that no magnetic scattering appears .
A second speciality of magnetic scattering as compared to nuclear scattering is thé existence
of thé socalled formfactor. The form factor describes thé fact that thé scattering amplitude
drops with increasing momentum transfer . This occurs because thé object, from which we
scatter, namely thé électron cloud of an atom, bas a size comparable to thé wave length of
thermal neutrons . Since thé distribution of thé magnetic field for spin and orbital angular
momentum is completely different (compare figure 3 .12 for thé case of a classical Bohr orbit),
different Qdependencies ofthé corresponding form factors result (compare figure 3 .13) .
324
Orbital magnetic spin
angular
,, momentum
momentum field distribution
Fit. 3.12: Schematic illustration of the magnetic field distribution due to spin  (S) and
orbital (L) angular momentum in the case ofa Bohr orbit The magnetic field due
to the spin moment is much more spread out than the one due to the orbital angular
momentum.
1 .0
ô
0 .8
E
ô 0 .6
a>
. 0 .4 ß
O C
0 .2
0 .0
= Chromium
0 .0 0 .2 0 .4 0 .6 0 .8 1 .0
sin(O/~ )
Fig. 3.12 : Formfactor ofCr [7, 81 . Due to the different distribution of the magneticfeldfor
S and L according tofigure 3 .11, a more rapid decrease ofthe scattering amplitude
as a function of momentum transfer resultsfor the spin momentum. For the xray
form factor, the innen electrons play an important yole, too. Therefore, the xray
formfactor drops sloiver as compared to the magnetic formfactor. Finally, on the
Â length scale of the thermal neutron ivave length, the nucleus is pointlike.
Therefore, nuclear scattering is independent ofthe momentum transfer.
325
Since the scattering amplitude is proportional to a Fourier transform of the scattering power
density in direct space, the scattering amplitude decreases faster with momentum transfer if
the scattering occurs from a larger object in direct space . Since the unpaired magnetic
electrons are located in the outermost electronic shells, the magnetic form factor drops faster
than the xray form factor. Compared to the natural length scale of the neutron wave length,
the nucleus is pointlike, which results in a scattering amplitude being independent of
momentum transfer . Finally, we want to mention that the magnetic form factor can in general
be anisotropic, if the magnetisation density distribution is anisotropic .
How the form factor comes about is most easily understood in the simple case of pure spin
scattering, i . e . for atoms wich spherical symmetric (L = 0) ground state, such as Mn2+ or Fei+ .
Moreover, the derivation is simplified for ionic crystals, where the electrons are located
around an atom . In figure 3 .13 we defme the relevant quantities for a derivation.
FilDefinition ofthe relevant quantitiesfor a derivation ofthe spinonlyformfactor.
We denote the spin operators ofthe electrons of atour i with sik. The spatial coordinates ofthe
electron number k in atom i are lk = R + t k, where R denotes the position vector to the
nucleus of atom i. Now we proceed to separate the intraatomic quantities . We can write the
operator for the magnetisation density as :
MS (Z:)= 211BY6(!:!:ik)»!iik
ik
(3 .52)
The Fourier transform of this magnetisation density is calculated to:
326
aQ . r 3 àQ . N . QR . aQ .t k
_MLQ) = fMS (N)e d r =le'Sik=je  t1e ' 'S ik (3 .53)
ik i k
To calculate the scattering cross section, we now have to determine the expectation value of
this operator for the quantum mechanical state of the sample averaged over the
thermodynamic ensemble . This leads to
M(Q) = 2 PB  fm(Q) 7,eiQ .Rt  Si (3 .54)
The single differential cross section for elastic scattering is thus given by :
2
_du = eiQRi ~ (Tnro)2 f.LQ)L Si1 (3 .55)
M
i
Here, fm(Q) denotes the form factor, which is connected wich the spin density of the atour via
a Fourier transform :
.fm (Q)= fps(?")eiQ .rd3r (3 .56)
Atom
With the form (3 .55), we have expressed the cross section in simple atomic quantities, such as
the expectation values of the spin moment at the various atoms . The distribution of the spin
density within an atom is reflected in the magnetic form factor (3 .56) .
For ions with spin and orbital angular momentum, the cross section takes a significantly more
complicated foira [4, 5] . Under the assumption that spin and orbital angular momentum of
each atour couple to the total angular momentum J (L/Scoupling) and for rather small
momentum transfers (the reciprocal magnitude of the scattering vector has to be small
compared to the size of the electron orbits), we can give a simple expression for this cross
section in the socalled dipole approximation :
_ 2 J 1 Q' ,I2
dS2(Ynro) ' .Îm(QJ~Ji1eaR .
i
(3 .57)
327
Here the magnetic form factor writes :
fm(Q) = (jo(Q)+c2(j2(Q) (3 .58)
gJ denotes the Lande gfactor, CZ = ? 1 and
gJ
(jl (Q) = 4z 1jl(Qr)R2 (r)r 2dr (3 .59)
0
are the spherical transforms of the radial density distributions R(r) with the spherical Bessel
functions ji(Qr) . For isolated atoms, the radial part R(r) has been determined by HartreeFockcalculations
and the fonctions (j0(Q)~ and (j2(Q)) in (3 .58) have been tabulated [6] .
After having introduced the principles of magnetic scattering, we will discuss applications in
chapter 16 .
References
[1] J . M. Cowley "Diffraction Physics"
NorthHolland, Amsterdam 1990
[2] B . W . Batterman, H . Cole "Dynamical Diffraction of X Rays by Perfect Crystals",
Reviews of Modern Physics 36 3, 681  717 (1964)
[3] V . F . Sears "Neutron Scattering Length and Cross Sections",
Neutron News 3 (1992), 26  37
[4] G . L . Squires "Introduction to the theory of thermal neutron scattering" Cambridge University
Press, Cambridge (1978)
[5] S . W . Lovesey "Theory ofneutron scattering from condensed matter" Volume 2 : Polarisation
effects and magnetic scattering, Clarendon Press, Oxford (1987)
[6] A . J . Freeman & R. E . Watson, Acta Cryst. 14 (1961), 231
[7] J . Strempfer, Th . Brückel et al Eur . Phys . J. B 14 (2000), 63
[8] J . Strempfer, Th . Brückel et al Physica B 267268 (1999), 56
328
Schweika Analysis
Polarization
W .
4 . Polarization analysis
W .
Schweika
4 .1 Introduction
Most typical neutron experiments are concerned only with the intensities related to a
specific change in momentum and energy of the neutron in a scattering process yielding
information about the structure and dvnamics of the considered svstem of interest . However,
since the neutron has a spin it interacts with the magnetic moment of the electron
shells, and the scattering amplitude depends also on the nuclear spins of a sample . There
are cases where one is able to distinguish magnetic from nuclear scattering, either from
the different form factor dependence or from a temperature variation across a magnetic
phase transition . Here we shall discuss the technique of using polarized neutrons and the
analysis of their final polarization after the scattering process . It is a powerful method
for distinguishing the varions possible scattering scattering contributions,  i. c . magnetic,
nuclear coherent, and nuclear spinincoherent scattering , and to separate them
from each other by experimental means without further assomptions . Its application to
neutron spin echo techniques will be discussed in chapter 11 .
The theoretical foundation for polarized neutron studies lias essentially been set by the
early works of Halpern and Johnson[1], Maleyev[2], and Blume[3] . A good introduction
is given in the classical work of Moon et al [7], sec also [4, 5] . This lecture will net treat
the full complexity of magnetic scattering (sec [2, 3]) . Emphasis will be given rather to
basic ideas following Refs . Schärpf [6] and Moon et al [7] .
4 .2 The motion of the neutron in magnetic fields and experimental devices
The essential characteristics of the motion of a neutron in a magnetic field is the precession
mode, which for simplicity can be considered in a classical treatment[6 ] . In tact,
even the quantum mechanical treatment, which introduces Pauli spin matrices into the
Schr5dinger equation, is effectively a classical treatment considering the origin of these
matrices . They result from the problem of mapping three dimensions onto two by intro
ducing a complex component and were treated by Cayley and Klein (1897) [8] describing
the classical problem of a spinning top .
Classical mechanics shows that a torque exerted on a magnetic moment tî by a magnetic
field H inclined at an angle B relative to the magnetic moment causes the magnetic
moment of the neutron to precess about the direction of the field with the Larmor frequency
WL . The precession frequency is independent of the angle B . Different to the
motion of a spinning top in a gravity field the neutron's motion shows no nutation, its angular
momentum L  hS and its energy is a constant . S ( 2) denotes the spin quantum
number of the neutron and h is Planck's constant divided by 27r . The relation between
angular momentuni L and magnetic moment tî defines the gyromagnetic ratio y
An applied magnetic field will tend to align this magnetic moment and exerts a torque . No
force is exerted by a homogeneous field, so that the resulting equation of motion simply
says that the change of L in time is normal to L and H, i. e . a precession :
L = yLxHLXW L (4 .2)
with  yH = WLand y/27r  2916 .4Hz/Oe .
A magnetic guide field defines a quantization axis and can bc used to maintain the
direction the spin and thus the polarization of the neutron beam, sec Fig . 4 .1 . The
neutron moments will align either parallel or antiparallel . Guide fields are typically weak
so that the sample magnetization is net significantly influenced, but sufficiently stronger
than for instance the magnetic field of the earth or any other stray magnetic fields frein
the surrounding . Such a guide field may vary is space and two important limits are of
interest (sec Fig . 4 .2 and Fig . 4 .3) :
slow field change :
this socalled adiabatic case means that H slowly changes its
direction with a frequency that is small compared to the Larmor frequency, cW « WL,
such that a neutron moving with a velocity EN keeps its precession mode around the
spatially varying H . This cari be achieved by sufficiently long path fer the variation
of the field or by a sufficiently strong the field H (a WL) .
sudden field change : If the field direction changes suddenly, the polarization of the
neutron cannot follow . Two opposite guide fields can be separated by a current
42
40
E¢. 0. or P
travel
03
E4 é0 Ki direction
E4 (»
0,
l
1 1
^4~ P
Fig .5a Guide field for longitudinal Fig .5b Guide f eld far longitudinal
polarisation, P Il H , the polarisation, _P antiparallel _N
small arrow is the spin of the
neutrons
Fig .Sc Guide fietd for transversal
polarisation, P parallel N
Eig .5d Guide field for transversal
polarisation, P antiparallel N
Figure 4 .1 : Neutrons in a guide field H with spins parallel or antiparallel[6] .
sheet, for example, and polarized neutrons parallel to the firnt guide field will be
kept in an antiparallel orientation to the second field when passing the sheet . This
case w » WL is also used in ends operating as spin flippers .
In neutron scattering experiments with polarized neutrons, the principle of slow field
changes is used, for instance, to align the polarization along a particular direction ai the
Sample position . As will be Seen in the examples below, the polarizations perpendicular
and parallel to the scattering vector and the magnetization of the Sample are of particular
interest . Usually, we assume that the field at the Sample position is sufficiently weck so
Chat the magnetization of the Samples remains undisturbed . Using three (orthogonal)
pairs of ends the polarization can be turned arbitrarily into any direction at the Sample
position to probe the orientation the magnetization of a Sample . While turning the
neutron polarization ai the Sample position by an additional field H and Chus keeping the
neutrons moments in guide fields one can only distinguish scattering processes in which
the spin direction is preserved (nonspin flip) or reversed (spinflip) for a given direction .
In general, there may be an arbitrary angle of rotation of the neutron polarization, and
it can be measured only if the Sample is in a fieldfree space . Superconducting sheets
are ideal for shielding the Sample environment from external magnetic fields (sudden
43
ir v s ftft 3956
2 s 2 0.81[X]
80 cm
Figure 4.2 : Polarisation of neutrons follows field direction in the adiabatic case : W « WL. [6]
use this principle .
guide field
neutron spin antiparalle
to guide field
neutron spin parallel
guide field'
field near the
current sheet
Figure 4 .3 : Neutron spin keeps its orientation for sudden field changes : W » W L .[6]
field changes) . Such an sample environment with zerofield is realized in a device called
cryopad ([9] F . Tasset, ILL) . It allows one to exploit all possible scattering channels with
independent initial and final polarizations along xyz in spinflip or nonspin flip mode
(which takes 3 x 3 x 2 = 18 measurements) .
An important device for working with polarized neutrons is a spin flipper, see Fig . 4.4 .
One cari use the Larmor precession in a coil to turn the neutron spin . The socalled
Vlezei coil is a long rectangular coil . The field inside (H = N  Ill) is perpendicular
to the polarization and the travel direction of the neutron . Guide fields outside are
necessary te avoid depolarization by the earth field or undefined stray fields, but need to
44
1'10 tarns
1 MM ~2( Al WIRE (enamel1ed)
Figure 4 .4 : Neutron Fspin flipper (Mezeiflipper) . The neutrons perform half of a Larmorprecession
inside a long rectangular coil . The field H, is perpendicular to spin orientation
and te the travel direction of the neutron and has to be adjusted to the speed of the
neutrons . In order te compensate the guide field one may either tilt the flipper or use a
correction coil[10] . (Fig . from [6] .)
be compensated inside the coil . Monochromatic neutrons passing through the coil they
experience a sudden field changes at the wires and perform a precession inside . A rotation
of 180 degrees (7rflip) is realized by field H, determined by yH,  d/v = 7r, which gives
H, = 67.825 Oe  (Â cm)/ (.\ d) ~ 20 Oe for A = 3.4Â and d = 1 cm . There are other types
of spin flippers using for instance radiofrequency resonators .
By experimental means it is possible to choose the initial polarization of the neutron as
either spinup or spindown, and the polarization analysis requires also the experimental
ability to determine the final polarization of the neutron after the scattering process . In
practice, there are three types of polarizing devices :
e a crystal monochromator and Bragg reflection, where the interference of the magnetic
and nuclear part of the scattering amplitudes is constructive for crie spin state
and destructive for the opposite spin state;
e supermirrors with a magnetic layered structure which shows total reflection for one
spin state only ;
e filters that produce by absorption or extinction a polarized beam in transmission .
3He is of particular importance . It exhibits high absorption for neutrons having
their spins antiparallel aligned te the spin of the 3He nucleus .
45
Some polarizers using Bragg reflections, for instance the (200) reflection from Co o.92Fe o .o8
alloy crystals, exhibit a very high degree of polarization (~ 0 .99 for the whole setup :
initial polarization  spinflipper  final polarization) . However, only a narrow band of
wavelengths can be used and also the accepted divergence is small, which could be demanding
in terms of scattering intensities . An experimental setup for polarization analysis
using the total reflection of long supermirrors or shorter benders (a stack of such
supermirrors) perform also reasonably well in terms of polarization (typically ~ 0 .95
or better), and in addition a comparatively wide band in wavelength or energy of cold
neutrons is accepted (particularly useful for timeofflight spectrometers) . For thermal
neutrons 'Hefiltern seem to be a very appropriate choice. The device does not interfere
with the divergence, which han been set otherwise in the experiment . The beam transmission
and degree of polarization can be optimized by varying the gas pressure and can
be matched to the spectrum of neutron energies . The most efficient performance is, however,
a compromise between intensity and a modest degree of neutron polarization (say
about 50%) . Of course, this requires to perform corrections due to the finite degree of
polarization . However, such corrections can easily be performed and the final result for
the scattering intensities depend just on the accuracy with which ones knows the degree
of polarization .
4 .3 Polarization and scattering processes
4 .3 .1 Coherent nuclear scattering
Within the firnt Born approximation the scattering crosssection is determined by
du Mn ) 2 ~kS~
d9 (2z1i
(4 .3)
First, we calculate the matrix element of the interaction potential V between the
initial and final states for pure nuclear scattering at a nucleus wich spin I = 0, i . e . the
scattering amplitude A(Q) (nee chapter 3) . With b(Q) _ ~, z btie i Q.r s the matrix element is
A(Q)  (Sz b(Q) Sz)  b(Q)(S,' l Sz)
NSF
SF
(4 .4)
46
It follows that the nuclear scattering for nuclei wich zero spin is purely "nonspinflip"
scattering, i . e . there are no scattering processes that turn the neutron spin around . In
particular this is valid for all isotopicincoherent scattering and coherent nuclear scattering
. Silice the coherent scattering amplitude represents the average nonfluctuating part
of the total actual scattering amplitude, it is the part that is also independent even of
any possibly existing nuclear spin.
4 .3 .2 Magnetic scattering
The matrix element of the interaction potential for pure magnetic scattering between the
states k and k' has already been introduced in the previous chapter 3 . The scattering
amplitude results to
A(Q)  (Sz
`ynro
ML(Q)IS,)
.  (Szior,I sz) MLa (Q) .
2Ms 2Ps a
`ynro _
Here y, 1 .913 denotes the magnetic dipole moment of the neutron expressed in
nuclear magnetons PN = 5 .051 . 10 27 JIT, and ro = 2 Z
is the classical electron radius .
Q , denotes the Paulispin matrices :
(4 .5)
0 1 0 i
i1 0 )
1 1 y, (
0
(4 .6)
Writing briefly the spinup and down states as 1+)  (
we obtain the following relations :
1
0
~ and 1) _ (
0 1 ~
respectively,
or X l +) = H , = W
or Y.H = i H , Or YH =  i H
(4 .7)
Or 'M  W ,  H .
Inserting there relations into Eq. (4 .5) we obtain the matrix elements (scattering amplitudes)
for spinflip and nonspin flip scattering :
+ + (NSF)
A(Q)
ynro
2/IB
MLZ (Q)
(Mlm(Q)  i VIL I (Q))
for
 (NSF)
+  (SF)
(4 .8)
(L ~, (Q) + i M L1(Q))
 + (SF)
47
Different to the coherent nuclear scattering now we cari also observe "spinflip" processes
that reverse the neutron spin direction . Recall that ML (Q) is the perpendicular
component of VI with respect to the scattering vector Q, and the neutron polarization
has been chosen parallel to an external field H z . We obtain two rules for the magnetic
scattering :
The "spinflip" processes are observed for the component 1!I+ (Q) that is perpendicular to
the neutron polarization . The "nonspin flip" processes are observed for the composent
of ML(Q) that is parallel to the neutron polarization .
4 .3 .3 Nuclear spindependent scattering
If the neutron is scattered from a nucleus wich nonzero spin the compound may form
a singulett or triplett state where the neutron spin Q is astiparallel or parallel to the
nuclear spin 1 with different scattering lengths b_ and b+ respectively. The case of nuclear
spindependent scattering cari be formally treated in analogy to the magnetic scattering
by introducing the scattering length operator
b=A+BuI (4 .9)
with A = (I+1)b + +Ib b+  b
and B
21+1
= 21+1 '
where I and o denote the nuclear spin operator and the neutron spin operator respectively.
The scattering amplitude A(Q) will have the came form as given in Eq . (4 .8) only
VIL (Q) has to be replaced by the nuclear spin operator I .
ABI,
A(Q) = (S (Z) JA+B or  I I s(z) )
B (l x  il,)
+
SF
While in Eq . (4 .5) M1 is assumed to represent the thermodynamic expectation value, the
thermal average has te, be calculated now for the different nuclear spin orientations and
for the firnt matrix element in Eq . (4 .10) . Except for some unusual cases, we may expect
that the orientation of nuclear spins is given by a random distribution, i . e .
(IX ) _ (I,,) _ (IZ) = 0
48
Therefore the nonspin flip matrix elements equal to A, arid (as derived before) the coherent
nuclear scattering is proportional to the square of b ol ,, identifying A = b = bcoh .
dQ (±± ,NSF )
dS2 coherent
 b2 L e.`i r)
r,r,
(4 .12)
The nonspin flip matrix elements vanish, however, for the incoherent scattering, which
is proportional to bz  b 2 , and we have to consider the thermal average of the squares of
the matrix elements . Since
(Ix) (Iy) (Iz) = 3I(II + 1)
(4 .13)
from Eq . (4 .l0) one obtains the spinincoherent scattering (per atom) :
dQ (±  :±,NSF)  (b2 _ b2)NSF  1 (B 2 I(I + 1))
d9 spinincoherent 3
(4 .14)
du (+~'  +  SF)
(b2  b2 )SF  2 (B 2 I(I + 1))
dP spinincolterent 3
(4 .15)
113 of the spinincoherent part of the nuclear scattering is nonspin flip scattering and
213 of it is spinflip scattering independent of the (direction) of an external field H .
In arialogy to the coherent scattering amplitude bcoh, orie may define the (spin) incoherent
scattering amplitude bin , \ B 2 I(I + 1) .
4 .3.4 Rules for separation
From the preceding discussion we cari summarize some useful rules for separating different
scattering contributions .
If we may neglect magnetic scattering, the coherent and spinincoherent
scattering is obtained from the spinflip and nonspin flip scattering :
du du NSF 1 du SF (4 .16)
d9 coherent d9 2 d9
If a part of the scattering is of magnetic origin, a field variation is required (perpendicular
and parallel to Q) to separate the magnetic crosssection :
dor 3 du SF (4 .17)
d9 spinincoherent 2 d9
field/polarization spinflip intensities nonspin flip intensities
H I I Q umag + 5Qinc + QBG 07coh + ()umag + 3Qinc + 07BG
2Umag + 3Qinc + QBG
(Tcoh + 2Umag + 3(Tinc + QBG
49
where QBG denotes the background .
Hence, the magnetic crosssection is separated by
dQ dor NSF d07 NSF dor SF dor SF
2 2
d9 mag (de L d9 ) (de I I de i
(4 .18)
and all nuclear scattering contributions and the background cancel in the differences of
Eq . (4.18), since they are independent of the magnetic field[11 ] .
For a multidetector instrument it is possible to fulfill the condition P L Q wich P = Pz
perpendicular to the scattering plane, however, P I j Q cannot be realized simultaneously
for all different scattering angles . However, a similar expression lias been obtained for
paramagnetic scattering [12] . Therefore, two measurements are required with the two
polarizations P x and P y lying in the scattering plane perpendicular to eacli other . Using
(MxMx ) _ (MyM y ) _ (MzMz) and COS2 a + sine a = l, we may substitute (valid for both
spinflip and nonspin flip term)
dQ dQ _ dQ dQ
d9 I I + d9 L d9 x + dQ y
4 .19
(trivial, if x lies in direction of Q) . Hence, the paramagnetic scattering is given by [12] :
d2 or
dQdW paramagnetic
d2a SF d2o SF d2a SF
2 (df2dwx + iS2dwy  2 df2dwz )
2 ( d2, NSF + d2, NSF  2 d2, NSF
d9dwx d2dwy dQdwz )
(4 .20)
Furthermore, the coherent scattering and the spinincoherent scattering can be separated
from each other and from paramagnetic scattering by the following useful combinations
[12] :
d207 NSF
dQdwcolterent
d9dwz
1 d 2 07 1 d2 07
2 dQdwparamagnetic 3 dQdwspinincolterent
(4 .21)
d 2 07
dQd~jspinincoherent
_
One may note, however, that  different from the Separation for (para)magnetic scattering
 the above relations do not compensate for possible background contributions .
Furthermore, the above equations hold for ideal experimental conditions for polarization
and flipping ratio .
3 d207 SF d2Q SF d20r SF\
  .
2 13 dS2dWz dPdwx dS2dW y I (4 .22)
In general, depolarizing effects may occur at all experimental devices,
and appropriate corrections need to be taken into account . Fig . 4 .5 illustrates that the
410
corrections for the ideal case can easily be performed . The example is given for the case
of coherent scattering and spinincoherent scattering . From the flipping ratio of nonspin
flip scattering to spinflip scattering from either a purely coherent scatterer or a purely
incoherent scatterer the polarization factor of the experimental setup can be determined .
One should note that multiple scattering may alter the expected ideal final polarization as
soon as spinflip processes are involved . Silice from polarization analysis the information
on both scattering channels is available, the possible corrections for multiple scattering
are more reliable as compared to unpolarized experiments .
coherent scattering
spinincoherent scattering
magnetic scattering
I_ 9  2 (I+_  I+
2(I1 + II++ ) '
I
N
C
N
i
i
i i
i
i
i
i
Figure 4 .5 :
1 0 1 0 1
P P P
Nonideal experimental conditions for polarization analysis shown for coherent,
spinincoherent and paramagnetic scattering .
The polarization factor of the instrument,
P < Pideat = 1, can be determined from the flipping ratio SF:NSF for a coherent scatterer,
and one can extrapolate to the ideal conditions .
Furthermore, one should mention the possible interference of nuclear and magnetic
scattering amplitudes ; an example will be given below . The interference properties are
especially of importance for polarizers . Since coherent nuclear scattering is only observed
in nonspin flip scattering, the interference terni cancels as well for the spinflip scattering .
In general, for studies of more complex magnetic systems, e .g. with with noncollinear,
chiral structures or excitations, interference of nuclear and magnetic interference a complete
vector polarization may be necessary [2, 3] . Therefore one has to determine the 3 x 3
Matrix given by the incident and final polarization vector .
4 1 1
4 .4 Applications
We now consider examples of experimental studies wich polarized neutrons and polarizatien
analysis[7] . A scheme of the experiment is shown in Fig . 4 .6 .
Figure 4.6 : The original experimental arrangement of Vloon, Riste and Koehler at the Oak
Ridge reactor (HFIR) : a triple axis instrument with additional equipments for polarization
analysis . CoFe crystals mounted in the gap of a permanent magnet are used on the
first and third axis for the production of the polarized, monochromized beam and for
analysis of scattered neutrons in energy and spin. At the second axis with the sample an
electromagnet is located with a horizontal rotation axis so that the field is easily changed
from vertical to horizontal . Radiofrequency coils with a vertical field are used as flipping
devices . [7]
The firnt example (Fig . 4 .3 .4 shows the isotopicincoherent scattering from Ni . Since
the Niisotopes do not produce nuclear spindependent scattering it serves as an example
for pure nonspin flip scattering . Apparently there are no relevant spinflip scattering
processes .
412
ABA (deg )
Figure 4 .7 : Isotopic incoherent scattering from nickel obtained by rocking the analyzer
crystal through the elastic position . Essentially all scattering is nonspin flip scattering
(++) measured with "flipper off" . In flipper on mode the spinflip data (+) are taken,
In contrast to magnetic scattering the result is independent of the neutron polarization
with respect to the scattering vector Q .[7]
Actually, this example is not trivial, and it is not so straightforward to reproduce this
result . Since at room temperature Ni is a ferromagnet, additional magnetic scattering
is to be expected if the magnetization has any component perpendicular to Q, and a
saturating magnetic field has to be applied to avoid any magnetic demain structure . Such
inhomogeneities typically cause depolarization effects . A much simpler example for pure
nonspin flip scattering would be Bragg scattering which is due to the coherent nuclear
scattering amplitude from a nonmagnetic material, for instance the DebyeScherrer rings
of aluminum or other materials . In practice, the ratio of NSF to SFintensities (ftipping
ratio) for such a measurement is useful to determine the degree of polarization for the
experimental setup .
4 13
Fig. 4 .3 .4 probably represents the first verification of the spinflip and nonspin flip
scattering from a spinincoherent scatterer . The example is Vanadium a typical material
used for absolute calibrations of neutron measurements . The scattering above the
background level shows nearly the ideal intensity ratio 2 :1 for spinflip to nonspinflip
intensities . In particular, hydrogenous materials have large spin incoherent cross sections .
Figure 4 .8 : Nuclearspin incoherent scattering from vanadium obtained by rocking the
analyzer crystal through the clastic position . The flipper off data are proportional te the
(++) cross section and the flipper on data are proportional to the () cross section . In
contrast to magnetic scattering the result is independent of the neutron polarization with
respect to the scattering vector Q .[7]
We recall that for a magnetic system the spinflip and nonspin flip scattering should
depend on the polarization of the neutron with respect to Q . This field dependence is
illustrated in Fig . 4 .9 showing the paramagnetic scattering from MnF 2 . In general, we
expect that the final polarization to vary between 0 and PZ,,tit2al . It is obvious that
this scattering can be distinguished from spinincoherent scattering . Indeed, one can
easily verify that the difference between the spinflip scatterings with polarization P I~ Q
and P L Q is proportional te the (para)magnetic scattering only, free from any other
scattering contributions like coherent nuclear scattering, spinincoherent scattering and
possible background . The saine is truc for the difference of nonspin flip scatterings with
P Ij Q and P L Q, and Fig . 4 .10 shows such a separation of the paramagnetic scattering
from MnF2 powder diffraction data . Measurements with the unpolarized beam show a
background intensity decaying with Q and various Bragg peaks on top . The Bragg peaks
414
i
Figure 4 .9 : Paramagnetic scattering from VInF 2 [7] . The full magnetic intensity is seen in
the SFchannel with P parallel to the scattering vector Q (= k) ;
rotating the analyzer crystal through the elastic position.
5000
É 4000
M
a 3~ai
i
data are measured by
Ô
32000
0
2000
4600
4200
rs
Min
POLARIZATION ANALYSIS
E 800
N
a 400
600
400
im
200
0 .
b
0 10 20 30
SCATTERIN6 ANGLE (dep )
Figure 4 .10 :
pattern . [7]
Separation of the paramagnetic scattering from VInF 2 in a powder diffraction
4 15
.
occur only in the nonspin flip channel, which verifies their nonmagnetic origin.
In the
spinflip channel we see the paramagnetic scattering with a decay that is characteristic
for the form factor of the ion Mn 2+ .
The next example in Fig .
4 .11 shows the separation between nuclear and magnetic
Bragg peaks for aFe 203 .
The magnetic Bragg peaks appear in the spinflip channel only,
while only nuclear Bragg peaks appear in the nonspinflip channel, if P I j Q .
800
. Co
n
ô
C
700
600
500
400
300
200
100
O
700
_
T114 410)1112)(1ÎOi(210)(220)1321)13~)(310)'
NUCLEAR + PEAKS
FLIPPER OFF
I %
W
AI(M)
;
à,
ß .
a~ 1
A9200)
Il I a
,y
1
I
(412)
600
t171)(100) I' 1(21OHtii) (223)(2f0 3f0)
c 500
400
n
300
(311} (333)(334)
r
I
MA6NE TIC PEAKS
PER ON
!NM 1
40 20 30 40
SCATTERING ANGLE (deq)
Figure 4 .11 :
Separation of magnetic and nuclear Bragg peaks for powder diffraction data
from aFe203 . [7]
So far we have discussed the nuclear and magnetic scattering separately.
in general there are possible nonzero matrix elements for both contributions .
However,
Therefore
interference phenomena may occur but only in the nonspin flip channel . In order to
maximize the magnetic signal one chooses the magnetization perpendicular to the scattering
plane .
In cases where the magnetic scattering amplitude is much weaker than the
nuclear amplitude the interference term may be large compared with the pure magnetic
intensity .
Since the polarization of the scattered beam is not changed, and thus already
determined we do not need to perform the polarization analysis in the experiment .
A
useful application of this effect is the determination of the distribution of magnetization
densities .
For instance, the form factor of chromium can be measured in the paramagnetic
phase, inducing a magnetization by an external magnetic field, as shown in Fig . 4 .12 .
D3
a
é
ô
v
08
0.6
0 .4
o Stassis
. . . . .
3d spi
. . . . .. . . 3d orbital
40% spin + 60% orbital
â
0.2
0 .0
......... . . . . .
a
00 0.2 0 .4 0.6 0.8 1 .E
1f2d (Ä t )
Figure 4 .12 : Induced magnetic form factor of Cr at a field of 4 .6 Tesla. Open and filled
circles are experimental data, lines denote theoretical calculations for spin orbital, and
total magnetic moments [13] .
4 17
The results for the magnetization density distribution are obtained by Fouriertransformation
and in comparison by a socalled maximum entropy method, which seems to
give a result of improved reliability .
Figure 4 .13 :
Magnetization density in the (110) plane obtained by Fourier transformation
(top), and by "Maximumentropy" reconstruction (bottom)[13] .
418
With triple axis instruments one can measure only stepbystep specific dynamic structure
factors S(Q, w) of interest . However, multidetector instruments are more efficient for
measuring powders, for timeofflight spectroscopy, or if langer regions in reciprocal space
need to be measured . The first instrument for such purposes is the D7, see Fig . 4 .14, at the
high flux reactor at the ILL in Grenoble ; 32 detectors are equipped for polarization analysis
. The polarizers are benders, curved stacks of polarizing supermirrors, which exhibit
good polarization and transmission properties for subthermal neutrons . In order to cover
Figure 4 .14 : The D7 at the ILL, a multidetector instrument for polarization analysis .
On the right hand side one bank is shown in the nonpolarizing version with analyzers
removed by pneumatic elevators and the collimators inserted instead of the guide fields .
With the spin turner coils the polarization of the neutrons can be rotated into the x,y, or
z direction . [14]
4 19
a large solid angle with polarizers in front of the detectors an enormous amount (6000)
of magnetic multilayers had to be produced . A 7rflipper (Vlezeitype wich a Brookhaven
correction coil) is used in the incident beam .
The following example [14] of a measurement at D7 demonstrates the capabilities of
such an instrument : the dynamic structure factor of liquid sodium, is separated into
the coherent and (spin)incoherent parts . The quasielastic incoherent scattering gives
information about the single particle motion in space and time, while coherent quasielastic
scattering is related to collective relaxations of the ensemble . The measurements
shown in Fig . 4 .15 have been measured on the D7 instrument in timeofflight spectroscopy,
while the presentation is given in the coordinates of energy and momentum transfer .
15
15
10
3 5
3
49.1
1 2 3 1 0 1 2 3
Seattering Vector [X1 ]
Scattering Vector [V]
Figure 4 .15 : Contour plots of (a) the (spin) incoherent scattering and (b) coherent scattering
from liquid sodium at T = 840 K over the plane of energy and momentum transfer
as separated by polarization analysis on D7 . The incoherent scattering is related to the
single particle motion ; the coherent scattering is related to the collective motion . [14] .
The instrument DNS [15] (see Fig . 4 .16) at the research reactor in Jülich is similar to
the D7 . The DNS has a comparably compact design . Different detector banks are used
for standard timeofflight (TOF) mode and polarization analysis (typically combined
with TOF) . They are placed to the right and left, respectively, to the incoming beam .
The polarizers and analyzers are made of a stack of sputtered magnetic supermirrors,
alternating layers of FeCoV/Ti:N with a Gd :Ti absorbing antireflexion layer underneath
[l6] . The monochromatic beam is vertically and horizontally focused . Different to the
present version of the D7 (there are plans for an upgrade) the polarizers have a geometrical
design te use beam focusing on the sample with a substantial gain in intensity . A 1lezeitype
(7r)spinflipper is used in combination with a Brookhaven correction coil, both made
of uncoated aluminum wires (for better transmission as compared to coated Cuwires, for
instance) . The degree of polarization determined frein the intensities of nonspinflip
Figure 4 .16 : The DNS instrument at Jülich equipped for 3dim polarization analysis . The
detector bank to the right of the incoming beam is for unpolarized experiments the one
to the left for polarization analysis . A focusing layout lias been used for the initial and
final polarizers .
4 2 1
scattering to spinflip scattering for a coherent scatterer is rather high, up to 1 III+
0 .98, while on average the performance is about 0 .95 °70 .
The following example is related to studies of structural properties of polymer glassec,
in which polarization analysis can be quite useful . Besides separating the coherent structure
factor, separated incoherent scattering intensities can be used for an intrinsic absolute
calibration . An example is shown in Fig . 417 . In this experiment[17] one bas also used
partial isotopic substitution of H by D to mark and to contrast the sidechains and the
backbone of different polymers (polyalcylmethacrylates) .
2
0
2
'H,
(Ï''CICD, CDCD CD . CD,CD,
0
Figure 4 .17 : Coherent structure factor of a partially deuterated polymer . Note that
by separatinn of the coherent and incoherent scattering one obtains a precise absolute
intrinsic calibration . Two measurements are displayed in the figure (bottom right) [with
.\ = 3 .3 Â (diamonds) and A = 5 .3 Â (circles)] demonstrating the excellent reproducibility
of the data. The peak at lower _C is due to interchain correlations between different
polymer "backbones" and the peak around Q 1 .4Â 1 can be related to inteachain
correlations along the polymer, the ones between the sidechains of a polymer .
422
Current methods for complete polarization analysis of magnetic neutron scattering are
based on zerofield techniques[9], which impose severe limitations and cannot be applied
on multidetector or timeofflight instruments . Recently, a new method for full vector polarization
analysis lias opened new possibilities[18] . Using precessing neutron polarization
on the DNS instrument (Jülich the off diagonal terms of the (3 x 3) polarization matrix
can be determined . It is noteworthy, that polarisation analysis is simultaneously achieved
for all scattering angles and energy transfers, which is of interest for diffuse (inelastic)
magnetic scattering, and also in view of new instruments at spallation sources . This
new method utilises precessing polarisation by operating the flipper in a F/2mode . By
varying the magnetic field integral the precessinn angle at the sample is determined, and
scattered neutrons with a finally nonprecessing polarisation can be analysed . Fig . 4 .18
shows a simulation of scattering processes changing the incident polarization from P X
into a final polarization P y for different scattering angles . Since the final polarisation is
parallel to the magnetic field the polarisation is adiabatically rotated and guided to the
final polarisation analysers .
pII
0
v
iiiif
®5111199®
Figure 4 .18 : Simulation of precessing neutron polarisation analysis for scattering processes
with changes in polarisation from P x to Py .
4 23
An experimental verification of this new technique is shown in Fig . 4 .19 . Here, the
magnetic (100) Bragg peak of an antiferromagnetic MnF 2 single crystal can produce such
a 90 degree rotation of the polarisation . The ordered magnetic structure is collinear, wich
spins pointing into cdirection, which is oriented in between the x and z direction of the
instrument . Varying the field strength of the ycoil, the initial polarisation at the sample
precesses perpendicular to y leading to a final polarisation as shown in Fig . 4 .19 .
neutron polarization analysis
Pxy from Pprecession in xzplane
Blly
M11C11Q
2 2 .5 3 3 .5 4
l y [A]
Figure 4 .19 : Measurement of offdiagonal elements of the polarisation tensor using the
(100) Bragg scattering of antiferromagnetic MnF 2 , in which the magnetic moments are
aligned parallel to the caxis . The precession angle in xzplane of the initial polarisation
depends on the field By (x I y ), and only neutrons with final polarisation Py are detected .
Appendix
Units :
magnetic field H :
Oersted Ampere/meter (SI) = 47r x 103
(cgs)
magnetic induction B = ,uo uH, po = 1.2566 x 10sm kg C2 (=1 in cgsunits) :
Tesla (SI) = kg / (sec2 Ampere) = 10 4 Gauss (cgs)
For cgsunits and vacuum (N = 1), H in Oe corresponds to B in Gauss .
Earth magnetic field : ~ 15 A/m ~ 0 .19 Oe .
424
References
[1] O . Halpern and M.R . Johnson, Phys . Rev . 55 898 (1939) .
[2] S .V . Maleyev, Zh . Eksperim . i Teor . Fiz . 33, 129 (1958) [English Translation : Soviet
Phys.JETP 34, 89 (1958)] ; S .V . Maleev, Zh. Eksperim . i Teor . Fiz . 40, 1224 (1961)
[English Translation : Soviet Phys.JETP 13, 860 (1961)] .
[3] M . Blume, Phys. Rev . 130, 1670 (1963) ; Phys . Rev . 133, A1366 (1964) .
[4] G .L . Squires, Introduction to the theory of thermal neutron scattering, Cambridge
University Press, Cambridge (1978) .
[5] S .W . Lovesey Theory of neutron scattering from condensed matter, Volume 2 : Polarization
and magnetic scattering, Clarendon Press, Oxford (1987) .
[6] O . Schärpf, in Neutron Spin Echo, p . 2752, Lecture Notes in Physics 128, Ed .
F . Mezei, Springer (1980) .
[7]
[8]
R.M . Moon, T . Riste, W.C . Koehler, Phys . Rev . 181, 920 (l969) .
F . Klein, The mathematical theory of the top, Princeton 1897 ; sec also [6] er H . Goldstein,
Klassische Mechanik, Akademische Verlagsges . Frankfurt am Main (1974) .
[9] F . Tasset, Physica B 241243, 177 (1998) .
[10] R. Pynn, Rev . Sei . Instrum . 55, 837 (1984) .
[11] G . Shirane, Y .J . Uemura, J.P.Wicksted, Y . Endoh, Y . Ishikawa, Phys . Rev . B 31,
1227 (1985) .
[12] O . Schärpf, H . Capellmann, Phys . Stat . Sol . (a) 135, 359 (1993)
[13] J . Strempfer, Th . Brückel, G .J . McIntyre, F . Tasset, Th . Zeiske, K . Burger, W .
Prandl, Physica B 267268, 56 (1999) .
[14] O . Schärpf, Physica B 182, 376 (1992) .
[15] W . Schweika and P . Böni, Physica B 297 (2001) 155159 . [Proc . PNCMI 2000] .
[16] P. Böni, J . Neutron Res . 5,63 (1996) ; D . Clemens, P . Böni, W . Hahn, M . Horrisberger,
P . SchubertBischoff and A . Vananti, in ICANSXIII and ESSPM4, Vol . 1,
eds . G .S . Bauer and R . Bercher, PSIProc . 9502 (1995) 312320 .
[17] G . Meier, U . Pawelzik, W . Schweika, W . Kockelmann, Physica B 276278, 369
(2000) .
[18] W . Schweika, Physica B (2003) in press .
Correlation Functions Measured
by Scattering Experiments
Reiner Zorn and Dieter Richter
5 . Correlation Functions Measured By Scattering
Experiments
Reiner Zorn, Dieter Richter
In this lecture static and dynamic correlation functions will be introduced . We will start by
introducing probability densities, relate those to the scattering cross section and define the
pair correlation function . Two examples will be given, one from the physics of liquids and
one from polymer physics . The concept of dynamic correlation functions will be explained
firstly by the example of correlation spectroscopy . Then the Van Hove correlation function
will be introduced which is the basis for the calculation of the double differential scattering
cross section . Finally, the concept will be applied to the example of an ideal gas .
5 .1 Probability Densities
We start by considering a homogeneous monatomic liquid with N atoms in a volume V .
We denote the probability to find a certain atom in a volume element dar at r by P(r)d'r .
Because of the homogeneity P(r) is constant and evidently
Then the number density of atoms at r is
1
P (r) (5 .1)
V
P(r) = NP(r) = N (5 .2)
We call the probability density to find a certain atom at r i and another at r 2 P(ri, r 2 ) .
This function fulfills the basic relations
P(rl , r2) = P (r2, ri ) and (5 .3)
IV d3r2P(ri, r2) = P(rj  (5 .4)
If there is no interaction between the atoms P(rl, r2) factorizes into
P(r l ,r2 ) = P(r1)P(r2) (5 .5)
In real liquids however usually an interaction exists which depends (only) on the distance
of the atoms r12 = r2  El . We express the deviation from (5 .5) by a pair correlation
function defined by
g(ri2) = P((~P~))
With the pair distribution function n(rl, r2) = N(N  1)P(El , r2) which expresses the
probability density for any pair of atoms to occupy positions rl
and r2 we obtain
2)
(5 g(L12) =
.7)
n('2r po
because in the lirait of large N we have N(N  1) ~ N2 .
The qualitative features of the pair correlation function are shown in figure 5 .1 . For r > 0
one finds g(r) = 0 because two atours cannot be at the saine position .
(5 .6)
Usually, this is
also true for distances r < ro because the atours cannot penetrate each other and have a
"hard core" radius ro .
For r > oc the lirait is g(r) = 1 because the interactions decay
with distance and the P(rl , r2 ) reverts to its default value 5 .5 . At intermediate distances
g(r) shows a peak because the probability density which is lacking at r < ro must be
compensated .
Its location is usually close to the minimum of the interatomic potential,
i .e . close to the average next neighbour distance rnn .
Using the pair correlation function one can formulate the differential neutron cross section
for a monatomic liquid'
Here (d (F /dÇZ) coh
du
CdZ)
coh
N
= Ibl 2 E exp N  (ri  ri» ~  (5 .8)
(i ' j= I
denotes the angle dependent coherent scattering cross section and b is
the average scattering length of the liquid atours . Q is the scattering vector, i .e . the
difference between incoming and scattered wave vector of the radiation, Q = k  k' .
average in the expression can be evaluated using the pair correlation function (5 .7) :
do,
()
dQ coh
_
 Ibl 2
+ ~E exp (1Q  (ri  rj
C1 i4j
1 Exactly speaking, this expression is valid only for monisotopic liquids . Otherwise,
there would be an additional incoherent terni like the one discussed for the dynamic
correlation function in section 5 .3 .
only visible as a flat background in the experiment .
the cross section is still correctly represented by (5 .8) .
The
Nevertheless, this terni is just a constant and therefore
5 2
The Q dependent (coherent) part of
S(Q)
rnn
=21r/r nn
Figure 5 .1 :
Schematic representation of interaction potential V (r), pair correlation function
g(r), and scattering function S(Q) .
= Ibl2 (N
+ f v d3rl IV d 3r2n(r l , r2) exp ( 1Q' (ri  r2)
= Ibl (N+P02Vfvd3r12g(rl2)eXP(iQ .r12)/
= IbI2N (1 + Po IV d 3 r12g(L12) exP (iQ . r12)/
(5 .9)
This equation states that the scattering cross section can be represented as the Fourier
transform of the pair correlation function . Assuming isotropy (as is found in the homogeneous
liquid discussed here) one can replace g(r 12 ) by the radial correlation function
y (r) :
(dS2)
coh
= I bI 2N Cl + 47rpo
f
r2d3rg(r) Sin
(5 .10)
Equation (5 .l0) follows from (5 .9) by radial averaging of exp (iQ  r 12) (i .e . an average
over all possible orientations of r12) .
53
The term in big parentheses of equations (5 .9) and (5 .10)
S(Q) = 1 + po fv
d ' r12g(L12) exp (1Q' L12)
(5 .l1)
is usually called structure factor or scattering law2 .
S(Q) is solely determined by the
properties of the Sample and does not depend on the radiation used in examining the
Sample .
For Q > oc, exp (iQ r12) becomes a rapidly oscillating function and the integral vanishes
.
Then one has
lim S(Q) = 1 . (5 .12)
Q> c>C
For Q ~ 0, S(Q) measures only the overall density fluctuation, i .e. the fluctuation of the
particle number :
Qmax = 27r/rnn
lim S(Q) = V 2 (6P2 ) = (N2)  (N)2 = PokBTrT (5 .13)
Q>o
Here, kB denotes the Boltzmann factor, T the temperature and K T the isothermal compressibility.
At intermediate Q, the structure factor of liquids shows a diminishing series
of broad peaks, remainders of the Bragg peaks of a crystalline structure .
The first peak
occurs at a scattering vector roughly corresponding to the next neighbour distance by
2 The usual definition of the structure factor found in the literature is
SI(Q) = 1 + Po IV d3 r12 (g(r12)  1) exp (iQ * r12)
subtracting the long distance limit 1 from g(r) . Because the Fourier transform of the
constant 1 is the delta function the two definitions differ only by a delta function,
S(Q) = S'(Q) + pod(Q) . This means that apart from the unobservable scattering at
zero angle (Q = 0) both are the Same .
The reason for this alternative definition is to avoid the singularity. Another way to
accomplish this is to use the density fluctuation Sp(r) = p(r)  po from the Start (equation
(5 .2)) . From this approach it becomes clear that the structure factor at Q 54 0
depends only on the fluctuation of the density but not on its absolute level .
54
White" neutrons
from reactor
Sample
Monochromator
Crystal
Figure 5 .2 : Schematic setup of a diffraction experiment . The inset shows the relation
between incident and final wave vectors k, k' and the scattering vector Q .
5 .2 Experimental Examples : Static Scattering
5 .2 .1 Placzek corrections
Figure 5 .2 shows the schematics of a scattering experiment for the determination of S(Q) .
By using a monochromator the incident neutron energy or the wave vector k is fixed . After
scattering the intensity is recorded as a function of the scattering angle 20 without energy
discrimination . This means that the diffraction setup fixes only the direction of kf but
not its magnitude . Therefore, for a given angle différent scattering vectors Q are mixed
as figure 5 .3 shows .
Strictly speaking, this invalidates thé relation (dQ/dÇZ) coh = IbI ZNS(Q) between (angle)
differential cross section and structure factor .
Nevertheless, for high incident energies it is an excellent approximation as long as thé
energy transfer due to inelastic scattering is small compared to thé incident energy E .
This condition is always fulfilled for xray scattering because thé incident energy lies in
thé keV range there and thé inelasticity of scattering is limited mainly to thermal energies
kBT which are of thé order of meV .
55
4
0
5 0 5 10 15 20
ho) [meV]
Figure 5 .3 :
Scattering vectors Q accessed by a diffraction experiment with the detector
at scattering angles 20 = 10 . . .115' vs . the energy transfer hw (incident wavelength
A; = 5 .1 Â) .
For neutrons on the other hand, incident energies are just in the latter range .
the errors which occur due to neglect of inelasticity are still not too large .
Fortunately,
Therefore, it
is possible to derive a correction formula by expanding the true differential cross section
under constant angle into a series in the ratio of the mass of the scattering nucleus and
the neutron mass mn/ms, . In this way one obtains to first order 3 :
al
(dd5~
ze = IbI 2N (S(Q) + .fp(Q» with .fp(Q) = mC (E  CQ~z ) (5 .14)
Here, E is the incident energy and k = 2m~É/1i the respective wave vector .
3 This formula is actually the specification of Placzek's original result [6] to the case of a
detector which is equally sensitive for all neutron energies ("black" detector) .
As pointed
out in [7]
the correction depends strongly on the energy dependence of the sensitivity.
Therefore, except for low Q values, formula (5 .14) is
not the one which is used in practical
applications .
56
2
0 0 2 4 6 8 10 12
0 (A 1 )
Figure 5 .4 : Structure factor S(Q) of liquid "Ar at 85 K . The points are frein a neutron
scattering experiment, the curve is generated by a molecular dynamics calculation using
a Lennard Jones potential [7] .
5 .2 .2 Experiments on Liquid Argon
As an example of the structure factor S(Q) of a monatomic liquid we consider the neutron
scattering results of Yarnell et al . [7] from liquid Argon . The result of the experiment is
shown in figure 5 .4 . The wavelength of the incident neutrons was A = 0.978 f1 . Under
this condition the Placzek corrections vary between 0.0012 near Q = 0 and 0.0426 at
Q = 9 .08Â 1 . The pair correlation function g(r) was obtained by numerical inverse
Fourier transform of S(Q)  1 and is shown in figure 5 .5 . The oscillations at small r
are a consequence of cutoff effects on the Fourier transform . They eccur below the
atomic diameter r o and therefore do not impede the interpretation . The determination
of g(r) is important for the calculation of equilibrium properties of the liquid and allows
scrutinization of theoretical models for the interatomic forces .
Two methods of theery based calculation of g(r) have to be emphasized : (1) In Monte
Carlo (MC) calculations a large number of possible atomic configurations is created .
Their probability is determined by the Boltzmann factor on the basis of interatomic
potentials . Finally, the ensemble average is calculated . (2) In Molecular Dynamics (MD)
calculations one starts from an initial configuration and solves (numerically) the equations
57
Figure 5 .5 : The pair correlation function g(r) of liquid Argon calculated by inverse Fourier
transform from thé data in figure 5 .4 [7] .
of motions using thé interatomic forces . These calculations yield thé time average4 . The
solid curve in figure 5 .5 shows thé result of an MD calculation with a LennardJones
Potential (V(r) oc (Q/r) 12  (Q/r) 6)thé agreement is excellent .
Unfortunately, thé pair correlation function is comparatively insensitive to details of thé
pair potential . To obtain exact information on V (r) it is necessary to do extremely
accurate measurements with errors in thé per mille range .
5 .2 .3 Scattering from a Polymer Chain
We consider a polymer, i .e .
monomers .
a long chain molécule consisting of equal building blocks, thé
In thé melt thé spatial arrangement of thé monomers is simply given by a
random walk5 . The mean squared distance between monomers i and j for such a coiled
chain is proportional to thé différence of indices
thé neutron scattering results shown here .
(rij 2 ) = ~2Ii  j
(5 .15)
4 The ergodic hypothesis ensures that thé results of both methods are thé Same .
a This is a result by no means trivial . It was actually confirmed for thé first time by
58
where rit denotes the monomer distance and P is the characteristic monomer length . This
is the same expression as for a random walk but with the time t replaced by I i  j I .
Because for not too small distances ri9 is the sum of many random variables the central
limit theorem is applicable and the final distribution of the distance is a Gaussian :
3/2 (_ 3ri j 2 \1I
g(ràj  ( 27r(ri j 2)) exp 2 (rij 2 )/ .
(5 .16)
Application of equation (5 .8) (radially averaged as (5 .10)) yields the socalled form factors
of the monomer
exp P(Q) = .~ 47r ri j 2d3ri j sin Qri~
JV2
9(ri j )  Q2 l i  j I~2) (5 .17)
Q i7
where N is now the number of mouomers . Analogous to the preceding derivation of (5 .9)
we take the diagonal part out of the sum and couvert the double sum into a single sum
over all differences k  Ii  j I :
P(Q) _
Cl + 2 ~ (1 
N/
exp Q 2 k~2 l
~ .
k/1
(5 .18)
Here it is taken account that in contrast to (5 .9) not all pairs are equally probable but an
index distance k occurs 2(Nk) times in the chain .
one obtains
Converting this sum into an integral
P(Q) = z
(ez  1 + z)  D(z) with z = Q26
~ 2 . (5 .19)
The expression D(z) is usually called the Debye function .
It describes the scattering of a
single polymer coil in the melt which is labeled e .g . by isotopic contrast . Figure 5 .6 shows
the scattering cross section of protonated polystyrene in a deuterated polystyrene matrix .
The solid curve represents a fit with equation (5 .19) .
At large scattering vectors the leading
asymptotic term of D(z) is 2/z and P(Q) becomes proportional 1/Q 2characteristic
for a Gaussian random walk . In a socalled Kratky plot (Q2  dor/dÇZ vs . Q) one expects
a plateau at high scattering vector Q . Figure 5 .7 shows this plateau for polystyrene .
At very large Q values deviations occur again which signalize the breakdown of Gauss
statistics for small distances .
s
Here the monomers are simply considered as "big atoms" neglecting their inner structure
.
One has to keep in miud that the thus obtained results only represent the actual
scattering law for small scattering vector when 27r/Q is larger than the size of a monomer .
59
Figure 5 .6 : Partial differential cross section for protonated polystyrene in a deuterated
polystyrene matrix [8] . The concentration of the protonated component is 5% (o) and
0.5% (o) respectively. The curve is a fit with the Debye function .
~E U 05
N
04
03
v
02
Y
H O
O
01 02 03 04
K .
A_
Figure 5 .7 : Kratky plot of the data from figure 5 .6 .
5.3 Dynamical Correlation Function
5 .3 .1 Correlation Speetroseopy
We consider an observable A of a system which fluctuates randomly because of the thermal
motion of the system . A could be e .g . the pressure on the wall exerted by a gas in a cylinder
or the particle density in a liquid . Figure 5 .8 shows exemplarily the timedependent value
of a quantity A fluctuating around its average value (A) .
51 0
, TIIIIV~i~.~1111
a"
Aj
A(t)
i ~M
~ jjj"
J~I'IIL~ Ir I iII~ I
V' ,i
~(8A 2
~ h`~mmm~i
1l
Ii `1l iû iül
Figure 5 .8 : Fluctuating observable A(t) of an ensemble of molecules as a function of time .
The time axis ils subdivided into discrete intervals of length At .
If one takes a time average over a long time interval as compared with the fluctuation
periods one obtains a stationary result which ils
interval
but in general A(t+T) :~ A(t) .
independent of the start of the time
1 fto+T
lim  J
dtA(t) = const .  (A) (5 .20)
Tcc T to
If T ils very small compared to typical times of the system
A(t + T)
approaches the value of A(t) which means that the both are correlated in time .
As a measure of this correlation the autocorrelation function ils introduced :
This function correlates the observable A with itself in a certain time displacement T and
then averages over all starting times .
1
t', +T
(A(0)A(7)) = Inn fo dtA(t)A(t + T) . (5 .21)
T
In a real experiment (figure 5 .8) this can be done by sampling values A Z at equidistant
times t 2 = idt . Let j denote the index ofthe starting time (t = j6t), n the distance counted
in time intervals (T = n6t), and N the number of intervals to be averaged (T = NSt) .
5 1 1
Then equation (5 .21) can be converted into a sum :
N
(A(o)A(T)) = lim 1 AjAj+n . (5 .22)
Ncc N j1
In optical correlation spectroscopy sums like (5 .22) are calculated from the photodetector
signal by special purpose computers .
per time interval, i .e . the light intensity .
In this case A is the number of photons detected
It is easy to see that the autocorrelation function has the following properties
(A(0)A(T)) < (A(0)A(0))  (A 2 ) (5 .23)
lim OO
(A(0)A(T)) = (A) 2 . (5 .24)
Figure 5 .9 shows a simulation of data of a light scattering experiment . Such data could
arise e .g . from scattering of polystyrene spheres in an aqueous dispersion .
The correlation function usually decays following a simple exponential law :
(A( 0)A(T)) = (A) 2 + ((A 2 )  (A)2)
exp ( T/TT)
(5 .25)
where Tr is the correlation time of the system . In general, also more complicated decays,
e .g . involving multiple characteristic times, are possible . But the decay always takes places
between the limits given by (5 .23) and (5 .24) .
Alternatively, one can consider the fluctuations 6A(t) = A(t)  (A), i .e . the deviations of
the observable from its average . For its autocorrelation function follows :
(SA(o)6A(t)) = (A(o)A(T))  (A)2
= (6A2) exp ( TI?T)
. (5 .26)
The general result is that the fluctuation autocorrelation function decays starting from
the variance of the observable, (6A2) = (A2)  2 (A) to zero .
The timedependent autocorrelation function describes the temporal fluctuation behaviour
of the system . In the case presented here of a polymer colloid the characteristic
time is directly connected to the diffusion constant : Tr1 = DQ2 .
51 2
(A(0)A(T»
Figure 5 .9 : Simulated result of a dynamic light scattering experiment . The circular
dots show the output of the correlator electronics . The continuons curve is the expected
exponential decay (5 .25) . The dashed line shows the underlying fluctuating intensity .
5 .3 .2 The Van Hove Correlation F unction
In order to consider inelastic scattering the differential cross section d6/dÇZ is generalized
with respect to its dependence on the energy transfer hrw . This leads to the double
differential cross section in quantum mechanical notation :
020, k'
 E PaPl
~ (A', 6 I b i exp(iQ  ri ) IA, 6 Î
2
S (hw + EA  Ey) . (5 .27)
Here, A and a describe the relevant space and spin quantum number respectively in the
initial state and A' and Q' those in the final state. PA and PQ are the respective probabilities
for the initial states A and a . The inner sum refers to all particles with scattering lengths bi
and singleparticle coordinate operators r i . k and k' are the wave vectors of the incident
and scattered neutrons . The delta function expresses energy conservation : the energy
transfer of the neutron hw is exactly compensated by the energy change of the quantum
state ofthe scattering system EyE A . In the following we will neglect the spin coordinates
for the sake of simplicity.
5 13
The route from expression (5 .27) to the Van Hove correlation function starts with an
integral representation of the delta function :
S (liw + EA  Ea,) =1 dt exp i + EA  EA, t I (5 .28)
27rh J Cw )
which results from the fact that the delta function is the Fourier transform of a constant
one .
With this expression the matrix element in equation (5 .27) can be written as a
Fourier transform in time:
E(A' Ibi exp(iQ  ri ) A)
2
S(hw+EA EA ,)
dt exp (iwt) exp i t )
exp i A, t )
27rh
Ebi(A ' Iexp(iQ  ri)IA)Ebi (AI exp( iQ  rj )IA' )
i
j
1 °° dt exp (iwt) E biM (AI exp (iQ  r j ) I A')
27rh oo i,j
(A'I exp(iEA,t/h) exp(iQ  r i ) exp(iEAt/h)la) (5 .29)
If H is the Hamiltonian of the scattering system, the fact that IA) are energy eigenstates
is expressed by
Iterating this equation n times yields :
HIA) = Eal AÎ . (5 .30)
HnIA) = EA
n
lA) . (5 .31)
By expanding the exponential into a power series one finally obtains from this relation
exp(iHt/tt) IA) = exp(iEat/1i) IA) . (5 .32)
With this result and the analogous one for A' it
in (5 .29) by the Hamiltonian H :
is possible to replace the eigenvalues EA
. . . (A' I exp(iHt/li) exp(iQ  r i ) exp(iHt/li) IA) . (5 .33)
In the picture of time dependent Heisenberg operators the application of the operator
exp(iHt/h) and its conjugate just mean a propagation by time t :
exp (iQ  ri (t)) = exp(iHt/1i) exp(iQ  ri (0)) exp(iHt/1i) (5 .34)
51 4
where we can arbitrarily set ri = r i (0) because of translation of time invariance . Using
this result the final expression for the double differential cross section is obtained :
k' 1 %
dtexp (  iwt)
8528w k27rh J.
(5 PA 1: bi b~ (A exp(iQ  r j (0» exp(iQ  r i (t» A) . .35)
ij
This equation averages over the scattering length distribution (which may depend on the
spin orientation distribution with respect to the incident neutron's spin) . This produces
coherent and incoherent scattering as explained in lecture 1 . In addition the initial states
of the scattering system are averaged weighted with the probability of their occurrence
PA . The latter is given by the Boltzmann distribution
PA = Z
exp (EA /kBT) with Z = exp (EA/k BT) . (5 .36)
We now denote this thermal average by angular brackets ( . . .) while that over the scattering
lengths be written as an overline . . . . Keeping in mind that for equal indices
bibi = Ibil 2 has to be averaged while for unequal indices the scattering lengths itself will
be averaged we end up with the usual separation into incoherent and coherent part :
k' z Ibl
 Ibl z p( J  ~ dtexp(iwt) .~ ex  iQ . _~(0))ex r_ p(iQ  _Z()) r_ t
27rh
k'
+ Iblz
k 2rh J
~ dtexp(  iwt) E ( A ex p(iQ
. ri( 0))exp(iQ . r j (t)) A . (5 .37)
z,9
The first term is the incoherent scattering . It involves the coordinate vector operators of
the Same atom at different times . The second, the coherent term correlates also different
atoms at different times . The material dependent parts are now defined as the scattering
functions
Si.,(Q' W) 
Scoh(Q,W)
1 f°°
dtexp(iwt) E(exp(iQ  ri(o)) exp(iQ  ri(t))) (5 .38)
27rhN oo i
1 dtexp(iwt) (exp(iQ  ri(0» exp(iQ  r j (t)» . (5 .39)
27rhN
1,3
In terms of the scattering functions the double differential cross section can be written as
z
as2a~ _
N ((Iblz  Ibl2) Sin c (Q, W) + Ibl
2
s~h(Q, W)) .
5 15
(5 .40)
In addition it is often useful to define the intermediate scattering function which denotes
the time dependent parts of definitions (5 .38) and (5 .39) before Fourier transform :
Sinc(Q,t)  N (exp(iQ Ei (o))exp(iQ ri(t))) (5 .41)
Scoh(Q,t)  N
E(exp(iQ  r i (0» exp(iQ r j (t») .
(5 .42)
2,7
If one compares this result with the definition of the structure factor (5.85 .11) one
recognizes that Sc oh(Q, w) is
time of a dynamical pair correlation function G(r, t) :
G(r, t) = C2r/ I d3Q
3
exp (
in an analogous way the Fourier transform in space and
E `exp (iQ  r i(0» exp (iQ  r j (t)) > . (5 .43)
N
The derivation of the relation between the coherent dynamical structure factor Swh(Q, W)
and the generalized pair correlation function requires a strict quantum mechanical calculation
.
This problem results from the fact that the coordinate vector operators commute
only at identical times . Therefore, in all algebraic manipulations the order of r i (0) and
ri(o) must not be interchanged .
To begin, one writes the operator exp (iQ  ri (0» as the Fourier transform of the delta
function :
exp (iQ  ri (0» = J
d 3 r'Ö (r  ri (0» exp(iQ . r') . (5 .44)
Using this expression equation (5 .43) can be rewritten as
3
G(r, t) = (1) 1 ~ (Id 3 r 'b (r i  ri
27r N i, j
(0))
J
d3Q exp (iQ . r  iQ . r + iQ . r j (t))
= (27r)3ö (r + r'  ri (t) )
N E J d 3 r' (6 (r  r' +r(0)) Ö (r'  rj (t)) ) (5 .45)
1,9
without changing the order of the operators at different times .
Now the particle density operator is
particle position operators :
introduced as a sum over delta functions at the
p (r, t)  Z 6 (r  Ei (t» .
(5 .46)
51 6
With this definition the pair correlation function can be written as timedependent
densitydensity correlation function :
(5 G(r , t) = N f d 3 r' (p(r'  r, 0)p(e , t)> .
.47)
With this form of the dynamic pair correlation function the dynamical structure factor
can beanalogously to equation (5.1l)written as the double Fourier transform of the
correlator of the particle density :
Scoh(Q, (5 W) = f~ dtexp(iwt) f d3r d 3r' exp (iQ  r)
00 J
(p(r' ?', 0)p(r , t» . .48)
We now define the density operator in reciprocal space as the Fourier transform of (5 .46) :
and obtain for the dynamic structure factor
pQ (t)  E exp (iQ  r i (t)) (5 .49)
Scoh (Q, W)
1
27fhN f c dtexp(iwt) (PQ(0)p_Q(t)) .
o0
(5 .50)
Correspondingly, the intermediate scattering function is
Scoh(Q,t) = 17 (PQ(0)PQ(t))
(5 .51)
which after insertion of (5 .49) turns out to be equivalent to (5 .42) .
Analogously, one can define a self correlation function by setting i = j in the preceding
equations leading to
G9 (r, t) = N
~ J d3r' (6 (?  e + ri (0 )) 6 (r'  ri(t»Î (5 .52)
as the equivalent of (5 .45) .
The pair correlation function has some general properties :
1 . For spatially homogeneous systems the integrand in (5 .47) is independent of r' which
can be arbitrarily set to the origin 0 :
G(r, t) = N
(p(r, 0>0, t)> = 1
(p(0, 0)p(r, t) ) .
(5 .53)
5 17
2 . The pair correlation function has the following asymptotic behaviour : For fixed
distance and t > oc or fixed time and r > oc the averages in equation (5 .47) can
be executed separately and in consequence
G (r, t) > N J d 3 r' (p(r'  r, o)) (p(r', t)) = po . (5 .54)
3 . For t = 0 the operators commute and the convolution integral of equation (5 .47)
can be carried out :
G(r, 0) = N
E (6 (r + Ei (0)  rj (0)) > . (5 .55)
i,j
For indistinguishable particles the relation to the static pair correlation function as defined
in (5 .6) can be drawn . Because of the identity of the particles we can set i = 1 in (5 .55)
and drop the average over i :
G(r, 0) = ~ (6 (r + rl(0)  rj (0)) > = S(r) + ~ (6 (r + r,(0)  r j (0)) > . (5 .56)
i
j 7~ l
We now consider the average number of particles 6N(r) in a volume SV at a vector
distance r from a given particle at rl .
It is obviously given by the integral over the second
term in the preceding expression which for small 6V can be written as
6N(r) = 6VZ (6 (r + rl (o)  rj(0))) . (5 .57)
j 7~ l
Using the definition (5 .6) and the expression for the number density in homogeneous
fluids (5 .2) one can relate 6N(r) also to the static pair correlation function :
SN(r) = poq(r)6V . (5 .58)
Finally, by comparison of the last three equations we get a relation between the dynamic
correlation function at time zero and its static counterpart :
G(r, 0) = 6(r) + pog(r) . (5 .59)
This equation expresses the fact that the diffraction experiment (g(r)) gives an average
snapshot picture (G(r, 0)) of the sample .
In the classical approximation the operators commute always, especially also at different
times .
Then the integrals of equations (5 .45) and (5 .52) can be carried out and yield
G"(r,t) = N
E6(r rj (t) +ri(0)) and (5 .60)
G9'(r, t) = N ~ ö (r  ri (t) + ri (0)) , (5 .61)
i
51 8
espectively. The former equation expresses the probability to find any particle at a time
t in a distance r from another at time 0 .
The latter equation denotes this probability
for the saure particle .
It therefore depends only on the particle's displacement during a
time interval Ari (t) = r i (t)  ri (0) leading to a simple expression for the intermediate
incoherent scattering function :
Sn, (Q, t) = NT E ( exp ( iQ  Ari (t)) i
In certain cases this expression can be further simplified using the "Gaussian approximation"
7 :
(5 .63)
Sncuss (Q,t) = eXp 1 Q2 (Ar2 (t)))
(5 .62)
Here (Ar 2(t)) is
the average mean squared displacement which often follows simple laws,
. e .g . (Ar 2 (t)) = 6Dt for simple diffusion Because one of the prerequisites of the Gaussian
approximation is that all particles move statistically in the Same way (dynamic homogeneity)
the particle average and the index i vanish . An analogous expression can be
derived for the coherent scattering .
In order to decide whether the classical approximation can be used the following rule has
to be taken into account :
Quantum effects play a rôle if the distance of two particles is of
the order of the DeBroglie wavelength AB = / 2m S~kBT or if the times considered are
smaller than hlkBT .
Figure 5 .10 schematically shows on the left side the behaviour of the correlation functions
G(r, t) and G,(r, t) for a simple liquid (in classical approximation) . On the right side the
corresponding intermediate scattering functions Scon(Q, t) and Sn,(Q, t) are displayed :
a For t = 0 the self correlation function is given by a delta function at r = 0 . The pair
correlation function follows the static correlation function g(r) .
The intermediate
scattering functions are constant one for the incoherent and the static structure
factor for the coherent .
e For intermediate times the self correlation function broadens to a bellshaped function
while the pair correlation function loses its structure .
The intermediate scat
For solids the longtime limit of this equation is called the LambMößbauer factor .
Its coherent counterpart is the DebyeWaller factor .
5 19
G(r, t)
G(r, t) i(Q, t)
r
Q
i(Q, t)
r
0. Q
Figure 5 .10 : Schematic Comparison of the correlation functions G (r, t), G, (r, t) and the
intermediate scattering functions Sc oh(Q, t), S;n,(Q, t) for a simple liquid at different times .
The solid lines denote the coherent case, the dashed lines the self/incoherent .
tering functions decay with respect to the t = 0 value . The decay is faster for higher
Q and (in the coherent case) less pronounced at the structure factor maximum .
The long time limit of the pair correlation function is the average density po while
the self correlation simply vanishes (in a liquid) . In consequence both the coherent
and the incoherent intermediate scattering function decay to zero for long times and
any Q .
5.4 Scattering from an Ideal Gas
We consider a gas ofN atoms in a volume V neglecting the spin coordinates Q and assume
that all scattering lengths are identical b i = 1 . The wave function of a free atom confined
520
to a volume V is simply a plane wave with wave vector K :
ID'(r) = WE) _ exp(iK  r) . (5 .64)
Using this expression, thé matrix element in thé double differential cross section (5 .27)
can immediately be calculated :
(KIexpiQrlr,)
VJv d3rexp(i(Q+  K)?')=6(Q+r,K) . (5 .65)
The resulting delta function expresses the momentum conservation . Only if momentum
is conserved the matrix element is 1otherwise zero .
In the second step we have to consider energy conservation .
wave vector K is
The energy of the atom with
(5 .66)
where ms , is thé mass of thé scattering atom . For thé évaluation of thé delta function
in (5 .27) we need thé energy différence between thé states K and W .
Because of thé delta
function factor (5 .65) only such states with K' = K  Q have to be considered and for
those thé energy différence is :
(5 E,  E =  (Qz + 2Q ) .
.67)
2m .,
With this result one can calculate the scattering function :
S(Q, w) = E Pub (hw  h (Qz + 2Q  E)~ . (5 .68)
2msc
In thé limit of a large volume V, K becomes a continuons variable .
thé component of K parallel to Q is relevant .
Therefore, (5 .68) can be written as a onedimensional
integral :
In addition only
S(Q, cv) = J
dKP,6
(hw
 1' (Qz +
2QK))
. (5 .69)
2m sc
The probability of a momentum state K follows from the Boltzmann distribution :
1 1i2K2
P, Z eXp ( 2mkRT
(5 .70)
with thé state surr being
z z
Z = ~ dr exp _ ~ r,
( 2m kBT)
5 2 1
_ 2~rme~kB T .
(5 .71)
Insertion of this result into (5 .69) yields :
2 2
S(Q,W) = 2~rm k T 1. dKexp (
~ ) ô
s~ B
2mS~ kBT (hW  2msc
(Q2 + .
2QK))
(5 .72)
Substitution of w  hW  2m_ (Q 2 + 2Qr,) into this integral allows the evaluation of the
delta function :
with ET
27rm s ,kBT
f 00.
S (Q, t) _ h 00
G(r, t) have an imaginary part .
dw,ZQ exp
1 (hu~  E, )2
47rE, kBT exp ( 4ErkBT )
(
2m~kBT (hMsc2Q (hW  w)  ~ ) 2
f . dw exp(iwt)1l 47rErkBT
exp ( ( 4ErkBT)2)
/
6(w)
= h 2Q2 /2ms, being the recoil energy experienced by the atom during the scattering
event . Thus, the dynamcal structure factor of an ideal gas is a Gaussian centred
around the recoil energy for a given Q . The width of the Gaussian 2ErkBT =
kBT/MS chQ increases with temperature and scattering vector Q .
Double inverse Fourier transform with respect to w and Q gives the correlation function
G(r, t) :
G(r, t)
(5 .73)
2
exp
Q
( 2 (kBTt2
 iht) ) , (5 .74)
9r
1 3
(2~) f d3Q exp(iQ  r) exp (2 kBTt2  lht))
m 3/2 ms~r
exp

2
2k (27rkBTt(t itt/kBT)) ( BTt(t  ili/kBT) )
Because of the quantum mechanical nature of the underlying dynamics both S(Q, t) and
The same result can be obtained via the Van Hove correlation function .
For this route
we start with equation (5 .39) for which we have to calculate exp(iQ  r (t)) for a free atom .
This can be done using the equation of motion
(5 .75)
ilid exp(iQ  r(t)) = [exp(iQ  r(t)), H] (5 .76)
where
H 2m
P2 (5 .77)
2 c
522
is the Hamiltonian of a free atom and p the momentum operator .
time dependent operator exp(iQr(t)) shall be calculated .
of motion
follows .
In the following the
This is done using the equation
(5 ihdt exp(iQ  r(t» = [exp(iQ  r(t», H] .
.78)
Here, the bracket on the right hand side is the commutator . In analogy to equation (5 .34)
holds .
1 [exp(iQ  r(t», pz] = 1 exp(itH) [exp(iQ  r(t », pz]
exp(itH) (5 .79)
2msc2msc
The commutator at equal times on the right hand side of the last equation can
easily be calculated . For this purpose one uses the coordinate representation p = ihV .
By calculation of the derivatives
[exp(iQ _ r(t», pz] = h exp(iQ  r(0» (hQ2 + 2Q  p) (5 .80)
Since p commutes with the Hamiltonian in the equation of motion the Hamiltonian
can be applied directly on r(0) :
ilid exp(iQ  r(t» =  h exp(iQ  r(0» (hQ2 + 2Q 
dt
2msc
p) (5 .81)
This differential equation can be solved immediately and one obtains for the time dependent
operator :
exp(iQ  r(t» = exp(iQ  r(0» exp
it
(2m .,
(hQ 2 + 2Q p)l
. (5 .82)
With this result the correlator in the scattering function (5 .39) can be calculated :
(5
z
(exp(iQ . r(0» exp(iQ . r(t»> =exp (exp
ihQ ihQ , p
(2m sc ) ( 2msc / ~ .
.83)
As in equation (5 .72)
Insertion into (5 .83) gives
the average is taken by using the Boltzmann factor yielding
p
expp 2msc
/  exp p
.
~
 2msc (5 .84)
(exp(iQ . r(0» exp(iQ . r(t»> = exp ~ Q z (tzkBT  iht) ~ . (5 .85)
2m sc
identical to equation (5 .74) .
Thus using the Van Hove correlation function we obtain
the same result as was originally derived directly from the definition of the scattering
function .
5 23
With this example we can also demonstrate that neglecting the operator character of the
position vectors leads to a wrong result .
classical expression (5 .60)
If we write the scattering function using the
S cl (Q' w)  27r t
dtexp(iwt) Cexp (iQ  (r(t)  r(0») > (5 .86)
is obtained . For a free atour we have r(t) = r(0) + tp/msc . Inserting this expression
into (5 .86) and averaging leads to :
1 _ W2msc l
Sc'MW)
2kBTQ2l  47rErkBT exp (
.
Comparison with (5 .73) shows that this result is wrong by neglecting the recoil energy
term . Instead of being centred at Er the expression (5 .87) is symmetric with respect to
W = 0 .
(5 .87)
References
[1] G . E . Bacon : "Neutron Diffraction" (Clarendon Press, Oxford, 1975) .
[2] G . E . Bacon (ed .) : "Fifty Years of Neutron Diffraction : The Advent Of Neutron
Scattering" (Adam Hilger, Bristol, 1986) .
[3] S . W . Lovesey : "Theory of Neutron Scattering from Condensed Matter" (Clarendon
Press, Oxford, 1984)
[4] G . L . Squires : "Introduction to the theory of thermal neutron scattering" (Cambridge
University Press, Cambridge, 1978) .
[5] M . Bée : "Quasielastic neutron scattering" (Adam Hilger, Bristol, 1988) .
[6] G . Placzek, Phys . Rev . 86 377 (1952) .
[7] J . L . Yarnell, M . J . Katz, R . G . Wenzel, S . H . Koenig, Phys . Rev . A 7 2130 (1973) .
[8] G . D . Wignall, D . G . H . Ballard, J . Schelten, Eur . Polym . J . 10 861 (l973) .
524
Continuation Description :
Grazing Incidence Neutron Scattering
0 . H . Seeck
6. Continuum description :
Grazing Incidence Neutron Scattering
O.H . Seeck, IFF8, FZ Jülich
6.1 Introduction
When studying solids or soit matter the explicit molecular structure is not always of
particular importance . Quite often the properties investigated are long ranged and not directly
connected with the atours or their positions . One example is a material with a continuons
ferromagnetic phase transition: Far below a well defined temperature (the critical temperature
called Curie temperature) the material is in a complete ferromagnetic state . Far above no
ferromagnetic behavior can be detected . Close to the critical temperature magnetic fluctuations
appear. The typical width of the magnetic areas is in the range of several nanometers up to
macroscopic distances depending on the temperature (sec Fig . 6.1a) . The width is basically
independent of the lattice spacing or the particular kind of atoms . Therefore, the knowledge of
the detailed molecular structure is not necessary to explain the physical properties of
ferromagnets .
Other examples are surfaces or layer systems . The properties of the samples such as film
thicknesses or inplane correlation lengths are usually also long ranged compared to the atomic
distances and the information about the exact atomic positions is not relevant (see Fig . 6 . lb) .
Figure 6 .1 : Sketch of systems with relevant mesoscopic or macroscopic properties . (a)
Ferromagnet close to the Curie temperature . Ordered regions with a correlation length
exist. (b) Monolayer system. The layer thickness d and the inplane correlation length ofthe
rougît surface ~, are much larger than the atomic spacing . The left picture of each example
shows the real atomic structure the right part the approximation as a continuous system .
A straightforward method to investigate mesoscopic length scales without taking into
account the exact molecular structure ofthe samples is the small angle scattering . `Small angle'
in this case means that the mean value of the wave vector transfer IQI of the scattered beam is
much smaller than the typicalreciprocal spacing of the atours in the sample (e.g., the reciprocal
lattice vector ja * 1 for a crystal with cubic synimetry) . In this case the effects of the atomic
structure on the scattered signal are negligible . This is schematically explained in Figure 6.2 .
real
space
Fourier U transformation
Q_
space
M v~
small Q /'U \
approximation
Q_
space
Fourier U backtransformation
real
space
Figure 6.2: Principles of small angle scattering . The method is not sensitive to the exact
atomic structure but only to mesoscopic or macroscopic length scales. Therefore, samples can
be treated as continuons systems. The operator © denotes the convolution of two functions.
A more detailed explanation is given in the text.
6 .2
Starting point is the exact atomic structure of the Sample . In this section a crystal with
some density modulations is chosen (Fig. 6 .2 top row) . The potential V(r) of such a System can
be written as a product of the undisturbed infinite crystal lattice potential Vatt (r) and the
modulation Vmod(r) . As it was shown in previous sections in Born approximation the scatternd
intensity
I(Q) IA(Q)IZ _ fV(r)exp(iQ .r)d'r2 = If Viatt(Y)Vod (E )exp(iQ  r)d 3r 2
= IF{Vatt(Y)V_d(Y)1(Q)IZ
of the sample can be calculated by performing a Fourier transformation F{ V(r) 1 of V(J . The
convolution theorem for Fourier transformations can be used to modify equation (6 .1) . This
theorem states that the convolution © of two Fourier transformed functions f=F{gi 1 gives the
same result as the Fourier transformation of the product of both functions gi . Thus,
F{g , 'gz }= F{g , }©F[92) = .f 0f2 = ff (q)f, (q  Q)d s q
(6 .2)
where the integral is the definition of the convolution .
It is also known from previous sections that for an infinite periodic crystal the lattice
potential Vatt (r) can be written as a surr of deltafunctions weighted with the scattering length
and located at the position of the atoms . The Fourier transformation of V,att (r) also yields delta
functions : the Bragg peaks at the reciprocal lattice positions . In contrast, the Fourier
transformation of Vmod(r) is usually a `smooth' function which is strongly decreasing for large
IQI " The result of the convolution is depicted in the second row of Figure 6 .2.
By doing a small angle scattering experiment only wave vector transfers Q with a mean
value close to 0 are considered. All other values are omitted. The result of the magnification
around Q=0 is shown in the third row of Figure 6 .2 . In good approximation it is identical to a
convolution of just a single deltafunction at 1=0 with the Fourier transformation of V,od(r) . In
real space (Fourier backtransformation) a single delta peak corresponds to an infinite sample
with homogeneous potential which turns out to be the averaged value of Vatt(r) . The fourth
row of Figure 6 .2 proofs that no information about the atomic structure is necessary to explain
a Small angle scattering pattern.
6 . 3
To study the morphology of surfaces or interfaces of thin layer systems such as polymer
films on silicon substrates or magnetic multilayer systems some specific kinds of small angle
neutron (or xray) scattering experiments can bc performed. Especially for buried interfaces
these surface sensitive methods are the only way to investigate the film properties without
destroying the sample. Therefore, they are very frequently applied and have an enormous
impact on solid states and soit condensed matter physics in general .
The socalled specular reflectivity is a scan with a wave vector transfer Q perpendicular
to the sample surface which is defined as the zdirection in this section. Because of the missing
Qz  and Q,component the reflectivity is only sensitive to the thickness, the potential and the
roughness of euch film . Inplane properties of the interfaces such as lateral correlation lengths
are accessible with different kinds of diffuse scattering experiments where at least one of the
components Qz or Q,, are not vanishing .
In the following, the specular reflectivity and the diffuse scattering are explained in more
detail. The usual experimental setup will bc shown and the basic theory of specular and diffuse
scattering will bc presented with some examples .
6.2 Experimental Principals of Surface Sensitive Neutron Scattering
A sketch of a typical neutron surface scattering experiment is displayed in Figure 6 .3, a
more detailed description is given in other sections . The direction of the primary beam is
defined by some slits. Before the primary beam bits the sample the flux is usually monitored.
The incident angle 6 which is determined with respect to the Sample surface is set by rotating
the Sample in the beam . The scattered beam is detected at an angle 6' (also with respect to the
surface) which is determined by 6 and the scattering angle 0=e'+6 . In the literature 0 is
sometimes called 26 (which is actually inaccurate because ~ is not necessarily equal to 26) .
Figure 6 .3 : Sketch ofa typical
surface sensitive neutron
scattering experiment. The
incident angle is denoted by
6, the outgoing angle with
respect to the surface by 6' .
The scattering angle is called
6 .4
For specular reflectivity measurements the condition 0=0' holds which is usually not true
for diffuse scattering experiments . The mean value of the wave vector transfer is given by
JQj= sin (2)
(6 .3)
with the de Broglie wavelength of the neutrons k=hl(2mE) 1/2 . As it was mentioned before for a
small angle scattering experiment IQI has to be much smaller than the typical reciprocal
distance of the atours in the Sample. Therefore, ~ also bas to be Small. Depending on the
chosen wavelength the angle ~ is almost never larger than a few degees . For a surface
sensitive experiment, which is performed in reflection and not in transmission (sec Fig. 6.4),
this means that 0 and 0' are also small and positive .
Fig . 6 .4 : Sketch of the wave
vectors for a surface sensitive
experiment. The parameters of
the transmitted beam are
labeled with the index t. The
potential of air is denoted by
Vo that one of the Substrate
with V I .
From simple geometrical considerations the components of the wave vector transfer can be
deduced. They are defined by
2n
Qx =(cos0'cos0)
Q v = 0
2n
(sin0'+sin0) (6 .4)
and can be used to estimate the accessible Qrange of surface sensitive experiments . At a
typical wavelength of the neutrons of about 0.2nm=2Â and angles not larger than 1 .0 degree
QZ would always be less than 0.1Â1 . JQxj would even be restricted to 5 .104Â1 . For
comparison: A simple cubic crystal with 3Â lattice spacing has a smallest reciprocal lattice
vector of 2.1Â1 .
6 .5
6.3 Specular Neutron Reflectivity in Born Approximation
For specular reflectivity measurements the exit angle 0' is
always identical to the incident
angle 0 .
Therefore, the Q~component is equal to zero and the reflectivity data does not contain
any particular information about the inplane structure of the Sample . In first order Born
approximation [1] the scattered intensity is given by
I (Q` )
1 ~f d
Qa dz (Z) exP(iQ`z)dz
2
(6 .5)
which means, that the specular reflectivity is basically determined by the Fourier transformation
of the gradient of the potential profile perpendicular to the sample surface.
The averaged
(continuons) potential of a particular material with N components is defined by
N
2nh,2
V = ~bjpj (6 .6)
mn J=1
where the b; are the scattering lengths and the pi are the particle number densities of the
components . A onecomponent sample with a perfectly smooth and flat surface which is
oriented in the (x y)plane would yield a step function for the zdependent potential :
z 2n h Zbp 1 1 0 : > 0
V (z) = (2  2 o(z)) _
mn C
{2nh 2bp / mn : Z :9 0
(6.7)
The derivative of V(z) is a deltafunction dV(z)/dzS(z) . With Eq . (6 .5) one gets I(Q^) _ Q^4
because the Fourier transformation of a deltafunction at z=0 is identical to 1 .
However, a perfectly smooth and flat surface does not exist. Instead surface roughness or
density gradients have to be taken into account [2,3] . As shown in Fig . 6 .5 roughness means
that thé zposition of thé surface is locally différent from thé mean position at z=0 .
Averaging
thé density in thé (x y)plane at each zcoordinate gives a smooth profile V(z) perpendicular to
thé surface.
The exact shape of thé profile depends on thé actual physical and chemical
properties close to thé surface.
For simple rough surfaces in good approximation an errorfunction
6 .6
v v z l 2r
V(z) = 2
2erfC~ with erf(z) = 6J J exp(t2)dt (6 .8)
0
is sufficient to modcl the profile . The parameter 6 is called rmsroughness and is a measure for
the root mean square width of V(z) given by the gaussian probability function
dV (z) (I
P(z) 
29L6 exp\ 262 ) .
(6 .9)
Figure 6.5 also shows that the profile does not contain any information about the lateral
structure of the rough surface . Therefore, the Rflectivity is insensitive to different inplane
length scales ~, . It even cannot be used to distinguish between a rough interface or a density
gradient caused by e .g ., interdiffusion . It will be explained later that this can only be donc by
using diffuse scattering experiments .
Z
~i . .,l , i : P,
Figure 6 .5 : Three différent surfaces with thé sanie nnsroughness G determined by thé root
mean square width of thé probability fonction (dashed line) of thé profile V(z) (solid line) .
The inplane structure is determined by thé lateral corrélation length ~n which is largefor thé
very left example quite smallfor thé rough surface shown in thé center and not definedfor thé
density gradient example (right) .
The reflectivity of a rough surfaces with an error fonction profile can easily be calculated.
The derivative of V(z) is determined by thé probability function P(z) [See Eq . (6 .9)] . With Eq .
(6 .5) this yields I(Qz) _ Qz4exp(Qa2( ) . Compared with thé perfectly smooth surface thé
reflected intensity is damped by a DebyeWaller factor : The rougher thé surfaces thé less
intensity is reflected at large Qz (sec Figure 6 .61eft) .
Reflectivity scans are not only extremely sensitive to surfaces roughnesses but also to film
thicknesses of layer systems . If a thin film with thickness d and an averaged potential Vl is
deposited on a substrate with potential Vz thé density profile V(z) is given by
6 .7
0 z>d
d V(z) = 2nh2b,P, / mz =V, : >_ z > 0 (6 .10)
0 21rh2b2 P2 /m =V2 . > z
if the interfacial rmsroughnesses ai and 62 are neglected. The derivative yields two deltafunctions
: dV(z)/dz(b2p2b,pl)S(z)+b,plô(zd) . Using Eq . (6 .5), the specularily reflected
intensity of a perfectly smooth monolayer system is given by
I(Qz )  Q4
[ (b2P2 b,P,) 2 + (b,P, ) 2 +2(b2P2  b,P, )(b,P, )cos(Qd)] . (6.11)
This means that films cause oscillations in the reflectivity. The period is determined by the fihn
thickness the strength (usually called `contrast') by the difference of the potentials Vl and V2
(see Fig . 6 .6 right) .
Figure 6 .6 : The left graph displays the effect of the surface roughness on the specularily
refected intensity : the rougher the surface the less intensity is refected at large Qz . The right
figure shows refectivities of perfectly smooth monolayer systems . The curves are shifted in
intensity for clarity. The thicker the film the smaller the distance of the socalled Kiessig
fringes . The less the contrast (given by [b2P2b,p, ]) the less pronounced the oscillations are.
In this way every additional layer appears as an oscillation in the reflectivity curve.
Interface roughnesses can also quite easily be included in the theory and yield a typical
damping of each oscillation. Multilayer systems with different parameters for each layer
generally show very complicate reflectivities . They are usually difficult to analyze especially
because of the socalled 'phase problem' which prevents an unambiguous solution of Eq. (6 .5) .
The ,phase problem" appears when performing the mean square of the complex function
6 .8
F{dV(z)/dz ) to calculate the reflected intensity [sec Eq. (6.5)] . The loss of the phase
information may end up in identical reflectivities even though the potential profiles are
different . E .g ., using Eq . (6 .11) it can easily be shown, that a monolayer system with bIp2=4
and blpl=3 exactly results in the saine reflectivity as b2p2=4 and blpl=l, if the film thicknesses
are identical.
6.4 Diffuse Neutron Scattering in Born Approximation
Performing a surface scattering experiment it turns out that some intensity is also
scattered in directions with 6 6' . In this case the wave vector transfer Q has a component in
Q,direction (see Fig . 6.4) . This offspecular signal is called diffuse scattering and is caused by
lateral structures (inplane, in the (x,y)plane) of the sample [4] . If the samples are perfectly
smooth or if there is no lateral structure (see Fig . 6.5 right) no diffuse scattering is expected.
In general, for rough layer systems the diffuse scattering is sensitive to the correlation
fonction C;k(R) between two interfaces j and k where R is an inplane vector (x y) . The
correlation function is defined by
Cjk (A)  fz; (r)zk (r + R)d2r (6 .12)
with the local deviation z;(r_) from the averaged position of the interface j . The correlation
function between two different interfaces is usually called `crosscorrelation' . If j=k holds
C;k(R)=C;;(R) is called `autocorrelation' . Qualitatively, C;k(R) is large if two areas of the
interfaces j and k, which are R apart from each other, `look similar' . E .g ., if the two interfaces
contain a periodic structure with the saine periodic distance D the correlation fonction exhibits
maxima at D,2D,3D . . . . For an autocorrelation function of a single rough surfaces one gets a
monotone decreasing function : For very small distances the parts of the surface look sirnilar,
the larger the distance the more different they become . The width of the curve is connected to
the lateral correlation length ~,,, of the interface (see e .g ., Fig 6.5) [5] .
The diffuse scattering can be used to investigate periodic inplane structures, inplane
correlation lengths of a single rough interface and correlations between two different
interfaces . Figure 6.7 depicts some examples . The complete mathematical formalism to deduce
the diffusely scattered intensity is quite complicate [6] . Therefore, the full theory is omitted in
this section . Instead, the diffuse scattering is explained using a simple monolayer system.
6.9
Figure 6 .7 : Sonie examples of monolayer systems with rough surfaces . a) Both interfaces are
not correlated at all. b) Perfect crosscorrelation between thé lower and thé upper interface .
c) A crosscorrelation is visible but it is not perfect: The interfaces do not exactly look thé
sanie . d) Perfectly anticorrelated interfaces.
In Born Approximation the diffusely scattered intensity of a monolayer system with the
interfaces j=1,2 and thé film thickness d can bc calculated by
In(Q"Q
Equation (6 .13) also shows that the diffuse scattering can be detected in the whole Q
space even at Q,e=0 which is actually the position of the specularily reflected signal .
This means
that reflectivity measurements (Q, scans at QX=O) always contain both the specular reflectivity
and the diffuse scattering at Q,e=0 .
To extract the specular reflectivity from the reflectivity
measurement the diffuse scattering has to be subtracted. This is usually donc by performing a
QZscan with a small offset 4Q~ so that the specular condition is not exactly matched. This socalled
longitudinal diffuse scan is subtracted from the measured reflectivity to get the true
specular reflectivity .
6
5
15
^®^ specular reflectivity
diff . int . a t 0,=0
c 2
ô
1
0
0
6 4 2 0 2 4 6 0.00 0.05 0.10 0.15 0.20
% [0.001Ä'] 0 . [Ä  ' l
Figure 6 .8 : Examplcs of diffuse scattering experiments. Left: Q xscan atfixed Qz from a single
rough surface . The solid curve corresponds to a sample with an inplane correlation length of
~p =5000A the dashed line to ~p=IOOOA. The peaks at the condition Qx=O (where 0=0') are
not diffuse scattering but caused by the specular reflectivity . Right: Specular reflectivity
(symbols) and diffuse scattering Qz scans at QX=0 (solid lines) of a monolayer system with
d=300Â, b2pz=4, 62=5A, b i p 1=3 and 6 1 =5A . The diffuse scans show the effect of crosscorrelations
. The measured reflectivity is detennined by the sum of the specular and the
diffuse scan .
Unfortunately, the intensity of the diffuse scattering is usually orders of magnitude
smaller than the specularily reflected signal . To get gond statistics and reliable data a very high
primary flux is necessary. This can easily be achieved with synchrotron radiation xray sources
but is hardly possibly for neutron sources (sec section 6 .5) . Therefore, it is extremely difficult
to extract quantitative information from the neutron diffuse scattering data .
6 . 1 1
6.5 The Regime of the Total External Reflection : Exact Solution of the Wave Equation
It is obvious that the Born approximation [Eqs . (6 .5) and (6.13)] fails for Q,>O because
the intensity would become infinite at Q=O. The reason is that multiple scattering processes are
neglected within the Born approximation . For surface sensitive experiments multiple scattering
processes become essential at very small angles [7] . An exact description of the scatternd
intensity can be deduced for a perfectly smooth surface from quantum theory .
Starting point is the Schrödinger equation
b z
2m
n
4+V(r) I`V(r) = EW(r) (6.15)
for the wave function of the neutrons `F(r) . The energy of the neutrons is given by
E = bzk z 1(2m,) with the mean value k=2ir1,~ of the wave vector k (the incident and the
outgoing beam have identical k because elastic scattering is assumed) . For a homogeneous
sample the potential is determined by Eq. (6 .6), thus
r ll r z l1
LA+Ckz 4nY,bj p~ I J
'F(r)=l A+kz C1Eb i
p i
IJ
'F(~=~4+kr ]`PL)=0 (6.16)
with the wave vector k, inside the medium (see Fig. 6 .4) . From Eq . (6.16) it is justified to
introduce the refraction index n,=k,/k ofthe material. In very good approximation one yields
z
n, =1
2 ~,b;p ; =18 1 (6.17)
for the refraction index which is a number close to 1 for neutrons of approximate 1Â
wavelength (the correction 8, is called dispersion and is on the order of 105 . . .106)
By introducing the refraction index the basic principles of optics can be applied for all
further considerations . First of all it is remarkable that for many materials n, is smaller than 1
(because b; is usually and pi always positive, thus 8, is usually positive) . This means that the
transmitted beam is refracted towards the sample surface (0,
ut is completely reflected . The critical angle can be estimated by and is on the order
of some 0 .1 degree depending on the density, the scattering lengths of the atours and the
wavelength of the neutrons . For 0 values beyond 0, the beam can penetrate the sample and is
only partly reflected. At the sample surface the reflection and transmission coefficients rf and tf
are obtained by the Fresnel formulars
k,
_ k
rf k + k,
and
2k_
k_ + k
(6 .18)
with k, =ksin0 and k, = k,sin0, = k(n,2cos20)'n (see Fig . 6.4) . The specular reflected intensity
I=Irla is determined by the absolute square of the reflection coefficient . It shows the typical
plateau below the critical angle, the regime of the total extenal reflection, and the rapidly
decreasing intensity beyond 0, . With appropriate approximations one gets I=8,Z/(4sin40)_Qz4
for incident angles 0 larger than 38, which is the confirmation of the Born approximation (see
Fig . 6 .9) .
Figure 6 .9 : Effect of the
total external reflection .
The large figure shows a
reflectivity of a smooth
surface in Born approximation
(Symbols) and the
exact Fresnel form (solid
line) . The dashed line
marks the critical Qz .
The left inset displays
absorption effects in the
reflectivity on a linear
scale. The same is depicted
for the transmitted
intensity in the right inset.
Not addressed yet in this section is the absorption ß, of the neutrons inside the Sample.
For most materials such as silicon the absorption is negligible but this is not the case for e .g .
cadmium or indium . Most straightforward, it can be introduced by including an imaginary part
to the reflection index
6 . 13
n, = 1 8, + i(3, (6.19)
The effect of the absorption is shown in Fig . 6 .9 . It basically smoothes the sharp features of the
intensity close the critical angle and also restricts the penetration depth of the neutrons to finite
values .
The diffuse scattering is also modified in the regime of the total external reflection [8,9] .
In good approximation one gets
I,i (Qx>Qz) tf(0)IzQzzexp ( QZ6i ) sii(Qx)tf(0 , (6.20)
)z
for a single rough surface. For layer systems this expression becomes much more complicate.
Eq . (6 .20) shows, that the transmission functions of the incoming and the outgoing beam have
to be taken into account. The transmission function tf exhibits a maximum at the critical angle
(or the critical Qz, respectively, see Fig . 6 .9) because for incident angles 0 = 0, an evanescent
wave appears which runs parallel to the surface (0' = 0) [10] . Therefore, the diffuse scattering
also bas maxima called Yoneda wings at the positions 0=0, and 0'=0, (sec Fig .6 .10) .
4
Figure 6 .10 : Diffuse scattering
scan at fixed Qz . The symbols
correspond to the Born
approximation (dashed line in
Fig. 6.8) . The solid line displays
0
the better approximation
2
including the scattering effects
due to the total external reflection
C
o,
at 0=0, and 0'=0, . They are
0 1
visible as the Yonedamaxima at
IQXI=0.0032 .E ' .
The peak at the center is the
0 4 2 0 2 4 specular reflected intensity (0=0') .
Qx [0 .001Ä  ']
In summary, the optical properties of the sample affect the scattering only if the incident
or the exit angle is comparable or smaller than the critical angle which is usually smaller than
6 . 14
0.4° . The full dynamical theory can only be deduced for the specular reflectivity. For the diffuse
scattering no exact solution exist right now .
6.6 Important Applications of Neutron Reflectrometry
For many standard scattering experiments on layer systems xrays are much more suitable
than neutrons because of the higher flux, the better collimation and the less divergence . In
numbers : A standard synchrotron radiation source bas a primary beam intensity of about 10' °
counts/sec at a typical spot size of (0.2x1)mm2 . The beam divergence which determines the Q
space resolution is less than 1/100 of a degree . For a modern neutron source one gets less than
10 7 counts/sec in an area of (0.5x20)mm2 with a divergence of larger than 0 .02° .
However, for some topics of research neutron scattering is superior . One example is the
investigation of materials which mainly contain hydrogen, carbon, nitrogen or oxygen such as
organic molecules . In this case the electron density [which for xrays replaces the potentiel
V(r)] is very low and the xray contrast becomes very small. In contrast, for neutron V(r)
strongly depends on the isotope of the elements . Therefore, by using deuterated or
hydrogenated organic materials the scattering contrast can easily be tuned without changing the
chemical properties of the semples . Figure 6.11 shows an example of apolymer bilayer.
hPS
12
10
ö
s
6
rn
4
0
50 100 150 200 250 300
Figure 6 .11 : Comperison
of an xray (left column)
and a neutron (right
column) reflectivity of a
polymer bilayer (210Â
polystyrene [PSI on 70Â
deuterated polyvinylpyrridine
[dP2VP] on a sifcon
z ra1 substrate) . The xray
contrast between the two
polymes given by the
electron density lis only
about 5% .
0.10 0,15 020 0 .25 A 30 2 0 .00 0.05 010 015 0.20 0 .25 0.30
0. rß  ' 1 0= rx ' 1
It can clearly be seen that the xray reflectivity only exhibits one signiflcant oscillation
period which is due to the whole fihm thickness . The xray contrast at the polymer interface is
6 . 15
too small to modulate the intensity. Advanced analyzing methods have to be used to extract the
information of the polymerpolymer interface [11] . This is different for neutrons : By
deuterating the bottom polymer the contrast is enhanced dramatically. The reflectivity shows
separate oscillations : a long period due to the thin dP2VP film and a short period which is
caused by the hPS film. The analysis is straightforward and usually very reliable .
Another very important application is the magnetic neutron scattering . Neutrons have a
spin of 1/2 which means that they are sensitive to the magnetization ofthe sample . A sketch of
a magnetic neutron reflectivity experiment is depicted in Fig. 6.12 . The sample is illuminated
with polarized neutrons . The polarization is determined by the direction of the neutron spins
with respect to an external fieldH: They are usually either parallel or antiparallel toH.
Figure 6.12: Sketch of a
neutron reflectivity experiment
on a magnetic layer.
The spins of the incident
neutrons s are oriented parallel
(either up or down) to an
external field H. After the
scattering the direction of the
spins s' may have flipped
depending on B which is
given by the magnetization of
thefilm and H .
After the scattering process the spin direction of the neutrons may have flipped. Thus,
four différent reflectivities can be measured :
" R++ : The spins ofthé incident neutrons are parallel to H. The spins of thé scattered neutrons
are also parallel toH (nonspinflip process) .
" R__ : The spins of thé incident neutrons are antiparallel to H. The spins of thé scattered
neutrons are also antiparallel toH (nonspinflip process) .
" R+ _ : The spins of thé incident neutrons are parallel to H. The spins of thé scattered neutrons
are antiparallel to H (spinflip process).
" R_+ : The spins of thé incident neutrons are antiparallel to H. The spins of thé scattered
neutrons are parallel toH (spinflip process) .
The four reflectivities can be deduced from thé Schrödinger equation considering thé external
field, thé magnetization of thé sample and thé spin direction of thé neutrons [12] . In thé
following only some qualitative descriptions are given .
6 . 16
1) If no magnetic induction B (which is determined by the external field H and the
magnetization of the sample) is present one yields R++ = R__ and R +_ = R_+ = 0 . Thus, there is
no dependence of the scattering on the spin orientation of the incoming neutrons .
2) If B = B (magnetic induction perpendicular to the surface) no magnetic scattering is
expected either. The reason are the Maxwell equations which do not allow a change of the
mean value of B in field direction (V  B = 0) . This means that B does not change at the
sample surfaces . Therefore, R++ = R__ and R+ _ = R_+ = 0 .
3) If B = Bil only nonspinflip processes appear (s = s') . The reason is the vanishing cross
product between s and B . This means that no interaction between the spins and the
induction is present so that the spins cannot flip. However, a magnetic contribution to the
refraction index has to be added for R++ and subtracted for R__ . Thus, R++ # R__ but still R + _
R+ = 0 .
4) IfB = B the spins can flip during the scattering process . Therefore, nonspinflip processes
appear with R+ _ # 0 and R_ + # 0 . In contrast to point 3) the nonspinflip reflectivities are
identical (R ++ = R) .
In summary, from all reflectivities R ++ , R__ , R+_ and R_+ the exact magnitude and orientation of
the magnetization profile of the sample can be determined with polarized neutron reflectivity .
References
[1] J . AlsNielsen, Topics in Current Physics. Structure and Dynamics of Surfaces
(Springer, Berlin, 1986) .
[2] P. Beckmann, A. Spizzichino, The Scattering of Electromagnetic Waves From Rough
Surfaces (Pergamon, New York, 1963) .
[3] L . Névot, P . Croce, Revue de Physique appliqué 15, 761 (1980) .
[4] S.K . Sinha, E.B . Sirota, S. Garoff. H.B . Stanley, Phys . Rev . B 38, 2297 (1988) .
[5] A.L. Barabâsi, H .E . Stanley, Fractal Concepts in Surface Growth (Cambridge
University Press, Cambridge, 1995) .
[6] V . Holt', J. Kubena,1. Ohlidal, K . Lischka,W. Plotz, Phys . Rev. B 47, 15 896 (1993) .
[7] J . Lekner, Theory of Reflection (Martinus Nijhoff, Dordrecht, Boston, 1987) .
[8] S . Dietrich, A . Haase, Phys . Rep . 260, 1 (1995) .
6 . 17
[9] V . Holt', U. Pietsch, T . Baumbach, XRat' Scatteringfrom Thin Films (High Resolution
XRat' Scattering from Crystalline Thin Films) (Springer Tracts in Modern Physics,
Vol . 149, Berlin, 1998) .
[10] H . Dosch, Critical Phenomena at Surfaces and Interfaces (Évanescent XRat' and
Neutron Scattering) (Springer Tracts in Modern Physics, Vol . 126, Berlin, 1992) .
[11] O.H . Seeck, I.D . Kaendler, M . Tolan, K. Shin, M.H. Rafailovich, J . Sokolov, R . Kolb,
Appl . Phys . Lett. 76, 2713 (2000) .
[12] C .F . Majkrzak, J.F. Ankner, N .F . Berk, D . Gibbs, Neutron and XRat' Diffraction
Studies of Magnetic Multilayers (in : Magnetic Multilayers, World Scientific,
Singapore, 1994) .
Diffractometer
Gernot Heger
7 . Diffractometer
G .
Heger
7 .1 Introduction
For pure elastic scattering the scattering function S(Q,w) is reduced to the special case
without energy transfer (Eo = E l and h is = E o  E l = 0) and equal length of the wave vectors
of the incident and scattered beams ( ko _ k ). S((Q,c)L = 0) and hence the scattering
intensity is only depending on the scattering vector Q = ko  k 1 . The coherent elastic neutron
scattering ( neutron diffraction) yields information on the positions (distribution) of the
atomic nuclei and the arrangement of the localised magnetic spins in crystalline solids, the
pair correlation function of liquids and glasses, and the conformation of polymer chains .
Depending on the scientific problem to be investigated adequate diffraction methods may be
quite différent . For fluids and glasses diffraction data ofhigh statistical relevance over a very
large 1 Q I range are required. The direction of thé scattering vector Q is not defmed for these
noncrystalline states and a good resolution I AQ I / I _QI is of no importance . Besides of thé
pure elastic scattering also inelastic contributions are involved .
Completely différent are thé needs for a diffraction study of crystalline solids . The diffraction
at thé crystal lattice gives rise to pure elastic scattering localised at thé nodes of thé socalled
reciprocal lattice. The scattering vectors Q for thé différent "Braggreflections" are well
defined . For thé séparation of reflections with similar Q values a good resolution AQ/Q is
very important. A measured dataset of Braggintensities (integrated intensities of Braggreflections)
as complete as possible over a large 1 Q I range is required . An experimental
stability and accuracy leading to a precision of thé intensity data of about 2% is desired and
may be achieved.
Diffraction measurements on polycrystalline samples depend only on thé length of thé
scattering vector 1 Q I . Very small line widths (according to an excellent resolution 1 AQ 1 / 1 Q I )
combined with well defmed reflection profiles are prerequisites for a quantitative lineprofile
analysis . The complete powder diagrams resulting from overlapping reflections are described
and analysed by means ofthé Rietveld method .
For all diffraction methods flrstly thé energy of thé incident neutron beam (expressed in
another way as its wavelength or velocity) must be specified . In thé case of angular dispersive
diffraction, thé 2axes diffractometer (see Fig . 1) is equipped with a crystal monochromator to
select a special wavelengths band (;, ± Ak/;,) out of the "white" beam according to the Bragg
condition for its scattering plane (hkl)
2dhk1' SinO yk1 = ;~ ,
with the interplanar spacing dhkl and the monochromator scattering angle 26hk1 = 20m. The
width ofthe wavelengths band which is important for the Qresolution, depends on the
divergences of the beam before and after the monochromator (collimations al and a2), on the
mosaic spread of the monochromator crystal AM, and on the monochromator angle 20m. In
order to increase the intensity of the monochiomatoc beam at the sample position the
monochromator cystal is often bent in vertical direction perpendicular to the diffraction plane
of the experiment. In this way the vertical beam divergence is increased leading to a loss of
resolution in the reciprocal space . Thc diffracted intensity from the sample is measured as a
function of the scattering angle 26 and the sample orientation (especially in case of a single
cystal) :
for a single crystal > I(Q), and for a polycrystalline sample > I( I Q 1 ) .
29 is defmed by the collimators a2 and a 3 . As there is no analysis of the energy of the
Detector
Fig . 1 . Schematic representation of a 2axes diffractometer .
72
scattered beam behind the sample, the energy resolution AE/E of a 2axes diffractometer is
not well defmed (typically of the order of some %) . In addition to the dominant elastic
scattering also quasielastic and some inelastic scattering contributions are to be taken into
account. The narre 2axesdiffractometer results from its two axes of rotation, the
monochromator axis defining 20m and the sample axis (20) .
In the case of energy dispersive diffraction, the timeofflight diffractometer uses the
complete energy spectrum of a pulsed neutron beam and the wavelengths of the scattered
neutrons are determined by velocity analysis . The measurement ofthe neutron intensity as a
function of velocity at fixed scattering angle 20 has to be calibrated according to the energy
spectrum of the neutron beam. Assuming no energy transfer at the sample the timeofflight
diffraction yields again I(Q) (and for a polycrystalline sample I( I Q 1 ) .
7 .2 Reciprocal lattice and Ewald construction
Bragg scattering (diffraction) means coherent elastic scattering of a wave by a crystal . The
experimental information consists of the scattering function S(Q,ca = 0) with no change of
energy or wavelength of the diffracted beam . For an ideal crystal and an infmite lattice with
the basis vectors a,, 22, a 3 , there is only diffraction intensity 1(H) at the vectors
H = hai*+ka2*+la3* (2)
of the reciprocal lattice . h,k l are the integer Miller indices and al*, g2*, a3*, the basis vectors
of the reciprocal lattice, satisfying the two conditions
a l **a l = a2 * .a2 =a3 * *a3 = 1 and a l*.22 = a l **a3 = ~!2
*al = . . . = 0,
or in ternis ofthe Kronecker symbol with i, j and k = 1, 2, 3
Sij = 0 for i 7~ j and Sii = 1 for i = j with Si, = a* . ai* . (3)
The basis vectors of the reciprocal lattice can be calculated from those of the unit cell in real
space
a,* = (axa
" The direction of the reciprocal lattice vector His normal to the (hkl) planes and its length is
reciprocal to the inteiplanar spacing dhkl : IHI = 1/dhkl .
" Duality principle : The reciprocal lattice of the reciprocal lattice is the direct lattice .
From the positions of the nodes of the reciprocal lattice obtained by diffraction experiments
one can determine directly the parameters ofthe unit cell of a crystal .
Although somewhat abstract, the concept of the reciprocal space provides a practical tool to
express geometrically the condition for Bragg scattering in the socalled Ewald construction .
In this way the différent diffraction methods can be discussed .
We consider the reciprocal lattice of a crystal and choose its origin 000 . In Fig . 2 the wave
vector ko (defined in the crystallographers' convention with ~kol = 1/A,) ofthe incident beam is
marked with its end at 000 and its origin P . We now draw a sphere ofradius ~lço I = 1/ ;, around
P passing through 000 . Now, if any point hkl ofthe reciprocal lattice lies on the surface of this
Ewald sphere, then the diffraction condition for the (hkl) lattice planes is fulfilled : The wave
vector of the diffracted beam k (with its origin also at P) for the set of planes (hkp, is of the
same length as ko (IkI = Ikol) and the resulting vector diagram satisfies k = ko + H. Introducing
the scattering angle 20 (and hence the Bragg angle 9yk1),we can deduce immediately from
21klsin0 = IHI the Bragg equation:
2dhk1'slnehkl
Fig . 2 .
Ewald construction in reciprocal space, showing the diffraction condition for the
hkl reflection.
74
In the case of single crystal diffraction a rotation of the crystal and therefore also of the
corresponding reciprocal lattice (which is rigidly attached to the crystal) is often used to set
the diffiaction conditions for the measurement of intensities I(H) .
If IHI > 2/a, (then dhkr < ;U2) the reflection hkl cannot be observed. This condition deines the
so called limiting sphere, with center at 000 and radius 2/; : only the points of the reciprocal
lattice inside the limiting sphere can be rotated into diffraction positions . Vice versa if ~, >
2dma,, where dma, is the largest interplanar spacing of the unit cell, then the diameter of the
Ewald sphere is smaller then IHI ,;. Under these conditions no node of the reciprocal lattice
can intercept the Ewald sphere . That is the reason why diffraction of visible light (wavelength
5000 Â) can never be obtained from crystals . T; determines the amount of information
available from a diffraction experiment . In ideal conditions ;,,; should be short enough to
measure all points ofthe reciprocal lattice wich signifcant diffraction intensities .
For a real crystal of limited perfection and size the infmitely sharp diffraction peaks (delta
functions) are to be replaced by broadened line shapes . One reason can be the local variation
of the orientation of the crystal lattice (mosaic spread) implying some angular splitting of the
vector H. A spread of interplanar spacings Ad/d, which may be caused by some
inhomogeneities in the chemical composition of the Sample, gives rise to a variation of its
magnitude IHI . The ideal diffraction geometiy on the other hand is also to be modified . In a
real experiment the primary beam has a finite divergence and wavelength spread. The detector
aperture is also finite . A gain of intensity, which can be accomplished by increasing the
angular divergence and wavelengths bandwidth, has to be paid for by some worsening of the
resolution fanction and hence by a limitation of the ability to separate different Bragg
reflections .
All of these influences can be studied by the Ewald construction . The influence of a
horizontal beam divergence on the experimental conditions for a measurement of Braggintensities
of a single crystal is illustrated in Fig . 3 where strictly monochiomatised radiation
(only one wavelength ;, with AA,/;, = 0) is assumed. A socalled ù)scan, where the crystal is
rotated around the Sample axis perpendicular to the diffraction plane, may be used for a
reliable collection of integrated intensities in adapting the detector aperture A20 as a function
of the scattering angle 20 . It is obvious that larger A20values will give rise to a higher
background and may lead to difficulties for the Separation of neighboured reflections wich
similar Hvectors in the reciprocal lattice . It is shown by this example that a larger beam
divergence with an increase in intensity can restrict the resolution conditions .
7 5
Braggintensities of single crystals are recorded in general by (0/n .20scans (0
Powder diffraction also may be discussed on the basis of the Ewaldconstruction . An ideal
polycrystalline sample is
characterised by a very large number of anbitrary oriented small
ciystallites . Therefore, for a powder only I H I is defmed without preferred orientation . In
Fig . 4 the corresponding sphere with radius 1111 = 1/dhkl is drawn around the origin of the
reciprocal lattice at 000 . For each Braggreflection the circle of intersection with the Ewaldsphere
yields a diffraction cone . All reflections with equal inteiplanar spacing are perfectly
superposed and cannot be separated.
7 . 3 Powder diffractometer
There are two principally différent powder diffraction techniques : thé angulardispersive
ADPmethod and thé energydispersive EDPmethod, better known as timeofflight method
in thé case of neutron diffraction .
In thé ADP measurement thé sample is irradiated by a
monochromatic beam (;, = const .) . To each dhki belongs a Braggangle 0yki.Most of thé
neutron powder diffractometers at
steadystate reactor sources work according to thé ADP
method (e . g . thé D2Binstrument at thé HFR/ILL in Grenoble) . The angular resolution of a
powder diffraction diagram depends on thé beam divergences before and behind thé
0 .6
4
r
D2B
2
Cornu, Xray }
Soie lier ~._ ._
0 .0é
CHESS
Diffraction Angle {°)
Fig .
5 . Comparison of thé halfwidths of powder lines for selected neutron powder
diffractometers : D2B at thé HFR/ILL in Grenoble(F), HRPD at NBSR in Lucas
Heights (USA), SEPD at ANL in Argonne (USA)  thé timeofflight data of this
instrument with Ad/d z 1 .5103 are converted in 20values  and Xray powder
diffractometers : conventional and synchrotron facilities (CHESS, USA) [1]
77
monochromator, on the mosaic spread of the monochromator crystal, and on the
monochromator's scattering angle 20m . In Fig. 5 for several Xray and neutron powder
diffractometers the halfwidth of powder lines (Braggreflections) A20 is given as a function
ofthe scattering angle 20 . A large 20Mvalue can be favourable to realise smaller line widths
A20 at higher diffraction angles as can be seen for the D213instrument (20M = 135°) .
The plan of the E9 instrument at the HMIreactor BER II in Berlin is shown in Fig . 6 . The
typical technical data of this new powder diffractometer are :
" collimations a1 = 10', a2 = 20', a3 = 10'
" germanium and graphite monochromators with mosaicspreads AM(Ge) ~ 20' and
AM(PG) z 30'
" monochromator's scattering angle 40'
For a ADPpowder diffractometer the measuring time can be reduced substantially by the
simultaneous use ofmany single detectors or of linear multidetector systems .
As an example for a 2axes diffractometer specially designed for the investigation of
amorphous systems and liquids the 7C2instrument installed at the hot neutron source of the
ORPHEEreactor in Saclay (F) is shown in Fig . 7 . Combined with an exchange of
monochromator crystals there are there différent standard wavelengths available : A,(Ge(111))
= 1 .1 A, ;,(Cu(111)) = 0 .7 A, A,(Ge(311)) = 0.57 A. The linear multidetector allows a
continuous intensity measurement over a range in scattering angle of 128° . The angular
resolution of this instrument is limited as there is no collimation in between the sample
position and the detector. But the I (Q I range is very large . For the shortest wavelength
k(Ge(311)) = 0.57 A the accessible values extend up to (~ ,aX = 2n I H 20 A ' .
SOI!R(:E
CHAUDE
3 TYPES DE COLLIMAIION (BARILLET)
z
MOPI~;,~iROMA!E'~lRî i!TÎL!~ïAEiLE
Ge 111 ; Cu 1 ;1 ; Ge 311
~(:OLUMAfEUR SOUS VIDE
MGNITEUR
UIAFFIP;ACME
COL AAIEUR INT RNF
NCEINTE A VIDE PCUR PA 'j EUR D'FCH,ANTILLON
FOUR OU CRYOSTA
 ECNAN [IL ON
Mlr_ IDEIECTEUR 640 CFI.ü!LES
Fig . 7 . Plan of the 2axes diffractometer 7C2 at the hot source of the ORPHEEreactor in
Saclay (F)
In the case of the EDP method a polychromatic white beam is used with the scattering angle
being fixed (20 = const .). The dhklvalues result from the timeofflight measurement of the
neutron velocities  converted to wavelengths  for the hkl reflections . This technique is
specially suitable for pulsed neutron sources . Moreover, it offers some advantages for
7 9
complex sample environments, such as extreme temperatures, magnetic fields, external
pressures, etc . due to its fiedd scattering geometry . The resolution of the timeofflight
analysis Ot/t depends on the wavelengthdependant pulse structure of the moderator, on the
length of the flight path, and on the scattering angle 20 (a backscattering geometry is
recommended). As there are normally relatively short wavelengths in the beam, too, also
higher indexed reflections with shorter dhkivalues mat' be reached . Some typical technical
data ofthe IIRPD installed at the spallation source ISIS/RAL in England are shown in Fig . 8 .
A special feature of this instrument consists in the vert' long flight path of about 100 m .
6m 9m
choppers
95K liquid
methane moderator
curved guide
Fig . 8 . FIRDP (highresolution powder diffractometer) at the spallation source ISIS/RAL,
England. A resolution of Ad/d z 4 .104 is achieved with a samplc position at 95 m .
6
allI li IlI IIIIIIIIHII1 I IIIII1 ICI I IIIIII II~1!Hi1 1111 0111r
50
Fig . 9 . Powder diffractogram of bcnzene : (a) section from 0.72 Â
Ili1'i 11111111 i
0Y5 0.76
d spacïng (Angstroms)
. r " L
k
0.73 0.74 0 .75 0,76 0.77
Fig . 9 . Powder diffractogram ofbenzene : (b) enlarged section from 0 .73 Â
the diffraction plane) two further rotation axes x and (p, which are perpendicular to each other .
The xaxis is also perpendicular to the ù)axis . Together with the rotation axis of the detector
20 ( I 1 te, the (oaxis) this mechanical unit is called 4circle goniometer (leading te, the narre
4circle diffractometer for this type of single crystal diffractometers) . The measurement of
integrated intensities 1(H) of individual Braggreflections is performed according te, the
o)/n .20scan techniques described in chapter 7 .2 . For a computercontrolled automatic data
collection a detailed knowledge of the crystal lattice is needed. Therefore, a single clystal
diffraction experiment starts by a systematic search of reflections in varying x and cp, with the
restriction ca = 0 (bisected condition) . From the accurate angular positions of typically 20
indexed reflections the lattice constants and the orientation matrix are determined .
As an example for a single crystal neutron diffractometer the Pl10/5C2instrument installed
at the hot neutron source of the ORPHEEreactor in Saclay (F) is shown in Fig . 10 . The
monochromatic neutron flux at the sample position is increased by a monochromator system
with vertical focussing . The use of small wavelengths allows the measurement of Braggintensities
up to large H values ( H maX = 2sin0 maX/;, = 2 .8 L1
Fig . 10 .
Single crystal diffractometer P110/5C2 at the hot neutron source of the ORPHEEreactor
in Saclay (F)
Attention : The lengths of both the vector H ofthe reciprocal lattice used in clystallography
and the scattering vector (~ of solid state physics are expressed in Â 1 . But there is a factor of
271 which means that 1 H = 2 .8 A1 corresponds to 1 Q 1 = 17 .6 A1 .
7 1 2
The influence ofthe primary collimation ul on the halfwidth ofBraggreflections of a perfect
Ge crystal is shown in Fig . 11 . The resolution curves for two différent wavelengths
k(Cu(420)) = 0.525 A and k(Cu(220)) = 0.831 A are plotted as a function of sin 0/ ;,.
Fig . 11 . Resolution curves of the single crystal diffractometer Pl10/5C2 at the hot neutron
source ofthe ORPHEEreactor in Saclay (F)
References
[1] R . J. Hill, The Riedveld Method, ed . R. A . Young,
Chap . 5, Oxford University Press (1993)
[2] W. 1. F . David and J . D . Jorgensen, The Riedveld Method, ed . R. A . Young,
Chap . 11, Oxford University Press (1993)
Smallangle Scattering and Reflectometry
Dietmar Schwahn
8 . Smallangle Scattering and Reflectometry
Dietmar Sehwahn
'
8 .1 . Introduction
The methods of elastic scattering with neutrons deliver structural information from
arrangements of atoms and magnetic moments in condensed material . Those arrangements
can be precipitated phases in mixtures of metals, low molecular liquids or polymers and one
gets information about size, number density and corrélations between thé objects . In
scattering experiments thé intensity of neutrons is measured as a function of momentum
transfer Q
Q = 4n sirr 0
with thé Scattering angle 20 and thé wavelength k of thé neutrons. Q is thé différence of thé
wave numbers k (absolute value k=2n/A,) of incoming and scattered neutrons . The
momentum transfer is inversely proportional te, thé length scale of investigation ; at Q of thé
order of 1 A  'one measures inter atomic distances and in thé région 10  A' _1()4Â '
mesoskopic objects of sizes between l0A _1()4Â . For all these investigations specialized
instruments have been developed . In this lecture we will introduce instruments for small angle
scattering and reflectometly with neutrons . With these instruments objects within thé bulk and
at thé surface are investigated. The main elements of these elastic methods will be separately
introduced in thé last part of thé lecture . We will discuss instruments working at stationary
nuclear research reactors . In future spallation sources will become thé more important sources
as they show a larger neutron flux with a periodic time structure ; those instruments need quite
différent conditions for optimization .
8 .2 . Intensity at Sample and Detector
In Fig . 8 .1 thé traces of neutrons for elastic Scattering are depicted in real and reciprocal
space. The intensity at thé sample (in linguistic usage : primary intensity) is determined
according te,
AI, =LFM2 (8 .2)
by thé luminosity ofthé source given in units [CM2 s 1 steradian 1]
L= (1) ( k ) a e (k/k T ) 2 Ak
(8 .3)
27c k T k
for neutrons with wave vector k, the irradiated area of the sample F, and the divergency of the
primary beam described by the space angle AS2 . The luminosity L is determined by the total
Sample
AS4, A;,/a,
Figure 8 .1 : Traces ofneutrons in real und reciprocal space
thermal flux of the neutrons 1), the temperature of the moderator (h/2n) Z kT/2m=k,T and
the resolution of wave length distribution according to Ak/k and determined by the
monochromator. The scattered intensity in a detector element with space angle AS2D and
scattering angle 20 or scattering vector Q respectively is given as
(0; Q) AS2D (8 .4)
Al, (o ; Q)=Al o D. T .
dE
with sample thickness D and diminution coefficient T ofthe primary intensity (transmission) .
The macroscopic scattering cross section dE/M is the experimental result and is usually
given in absolute units [1/cm] .
8 .3 . Small Angle Scattering with Neutrons
The method of small angle scattering (SANS) is a broadly used tool in research. There are
three different SANS techniques : The pinhole SANS, the double crystal diffractometer, and
the focusing SANS . The First two types of instruments are being used in our laboratory in
Jülich, and a first focusing SANS instrument is presently built and will start operation in our
laboratory within the next year.
82
8 .3 .1 . PinHole SANS
The principle lay out of a pinhole SANS is depicted in Fig . 8.2 . Alter the fission process,
thermalization, and a further moderation in the cold source the neutrons are guided through
neutron guides to the instrument . Monochromator and collimator are filters for neutrons with
a predetermined wave length and divergency . The collimator consists of two apertures of
Selector Apertures Sample Detector
Lc=120m
wiw
LD =120m
Figure 8 .2 : Principle design ofpin hole SANS
neutron absorbing material as fi . Cd and as monochromator one has a velocity selector,
delivering a monochromatic beam of wave lengths between 5 and 15 Â wich a relative mean
square deviation of about < 8 ;~ z > o.s / < ;, >=0.1 . After passing both apertures the neutrons
irradiate the sample and part of the neutrons are scattered. The thickness ofthe sample should
be adjusted in a way, Chat only about 10% of the neutrons are scattered in order to avoid
remarkable effects from multiple scattering . The scattered neutrons are counted in a two
dimensional local sensitive detector. The neutrons not scattered by the sample remain in the
primary beam and are absorbed in the beam stop in front of the detector. The resolution
function of this experiment is given as
Q 2 k [( dD ) 2 (dE ) 2 S ( 1 1 ) 2 2 ( 87,' ) 2 j .
12 LD L S L s LD <
(8 .5)
The symbols Ls und LD represent the distances between the two apertures and between
sample and detector, the symbols dD and dE the diameter of the two apertures . For a given
instrumental setting neutrons can be detected in a limited angular interval ; the setting is
adjusted by the distance between sample and detector between 1 .25 und 20 m leading for the
83
possible neutron wave lengths between 5 and 15 A to a Q inteival of 10'Â'0 .3ÂI . The
resolution has always been adjusted to the instrumental setting and which is determined by the
length of collimation L ., The space between selector and first aperture is always bridged by
Figure 8 .3 : Sample intensity for different length ofcollimation
neutron guides which in segments of lm length can be posed in or out the beam; in this way
the primary intensity can be remarkably enhanced by a beam with larger divergency . This is
shown in Fig .8 .3 where the measured primary intensity is depicted versus the length of
collimation . The optimized conditions of the instrument are achieved, when all elements of
resolution in Eq .(8 .5) contribute the same amount to the ,desmearing" of the scattered
intensity . Optimal conditions are accordingly obtained for the following instrumental setting :
LD =Ls und dE =d D =2d s . (8 .6)
One always tries to perform measurements with as much intensity as possible with
sufficiently good resolution . Such an optimized instrument has a resolution of
8Q opt.=(k/ ~3 )  d,/LD (sec Egs.(8 .5) und (8 .6)) and delivers an intensity at the sample
according to
AI, =LAS2 L2 LD =L(Q) 4 L D . (8 .7)
D
The last relationship shows that the intensity at the sample is proportional to the square of its
length and is the reason of 40m long pinhole SANS instruments . The upper limit is
84
determined by the maximum divergence of the neutrons according to the total angle of
reflection.
A further important criterion for the quality of a SAS diffractometer is the sharpness of
the primait' neutron beam prepared by the collimator . In Fig.8 .4 primary beam for a given
72
N
103
" Si~
: , 2F,
r2
1 1 1
,
2F,/2
20 15 10 5 0 5 10 15 20
Position [cm]
Figure 8 .4 : Resolution curvefor a given configuration
configuration bas been depicted in a semilogarithmic presentation. One recognizes, that at
twice the full half width the primary intensity has been decreased to values between
10 5 und 10 6 . This result demonstrates that the instrument is in a good condition ; the
background near the primary beam is sufficiently small, so that also in thfs region scattered
neutrons can be sensitively detected and analt'zed.
8 .3 .2 . Focusing SANS
The principle of a focusing SANS has been depicted in Fig.8 .5 . The monochromatic neutrons
enter the instrument through an aperture with a diameter of about lmm and enter the focusing
mirror with the full divergence of the neutron guide . From the mirror the neutrons are
reflected and in the focal point the neutrons are detected from a local sensitive detector . The
resolution element of this detector has the saine size as the aperture of about lmm. Just
behind the minor is the position of the sample . The instrument with the lengths given in the
85
figure and with neutrons of about 15A wave length covers a Q range of (10 3 10 4 )A  ' ; it
measures in the resolution range of fght scattering . The intensity at the sample is given as
Figure 8 .5 :
Schematic design of a focusing SANS
AI o =LM2 L2 LD=L(4rc)(~Q) Z Lô (8 .8)
D
Within these small Q ranges this instrument is superior to the pinhole instrument because
neutrons with the maximum space angle 4y ~ of the neutron guide are used. The concept of
10 11
0 I I
a 10 _
â
I o,
AQo .5=3 .8510AI
',.
6
3 0 3 6
Abb .8.6 : Resolution curve ofafocusing SANS
Q L104A1 j
86
the focusing SANS is known for long time . However, only quite recently it is possible to
build such instruments with the necessary good quality as shown from the experimental
resolution culve depicted in Fig . 8 .6. The reason is the high demand on the surface quality of
the focusing minor ; those mirrors can be built today as the result of an extended project for
the development of Xray satellites .
8 .3 .3 . Double Crystal Diffractometer
From all three SANS instruments the double crystal diffractometer (DCD) bas the highest
resolution . Its concept is depicted in Fig .8.7 . The central part of this instrument are two
Figure 8 .7 : Schematic design ofa double crystal diffractorneter
perfect Silicon single crystals, mounted on an optical bench . The reflectivity of a perfect
crystal is described by the Darwin curve according to
1 ly l
< 1
R(y)= 1 _(l _ (8 .9)
2)0.5
y lyl > 1
and depicted in Fig . 8 .8 . The parameter y is the scattering angle which is normalized in a way
that the inteival where neutrons are fully reflected are within ~yj
1 .0
Danvinkurve
0 .8
0 .6
0 .4
0 .2
3x
0 .0 r .
. . ~~ . . . . . 1 . . . . 1 . . . .
3 2 1 0 1 2'
3
y
Figure 8 .8 : Darwin curve after single and triple reflections .
Fig .8 .9 and which is the scattered intensity from the second crystal . In the region IyI
three times, then one measures a Darwin curve multiplied three times with itself and gets a
reflection curve as depicted in Fig . 8 .9 with the region of total reflection and much sharper
2.0
0.5
i
0.0
54321012345
8[48]
Figure 8 .9 : Theoretical curves of resolution of the double crystal d~actometerfor singlesingle
(ss) and tripletriple (tt) refections .
Experim . Resolution : Si el ; 9~=4.48Â
0
4S(ss)54.2gad
4S(tt)=25.8gad
10 90 60 30 0 30 60 90
Scattering Angle b [Wad]
Figure 8 .10 : Experimental resolution afer singlesingle and tripletriple refections within the
channel cut crystal.
89
tails. This reflection curve leads alter folding to a much sharper resolution curve .
Experimental resolution curves of singlesingle and tripletriple reflections are shown in
Fig .8 .10 . One clearly see the effect of multiple reflections .
8 .4. Reflectometer
Investigations of surface properties by surface reflection of neutrons or Xrays is a relatively
new technique and is presently very active field in research . In Fig . 8 .11 the specular
Figure 8 .11 :
Traces ofneutrons and diagram ofmomentum ofspecular refection
reflection of neutrons at a surface is shown and in Fig . 8 .12 a reflectometer for neutrons has
been schematically depicted . Similarly to the pinhole SANS instrument in Fig .8 .2 the
divergency of the monochromatic neutron primaiy beam is determined by two apertures . In
this example the monochromatic neutron beam is determined by a single crystal within the
neutron guides . A linear position detector measures the reflected neutrons . Specular reflection
as shown in Fig . 8 .11 is defmed by the saine incoming and outgoing angle. In this case the (Q
vector has an orientation perpendicular to the surface and only heterogeneities in direction
perpendicular to the surface e .g . parallel te, Q are measured. An example is shown in Fig . 8 .13
giving the reflection profile of a Nickel metallic film coated on glass . In this case one
measures the heterogeneities formed between Nickel and glass and in addition the surface
roughness between Nickel and vacuum according to thé différent values of thé cohérent
scattering length densities . The intensity profile shows total reflection at small angles and then
at larger angles strongly decreases with periodic oscillations . From this profile one can
determine thickness and roughness ofthé metallic film.
8 1 0
Figure 8 .12 : Schematic design ofa diffractometerfor neutron refectometry .
Nickelschicht auf Glas
0.00 0.02 0.04 0.06 0.08
Q = 41r/Ä*sin0 (A')
" Messung (HADASReflektometer)
Fit : d = 837,5 A ; 6 = 14,5 A ; SQ = 2,08e s A'
 Simulation : d = 837,5 A ; a = 14,5 A ; SQ = 0
 Simulation : d = 837,5 A ; a = 0 ; SQ = 0
 Simulation : nur das Substrat
o Messung an der Substratoberflaeche
Figure 8 .13 : Curve ofrefectionfrom a Nickel surface measure at the "HADAS" instrument.
8 1 1
For the Nickel film one gets a thickness of 838 A and a roughness of 15 A . The open dots in
Fig . 8 .13 show the reflection from glass alone . One clearly observes a smaller angle of total
reflection and a decrease equivalent to the Darwin cuive in Eq. (8 .9) . At relatively small
intensities of 103 scattering from background becomes visible .
One can also study heterogeneities within the surface which are f i .
formed by phase
separation. In those cases one also observes nonspecular reflection in direction parallel to the
surface.
8 .5. Important Elements of Small Angle Scattering and Reflection
The most important elements of small angle scattering and reflection are (1) the neutron
guides for an effective transport of neutrons, (2) the velocity selector and the perfect single
ciystals for monochromatization ofthe neutrons, and (3) the local sensitive detector for a fast
detennination of the scattering angle .
8 .5.1. Neutron Guide
The phenomenon of total reflection is demonstrated in Fig .8 .13 on a Nickel film . This effect
is used to transport neutrons through neutron guides over long distances without much loses .
The angle of total reflection is given as
o c = ;~ (P / 7L) o .s (8 .11)
with the coherent scattering length density p . Natural Nickel is a good choice for coating
material in order to have a large angle of total reflection (see Figure 8 .13) ; an even better
choice is the isotope Nickel 58 because of its large coherent scattering length. So, for natural
Nickel one gets a total angular of reflection of Oc = 6' . A, [A] and for the isotope 58 a
O c =7.1' .k[A] .
About 30 years ago neutron guides were invented at the research reactor in
München ; Neutron guides lead to a much broader use ofneutron scattering wich instruments
posed far from the source and with much better conditions .
Neutron guides coated with a socalled super minor transport neutrons with even
larger angles of divergence. In addition to Nickel those minors consist of altemating layers of
two different metals (their coherent scattering length density must be sufficiently different)
wich an ingenious sequence of different thickness, in order to excite Bragg scattering in a
continuous range of Q perpendicular to the surface . In this way the angle of reflection of
Nickel can bc increased by more than a factor of two ; however, the best achieved reflectivity
of super minors is still slightly less than one so that one gets appreciably losses of neutrons if
transported over long distances . .
812
Neutron guides also enable to transport neutrons on curved traces . The bending radii
can be made very small by socalled
bender guides consisting of several small and parallel
channels . Bender with proper materials for the layers are also used as a polariser .
8 .5 .2 . Velocity Selector
mhC , tetnßhe: ao m .,
'.Zwicht : 3,e ..
Figure 8 .14 : Rotor ofa velocity selector built at FZJülich .
91~ FÄl
Figure 8 .15 : Timeoffight spectrum from a velocity selector. The neutron wave length is
evaluatedfrom the velocity, e.g. from the fight time and the distance between chopper and
detector. The small dip in the intensity at 7.94Â is caused from Bragg scattering in the
Bismuth filterjust behind the cold source and is used as a reference value .
8 13
I
The rotor of a velocity selector is shown in Figure 8 .14 . This rotor is mounted in a housing
and can rotate with a speed up to 30000 ipm. It is transparent for a given wave length
depending on the speed of the rotator . A distribution of neutron wave length aller passing the
selector is shown in Figure 8 .15 . The neutron wave length is inversely proportional to the
frequency of rotation ; the exact relationship and the halfwidth of the wave length distribution
is determined by the tilt angle and the width ofthe channels .
8 .5.3 . Local sensitive Detectors
Local sensitive detectors are necessaiy for an optimized use of small angle scattering and
reflection instruments . The resolution element of a detector for the pinhole SANS is typically
0.5lcm, for the focusing SANS and reflectometer lmm. A two dimensional local sensitive
detector has at least 64x64 resolution elements . There are detectors on the basis of gas and
scintillation detection.
8 .5.3.1 . Gas Detector
The presently mostly used detector for SANS are 3 He gas detectors . The neutron is absorbed
by an 3 He gas atom which then decomposes according to
3He+n 3
H+ 1H+0.77MeV (8 .12)
cathode
neutron
primary
ion izetion
La L,~ Me
avalanche
I
I
I
1 H
drift
~ region
'TJT7TTTTT7
onode
Figure8 .17 : Process ofdetection of the 'He gas detector
814
into two ionic particles with kinetic energies of 0.573Mev and 0.191Mev for the proton and
the 3 H (tritium), respectively . As shown in Figure 8 .17, both ions cause a "primary"
ionization cloud within the suiroundings where the neutron was absorbed. These ions are
accelerated by an electric field and produce by a socalled "secondaly" ionization process an
avalanche of ions . Only the electrons give a signal at the anode because they achieve a much
larger acceleration according to their small mass. The size of the voltage pulse at both ends of
the anode is used for determination the position of absorption and thereby the scattering
angle . In a twodimensional detector there are two perpendicularly arranged wire lattices,
from which by coincidence measurements the position ofthe absorbed neutron is determined .
8 .5 .3 .2. Scintillation Detector
Another type of detector are solid state detectors using the principle of scintillation.
reaction equation is the following :
6 Li+n 4He+ 3H+4.79MeV (8 .13)
The
A Li glass with 6.6% 6 Li is mixed with Cerium (Ce) . By absorbing a neutron in 6Li two
ionic products of reaction are formed, which interacting with Cerium produce about 4000
photons of 400nm wave length per neutron. In the disperser the photons form a light cone of
90° as depicted in Figure 8 .18 . The light cone is adjusted by the thickness of the disperser and
by the slit between scintillator and disperser (total reflection) so that the light overshadows
two photo multiplier . The photo multiplier have a diameter of 8cm and in total 8x8 photo
Neutron capture event
Reflector
Scin tillator
Air Gap
Light Disperser
Light Cone
Figure 8 .18 : Process of detection ofa 6 Li scintillation detector
8 15
multiplier are arranged in a quadratic array . The resolution of one pixel is 0 .8 cm . Such a
resolution becomes possible by an algorithm calculus from the light intensities of several
photo multipliers . In a first stage a rather rude determination with an uncertainty of 8cm is
made by the position ofthe photo multiplier with the largest light intensity . In a second stage
he neutron position is determined by also considering the intensity of the neighboring photo
multipliers . An important advantage of this detector is the large atomic density of the
absorbing material and its consequently large detection probability; a lmm thick absorbing
material of a scintillator bas a 93% detection sensitivity of 7 A neutrons . Such a detector
(Anger camera) was developed at the Forschungszentrum Jülich and is used in our KWSI
small angle instrument .
References :
Books :
J.S . Higgins und H.C. Benoit, Polymers and neutron scattering. Clarendon Press, Oxford
(1994)
C.G: Windsor, Pulsed Neutron Scattering. Taylor & Francis, London(1981)
P . Convert and J .B . Forsyth (eds .), PositionSensitive Detection of Thermal Neutrons .
Academic Press, London (1983)
X.L . Zhou and S .H. Chen, Theoretical Foundation of XRay and Neutron Refectometry .
Elsevier, Amsterdam (1995)
Articles about single subiects :
W. Schmatz, T. Springer, T . Schelten and K . Ibel, J . Appl . Cryst . 7, 96 (1974)
D . Schwahn, A . Miksovsky, H . Rauch, E . Seidl and G. Zugarek, Nucl . Instrum . Methods,
A239, 229 (1985)
B . Alefeld, H .J . Fabian, D . Schwahn and T. Springer, Physica, B156&157, 602 (1989)
D.Schwahn, G.Meier and T .Springer, J. Appl . Cryst. 24, 568 (1991)
M . Heiderich, R. Reinartz, R . Kurz and J . Schelten, Nucl . Instrum . Methods, A305, 423
(1991)
8 1 6
Crystal Spectrometer :
Tripleaxis and Backscattering Spectrometer
F . Güthoff and H . Grimm
9 . Crystal spectrometer :
tripleaxis and backscattering spectrometer
F .
Güthoff, H.Grimm
It has been emphasized in the preceding lectures that thermal neutrons provide wavelengths
k comparable to interatomic distances and energies hw in the order of collective excitations
of condensed matter. In order to determine the properties of a sample  as represented by the
scattering function s(_Q>ü) °c dZ6 /dÇ2dE'  a variety of instruments may be used . The evaluation
ofthe single differential cross section represented by d6 / dÇ2 is the topic of diffractometers
. However, since  in general  the scattering ofneutrons by the sample is connected with
an energy transfer it suggests itself to analyze the neutrons scattered into the solid angle dS2
in addition with regard to their energy . Introducing and investigating the double differential
cross section dZG / dS2dE' thus corresponds to the switching from diffractometer to spectrometer.
In order to determine which energy transfer E  E' = ho) is associated with which
momentum transfer _Q, the neutrons have to bc characterized before hitting the sample by
means of the socalled primary spectrometer and after leaving the sample by the secondary
spectrometer . It will be shown in the lecture on timeofflight spectrometers that the energy
of neutrons can be determined via selection of velocity and travel time . Recall that thermal
neutrons (300K) having an energy of kBT =%2 mv2  25 meV travel with a speed of about
2200m/s . According to de Broglie one may associate a wavelength ;, to a moving particle
with mass m . This fact is used by crystal spectrometers which  by means ofBragg scattering
select neutrons of energy
n ;, =2dsin0 (1)
h 2k2
2m
h z
2
2M;`,
(2)
under Bragg angle 0 for given spacing d of the selected atomic planes .
wave vector is related to the wavelength by k = 2n / ;, .
The modulus of the
Two types of crystal spectrometers will bc introduced in this lecture . The tripleaxes spectrometer
represents one of the earliest neutron spectrometer types . It was developed by B . N .
Brockhouse . By means of this facility his essential studies [I] resulted by the end of the
fifthies laying ground for his winning of the Nobel prize for physics in 1995 . In contrast, the
backscattering spectrometer is of more recent origin (the first facility of this type was put into
operation in Jülich at the beginning of the seventieths by B .Alefeld) and was stimulated by
ideas of MaierLeibnitz [2] .
Both types of spectrometers can be  similar to timeofflight machines  positioned at cold
and thermal neutron sources . Especially for tripleaxes spectrometers the possibility is realized
to use them at hot sources where neutron energies range up to leV .
10 .1 Common features of crystal spectrometers
One of the most important properties describing and characterizing spectrometers is the resolution
function . It is essential to determine and to optimize this function since it determines
the type of dynamical behaviour which may successfully be measured . For a substance to be
investigated, this might mean that several différent spectrometers are to be employed in order
to determine thé whole range of interesting excitations . According to thé expected excitation
energies not only a change in thé modération of thé neutron source but also switching to a
conceptually différent spectrometer might become necessary . However, already for a given
spectrometer, resolution and flux may be varied by an order ofmagnitude taking advantage of
available measures . Amongst other aspects, thé knowledge of thé instrumental resolution
function is of central importance in view of thé rather limited neutron flux, since  for example
 thé size of thé measured signal varies proportional to thé inverse fourth power of thé
chosen average collimation for a tripleaxes spectrometer. Thus, for each experiment, a suitable
compromises between resolution and intensity have to be chosen . A comparison might
elucidate this point : e .g . 10 17  1021 quanta/s are typical for a LASER beam whereas a reactor
like thé DIDO offers normally 10 6  10 7 neutrons /cm2 s (monochromatic) at thé sample
position . In order to make thé most efficient use of those neutrons, différent strategies  discussed
below  are pursued by thé various crystal spectrometers .
For a crystal spectrometer one may Write thé measured intensity scattered into thé solid angle
Abt with thé energy spread Ahoi in thé form :
Nd2a
AI = A(k)  k  p(k)  AV .
 p ' (k ' )  AS2 . AhùL) .
 dMdw
pximaryside
sample '
dry side
The frst part ofeq . (3) up to thé cross section of thé sample represents information about thé
spectrum of thé neutron source A (k) and thé reflectivity of thé monochromator p(kb ; thé number
of scatterers in thé sample is N. The last part refers to thé signal measured by thé secondary
spectrometer . Since monochromator (primaiy side) and analyzer (secondary side) act by
thé saine physical principles it is advantageous to describe thé instrumental factors and thus
thé resolution in eq . (3) more symmetrically . To this end we use thé already introduced relation
between cross section and scattering function
d Za
df2dc L)
k'
= S(g,0 )
k
hz
h,
and with the hel of
4k~ Akl
AS2~ ~CAw
~ Z '
p =
AV we can rewrite eq.
=
k z ~ m kAki m . k'
(3) to
AIccA(k)NS(Q, üL )p(1)AVp(,L)AV' ,
where  as will be shown below  the volume elements in
AV = Ak11 . Ak . Aki .
wave vector space are given by
In this section, now, the most important elements for the tripleaxis and the backscattering
spectrometer shall be introduced . It will become obvious that exploiting an essentially identical
principle leads to quite différent setups and properties . As a first step the general influence
of various components on the resolution will be descrbbnd by means of the tripleaxis
92
machine which will be followed by an optimization of the physics involved (one sided in a
certain sense) in the shape of the backscattering spectrometer.
10 .2 Principle of the crystal spectrometer with three variable axes
Fig. 1) shows the principle layout of a tripleaxis spectrometer. Neutrons of a defmed wavelength
Â are selected from an incident "white" beam by means of a single crystal (monochromator
M, ferst axis) under the associated angle 20, according to eq . (1) . The sample S
under inspection is positioned in the diffracted beam. The secondary spectrometer moves
around the sample thereby selecting neutrons scattered by an angle 20, (second axis) which
are further sorted with regard to their energy via the angular setting 20, of an analyzer crystal
A (third axis) and counted by detector D . The scattering vector 2 as well as the energy transfer
ho) are determined by the angles 20, and 20, for given incident wave vector k (see
also Fig . 2) .
Fig. 1)
schematic layout of a tripleaxis
spectrometer
with :
collimators a ,, monochromator
M, sample S,
analyzer A, detector D,
incident (scattered) wave
vector k (k
Thereby, the wave vectors k and k' are connected with the variables Q and ho) by the conservation
of momentum and energy . In the resulting scattering triangle (Fig. 2) the deviation of
the foot F from Y Q determines the energy transfer hco . The sense of this deviation determines
whether the neutron bas gained (k < k, EE'=hco < 0) or lost energy (k > k, hco > 0)
by the scattering process . In order to influence the divergence of the neutron beam, collimators
a are inserted before and alter the crystals by which neutrons are selected . Detection of neutrons
is by materials with an exceptionally large absorption cross section . The involved nuclear
processes are e.g . 1OB(n,a), 6Li(n,a), and 3He(n,p) . The most common type of detectors
is conceived as proportional counter filled with 3He having an absorption cross section of
5300 barn for neutrons with 25 meV . With the typical active length of about 5 cm and a filling
pressure of about 5 bar, the counting probability reaches >95% for thermal neutrons (the absorption
cross section is reciprocal to the speed of the neutron) .
It is meaningful to insert a neutron monitor at the exit of the primary spectrometer . This device
is principally similar to a counter absorbing and detecting, however, a small fraction of
the incident neutrons, only . The measured spectra may thus be normalized to the number of
incident neutrons which is essential for long measuring periods since the neutron flux may
9 3
undergo appreciable fluctuations . In addition, for a reactor of the type DIDO, the average neutron
flux increases by about 10% during a normal cycle .
The term tripleaxis spectrometer indicates already the versatility of this instrument (not only
in real space) which distinguishes this concept front other types of spectrometers . As long as
the radius of action is not barred by the radiation shielding, arbitrary points in Q, _w  space
may be selected. For fixed incident wave vector, those points belong to a parabolic surface
which is defmed by momentum and energy conservation as shown in Fig . 3) .
Q=kk'
AE=hco=Z~~(kZk f z)
.
AE=ti(kkZ)/2m
1/2Q = 1/2(kk`)
1/2 hoo
Q
h2 Q3 / 2m
Fig . 2)
Geometrical relation between
wave vectors k and k' on the one
hand side to momentum h Q and
energy transfer hco on the other
hand . Since (k k~ represents 6
dimensions, yet (_Q, 0) ) 4 dimensions,
only, arbitrary solutions of
vector P on the plane perpendicular
to Q result for a given (_Q, OJ )
point.
Fig .3 ) representation of the theoretical
measuring range of a neutron
spectrometer with fixed incident
wave vector k.
9 4
10 .3 Beaur shaping
Due to the fact that neutrons are uncharged and thus may penetrate materials rather easily,
neutrons may bc bundled or focused to a limited extent, only . This aspect aggravates with increasing
neutron energy . Already in the source, there arises the problem to guide a suitable
number of neutrons through "holes" (beam tubes) in the biological shielding to the experimental
setup. From the total solid angle of 4n , only the fraction travelling in the direction of the
beam tube will contribute to the flux . The used divergence of the beam is can merely bc chosen
by annihilating all those neutrons by absorbing materials travelling outside a defmed angular
range . Thus a beam tube represents the simplest version of a collimator . It is comparable to
a system of two diaphragms positioned in a distance of some meters . With a typical length of
3 m for the beam tube and a cross section of 0 .1 m there results a divergence of about 2° for
the neutron beam .
Now it turns out that it is less meaningful to collimate the neutron beam in the vertical plane as
tight as in the horizontal (scattering) plane . Tilting the scattering triangle (Fig . 2) slightly out
ofthe scattering plane influences the selected (,0, 0) point either not at all or in second order,
only . If collimation shall be achieved within a short distance, thereby making allowance for a
desired anisotropy, one uses a socalled Soller collimator. To this end, a set of coplanar foils
coated with absorbing material is mounted vertically with a distance of say 1 to 5 mm .
Choosing about 30 cm for the length of the foils, one may achieve a horizontal divergence of
the neutron beam in the order of 10 minutes of angle . Yet one has to take into account that
switching to half of the divergence entails about the saure reduction of the neutron flux! The
facts that the foils have a finite thickness and that their absorption is less than 100% modifies
the ideal triangular transmission curve by rounding the top and by the appearance of tails beyond
the base . This modiffed curve may well be represented by a normal distribution  a useful
property for folding operations. In regard to the interpretation of measured data the more
sharply limited resolution triangle as realized by the chopper of a timeofflight machine
would be more desirable . Since a well defmed cutoff clearly separates the change from elastic
to inelastic scattering the difficulties in interpreting the quasielastic transition region which
involve the knowledge ofthe exact shape of the resolution function are greatly reduced .
The anisotropy of the divergence may be exploited by a vertically focusing arrangement of
monochromator and/or analyzer ciystal in order to increase the neutron flux at the sample as
shown in Fig. 4). It is well known from optics that the inverse focal length is given by
1 /f = (Ll +i2 ) and that the ratios of heights for image and source is equal to that of their distances
L IL, . Since, in general, the Bragg angle 0 7~ 0°, the focal length depends on the
Bragg angle and the radius of vertical curvature by
f _
R
sin0
The distances 4,4 for a given spectrometer are to be considered as fixed quantities and thus
the curvature R of the crystal bas to be variable . This may e .g . bc realized by the parallel arrangement
of lamellae of single crystals which can be tilted individually . An additional gain
factor results from the height ratio of monochromator to source . Depending on the relative
heights of sample and crystals an increase ofthe neutron flux at the sample by a factor of 2 to
6 might be achieved. The possibility of a horizontal focusing  whereby the influence on the
resolution is no longer negligible  will be discussed further down.
9 5
Fig. 4) vertical focusing :
The gain factor P for the intensity at
the simple is givenby the ratio of
heights for source and image (hi/hz)
and the height of the deflecting crystal
hm in nuits of the height of the source
by :
_ crysFal~,~~e _ h~ Li_±Lz
cystaln~~ L2 hl
Similarly to e .g. light, one may mirror and thus guide neutrons . On the basis of the Fermi
pseudopotential V one obtains the index of reflection for neutron by
k V I 2A 2M ' p(z) b, (r) ~ 2 = 1 E
p(r) b, (~)
b2 k2
ko
( 2m ) ' =1 2;
where b,oh (r) denotes the average scattering length and p(r) the particle density . The losses
due to the total reflection are small even for a rather modest quality of the mirroring surface .
By suitable coating the simple beam tube may become a neutron guide and the 1/r2law is
thus circumvented. According to eq. (9) one should use materials for such mirrors which possess
a large coherent cross section together with a large atomic density which is fulfilled for
the isotope S 8Ni with b =14 .4 10  ' S m . Since the limiting angle for total reflection is ex
tremely small (0, / Â z 0 .1°/101°m), simple homogeneous coating could be used successfully
for cold neutrons, only (the technique to produce super mirrors opened the possibility for
guiding neutrons with energies up to the thermal range) . By means of the neutron guides instruments
having still a high neutron flux can be set up at larger distances from the reactor
core . If , in addition, such a neutron guide is slightly curved one can avoid the direct view onto
the core which reduces the background . Simultaneously, one obtains an efficient ;,/2filter by
suppressing the unwelcome faster neutrons. A marginal note might be added : in the case of extrente
cooling of neutrons one may keep and store them in "bottles" since they are totally reflected
under arbitrary angles .
10.4 Resolution for diffraction by a crystal
As we have seen already, single crystals offer the possibility to corrtrol the travelling direction
of neutrons . Thereby use is made of their coherent, elastic scattering properties which  according
to eq . (1)  allow for deflecting neutrons from an incident "white" beam under the angle
20 . This Bragg scattering becomes possible as soorr as the scattering vector corresponds
to a reciprocal lattice vector, i .e .
Q=_kk' =G (10)
and eq. (7) satisfies the condition DE = 0, or expressed differently by :
9 6
G.k=zGz . (11)
This case is fulfilled if as shown in Fig . 5)  the projection of the wave vectors onto
Cz is just equal to 1 / 2  G .
Fig 5)
illustration for the
selecticn of scattered
wave vectors and
1/2G = k . sinO
their divergence as
determined by the
k ` k` modulus G and the
  2  scattering angle .
       kAG/G °G/ G is of the order
of 104 and is thus
negligible for tripleaxis
spectrcmeters .
k . cot 0
The variance of a selected k vector is given by the derivative of Yz G= k sin0 , or
4k  4Z  1 4E  OG + cot0  40 .
k Z 2 E G
With increasing wavelength ofthe neutron the energy resolution will be improved.
2 .0
n É
m
w 1 :0
m
x
C
O
(12)
c 0 .5
Fig . 6) schematicrepresentation of the variance 4~.
as a fonction of scattering angle and material
9 7
1 2 3 A 5 6 7 8
neutron wave vector k ,(A 1 )
Fig . 7) monochromatic flux at the
IN8 (ILL) for various materials as
afonction of k [3]
Back to the "bottled" neutrons : in this case it is the half life time of the free neutron of about
13 minutes which fmally limits the variance ofthe energy .
The probability for a kvector to obey the Bragg condition is both given by the "thickness" of
thé bisecting plane (constructive interférence ofthé contribution of thé lattice planes) and by
thé variance of thé orientation of G . The former condition means a relative sharpness of thé
modulus of CL in thé range of 10 ° to 10  ', whereas thé latter is fulfllled with an accuracy of
about 10 8 for an illuminated crystal surface in thé order of cm2 . Simultaneously, eq. (12)
expresses thé dependence of thé résolution on thé material of thé crystal, i .e . thé lattice parameter.
This is exemplified in Fig . 6). The smallest variance in k (or ' ) results for a Bragg
angle of 90° . This range of O  90° is not accessible for usual tripleaxis spectrometers .
Ideal crystals would be nearly prohibitive for measurements with the tripleaxis spectrometer
since their variances in the lattice vector are too small as to reflect sufficient intensity . Therefore,
the perfection of the crystals is artificially degraded by various methods . Possible methods
are elastic bending of the crystals or a continuous variation of the lattice parameter in socalled
gradient crystals . The breakthrough in the successful preparation of gradient crystals
which implies a complicated and costly procedure was achieved satisfactorily in 1995 in BerlinAdlershof
with GeSi crystals . A comparably widespread method is the deformation of
perfect crystals, thereby generating an imperfect mosaic crystal by introducing dislocations .
On may imagine such a crystal as being composed of small perfectly crystalline blocks  the
1
Fig . 8) Braggreflexi onby a
crystal width mosaic spread il
and collimations ŒO und a,
mosaic pebbles  whose orientation is normally
distributed. A common fullwidthhalfmaximum
or mosaic spread is in thé Order of 30' .
Fig. 8) illustrates the operation of such a crystal as
monochromator . The neutron beam incident on the
crystal is given a divergence a. . A perfect crystal
would reflect just one wavelength for each angle
OM , as expressed by the section of the dashed line
(bisecting plane) limited by a, (
tribution of bisecting planes (ntosaic) which spans the hatched area being proportional to
k 2 cot0, . Together with the vertical divergence iß delivering a contribution of ßk there results
a resolution volume being proportional to k' cot 0,,, . The variance ofthe scattering angle
AO in eq . (12) follows to (without derivation) :
a 2 a 2 + a 2 2 + a2 172
2 2 2
ao+a, +41
(13)
This dependence shows that the gain in intensity by the mosaic crystal is not to be "paid" by a
worse energy resolution for ao = a, ! Generally, the influence of ri on AO is weak . (Fig . 9)
Which crystals should now be used as monochromators for neutron? Apart front the lattice parameters
further criteria are to be considered : those are the reflectivity, the suppression of
A,/2contamination, and last not least the availability as given by the technical and fmancial effort
for their production in suitable quality and size . For example, for the saine reflected
wavelength, Cu bas a better resolution as graphite (PG means pyrolytic deposited graphite),
however, an appreciably lower reflectivity (see table 1) and Fig . 7)) . The elastic form factor of
the crystal
plays an important role saine it represents the coherent scattering length and the extinction
cules . Eq . (14) delivers for the diamond lattice the form factors :
2 h+k+1= 4n
F(Q)=_b 1±i = 2n + 1
0 = 2(2n + 1) !!
Thus Ge and Si have the desired property to suppress the ~,/2contamination of the reflected
beam by means ofthe forbidden (222)reflection when using the (111)reflection.
1 .0
Fig . 10) transmission of
PGfilters [4]
0.8
a .s
0.4
0.2
0.5 1 .0 1 .5 2.0 2.5
wavelength ~ iA
99
Choosing PG or Cu one gets contributions of higher order apart from the wavelength scattered
first order . It is important to eliminate those contributions carefully in order to avoid any
ambiguity of the measured signal . One may circumvent this problem by inserting suitable materials
as filter, however, at the expense ofweakened intensity . In addition, there result limitations
in regard of the freedom to ctroose the wavelength as can be seen by the example of the
frequently used PGfilter . The corresponding transmission curve is shown in Fig. 10) . The
goal is to choose a wavelength À for which the filter offers an especially large transmission
and, however, a large absorption for integer fractions Â /n . With the choice of' =2.37  1010
m, neutrons with 2 Â and 3Â =2 .37  10 10 m will be largely suppressed. The wavelength
Â =l .55  1010 m offers itself, as well . Above Â  4  1010 m , as in the case of a tripleaxis
spectrometer at a cold source, one uses a Berylliumfilter cooled by liquid nitrogen as a cutoff
for shorter wavelengths .
Table 1) properties of frequently used mosaic crystals
material graphite (PG) Ge Cu
reflection (hkl (002 (111 (220)
À range / 1010m upper limit 6.708 6.533 2.556
( ~t 2d)
lower limit 1 .16 1 .13 0.444
(0=10 .)
peak reflectivity Â = 1 10 10 m   14
(0/) = 2 10 10 m 74 24 32
= 3 10 10 m 82 34 
= 4 10 10 m 87 43 
absorption 5104 0.058 0 .19
details (222) forbidden "bad" mosaic distribution
costs 20000 15000 5000
per crystal in DM (coarse)
Mosaic distribution of a crystal and beam divergence are not the only means to influence
resolution and intensity . Those properties may be varied also directly by the choice of k . In
order to offer more neutrons at the conespondingly large or small incident energies, one shifts
the maximum in the energy spectrum of the reactor neutrons by cooling (D2 at 25 K) or heating
(C at 2000 K) of a moderator. A spectrometer placed at a cold source (small k), has a
higher resolution as compared to ttrose placed at thermal or hot sources . Thus, by selecting different
moderation, one may vary AE between orders of 0 .01 meV, 1 meV, and 100 meV .
One notes that nearly all introduced components affect the resolution function of the spectrometer
. This function  a four dimensional ellipsoid  results by projecting the product of the
volume elements AV and AV' onto the (L), ü) space (integration over the two dimensional
vector P in Fig . 2)[5] . In the upper part of Fig . 11), the orientation of the volume elements
with respect to k and k' are indicated as well as projections of the resolution function . Inclination
and widths of the ellipsoids depend strongly on the scattering sense  part (II) of the figure
. Part (III) shows that there results an appreciable increase of the wave vector spread for
scattering twice in the Same sense . Il is just those different projections on the various (Q, 0J)
910
directions which is exploited for the measurement of phonons. By adapting the slope of the
resolution ellipsoid to the slope of the dispersion curve in question one achieves a focusing effect
 as shown schematically in Fig . 12). This exemplifies an important possibility to influence
the quality of the measurement.
The following two figures shall demonstrate
how one can obtain a complete picture of the
dispersion surfaces by measuring phonons at
selected symmetry direction and making use
of a lattice dynamical calculation . In contrast
to TOFinstruments recording simultaneously
many points on the surface shown in
Fig. 3) (e.g . 128 angles * 1024 time channels),
one may measure just one point with a
conventional triple axis spectrometer . Fig .
13a) shows a seau in energy direction, i .e . a
series of such points, whereby the vector
is kept fixed in the system of the inspected
crystal. Thus the widths of the observed
peaks represent the frequency or energy
width of the phonons folded with the resolu
tion . The scan also demonstrates the general (II)
case that several phonons will contribute to \
a seau according to their dynamical structure R j
factor . In fact, the Same peak positions but
quite different intensities will be observed at
equivalent positions in other Brillouin zones .
On the one hand side this equivalence serves
as experimental cross check for the peak positions
(eigenvalues) and on the other hand
one may derive the eigenvector from the observed
intensities for a selected phonon .
1 no)
The dispersion  often illustrated as curves
along symmetry directions (e .g. Fig . 13b)) 
represent of course dispersion surfaces being
periodic with the Brillouin zone . In general,
this surface needs not to be determined completely
by further scans . One rather fils a lat
tice dynamical model (see lecture on inelastic
neutron scattering) to the observed peaks and
may extent this calculation to arbitrary wave
vectors which "predictions" might in turn be
tested experimentally . The dispersion surface
for Barium is shown in Fig . 14) in the (O31)
plane [8] . Directly measured have been the indicated
points, only . The remainder results Fig . 11) dependence of widths and inclinations of the resolution
ellipsoid from the configuration of the spectrometer ((I)
from a fitted lattice dynamical model .
and (11) from B . Domer [6], with ki  k and kf  k~
911
scan direction
v
scan direction
dispersion curve
ti .
q
intensity
Fig. 12) Effect of focusing for measurements
of phonons . The integrated intensity is the
same in both cases . The focused mode (upper
part) exhibits a smaller width and a better signaltobackground
ratio.
N
2
h
T
U
c
N
3
a
.
E
N QV)
C
0
U
wavevector q Fig. 13) Phonon dispersion for A1203 (sapphire)
along the (010)direction at 20 K . The points
(phonons) in
a) result from the maxima observed in many separate
scans . E.g. the results within the marked region are obtained from scans as shown in b). Such scans display however
not always all theoretically expected phonons simultaneously . The solid line in a) represents the fit of the
experimentally obtained data to a lattice dynamical model ; in b) the line corresponds to the fit of the response
fantion broadened by the resolution function of the instrument to the observed scattering intensity (inmany cases,
a one dimensional folding with a Gaussian is sufficient for fitting the measured spectra) . [7] .
9 1 2
Fig . 14) Dispersion surfaces for Barium in
the (110)plane . The solidlines correspond
to the main symmetry directions,
the points to the various observed pealc
positions of intensity . The transition from
lighter to darker points corresponds to that
from longitudinal to transverse polarisation
of the phonons .
A fmal aspect for optimising the spectrometer shall now be mentioned . Considering the dispersion
for Barium it becomes obvious that the dependence on wave vector for the so called
acoustic phonons is not exceedingly large towards the zone boundary . Optical phonons (sec
the lecture on phonons and magnons) exhibit this property in most cases even more clearly .
This means that one could achieve more intensity or shorter measuring times by reducing the
resolution and keeping the energy resolution constant, i.e . keeping the distinctness of the
various phonon branches . This can be achieved by means of a horizontally culved monochromator
and/or analyzer as drafted in Fig . 15) . About a factor of five in irrtensity may bc
gained by this horizontal arrangement. Experiments using doubly focusing deflection crystals
exist since a couple of years requiring, however, a high degree of skill and experience .
k
1
1
0#0#0#0#0 0=0=0=0=0
1 2 3 4 5 1 2 3 4 5
k#k#k#k#k
k=k=k=k=k
1 2 3 4 5 1 2 3 4 5
Fig. 15)LA hand side : energy and resolution are determined by the deflection angle O as well as by the collimators
absorbing all neutrons travelling outside the accepted divergence . Right hand side : for the so called
monochromatic focusing, all deflection angles and thus the energy of the neutrons are equal due to the curved
crystal such that the divergent (i .e . relaxed Qresolution) but monochromatic neutrons merge together at the focusing
point . Caution! the average energy of the setup bas now become dependent on the sample position due
to the omitted collimators . The resolution will depend on the size of source and sample relative to the radius of
curvature .
9 13
10.5 BackScattering Spectrometer
It follows from Fig .6) and eq . (12) that for a given divergence
of the neutron beam a crystal will achieve the optimum
resolution in the modulus of k_ for the case of backscattering,
i .e . for 0 = 90° . This is the basic idea for the
backscattering( ;r )spectrometer which realizes this optimum
deflection angle both at the monochromator and the
analyzer . For the case of backscattering one may rewrite
eq. (12) to :
Aḵ div
_4k 1 1 
(AO)2
4, j d , cos(AO / 2) 8
(15)
Fig. 16) Braggreflection in the case of
near baclcscattering
Assuming that the divergence of the beam is determined by a neutron guide, one gets from eq .
(9) and for the isotope 58Ni
AO,,; 
2 (4zpb )
k
(16)
Inserting AO,,,; into eq. (15) delivers ° o ~dN  5105 and with eq. (12) an energy resolution
of AE = i AkN; 2  E / k2  2 .410 7 eV. This contribution to the energy resolution is thus independent
of the selected energy . Even with a triple axis spectrometer at a cold source this extreme
value of AE is out of question . An additional contribution to the variance of k results
from primary extinction, i .e . the fact that a final number of lattice planes contributes to the
Braggreflection, only. Perfect crystals are used in order to maximise this number . This second
variance is expressed in Fig . 5) by the thickness ofthe bisecting plane . The primary extinction
is proportional to the number of unit cells per volume NZ and the absolute value of the structure
factor FG, and inversely proportional to G2. For perfect crystals like e.g . Si the additional
variance is of about the saine order as that due to the divergence of the kvector . The maximum
error for the energy results then from the sum of both contributions, i.e . adding the extinction
in eq. (15) (without derivation).
AE Ak (AO)2
=2(
E ZCk
8 +
0 div
16 ZNZF, 1
G Z (17)
Yet, how is it now still possible to vary the incident energy at such a spectrometer being restricted
to the deflection angles 0=90' ? To this end one needs  according to eq. (1)  a
variation of the lattice parameter or the reciprocal lattice vector !2 . This can be achieved by
heating the monochromator crystal or simply by moving the crystal (periodically) parallel to
the direction of G with a velocity v,, . The change of energy (in the laboratoty system, Doppler
effect) is then
AE= 2E vo / v (18)
9 1 4
whereby E and v,, denote energy and speed ofthe backscattered neutrons and vD die velocity
of the Doppler drive . Moving a crystal  set to neutrons with ~ z 6.3 101° m by using the
Si(111) reflection  with a velocity amplitude of 2 .5 m/s results in an energy range of
f 15 p eV .
Supermirror
Guide
Deflector
Monitor
Chopper
Sample
Detectors
Doppler
Monochromator Drive
Neutron Guide
Fig.
17) layout of the backscattering spectrometer in Jülich
Fig. 17) now displays the realisation ofthe above considerations by means of an experimental
facility . Not unexpectedly, this set up is quite different from that of triple axis spectrometer .
The backscattered and Doppler shifted neutrons have to be deflectod by a second crystal off
from the neutron guide towards the Sample position . This so called deflector is positioned next
to the neutron guide which entails a slight deviation from perfect backscattering and thus the
optimum energy resolution . Exact backscattering has been attempted in the first experimental
set up by placing a deflector covering 1/10 11' of the beam size inside the neutron guide . Despite
the somewhat better resolution this option results in too a low flux for most applications . After
deflection, the neutrons travel through a conical shaped, supermhror coated neutron guide
which focuses the beam onto the Sample. A chopper wich about 50% dead time interrupts the
continuous beam and triggers the gate of the counters . Thereby one avoids counting of those
neutrons being scattered directly from the Sample into the nearby counters, whereas neutrons
having passed the analyzers are detected according to the Doppler velocity . The analyzers
(elastically curved Si single crystals) are arranged at a fixed radius around the Sample and focus
the backscattered neutrons on the associated detectors . Note, that the energy resolution of
the backscattering instrument also depends on the flight path. It increases wich increasing
flight path since the detectors have a finite volume which means slightly different detection
times. The accuracy of the counting electronic may thereby be considered as perfect .
9 15
After all ttrose constraints on the detected neutrons it might astonish that there remains sufficient
intensity for measurements . We had learned about the cost of intensity for optimizing the
resolution . In order to aehieve a useful signal/noise ratio here, one has to relax the resolution
in the momentum transfer . Taking the width of 45 cm for an analyzer plate being positioned
at a distance of 150 cm to the sample, one gets an angular resolution of about 9° . For an average
Q value, given by Q=4Y slnO s = 1 .41  10 10 m7l for O s = 90' and a wavelength Â _
6 .3  10 10 m, ttris means a resolution of f 0 .1  10 10 m1 . For comparison : at the triple axis
spectrometer one has a resolution in Q of about 0 .01  10 10 m1 . On the other hand, most
problems investigated on a backscattering spectrometer exhibit smooth functions on ~Qj, only,
which allow for such a relaxed Q resolution. The isotropie scattering also permits the simultaneous
recording of several momentum transfers by arranging many counters and associated
analyzer plates around the sample. In ttris respect the efficiency of a backscattering instrument
is higher than that of a triple axis spectrometer which uses on detector, only . .
Fig. 18)
Rotational tunneling of
the methyl group in
Paraoetamol .
energy transfer / geV
Finally, as an example for a measurement on the backscattering instrument in Ellich, the temperature
dependence of the spectrum of Paracetamol is shown in Fig .18 . In this case, one is interested
in the rotational or more exactly  permutational  tunneling of the methyl group of
the molecule . Eigenvalues and eigenvectors of the associated hamiltionian result from the
Mathieu equation for threefold symmetry . The goal is to determine those eigenvalues (here
about 3~teV for the AE transition, A = totally synznzetric, E = doubly degenerate) and thus
to obtain rather precise information on the intea and intermolecular interactions . A remarkable
observation thereby is that the excitation energies are much smaller than the thermal energy
of say 10 K of the sample (1 lteV z 1/100 K) . This may be understood by considering
thé basically différent coupling of phonon (spin = 0) and neutron (spin ='/z) to thé eigenstates
with différent symmetries (see lecture on Translation and Rotation) .
9 1 6
[1] B . N. Brockhouse, in Inelastic scattering of neutrons in solids and liquids (IAEA), Vienna,1961
p . 113
[2] H . MaierLeibnitz, Nukleonik, 8, 61 (1966)
[3] The Yellow Book, ILL (1988)
[4] V . J. Minkiewicz, G . Shirane, Nucl Inst. Methods 89,109 (1970)
[5] H . Grimm, Nucl. Inst. Methods 219,553 (1984)
[6] B . Domer, Coherent Inelastic Neutron Scattering in Lattice Dynamics, Springer Tracts in
Modem Physics, Vol . 93 (1982)
[7] H . Schober, Dissertation, Universität Regensburg (1992)
[8] J. Mizuki, Y. Chen, K.M . Ho, and C. Stassis, Phys . Rev . B 32, 666 (1986)
10
TimeofFlight Spectrometers
Michael Monkenbusch
10 . Timeofflight spectrometers
Michael Monkenbusch
10 .1 Introduction
The information that may be extracted from a neutron scattering experiment can be expressed
in terras of the scattering function S(Q, w) .
of scattering experiments are contained in S(Q, cw) .
All properties accessible by these kinds
The resulting intensity represents the
double differential cross section :
2 r
_ 2
dS2dE'
N k b
(Qiw)
where k', k is the modulus of the scattered and incoming neutrons respectively.
N denotes
the number of atoras in the sample and b is the scattering length' .
The energy transfer
during scattering is hw = (E  E'), here E ,
E' denote the energies of the incoming and
scattered neutrons respectively. The variables of the scattering function depend on k, k' ;
Q  1  l' is the momentum. transfer and
hw = (h2/2mn )(k 2  k'2 ) (l0 .2)
the energy transfer that occurred during the scattering process .
Since the modulus of the
wavevector k of the neutron is related as well to the neutron velocity, v_ (momentum) as
to the wavelength (1/wavenumber) :
v_m, = hk (10 .3)
27r
= k (10 .4)
it is possible to deterraine the energy transfer (10 .2) as well by employing the wave
properties of the neutron by analysis of the wavelength A' as by using the particle
character by measurement of the velocity v' of the scattered neutrons .
The first method
is applied in crystalspectrometers like the classical tripleaxisspectrometer or the
'For compounds containing different types of atours (elements or isotopes the corresponding expression
consists of the sum of partial structure factors multiplied by the corresponding scattering lengths
bibj in bilinear combination . For the discussion of instruments the simple version is sufficient .
101
ackscatteringzspectrometer ; for details sec chapter 10 . The second method leads
to the spectrometer types that are the topic of this chapter, namely different variants of
timeofflight (TOF)spectrometers . Also the neutron spinecho spectrometer,
NSE that is described in the next chapter employs somewhat less obvious directly the
velocity change of the neutrons to infer the energy transfer . The generic geometry of
a scattering experiment in reciprocal (i .e . velocity, momentum or wavevector) space is
illustrated in Fig . 1 . The scattering triangle consisting of the incoming wavevector k,
Figure 10 .1 : Scattering triangle .
the wavevector of the scattered neutrons k' and the resulting momentum transfer ( . ),
Q, the figure shows the general situation of inelastic scattering (here : energy gain of the
neutron) . 20 is the scattering angle, Qe indicates the momentum transfer for elastic
scattering (i .e . without energy transfer) .
A nuclear research reactor as neutron source basically yields a thermal (Vlaxwellian)
spectrum of neutron velocities, the temperature of the moderator (D 2 0cooling water
approx . 60°C) determines the temperature of the neutron cloud . Vlany facilities contain
additional small moderators of different temperature that supply single beam tubes with
neutrons of a different spectral distribution (different temperature) . In particular the so
called "cold sources" have to bc mentioned . In Jülich the "cold source", which supplies
the neutron guide hall (ELLA) with long wavelength neutrons, consists of a small volume
filled with liquid H 2 corresponding to a temeparture of 20 K . The following table enables
a quick survey over the average values of the corresponding neutron spectra .
10 2
Tnloderator /K V7 2/m/s A/nm Aiw/eV v = w/2z/s1
330 2870 0 .14 28 x 103 6 .87 x 10 12
20 706 0 .56 1 .7 x 103 0 .42 x 10 12
5 177 2 .24 0 .4 x 103 0 .1 x 10 12
For specific experiments of course also neutrons of deviating velocities within a band
around the average are employed, however far from that the available number density
resp . the flux drops strongly. Typical neutron velocities are in the order of 1000 m/s
the corresponding timeofflight per meter is 1 ms/m, i .e . such neutrons need a couple of
milliseconds for their journey through a spectrometer .
10.2 The classic timeofflight spectrometer
Figure 10 .2 illustrates the generic setup of a classical timeofflight (TOF) instrument .
Chopper
HISTOGRAMM
SPEICHER
inkrementierend
Figure 10 .2 : Generic setup of a classical TOF instrument .
103
From the thermal spectrum of the neutron beam entering from the left a monochromator
(of any type) filters a limited wavelength band .\+0A .
By doing this typically a bandwidth
of AA/A ~ 102 is achieved .
The thus monochromatized beam enters a socalled chopper
which opens the beam path periodically for a short moment .
Typical frequencies are
between 20 and 200 Hz, the ratio of timeopen:timeclosed is around 1 :100 .
The resulting
pulse widths are of the order of several (tens) of microseconds . After an as short as
possible flight path the neutron bunches hit the sample and are scattered according to
the double differential cross section of the Sample material .
In this process some neutrons
exchange kinetic energy with excitations in the Sample, i .e . change their velocities . After
scattering into different directions the neutrons transverse the flight space between sample
and the detectors .
The path length between sample and detector is usually kept the saute
for all detectors placed at the periphery of the flight space. The detectors most often
consists of 'He (10 bar) filled counting tubes of 30 . . . 40 cm length . Up to 1000 (and
more) tubes are used in some installations to cover as much solid angle as possible .
The elastically scattered neutrons (like those from the direct beam) reach the detectors
after the time tcp + t o = dchopperSample /vo + L/vo , those scattered inelastically arrive
earlier (energy gain of the neutron) or later (energy lors of the neutron) . Each pulse
from a counting tube causes via the associated electronics an increment of one Gell in
the histogrammic memory. The address of this cell is derived from the time difference
between chopper opening and arrival time of the neutron (pulse), i .e . TOF, and the
detector number (> scattering angle) . Thus the distribution of flight times evolves as a
histogram of 512 . . . 2048 channels with a width of around 10ps each . For each detector
(resp . group of detectors) such an histogramm vs . time is obtained . A monitor (Mo) in
the direct beam serves to normalize the histograms to the incoming neutron flux . 2
2A "monitor" is a detection device (counting "tube") that covers the beam cross section and has a
high transmission for neutrons (> 90%) and low detection probability (103 . . . 10 7) . In the figure only
one monitor behind the sample is shown for clarity . In general another monitor (more important) is
located between chopper and sample, it measures the incoming flux without the influence of the sample
transmission .
10 4
10.2 .1 Interpretation of spectra
As displayed in the pathtime diagram in fig .
10 .3 pulses of neutrons with defined velocity
are periodically transmitted by the chopper with the frequency 3 NQ = 1/T .
The slope
of the dashed lines corresponds to the average velocity vo .
The neutron pulse needs a
constant time tcp for the distance from the chopper to the Sample dChopperProbe .
After
dcp+L
d cp _~t4, :'l Probe
~ ~ l Chopper 2)
I, I,
Zeit
Chopper
Figure 10 .3 : Path(Flugweg)time(Zeit) diagram .
This velocity spread is indicated by the filled grey triangles . The analysis of arrival
3According to the technical realization there is
an integer factor bet%veen rotation frequency of the
chopper and pulse repetition frequency; e .g . a Fermi chopper that opens twice per one revolution (See
10 .2 .4) .
105
times is performed at the detector distance dcp + L .
A possible resulting "spectrum" is
indicated on top of the detector distance line.
The extrapolation of the dashed line to the
detector position indicates the location of the "elastic line", i.e .
the time channel where
neutrons without energy transfer arrive 4 .
The left vertical edge of the triangle defines
the "beginning" of the timeofflight spectrum, i .e .
the earliest possible time of arrival
occurring only for nearly infinite energy gain of the neutron .
In reality there are no infinite
large energy gains and the proper spectrum Starts somewhat later .
The right edge of the
"velocity fan" symbolized by the triangle is less well defined, in principle the neutron may
transfer only a part of its energy but also virtually all of its energy to the Sample, thus
virtually hortizontal pathtime curves may result . Le . strictly speaking the spectrum does
not end at some maximum channel number . However it is immediately recognizable that
fortunately this effect goes along with a corresponding "dilution"
of the intensity which
becomes virtually structureless on the scale of the histogram channel Windows ("frames")
causing a constant background in all channels of a "frame" that may be subtracted during
data treatment . Thereby it becomes possible to repeat the uptake of a "frame" with a
frequency S2 and to accumulate the spectra into the histograms mentioned above . Each
chopper pulse resets the clock to time zero and the channels of the histogram cover the
time interval T in terms of bins of width O7K ~ TIN .
If due to resolution requirements
5 or due to other technical demands 9 lias to be chosen such that the above discussed
"frame"overlap effect still distorts the spectra, it is possible, as indicated in fig . 10 .4, to
use an additional coarse chopper to transmit only every 2nd or nth pulse .
By doing this
sufficient spacing between "frames" may be gained to collect
an undistorted spectrum,
however with an nfold reduction of effective data collection rate .
10 .2 .2 Timeofflight spectra
In fig. 10 .5 several spectra as they are accumulated in the histogrammic memory are
displayed .
The timeofflight scale of the horizontal axis refers to the distance L between
Sample and detectors . This timeofflight is directly proportional to the wavelength A'
of the scattered neutrons as is indicated by the diagonal representing this linear relation
4 Generally the scattering without (sizeable) energy transfer is the most probable process .
5The pulse width (opening time) of a chopper depends for a given design on its rotation frequency.
106
~ Probe
' (Chopper 2)
Zeit
I
Chopper
Figure 10 .4 :
Pathtime diagram for a configuration with "Frame overlap choppers", chopper
2 .
using the right hand vertical scale. This diagonal straight Elle intersects the level A o =
0.6nm at the location of the "elastic channel" where neutrons are collected that did not
change their velocity during scattering . Silice in liquid water which was the sample all
molecules may diffuse without restriction only a so called quasielastic line is observed
which corresponds to a Lorentzian with a width proportional to QZ . The maximum of
intensity is nevertheless at the elastic channel ( quasielastic) . The difference between a
solid with atoms/molecules fixed at lattice sites and a liquid is illustrated by the right part
of the figure. Imidazole in the solid state exhibits an intense line at the elastic channel
with a width corresponding to the instrumental resolution. In contrast molten imidazole
(especially for the relatively large scattering angle displayed here > large Q) shows only a
broad quasielastic intensity distribution . At shorter times offlight corresponding to larger
107
energy transfers (gains) structures in the spectra are visible that stem from molecular and
lattice vibrations . Note the second left scale in combination with the dashed fine that
illustrates the strongly nonlinear relation between energy and timeofflight . For energy
gains AE » 1BT the scattering energy dies out due to the exponentiel Boltzmann factor .
At ambient temperature 1BT is equivalent to 25meV . Well above that energy gain the
unavoidable virtually constant background due to "frame overlap" may be determined .
2 4 6 0 0 .002 0 .004 0 .006
Flugzeit/ms
Flugzeit/s
Figure 10 .5 : Left : TOFspectra from liquid water at ambient temperature for different
scattering angles between 30° and 140° . Parameters : A o = 0 .onm, AT = 18ps, L = 3 .05m,
N = 512 . Right : TOFspectrum from imidazole (C 4H4NH) as crystalline solid at 300K
(the dashed fines displays the saine data scaled by x0 .1) and as melt at 403K at a
scattering angle of 95° .
Technically a TOF spectrum is accumulated at a fixed scattering angle for each detector .
That corresponds to the situation of the scattering triangle as depicted in fig . 10 .1 . A
glimpse on this figure makes clear that different momentum transfers Q and Q (depending
Le 
on energy transfer) for elastic and inelastic scattering have to be assigned to the different
time channels of the histogram from one specific detector .
modulus Q as for the direction of Q .
That applies as well for the
The sequence of curves in the left figure 10 .5 shows
the values of Q as function of scattering angle (different curves) and time channel .
property that the values become very similar for large energy gains also expressed by
10 8
The
the similar intensity distribution of that part of the spectra for different angles follows
from the fact that the main contribution to Q at high energy gain stems from the length
difference of k and k' (sec fig . 10 .1) . The variation of IQI may be compensated within
certain limits by combining the data from different detectors (angles), however that does
net apply for the direction change of Q . Therefore TOFinstruments in contrast to tripleaxis
spectrometers are better suited for isotropic samples (liquids, powders, amorphous
substances) than for single crystals or other highly oriented samples .
10.2 .3 Transforms
Since the physics of the systems under investigation is
usually expressed in terms of
S(Q, cw), a transformation of the raw data representing 1(28, t) into the (Q, cw)space is
necessary. With t = L /v' and t o = L/v inserted in Eqn . 10 .2 yields
and
2 2
w (t) = m n L2t  to
t2 t2
t 2
2h
+t2  2cos(20)tot
t 2 t 2 0
The nonlinear mapping frein channels to energy given by Eqn .
varying energywidth of TOFchannels, K.
er somewhat simpler
with
z(2o, K) a
KD7
(K1)4r
kt
47rb2S(Q, w(t))
dt dt
(10 .5)
(10 .6)
10 .5 also causes a strongly
(10 .7)
I(20, K) x k/47rb2S(Q, w(KO7))wOT (10 .8)
and
the result
k'
k
to
t
dcw(t) = Mn L2 1
dt fii t3
(10 .9)
(10.10)
I(2(9, K)
1
S(Q, w(KOT) (10.11)
109
is obtained, all constant factors are omitted and lumped into a still undetermined proportionality
factor 6 . Note the factor t ' between S and I which causes a significant
intensity enhancement for the early arriving time channels, however intimately connected
with a corresponding loss of energy resolution . Application of the transforms Eqns . 10 .5
and 10 .11 allows a display of the spectra in terms of S(20, cw) . Figure 10 .6 shows a
corresponding S(20, cw) derived frein the water data (medium angle data in fig . 10 .5) .
1 .5
1 .5
0 .5
0 .5
0
4 2 0 2 40 20
AE/meV
AE/meV
Figure 10 .6 : TOF spectrum from liquid water (see fig . 10 .5) converted to S(2(9, w)
displayed over two different energy ranges .
The diffusion is easily recognizable but the structure due to (internal) vibrations is lest in
this type of representation. As soon as a model for S(Q, cw) is available, it is in most cases
more advantageous to apply the inverse transform to that model to compute I(28, K)
and to compare this result with the raw TOF data . This procedures also allows for a
simpler more direct application of resolution corrections .
Remark : application of a coordinate transform (here (Q, w)  (20, K) resp . (Q, w)
(20, K)) requires besicles the observation of the (nonlinear) coordinate dependence the
application of a Jacobian determinant as factor to preserve "volume" . For the timefrequency
part this is also donc here (t4 factor) . The transform 20 > Q, however
'Fer practical purposes the proportionality factor is determined by an absolute calibration using a
standard sample, e .g . vanadium which is a purely incoherent elastic scatterer .
1010
is performed without Jacobian due to an asymmetry in definitions of S(Q, w), namely
du(20)/d52 = S(Q(20)) !
10.2 .4 Fermi chopper
One possibility to open the beam for a short time to create the required neutron pulse
consists in the placement of a short rotating collimator in the beam such that it transmits
neutrons only for a narrow interval of the rotation angle . The collimator consists of of
a parallel arrangement of neutron absorbing sheets (cadmium, gadolinium, boron) . The
gaps are filled with a material which is transparent for neutrons (aluminum) . Such a
chopper is sketched in fig . 10 .1, this type of chopper is called "Fermi chopper" . The
divergence Aa is determined by the distance between neigbouring sheets D and their
length l in beam direction, OcxFWHAI = arctan(D/l) (typical values are 1° . . . 2°) . The
duration of the opening OT is given by the rotation frequency 52
OaFWHM
Note that the neutron pulse frequency for a chopper with straight collimator slits is 252,
because the collimator axis is twice per revolution parallel to the beam axis . Silice the
neutrons have a finite velocity, the chopping collimator must not be too long, because otherwise
the transmission direction drops too muck even before the neutrons that entered,
rohen the collimator orientation corresponded to transmission, have emerged from the
collimator . It is also possible to use a "collimator" with curved slits, which accounts for
the above mentioned effect, however such a curvedslitchopper exhibits a wavelength dependent
transmission characteristic . Sometimes this is a desired characteristic to suppress
unwanted orders of monochromator Bragg reflections .
10.2 .5 Disc choppers
Besides the Fermi choppers also so called "dise choppers" are used . Figure 10 .7 shows a
front view with respect to the beam direction of such a chopper dise .
The dise is covered by a neutron absorbing layer (dark grey) and contains for counterbalancing
two window zones, A and B . The beam cross section is indicated as striped area
in A . The typical diameter of such dises is 0 .5 . . . 1m . From the figure it is immediately
visible that the ratio pulse width to pulsepulse distance for a copper of this type is rather
Figure 10 .7 : Disc chopper .
10% than 1% . A reduction of the window site would not help to improve this ratio,
silice that would also impose a reduced beam width on the system which would reduce
the available intensity to an unacceptable level . To achieve nevertheless a reasonable
temporal resolution wich the required pulsepulse distance (to avoid "frame overlap"),
it is necessary to combine several dise choppers where slow choppers select only one of
several openings of faster ones (rotating with a integer multiple n of the pulse repetion
frequency S2) . The resulting pulse bas according to the higher rotation frequency nQ a
length which is shorter by a factor 1/n . Also counter rotating dises are employed . The
multiple dise chopper technique requires exact electronic control of the relative rotation
phases of the choppers .
10 12
10.2 .6 Crystal monochromators
The monochromator indicated in fig . 10 .2 has the function to select neutrons from a
narrow band of velocities (approx .
1%) out of the Maxwellian spectrum of the incoming
primary beam . It may be realized by different means . First the crystal monochromator
is described . It uses the matter wave properties of the neutrons to select neutrons of a
defined wavelength (i .e . velocity) by interference in a crystal lattice (Bragg reflection) .
Neutrons with a wavelength of
A  2d sin(OA11/2) (10 .13)
n
are reflected in direction of the sample; here d is the distance of lattice planes of the
monochromator crystal (often pyrolytic graphite 002, d = 0.6708nm), n the diffraction
order and OAvt the angle of reflection . Le . a simple crystal monochromator rotates the
beam direction by Ont ;
if the wavelength should be changed the bulky rest of the spectrometer
must be rotated around the location of the monochromator crystal.
Sec figure
10 .9 in the following section . 7 In addition Eqn . 10 .13 implies that generally several
diffraction orders are reflected .
To suppress the unwanted orders mainly three methods
are used :
1 . Filter : if the desired wavelength A is long enough it is possible to use a block of
polycrystalline material (mostly beryllium) which has negligible neutron absorption .
The shorter wavelength neutrons are Bragg reflected by some crystallites
in the
block and removed from the beam direction while the long wavelength neutrons
with A > 2d,ax are transmitted with low losses .
2 . Curved slit choppers : by curving the slits of a Fermi chopper it is possible to
achieve that the chopper is only transparent for a certain band of neutron velocities .
This band may be selected such that only the selected diffraction order is included .
3 . Second (coarse) chopper : by a second (coarse) chopper at seine distance from
the main chopper it is possible to select the desired diffraction order via the TOF
TThis may be avoided by the use of t%vo crystals in a parallel arrangement . The second crystal performs
a reflection that restores the original beam direction and rotation and translation of the crystals in such
a "double monochromator" are performed such that the direction and position of the monochromatized
beam stays the came for all wavelengths . However this advantage is connected with an intensity loss .
More about crystal monochromators may be found in the chapter "Crystal spectrometers" .
1013
etween the two choppers . See also section TOFTOF .
10 .2.7 Time focussing
It seems unsatisfactory that by a TOF spectrometer ai a continuous source (reactor) only
a sinall fraction (1%) of the continuous primary beam is utilized . On the other hand the
TOFanalysis correlates the energy resolution with the length of the neutron pulses OT .
However there is trick to partly compensate for this correlation and to achieve a multiplication
of the intensity without resolution loss (at the elastic line), see fig . 10 .8 . The
chopper opening may last longer if there is a correlation between time and wavelength
(velocity) of the neutrons during the opening interval such that all neutrons arrive at the
saine time at the detector as indicated in fig . 10 .8 . By this means the elastic line remains
Zeit
Figure 10 .8 : Pathtime diagram, time focussing .
narrow but the focussing effect depends on energy transfer and becomes ineffective for
1014
larger energy transfers . However it is possible to move the focusing point to some inelastic
energy transfer by chosing a different chopper frequency.
Figure 10 .9 shows a technical
realization of the time focusing principle .
Figure 10 .9 : TOFspectrometer with timefocusing .
Instead of only one monochromator crystal several crystals one after the other form the
monochromator, each crystal reflects a slightly different wavelength A l > A2 . . . > 1\5, such
that the slowest neutrons (A 1 ) are transmitted first when the chopper channel approaches
transmission during a revolution ; thereafter the gradually faster neutrons ( .~ 2 * * * 4) follow
subsequently.
For a set of matched distances between crystals and between monochromator
and chopper and frequency Q of the chopper a pathtime behaviour as illustrated in
fig . 10 .8 may be achieved . By the use of 5 instead of one crystal about 5 times as much
neutrons bit the sample .
10 15
10 .2 .8 TOFTOF : TOFmonochromator
Instead of a crystal monochromator (see above) the incoming wavelength (velocity) may be
equally well selected by the timeofflight between two choppers (see fig . 10 .10), therefore
the abbreviation TOF(monochromator)TOF(analyzer) .
Figure 10 .10 : Pathtime diagram for an instrument wich TOFmonochromator .
A technical realization of this principle is e .g . the IN5 spectrometer at the ILL in Grenoble .
It is equipped with a system of disc choppers . Besides the flexibility to choose wavelength
simply by changing the chopper phasing a better defined resolution function, due to
convolution of several real triangular window opening functions, is advantageous . In any
case this method of monochromatization automatically yields a pulsed beam hitting on
the sample .
1016
10.3 Inverted TOFspectrometer
In the spectrometer types described above the sample was "illuminated" by pulses of neutrons
with a single defined wavelength (velocity which have been prepared by a choppermonochromator
combination . The analysis of the velocities of the scattered neutrons was
effected by TOFmeasurement .
It is also possible to invert this sequence, the incoming velocity (i .e . wavelength, energy,
k) is determined by the TOF between chopper (pulsed source) and sample . Then to
obtain a defined energy and momentum transfer only scattered neutrons of a given final
wavelength that may pass an analyzer are detected .
1111III
M/F
1 1 1 1 1 1'
LLU 1 4
~ Probe
Zeit
Figure 10 .11 : Pathtime diagram of a TOF spectrometer with inverted geometry .
The corresponding pathtime diagram is displayed in figure 10 .11 . Neutrons emerging
the pulsed source fly according to their individual velocity in direction of the Sample,
10 17
the associated paths are indicated by the grey triangle .
The intensity within the range
of this triangle is of course not uniform but depends on the spectral properties of the
source .
s
Neutrons that have been elastically scattered by the Sample (path 2) pass the
analyzer/filter M/F and lead to the elastic line in the TOFhistogram .
Neutrons that loose
energy (path 1) are faster before the Sample scattering and arrive earlier at the detector
than the elastically scattered ones .
Analogously path 3 represents neutrons that gained
energy during scattering .
Compared to a "normal" TOF instrument the energy gain and
energy loss sides of the histogram are reversed .
Therefore also high energy excitations
that are thermally not occupied may be measured .
(Spallationstarget)
Chopper
Figure 10 .12 :
Setup of a TOF spectrometer with inverted geometry.
Figure 10 .12 shows a corresponding setup .
The pulse at the chopper contains neutrons
from a broad velocity distribution (Maxwellian spectrum at moderator temperature) .
During the path from chopper (pulsed source) to Sample this pulse separates into different
wavelengths A, resp .
different incident energies, that arrive ai different times ai the
sample .
Since a wavelength selection (to Ao) is performed between Sample and detectors,
all detected neutrons have the saine velocity and the distance Sampledetector adds a
a In particular overlap of the triangles ( "frame overlap") may lzappen, wlziclz may be suppressed by
filters tayloring tlze incoming spectrum .
10 18
constant offset to the TOF . To be able to correct the TOFhistograms with respect to
the spectral distribution of the incoming pulse, it is important to detected the incoming
neutron flux by a monitor (Mo) located close to the sample position accumulated in a
separate TOFhistogram . This type of TOFspectrometer is preferentially used at pulsed
sources, ideally it may be possible to omit the first chopper by taking the pulse as generated
by the pulsed source (spallation target) . e All neutrons from the pulse (flying
into the right direction) are utilized . This method has a few specific advantages and
disadvantages, advantages are :
1 . The pulse contains neutrons with high incident energy that may perform energy
loss scattering, the resolution at high energy loss is relatively good, especially if the
pulsed source supplies very short pulses ai high neutron energies .
2 . If the analyzers are used in near backscattering configuration high resolutions (comparable
to those on truc backscattering spectrometers, See chapter 9) can be attained
.
The utilization of the full spectrum has however also disadvantages :
1 . The full "white" pulse enters the shielded sample detector spacc . Any parasitic
scattering and any imperfection of the analyzing filters or failurc to absorb neutrons
of "unused" final wavelength or direction leads to ilicreased background . In addition
the background depends on the sample which makes correcting subtractions difficult .
2 . Samples are hit by a higher integral flux and therfore become more radioactive .
In general also "normal" TOF instruments perform better on a pulsed source in comparison
with a reactor (if the average fluxes are equal) silice by synchronizing source and
chopper only a small part of the generated neutrons (with the desired wavelength) are net
used . The distance sourcechopper may serve at the saine time as TOFmonochromator .
In total the efficiency is comparable with the inverted type because in both cases on
one ride of the sample the spectrum is restricted by filters/monochromators and on the
other side the full spectrum is utilized and sorted according to the TOF . Energy transfer
analysis without filter on any ride is impossible .
'Te suppress background or to prevent "frame overlap" it may be nevertheless advisable to use an
additional chopper .
10 19
10 .3 .1 Analysis by filters
The analyzer that is indicated by the grey segment labelled M/F in fig. 10 .12 may either
consist of an array of crystals reflecting scattered neutrons of the selected wavelengtli
A o ente, the associated detectors or of a filter . Especially in the early days of neutron
scattering filters made from polycrystalline blocks of Be , BeO etc . were used . These
filters are transparent only for neutrons wich energies below the "Braggedge'" , i .e . for
wavelengths larger than twice the largest lattice spacing . All faster neutrons will be
reflected by some crystallite in the block . By integrated absorbing plates the thus reflected
neutrons are removed . For the filter to be sufficiently transparent below the Braggedge
the used material may only have a very low absorption cross section . In addition
the thermal diffuse scattering by fluctuating lattice deformations (phonons) bas to be
suppressed by cooling (liquid nitrogen) . Below the Braggedge these filters transmit all
neutrons from nearly zero energy to the edge energy of a few meV . For the spectroscopy
of high energy excitation this is accceptable since the energy transfer is then determined
by the incident energy of a few 100 meV . High resolution quasielastic scattering bas to
be donc with other instruments . By employing the difference between data obtained with
two different filters (e .g . Be and BeO) the effective window of final energies may be
narrowed, however two measurements are needed and the final signal is obtained from a
small difference of two larger counting signals with the corresponding statistical errors .
10 .4 Resolution and intensity
One important quality of a spectrometer is its resolution in (Q, w)space . For TOFspectrometers
unlike for tripleaxis instruments for many applications mainly/only the
energy resolution is important silice the scattering intensity bas to be collected and accumulated
in a large solid angle anyway to yield a sufficient number of counts . The energy
resolution is determined by the accuracy of the TOFmeasurement and by the width of
the incoming (or analyzed) wavelength band . The latter is given by the beam divergence
in combination wich the mosaic width of the crystals (sec also chapter on tripleaxis spectrometres)
. The TOFuncertainty is given by the chopper pulse length and the accuracy
of the flight path . The flight path cannot be defined wich arbitrary accuracy, rince finite
1020
sample size of cm and a detection position uncertainty of some mm in the detectors l° . If
all timing uncertainties are lumped into At, a classical TOF instruments bas the following
resolution :
Ow  ()WOt) 2 + (OW 0A)2 (10 .14)
From Eqns . 10 .2  10 .5 follows :
Ow (
2
~t3 Ot) 2 +
(m~~3 0A)2 (10 .15)
n
Because A' a 1/v' oc t and close to the elastic line (Y ~ A) it follows that Ow oc 1 /,\ 3 , i .e .
the most efficient measure to increase the "elastic" resolution is the use of a long neutron
wavelength/ For a matched setup the relative timing uncertainty Ot/t o and the relative
wavelength width 0A/A should be about equal .
Egn .10 .15 shows in addition that the
timing uncertainty term oc Ot dominates the resolution width for short time t, i .e . large
energy gain of the neutron .
If path uncertainties AL are treated separately, Ot represents
only the chopper opening and Eqn . 10 .15 reads :
( mnLOL)2 + (maL Ot)2 + ( 47 2 1i oa)2 (10 .16)
Ät~t 2
3 mn\3
For the inverted spectrometer the expressions stay the saine except for the exchange of A
and Y .
10.4 .1 Intensity
The available neutron sources are rather weak compared to sources of electromagnetic
radiation (laser,
synchrotron), they emit neutrons in form of a thermalized gas with a
broad distribution of velocities and into all directions . Preparation of collimated and
monochromatic beams is only possible by selection, i .e . removing all unwanted neutrons .
The resulting beams even ai high flux reactors contain only relatively few neutrons . 11
For this reason the available neutrons have to be utilized as efficient as possible .
Even
"For sample in form of thin plates the path uncertainty due to scattering position in the Sample may
be reduced for (only) one scattering angle (region) to the plate thickness .
"The typical neutron flux in front of the chopper of a classical TOP instrument is in the order of
10 °n/cm2 s, after chopping only 1O sn/cm2 s hit the sample and are available for scattering . In comparison
a beam of a small 1 mW HeNe laser is strictly collimated and monochromatic and represents an integral
flux of 3 x 10 15Photonen/s with a cross section of maybe lmm 2 , i .e . 3 x 10 17photons/cm 2s .
102 1
if an increase in resolution may be achieved by stricter wavevector 1 selection (velocity,
direction) and by reduction of the chopper pulse length, it is offen not advisable to
enhance all elements of the resolution up to the technological limits because this goes along
with a drastic loss of intensity (detector count rate) . Design of (neutron)spectremet ers
means the search for the Best compromise between resolution and intensity .
The optimum
depends on the nature of the problem, i .e . the features and structures expected in S(Q, 4 .
TOF spectrometers as described in this chapter are preferentially used to investigate
isotropie to weakly anisotropie samples with only weak structures in S(Q) . This enables
the utilization of a large solid angle for detectinn which compensates for the loses caused
by energy analysis . In the schematics of the spectrometers this is already indicated by
the large number of detectors . Modern TOF instruments contain more than 1000 single
counting tubes covering a detecting area of 30 x lcm 2 each . The total area coverd by
1000 detectors is about 3m2 , for a flight path of 3 m this corresponds to a solid angle
of 0.333 or 1000 degrees squared . Thereby an intesity gain of a factor 500 is obtained
compared to a triple axis spectrometer with a detecting area of 2 degrees squared, the
loss caused by the fact that the chopper opens only for about 1% of the time is more
than compensated . In addition the TOF instrument has a multiple advantage : all energy
transfers are detected simultaneously and not sequentially as in the case of a tripleaxis
spectrometer . However it is seldom useful to surr the data of ALL detectors into one
spectrum but different scattering angle regions have to be evaluated separately. Still
they are measured all at the saine time! Generally the TOF instrument is more efficient
than a tripleaxis spectrometer for isotropie samples . As soon as single crystals or very
anisotropie samples with a strong dependence of the spectra on Q are to be investigated
the conventional tripleaxis spectrometers are better suited .
Contents
10 .1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 101
10 .2 The classic timeofflight spectrometer . . . . . . . . . . . . . . . . . . . . 103
10 .2 .1 Interpretation of spectra . . . . . . . . . . . . . . . . . . . . . . . . 105
10 .2 .2 Timeofflight spectra . . . . . . . . . . . . . . . . . . . . . . . . . . 106
10 .2 .3 Transforms . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 109
10 .2 .4 Fermi chopper . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1011
10 .2 .5 Disc choppers . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1011
10 .2 .6 Crvstal monochromators . . . . . . . . . . . . . . . . . . . . . . . . 1013
10 .2 .7 Time focussing . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1014
10 .2 .8 TOFTOF : TOFmonochromator . . . . . . . . . . . . . . . . . . . 1016
10 .3 Inverted TOFspectrometer . . . . . . . . . . . . . . . . . . . . . . . . . . 1017
10 .3 .1 Analysis by filters . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1020
10 .4 Resolution and intensity . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1020
10 .4 .1 Intensity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1021
Neutron Spichecho Spectrometer, NSE
Michael Monkenbusch and Reiner Zorn
11 . Neutron spinecho spectrometer, NSE
Michael Monkenbusch, Reiner Zorn
11.1 Introduction
The attempt to increase the resolution of timeofflight (TOF) instruments described in
chapter 10 far beyond the ~ 1% of the present realizations would lead to an unacceptable
loss of intensity (as expressed in terms of detector count rate) . E .g . a factor 0 .1 which had
to be applied as well to the monochromatization as to the pulse length (chopper opening
time) would on the one hand increase the resolution accordingly by a factor of about 10
but at the same time the intensity is reduced by O .lmonochr . x O .l eho pper = 102 . Still other
necessary measures to preserve the increased resolution as the reduction of sample size
(definition of flight path) are not contained in this reduction factor .
The same situation is
also given if monochromator and analyzer consist of crystals .
In general an improvement
of the spectral resolution requires the narrowing of the filter transmission functions before
and after the sample scattering by the desired improvement factor .
However this means
an intensity reduction by the square of the resolution improvement factor .
This situation
would immediately improve, if it would be possible to equip each neutron with an
individual stop watch which could be read in a way that the run time difference between
test tracks before and after the sample is obtained at detection .
If this stop watch has
a sufficient time resolution it would be possible to observe very small velocity changes
even if a beam with a wide range of initial neutron velocities is used .
This would allow
to escape the intensity trap .
In the neutron spin echo (NSE) spectrometerwith some restrictions (with important
consequences for the application)it is indeed possible to use the neutron spin directions
as kind of individual stop watch pointers . The clockwork of this watch is then effected
by the precession of the neutron spins in an external magnetic field' .
The restrictions
1 It is somewhat involved to extract this analogy starting from a quantum mechanical
view with spin eigenstates and eigenvalues .
Implicitly we are talking about the behaviour
of the ensemble average of the spin vectors which obeys the "classical" Bloch equation
affecting application are caused by the fact that the "spinstop watch" can only be read
up to an unknown integer number of complete precession turns .
The reading is performed
by the cosine type transmission function of an analyzer and yields only ensemble averages
and not individual rotation angles .
The intensity at the detector is modulated accordingly.
In addition inelastic scattering does not produce only one defined velocity change but Av
is distributed according to S(Q, w ~~ kAv) . The detector signal is then proportional to
the integral of intensity contributions modulated by the cosine of the precession angle and
weighted according to the Ov of S(Q, w) .
Therefore, the signal of the NSE spectrometeras
explained in this chapteris completely different from the TOF histograms of classical
TOFspectrometers (chapter 11) .
Instead it is proportional to the cosine Fourier transform
of S(Q, cv), i .e . the intermediate scattering function S(Q, t) . A detailed derivation and
discussion is given below . But first of all the actual setup of an NSE spectrometer is
presented .
11 .2 Setup and Function
Figure 11 .1 shows the schematic setup of a NSE spectrometer (upper part) together with
the propagation of the neutron spin in the instrument (lower part) .
Longitudinally polarized neutrons2 (i .e . spin expectation value parallel to the beam diconcerning
its precession in the magnetic field . As long as the kinetic energy of the
neutrons is much bigger than the magnetic level splitting the classical picture is completely
sufficient . It is much easier to understand the NSE spectrometer in this way than a
quantum mechanical treatment .
2 The polarized neutron beam is obtained by reflection by a magnetic multilayer mirror .
The layer stack consists of alternating nonmagnetic (e .g . Fe, Si or Ti) and magnetic (Fe or
Co) layers .
The effective index of refraction of the magnetic layers depends on the relative
orientation of magnetization and spins of the neutrons such that there is a modulation
of index of refraction for neutrons in one spin state only.
Those neutrons are reflected,
the others are transmitted . For layer distances of 5 . . . 10 nm reflection angles of a few
degrees result for wavelengths around 10 A .
Both the reflected and the transmitted beam
are polarized (with opposite spin directions)
11 2
2
0 L Tr 0 L
2
ArDet
Figure 11 .1 : Spin rotations and setup of a generic NSEspectrometer . Upper part : Spin
rotation, middle part : magnitude of the magnetic field, lower part : schematic setup of
the Jülich NSEspectrometer .
rection) enter the spectrometer from the left . In the first socalled 7r/2flipper the spin
is rotated such that on exit it is orthogonal to the longitudinal magnetic field of the
precession path . That defines the start of the "spin stop watch ", immediately after the
flipper a precession of the spins around the axial magnetic field begins .
The precession
frequency increases
during the approach to the centre of the main precession solenoid
where it reaches its maximum of up to a few MHz .
The accumulation of precession angle
continueswith decreasing frequencyuntil the neutrons reach the 7rflipper close to the
sample (S) . The total precession angle at that point is :
where ~ = 27r x 2913 .06598 x 104 s'/Tesla is the gyromagnetic ratio of the neutrons and
IBI is the modulus of the magnetic induction along the path 1 .
The "stop watch" does not proceed uniformly but with a position dependend frequency
that is proportional to the local magnetic field along the neutron path, see figure 11 .1 .
This may also be considered as a field dependend distance streching, which releases e .g .
the mechanical positioning accuracy requirements for the flippers since they are located
in low field regions .
The total number of precessions a neutron spin undergoes on passage
113
through one arm of the spectrometer lies between 10 and some 10 4 .
300
0
Figure 11 .2 : Field along the axis of a main precession coil .
Close to the Sample (ideally : at the sample position) the socalled 7rflipper is located, it
rotates the spins by 180° around a vertical axis . In this way the total precession angle is
transformed to `F1 = + ce > ce . The precession angle ce isaccording to equation 11.1
extremely dependent on velocity and therefore very different for different neutrons in
a beam with finite width of the wavelength distribution . As a consequence the spin
vectors at the sample position (7rflipper) are evenly distributed on a disc orthogonal to
the field direction . If no velocity change occurs during scattering at the sample (elastic
scattering) each neutron enters the secondary arm of the spectrometer with unchanged
velocity. The precession field and path length of the secondary arm exactly match the
corresponding elements of the primary arm before sample and 7rflipper . Accordingly, the
precession accumulated in the secondary arm is q~ 2 = +ce and the total precession angle
at the second 7r/2flipper is q~ 1 + kP2 =  a + a = 0 . Le . all spinsirrespective of their
11 4
initial velocityreassemble at the saine vertical position they had at the start point . The
rotation imposed by the second 7r/2flipper couverts this back to the initial longitudinal
polarization that is fully restored .
The flippers limit the the two race tracks and realize
"start", "time reversai" and "stop" of the "spin stop watches" . The second 7r/2flipper is
the last element used to manipulate the spins .
It couverts the average precession angle to
a longitudinal polarization component .
Since the field after the second 7r/2flipper is again
longitudinal, further precessions do not influence the analyzed longitudinal polarization
component (the stop watch is stopped!) .
The analyzer accepts neutrons of one longitudinal
spin state for the detector .
After ensemble averaging this means that the cotait rate at
the detector is proportional to (1 ~_ cos(T))/2 s, where T is the expectation value of the
angle between spin and axial direction .
11 .2 .1 Flippers
Ignoring technical details the main elements needed to perform the spin operations necessary
for a NSE spectrometer are :
o 7r/2flipper (start)
first precessions field
o 7rflipper ("time reversal" )
e second precessions field
7r/2flipper
While in the precession fields the spin vector (its expectation value) continuously rotates
around the field vector on a cone with constant angle (angle fieldspin, ideal value =
90°) even if the field which the neutron experiences during its flight performs (sufficiently
slow, i .e .
adiabatic) direction changes', the flippers rely on a sudden change in the field
3 The sign in front of the cosine depends on the technical realization of poiarizer
and analyzer (both reflecting, transmitting, one reflecting one transmitting) and on the
orientation of flippers . It may be selected by choosing the signs of the flipper currents .
4 The cone of precession follows the direction of the precession field quite accurately
if the effective frequency of the field rotation is
much smaller than the local precession
115
direction that gives rise to a new drastically changed cone angle . In figure 11 .3 a 7r/2
flipper is shown together with the field vectors that have to be generated for an adequate
function of the flipper .
Figure 11 .3 : Schematics and function of a 7r/2flipper .
The rectangular flipper exposes its large sides to the beam . The box consists of electrically
conducting and neutron transparen material (aluminum wire) which carries a current I, as
indicated by the broad arrows . All side walls realize a thin homogeneous current density
frequency . Such a change in field is called adiabatic . In particular this means that faster
direction changes are the more adiabatic the larger the field is . For a NSE spectrometer
care must be taken that except at the entry and exit of flippers the conditions are
adiabatic . The magnetic field of the spectrometer is of course static, however the neutron
spins experience a time varying field due to the passage of the neutron through the
spectrometer .
11 6
distribution (current sheets) that leads to a homogeneous field B, r / z in thé inside of thé
flipper .
For a sufficient length of thé flipper thé stray field emerging from thé ends of
thé flipper coil is negligibly small in thé beam area in front of thé flipper . To obtain
thé desired operation thé 7r/2flipper has to
be embedded in an external longitudinal
field The resulting field in thé interior of thé flipper Bi ,, t
has an angle of 45° to thé
longitudinal axis .
The magnitude of thé field must be set such that thé neutrons perform
a precession of exactly 180° during thé time they need to transverse thé flipper .
In this
way a longitudinal spin vector is rotated into an orientation perpendicular to thé axial
field . Then thé precession cone has thé maximum angle of 90°, i .e . it is a disc (dial of thé
"stop watch") .
For a typical flipper thickness of 1 cm thé interior field is in thé order of
0 .1 mTesla = 10 Gauss (For comparison thé earth's magnetic field is ~ 0 .5 Gauss) . Since a
fixed precession angle around Bi t=const must be accumulated during thé passage time of
thé neutron through thé flipper, thé flipper function is moderately wavelength dependent .
For thé ease of setup and stability of operation of thé spectrometer it is
advantageous
that thé flippers are embedded in a comparatively small external field
(< 103 of thé
maximum precession field) . Le . close to thé flippers thé "spin clock" runs slowly and
small path différences due to positioning inaccuracy and thermal expansion only lead to
very small errors in precession angle .
The technical realization of thé 7rflipper is identical to thé one of thé 7r/2flipper, however
its functionas indicated by its naineis différent . It performs a 180° rotation around
an axis perpendicular to thé beam axis (e .g .
a vertical axis) which is virtually parallel to
thé axis of thé flipper coil .
To do so thé internal field has thé saine magnitude as in thé
7r/2flipper however thé embedding field
is close to zero and therefore thé internal field
vector is virtually vertical 5 .
a
Unfortunately it is not possible to embed thé 7rflipper in a zero field environnent, as
everywhere in thé beam volume this would lead to a violation of thé adiabatic condition .
While thé beam enters such a zero field région if would suffer uncontrolled inhomogeneous
tilts and rotations of thé precession cone that would effectively lead to a depolarization .
Smallest external stray fields would exert a big influence on thé signal .
A defined spin
operation would not be possible .
For that reason a minimal field in thé range of a few
(1 . . . 2 Gauss) is mandatory not to loose thé defined polarization . Without further action
thé 7rflipper function is deteriorated by this finite external field . But by a slight tilt of
117
11 .3 The detector signal
As mentioned above the detector signal results from the transmission function of the analyzer
shaped as the cosine of the net precession angle in combination with the distribution
of net precession angles due to the distribution of velocity changes during scattering . The
velocity distribution is proportional to the spectral part of S(Q, W) . In the following this
is derived in terms of mathematical expressions . First the field integrals along the primary
and secondary paths of precession are defined :
I(Z)
1 IBldl (11 .2)
l((7r/2)1)
J2 =
l((z/2)z)
IB I dl (11 .3)
for a symmetric setup J 1 = J2 ; l(7r, (7r/2) 1, 2 ) denotes the positions of the corresponding
flippers . The precession angle accumulated on a path i is
v
where v is the neutron velocity (typically several 100 m/s) .
the sign of ~P 1, a total precession angle of
Because the 7rflipper inverts
lyii
v
+
'Y j2
v + Ov
results, where Av is the velocity change of the neutron due to inelastic scattering . The
transmission function of an (assumedly ideal) analyzer is
Ta =
From that the detector intensity
'Y J2
2 1+cos(`Yv1
~ + v+Av
I = 77S(Q) fi 1 + cos Yv 1 + w,,(Av)wA(v) dAv A (l1 .7)
2 ~ ( v +JOv )]
the flipper or by a tiny extra component of the external field in direction of the flipper
axis the ideal function may be restored .
internal field
The condition to be fulfilled is that the resulting
is orthogonal to the embedding field which may be slightly tilted from its
horizontal orientation by the added small extra field component .
11 8
esults, where il is an irrelevant calibration factor and w, resp . w A are normalized distribution
functions . w", represents the spectrum of the sample as found in the scattering
function and wA takes account for the fact that the NSE spectrometers usually are operated
with a broad incoming wavelength distribution (O,\Fwxml,\ = 10 . . .20%) . Observing
the linear dependences of k, A and v and series expansion of the squares in the
expression for the double differential cross section 10 .2 and insertion into equation 11 .7
leads to :
yJ1
'Y J2
+
S , w wa dw dA
Il 2 [ ( (h/m )A1 (h/mn) ,\1 + ,\wl27r)] (Q ) (,\)
I = 1 1 + cos 
11 .3 .1 Symmetric Case
At the point of symmetry J1 = JZ = J it is possible to collect the Adependend terms in
equation 11 .8 and to write them as series expansion for small w :
3
h27r .\ 1 + .\ 1 + ,\(m /h)w/27r ,.J 
11 .9
To see the salient features of the spectrometer signal more clearly the finite wavelength
distribution is temporarily ignored
The underbraced product has the unit "time", the integral in equation 11 .10 represents
the cosine Fourier transform of S(Q, w) with respect to w, the resulting function is called
intermediate scattering function, S(Q, t) s From equation 11 .10 it is further reckognizable
that the time parameter t = yJm,,
(hz 27r) depends on the third power of the wavelength
A (i .e . long wavelength very long Fourier times) . In addition t oc J, i .e . mainly
s Strictly this is only true for a S(Q, w) that is symmetric with respect to w, i.e . in the
classical approximation . For any practical problems however this is well fulfilled since the
minute energy transfers corresponding to the NSE time scale are very small compared to
kBT .
=
=
z
rl2 [S(Q) + f cos `yJh 27r
A
3 w) S(Q, w)dw]
2
t
(S(Q) + S(Q, t)) (11 .10)
119
proportional to the current throught the main precession solenoids . This current usually
is the parameter used to stepwise scan the Fourier time during an experiment to get a
table of S (Q, t) vs . t .
11.3 .2 Mastic Scattering of a Finite Width Wavelength Distribution
For a transmitted beam or elastically scattered neutrons from a reference sample w = 0
holds, i .e S(Q, w) = S(w) . With that equation 11 .8 becomes
I = 1
f [1 ~ cos(A Y(m,/h){J2  Jl})] w a (A)dA (11 .11)
For this case the intensity is proportional to the Fourier transform of the wavelength
distribution . Here, the underbraced part is the external control parameter . It contains
the difference between the field integrals along the primary and secondary paths JZ  Jl .
This difference can be easily controlled by sending a current through an auxiliary coil
of a few windings around one of the precession solenoids . For a Gaussian wavelength
distribution the envelope of the Fourier transform is again a Gaussian whose width is
inversely proportional to the width of the wavelength distribution . Since wA is centered
at a finite nominal wavelength \o the envelope is multiplied by a cosine with a period
oc I/A o . This function follows immediately from equation 11 .11 if wA = ô(,\) is assumed .
Figure 11 .4 displays the results of an extensive measurement using the attenuated direct
beam with a central wavelength of \o = 0.7nm and O,\Fwxm/,\o = 0 .1 compared to a
calculation (fit) assuming a Gaussian wavelength distribution .
At the echo point (i .e . a phase coil current close to 1 .5 A creating perfect symmetry) the
count rate has a minimum . Ideally the count rate should be zero there, but because all
elements that contribute to the polarization manipulation and analysis are imperfect a
residual intensity is left that has to be determined by calibration measurements . From the
the functional dependence of the intensity on the phase current it is possible to determine
the wavelength distribution .
10000 
8000 
co 6000 
C
ô 4000
U
2000 
0
2 0 2 4
Phase current (40 turns) / A
Figure 11 .4 : Echo shape : count rate as function of the magnetic symmetry (oc phase coil
current) .
11.4 Experimental Procedures and Evaluation
In principle the information on S(Q, t) according to equation 11 .10 is contained in the ratio
of the intensities at the symmetry point and the average intensity (17/2) S(Q) . However
there are practical reasons that prevent the reliable setting of the symmetry point alone .
The location of the symmetry point (i .e . phase zero current in the phase coil) is extremely
sensitive to tiny variations of the magnetic environment caused e .g . by displacement of
larger iron parts at neighbouring instruments, movement of the crane of the instrument
hall and thermal displacements of coils .
Therefore, the position of the symmetry point has
to be measured as well as the intensity for each Q, t setting .
In figure 11 .5 the minimum
of single countings is indicated, intensity must be determined for three points Pl . . . P3
separated by a symmetry change corresponding to a quarter precession each . From these
three values it is possible to extract the average intensity I(Q, 0), the echo amplitude
I (Q, t) and the exact symmetry point location . This also holds if any perturbation shifts
the location as indicated by the three hollow circles in the figure .
P 1__________
I(Q,t)
j11
I(Q,0)
Symmetry
Figure 11 .5 : Schematic echo form, idealized .
For an ideal spectrometer I(Q,t)II(Q,0) = S(Q,t)IS(Q) would be the desired value of
the normalized intermediate scattering function . In reality resolution effects and polarization
losses reduce the value of I(Q, t)/I(Q, 0) compared to S(Q, t)/S(Q) .
Figure 11 .6 shows data from actual experiments that are used to determine the echo
amplitude and average intensity . Here the shape of the echo signal (intensity vs . symmetry
current) is sampled for a considerably larger number than the minimum of three points .
The parameters amplitude, average and phase zero current are determined by a nonlinear
fit . Behind the oscillating echo form there are two further groups of points showing the
minimum and maximum of intensity which indicates the efficiency of the polarization
analysis . These intensities are measured by deactivating the 7r/2flippers (minimum) and
e0
oX n .5 1 .0 1 .5
so
0 .0 0 .0 1 .0 i .5
50
6c
an
4a
80
ô
~ 20
so
20
10
w
10
0
0
0A 0 .5 1,U 1 .5 13 .0 0 .5 1 .U 1 .5
phase eurrent /A phase carrent /A
20
9.5 1 .0 1 .5
15
w
5
0
0.5 1 .0 1 .s 0.5 1 .0 1 .5
phase carrent /A phase torrent /A
Figure 11 .6 : "Phase scans" used to determine thé écho amplitude at thé Jiifich NSE
spectrometer . Symbols indicate count rates normalized to a monitor rate . The oscillating
fines are "fitted" écho signals (assuming Gaussian distribution of wavelengths) . At thé
end of thé scans groups of points corresponding to thé minimal (7r/2flippers off, 7rflipper
on) and maximal (all flippers off) obtainable count rates are located .
The horizontal lines
correspond to thé average and thé minimum and maximum intensities . The experimental
value of interest is computed from thé ratio of thé écho amplitude and thé maximum
possible updown différence . The fines starting at one point at thé beginning of thé scan
are measured magnetic field components (différences to thé starting value) at thé sample
position, they serve to monitor variations of thé magnetic environment .
then additional deactivation of the 7rflipper (maximum) .
An ideal spectrometer would
have zero transmission in the one case and 100% transmission of neutrons in the other
case .
The nonideal behaviour is caused by depolarization effects at the technical elements
of the spectrometer, the wavelength dependence of the flipper operations and the finite
efficiency of polarizers and analyzers .
Also for an ideal spectrometer being free from the
above effects a finite minimum and less than 100% maximum intensity will result for spinincoherent
scattering which is always accompanied by spin flips for 2/3 of the incoherently
scattered neutrons .
To account for the polarization losses the difference between the thus determined "up"
and "down" cotait rates is used to normalize the echo amplitude (instead of taking just
the average intensity) .
11 .5 Field Integral Homogeneity and Resolution
Besides the decay of S(Q, t)
as a consequence of the dynamical processes in the sample
the measured echo amplitude suffers a further reduction due to resolution effects (different
from the above mentioned depolarization effects) that must be accounted for in the data
evaluation .
Up to this point we tacitly assumed that the values of Jl and JZ are the saine for all
neutrons in the primary and scattered beams .
This would however only be approximately
true for very narrow beams which therefore would carry only very few neutrons .
Useable
beams must have a width of several cm and contain neutrons of different direction (divergence)
.
In particular the use of a large area sensitive detector leads to rather divergent
rays in the secondary arm .
Note that a field of 1000 Gauss=0 .1 Tesla acting along a track
of 2 m yields 3000 Hz/Gauss x 1000 Gauss x 2 m / 400 m/s = 15000 full precessions for
neutrons with a velocity of 400 m/s (A = 1 .Onm) .
The condition that the precession angle
accumulated along different rays in the beam must be equal within 0 .1 precessions then
translates into the requirement that the field integrals along the different rays must be
saine within 1 : 10 5 . As soon as the precession angles resulting from different rays differ
by 180° the signal ist lost completely.
required homogeneity by a factor 100 .
Simple cylindrical precession coils fall behind the
Only by use of special correcting elements ("Fres
nel" coils) the required homogeneity may be achieved . The correction elements positioned
in the neutron beam have to realize radial current distributions around the magnetic axis .
Three radial elements per arm in principle allow for a full correction .
However the making
of such elements that are transparent for neutrons and are able to carry the required high
current densities with the required accuracy is difficult .
Currently the improvement by a
factor of 100, sufficient for operation with the above parameters, is barely achievable .
Figure 11 .7 : Correction element for the field integral homogenization, material : aluminum
.
Fig .
11 .7 shows the shape of the radial correction elements which are used in the Jülich
NSE . The uncorrected inhomogeneity is proportional to the main precession fields and
therefore proportional to the Fourier time t .
In the current setup the residual inhomogeneity
(after correction) sets the limit for the maximum Fourier time .
Figure 11 .8 illustrates
how the echo amplitude decreases due to resolution effects even
with correction elements .
Without correction the amplitude would drop to values below
0 .1 above Fourier times of a few us . The resolution functions as show in figure 11 .8 can
be determined using the scattering from a reference sample which is
known to exhibit
elastic scattering only (> 99.9%), here : microcrystalline MgO . The experimental results
(normalized echo amplitudes) of all samples have to be divided by the normalized echo
ô 0 .8
0
0
Im 0 .6
X ,a,
`RMRXI km,
,zum
0 .4
ccc .g1l
Figure 11 .8 : Resolution function of the Jülich NSE for beams of different divergence .
Solid lines : configuration with three correction coils, dashed lines : only two correction
coils .
amplitudes from the reference sample to yield S(Q,t)/S(Q) .
result of a typical experiment is shown in figure 11 .9 .
An example for the final
11 .6 Practical Aspects, Peculiarities
From the above description it follows that the NSE spectrometer measures the Fourier
transform S(Q, t) of the spectral part of S(Q, w) directly . As a consequence the average
count rate at the detector corresponds to half of all neutrons scattered from the Sample
into the solid angle of the detector (Fourierintegra4 . Therefore weck spectral features
are buried under the noise due to counting statistics . However the method is perfectly
adapted to relaxations that are performed by most of the scattering structure since the
Figure 11 .9 : S(Q, t)IS(Q) of a 2 .5 % polymer solution with a fit to the Zimm model that
theoretically describes S(Q, t) for a dilute polymer solution . The data have been measured
using the area detector at only two angular positions of the secondary spectrometer arm
within 8 h time . The hollow symbols have been obtained at an arm setting of Q = 0.05À1
and correspond to Q/Â 1 = 0 .038, 0 .05, 0 .061, 0.072 . The filled symbols were measured
at Q = 0 .08 .1 1 and correspond to QIÀ 1 = 0 .067, 0 .08, 0 .09, 0.102 .
relaxation functions are measured in the time demain directly and resolution correction
consists of a division instead a deconvolution in the frequency space .
One vert' important field for NSE investigations are "soft matter" problems. These comprise
polymer melts and solutions and other complex fluids . The NSE methods opens a
dynamics window in the SANS scattering vector regime . Since in that regime the dynamics
is determined by the balance between elastic (entropic) forces and friction and
in comparison inertial forces are negligible the observed fluctuations are pure relaxations
and well suited for investigation by NSE .
Many isotopesespecially normal hydrogen (protons)scatter neutrons incoherently.
This is often utilized in TOF investigations since the incoherent scattering from hydrogen
is dominant and more easy to interpret than the coherent . The spin incoherent scattering
is caused by the dependence of the scattering length on the relative orientation of nuclear
and neutron spins . The fluctuating part of the scattering length due to random spin
orientation contains no interférence of scattering from différent nuclei, i .e . thé scattering
intensity distributes evenly over 47r solid angle and is "diluted" accordingly . The intensity
is very small compared to typical SANS intensities . The dynamics of thé incoherent
scattering reflects thé tagged particle motion (self correlation) . For thé NSE method it
is important to note that thé spindépendent scattering flips 2/3 of thé neutron spins .
This means that a considerable loss of polarization is encountered, only 1/3 of thé neutrons
contribute to thé echo signalthé rest is background . This 1/3 stems form thé spin
flipped neutrons, i .e . thé écho amplitude is also inverted (négative) . It is evident that
for this reason NSE experiments with incoherent scattering are much more difficult to
perform . If coherent and incoherent scattering contributions are simultaneously present
this may lead to peculiar effects since thé amplitudes may cancel each other depending
on theirpotentially différentdynamics .
Contents
11 .1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 111
11 .2 Setup and Function . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 112
11 .2 .1 Flippers . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 115
11 .3 The detector signal . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 118
11 .3 .1 Symmetric Case . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 119
11 .3 .2 Elastic Scattering of a Finite Width Wavelength Distribution . . . . 1110
11 .4 Experimental Procedures and Evaluation . . . . . . . . . . . . . . . . . . 1111
11 .5 Field Integral Homogeneity and Resolution . . . . . . . . . . . . . . . . . . 1114
11 .6 Practical Aspects, Peculiarities . . . . . . . . . . . . . . . . . . . . . . . . 1116
12
Structure Determination
Gernot Heger
12 . Structure determination
G .
Heger
12.1 Introduction
The analyses of ciystal structure and magnetic ordering is usually based on diffraction
phenomena caused by the interaction of matter with Xrays, neutrons, or electrons .
Even
though electron microscopy can achieve atomic resolution, more detailed information on the
3dim . atomic arrangement of ciystals with its symmetiy and chemical bonding as well as
magnetic structures and spin densities requires diffraction methods. The basic theory of
diffraction is the saine for all types of radiation . Complementary information is achieved due
to thé différent character of Xrays, neutrons and electrons, and hence their différent
interactions with matter and further practical aspects.
Considering only Xrays and thermal neutrons one fends that their wavelengths are similar
(0 .5 Â < ;, < 2 .4 Â) . While thé electromagnetic Xray radiation yields thé total électron
density distribution, thé nuclear scattering of neutrons probes thé density distribution of thé
nuclei and thé magnetic neutron scattering thé spin density ofunpaired electrons .
Xray diffraction using conventional laboratory equipment and/or synchrotron installations is
thé most important method for structure analyses. The purpose of this paper is to discuss
spécial cases, for which, in addition to this indispensable part, neutrons are required to solve
structural problems . Even though thé huge intensity of modem synchrotron sources allows in
principle thé study of magnetic Xray scattering thé investigation of magnetic structures is
still one ofthé most important applications ofneutron diffraction .
12.2 Structure factor and Bragg intensities
The characteristic feature of the crystalline state consists of its periodic ordering, which may
be represented by a (translational) lattice . In the 3dim . case three basis vectors a, b and c
deine a parallelepiped, called unit cell . The general lattice vector
ti=ua+vb+wc (1)
results from a linear combination of the basis vectors with coefficients u, v, and iv being
positive or negative integers (incl . 0) . According to their pointsymmetry properties seven
crystal systems are distinguished :
Triclinic, Monoclinic, Orthorhombic, Tetragonal, Trigonal, Hexagonal, and Cubic.
121
Besides of the related seven primitive lattices, with only one lattice point per unit cell,
multiple lattices with centred unit cells are possible . In this way a total of 14 Bravais lattices
is defined.
The position of atour j in the unit cell is given by the vector
ri =xja+yb+zjc . (2)
The coefficients xj , y, and zj are called atomic coordinates (0
Important: Thc measured Bragg intensities 1(H) from diffraction experiments yield only the
modulus of the structure factors, IF 1(I) j oc «H), and not their phases cp(HH)
(see Eq .
5), which would be required for the inverse Fourier transform of the data (Fourier
synthesis) to give directly the arrangement of the atours in the unit cell . The lack of the phase
information is known as the phase problem of ciystallography.
In a diffraction experiment normally only relative Bragg intensities are measured . A SCALE
factor is assumed to be rigorously the saine for all reflections of one data set . For merely
nuclear neutron scattering and single crystals the integrated relative intensities are given by
I(H) = SCALELAIF(H),2 .
The Lorentz factor L is instrument specific . The absorption correction A depends on the
geometiy and linear absorption coefficient ofthe sample .
The geometrical diffraction conditions and hence the reciprocal lattice yield the periodicity of
a ciystal . Information on the ciystal system, the Bravais lattice type and the basis vectors a, b,
c of the unit cell (lattice constants a, b, c, a, ß, y) may be directly deduced from the reciprocal
lattice . The 1F(H)1 2 values associated as weights to the nodes of the reciprocal lattice give the
diffraction symbol and hence valuable information on the spacegroup symmetry . Here
systematic absences (zero structure factors) can be related to the choice of a nonprimitive
Bravais lattice,
or to the presence of nonsymmorphic symmetry operations (symmetry
operations with translation components) .
12.2 . 2 Magnetic scattering
The dipolar interaction between the neutron magnetic moments and the magnetic moments of
atours/ions (and nuclei) mi leads to the magnetic neutron scattering in addition to the nuclear
contribution .
In the case of an ordering of the magnetic moments over the whole ciystal
(periodic magnetic structure) the magnetic structure factor is given by
FM(H) = 1 bmj(I1) exp[27ci(Hri)]Tj(H)
i
(9)
with the magnetic scattering amplitude
hM~(~ = (e2y/2mec2 ) . fMi(H)'6'm (H) . (10)
1/26 is the neutron spin operator and ~JH) the projection of the magnetic moment mj onto the
scattering plane (hkl). The magnetic form factor fmj(H is the Fourier transform of the
normalised magnetisation density Mj(r) of the atour or ion j
12 3
fM(H) = Jv Mj(r)exp[2ni(Hr)] &r (11)
with fm(0) = Jv Mft)dr = 1 .
This is a fonction of the reciprocal lattice vector H, whereas the atomic scattering factor f of
Xray diffraction
f (IHI) = fv pi(r)exp[2ni(Hr)] &r, (12)
for a spherical electron density pj(r), depends only on the length of H.
The intensity of magnetic and nuclear neutron scattering is of the saine order of magnitude .
For unpolarised neutrons the Bragg intensity of nuclear and magnetic neutron diffraction is
simply an incoherent superposition
I(H) = IN(H) + IM(H)  IFN(H)I Z + IFm~H)I Z . (13)
For polarised neutrons on the other hand the coherent superposition gives
(14)
[IF(H)IZ] } = IFN(H) ± Fm(H)I Z
with thé interférence terms ± 2 . IFN(H) . FM(H)I according to thé two possible directions of
polarisation (+ and ) . In measuring thé flipping ratio at superimposed Bragg reflections, that
means thé ratio of thé intensities for thé two polarisations up and down, even small magnetic
structure factors can bc determined quite accurately .
The analysis of a magnetic structure starts with thé determ nation of its periodicity with
respect to that of thé crystal structure . The identification of magnetic reflections is usually
accomplished by a careful comparison of powder diagrams recorded below and above thé
magnetic phase transition temperatures . A more detailed study of thé scattering vectors, e .g .
for incommensurate structures, may require also singlecrystal experiments . The nuclear
structure factors FN(H) can bc calculated from thé known crystal structure . In this way thé
SCALE factor of thé data set can bc obtained and thé absolute values of thé magnitudes ofthé
magnetic structure factors IFM(H)I can be determined. The individual orientations of thé
magnetic moments mj with respect to thé basis vectors of thé crystal lattice and their
magnitudes are then to be calculated.
12 .3 Contrast variation
Neutron diffraction
can bc used for an experimental distinction of atoms/ions with almost
equal Xray scattering amplitudes . In thé case of mixed systems it is furthermore possible to
détermine a fractional site occupation. Another application of neutron diffraction is thé
12 4
determination of accurate atomic parameters (positional and thermal parameters, site
occupations) of lighter elements in the presence ofheavy ones .
The contrast in conventional Xray diffraction is directly related to the ratio ofthe number of
electrons Zj of thé différent atoms or ions j involved . The atomic scattering factor f in thé
structurefactor formula, which represents thé Fourier transform of thé atomic electron
density distribution, is proportional to Zj (f = Zj for sin9/A, = 0) . Standard Xray techniques
can hardly differentiate between atoms/ions of a similar number of electrons, and only an
average structure  including a total occupation probability of mixed occupied sites  may be
obtained in such cases .
For neutrons thé atomic scattering factor f is replaced by thé nuclear scattering length (or
coherent scattering amplitude) bj, which is ofthé same order of magnitude for all nuclei but
varies from nucleus to nucleus in a nonsystematic way . b,, values, which can be either
positive or negative, depend on thé isotopes and nuclear spin states of thé element j . A
nucleus of an isotope with spin I may have two différent neutron scattering lengths : one for
thé combined spin state J = I + %2 and one with J = I  '/z . An important and fundamental
example is provided by thé simplest of all nuclei, thé proton with spin I = 1/2 . The two spin
states, J = 1 (triplet) and J = 0 (singlet), with statistical weights 3/4 and 1/4 respectively, have
thé scattering lengths for afree proton :
b SH=23 .7 fin, b'H=+5 .38 fin, bfre,H = 1/4b'H + 3/4b'H = 1 .89 lin (with 10 15 m = 1 lin).
The value for thé bound proton in a ciystal structure, which is to be used in thé structure
factor calculations, amounts to bl, = 2 bfreeFl = 3 .741 fm.
The natural isotope mixture and a statistical spinstate distribution lead to thé commonly used
general formula bj = with thé sum of thé différent isotope fractions
a+13+y+. . . = 1 (boa, bop, bj,, being thé individual scattering lengths of thé différent isotopes of
thé element j) . The natural nickel isotopes, for instance, have extremely différent coherent
scattering amplitudes :
b( 58Ni) = +14 .4 fin, b(6°Ni) = +3 .0 fin, b(61Ni) = +7 .6 fm,b(62Ni) = 8 .7 fin, b(64Ni) = 0.37 fin
resulting in an overall scattering length bNi = +10 .34 fm .
Neutron experiments frequently make use of compounds containing single isotope elements,
like fully deuterated samples . Incoherent scattering due to a statistical distribution of isotopes
and nuclear spin states is not discussed here . It may influence thé effective absorption and thé
background conditions ofneutron diffraction studies .
12 5
12 .3 .1 Example ofcontrast variation :
Crystal structure and magnetic ordering of (Mnl%Cr%) 1+sSb
A special possibility of contrast variation, the combination of Xray and neutron diffraction
information, is demonstrated for the example ofthe intermetallic compounds (Mnl_XCr,)1 + sSb,
with 0
The knowledge of the overall occupation probabilities M, and Md  from conventional Xray
studies  allows thé évaluation of thé Cr : Mn ratios of thé différent sites 2(a) and 2(d) from
thé corresponding effective scattering lengths detennined by neutron diffraction. In thé
structure analyses based on thé neutron data beff = bmPP is obtained individually for thé two
sites
(PPa = a and PPd = d stands for refmed pseudooccupation probabilities) . According to
we can calculate
bef~2a) = a[(1y)bm, + ybcr] and ber~2d) = d[(1z)bm, + zbcr]
y = [b ef{2a)/a  b ue,] / [ber  bue,] and z = [b ef{2d)/d  bm,] / [ber  bm,] .
The detailed site occupations lead to thé general formula
(MntyCry)a(NlntzCrz)dSb
site 2(a)
site 2(d)
corresponding to a chemical composition of Mn[( l  y)a + (1 z)d]Cr[ya +zd]Sb . It is evident, that thé
individual (Cr,Mn) distribution on thé two crystallographically différent sites 2(a) and 2(d) is
not accessible merely by a chemical analysis . For most of thé samples studied, thé site 2(a)
was found to be fully occupied : a ~ 1 .0 . But thé formula (Mn l  XCr.) 1+8Sb used normally is
only correct for thé spécial case of equal Cr : Mn ratios on both sites :
x = y = z and 1+S = a+d.
1_ 300
PilnSb 02
12 7
Fig . 2 . Magnetic phase diagram of the System MnSb  CrSb . The vectors indicate the spin
orientations in the different magnetic structures .
The detailed information on the (Cr,Mn) distribution is needed to explain the magnetic
properties of these intermetallic compounds, for which only the spins localised on the 2(a)
sites are involved in the magnetic ordering leading to a complex magnetic phase diagram of
the MnSb  CrSb system ( sec Fig . 2) . An overall Cr : Mn ratio from chemical analysis is not
sufficient . The ferromagnetic Mnl+sSb changes its axis of easy magnetisation from parallel to
the hexagonal caxis at high temperatures to Ic at low temperatures . The magnetic spins of
the uniaxial antiferromagnetic Crl+sSb are oriented parallel (or antiparallel) to c . For mixed
crystals (Mnl_,Crx )1 +sSb in between the pure end members there exist various ferro and
antiferromagnetic states with inclined spin orientations, wich noncolinear magnetic
arrangements, and regions wich coexisting magnetic ordering .
In general, a mixed occupation of one ciystallographic site with three kinds of scatterers  e .g .
Mn, Cr, and "vacancies"  requires at least two independent and sufficiently different
experimental data to determine the fractional occupancies .
12 .4 The hydrogen problem in structure analysis
The detennination of the structure parameters of hydrogen atoms is a special problem
involving différent aspects of Xray and neutron diffraction. It is obvious that H/D atoms with
Z = 1 give only a small contribution to thé electron density and, therefore, they are hardly
visible in Xray structure analyses . This holds especially when heavy atoms are present . But
there is a more general problem : thé single electron of H/D is engaged in thé chemical
bonding and is not localised at thé proton/deuteron position . This position, however, is of
importance when hydrogen bonds  eventually related to thé lattice dynamics or structural
phase transitions  are discussed.
Xray studies of electron densities of simple molecular crystals, for which theoretical
calculations for isolated molecules are possible, are of special interest in order to compare
experimental and theoretical results for a better understanding of chemical bonding in
crystalline solids . Molecular crystals consist normally of light atoms often including
hydrogen . A combination with neutron diffraction experiments is important to determine thé
structure parameters of thé H/D atoms properly . More generally, thé structure analysis by
neutron diffraction yields separately and independently from thé Xray data thé structure
parameters of all atoms including thé mean square displacements due to static and dynamic
12 8
(even anharmonic) effects. This complete information can be used in a socalled XN
synthesis to obtain experimental electron deformation densities from the measured Xray
Bragg intensities .
12.4 .1 Example of the determination ofH/D positions :
Study of hydrogen bonds in Na2S "9D20
One of the most important fields of application of neutron diffraction is the determination of
H/D sites and of their DebyeWaller factors . As an example for a study of a variety of
hydrogen bonds, where the structure model was established by conventional Xray analysis
and neutron diffraction served especially to localise the hydrogen atoms, the case of fully
deuterated Na2S9D20 was chosen [2] . Its crystal structure (noncentrosymmetric space
group : P4 122 or P4322) is dominated by discrete [Na(D 20) 5 ] and [Na(D20)4 ] spiral chains of
Na(D20) 6 octahedra (see Fig. 3) . There are five différent water molecules (see Fig. 4) with
OD distances between 0.949 A and 0.983 Â, and D0D angles from 104 .6° to 107 .5° . These
water molecules are furthermore involved in six différent OD. . .S bridges to thé S 2 ions .
Details of thé various OD . ..O/S hydrogen bonds (given in Table I) were combined with
results from Raman spectroscopy from which thé uncoupled OD(H) stretching frequencies
could be reasonably well assigned to thé vine différent OD(H) groups of thé ciystal structure .
Fig . 3 . Na2S9D20 : A partial view of the crystal structure
Fig . 4 . Coordination ofthe D20 molecules in Na2S 9D20 .
A B C
AB
BC
AC ZBAC ZABC ZBAB' ZCAC'
L AL ~ LA L'
0(l) D(1)_ ..S
D(V) S
0(2) D(21).~ .0(5)
D(22). . . S
0(3) D(31). . .S
D(32). . .0(4)
0(4) D(41) . . .S
D(42), .,S'
0(5) D(51), . .0(3)
D(52) . . .S
mean values
mean values 0D .. .O
mean values 0D . . .S
0.9617) 2 .359(5) 3.319(5) 1,4(4) 178.0(6) 106.3(7)
0.961(7) 2,359(5) 3.319(5) 1 .4(4) 178A6)
0.964(7) 1 .793(7) 2.752(7) 1W4) 172.4(6) 106 .l(7)
0.962(7) 2.550(6) 3.5M5) 52s) 172.8(6)
0,977(7) 131l(5) 3.284(5) 47(4) 173,3(5) 10T5(7)
0.953(7) 1 .797{7) 2,730(7) 9.6(4) 169.3(6)
0,983(7) 2.294(5) M74(4) 3.4(4) 179.l(5) 104 .6(6)
O.973(7) 1359(5) 3 .333(5) 03M 179.6(5)
0 .949(7) 1,ffl(7) 2,768(7) 9 .2(4) 166 .l(6) 105 .5(6)
0 .967(7) 14o(5) 3,401(5) 5Y(o 172,1(5)
0 .965 106,0
0,955 1309 2,750 1679
0970 1386 3353 1751
103M2)
Na(1) 2.411(4) 116.1(2)
Mai lois)
111 .5(2) Na(2)
Na(T)
1588(5) 976(2)
2,380(5)
116 .9(2) Na(1)
0(5)
1397(5) 104 .8(2)
2 .768(7)
104 .1(2) Na(2)
0(3)
1418(51 105 .5(2)
2 .730(7)
103 .4(2) Na(1)
0(2)
1485(5) 101 .7(2)
2,752(7)
107,9 2,447
Table 1 .
hiteratomic distances (Â) and angles (') for the hydrogen bonds and the ligands te,
the water molecules in Na2S9D20.
imil
Remember: The scattering lengths ofthe proton and the deuteron are bx = 3 .74 fin and bD =
+6 .67 fin, respectively . Their magnitudes are comparable to the average of all b; magnitudes
and, therefore, H/D can be considered as "normal" atoms for neutron diffraction . The différent
signs of bu and bD may be of interest in Fourier maps for contrast reasons . Experimental
conditions like background and effective absorption are strongly affected by thé huge and
exceptional incoherent neutron scattering crosssection of hydrogen (ß;n,(H) = 79 .7 barns as
compared to 6; c(D) = 2 .0 barns).Very often deuterated compounds are preferred in order to
profit from thé larger bD value, but mainly to reduce thé background from incoherent
scattering . This volumedépendent background may become crucial for neutron powder
diffraction experiments, for which normally sample volumes of more than 1 cm3 are required .
12 .4 .2 Example ofa study ofH/D ordering :
Ferroelectric phase transition in KH 2PO4 (KDP)
The hydrogen problem is of special importance for structural phase transitions driven by
proton ordering . As a well known example thé fenoelectric transition in KH2P04 (KDP) is
presented . A characteristic feature of its crystal structure consists ofthé P0 4 groups linked by
strong hydrogen bonds (see Fig . 5). At room temperature KDP crystallises in a tetragonal
phase (space group : 1 42d), where thé protons in thé 0 . . .H...0 bonds are dynamically
disordered according to a doublewell potential . At T c = 122 K, KDP transforms to a
Fig . 5 . Crystal structure of KH2P0 4 .
1 212
fenoelectric phase of orthorhombic symmetiy (space group : Fdd2) in which the protons order
in short asymmetric OH . ..0 bonds [3] . The contour plots of the proton distribution at
différent temperatures are shown in Fig . 6.
(a) TC + 2K (b) Te  1 .3K
,~r
(c)
Tç  10K
Fig . 6 . Contour plots ofthé refined proton distributions in KH2P04 at :
(a)Tc +2K,(b)Tc 1.3K,(c)T c 10K,(d)Tc 2OK.
12.51VIolecular disorder
Disordered structures and pseudosymmetries related to dynamical reorientation and/or
structural phase transitions are of great current interest . In principal, the dynamical disorder of
molecules is due to the fact that the intermolecular bonds are very much stronger than the
external ones between the molecular groups and the surrounding crystalline frame . It is
obvious that the chemical bonding scheme predicts the symmetry of a crystal structure, and
not the other way around . We can state, however, that in the case of an incompatible pointgroup
symmetiy of a molecule with respect to its site symmetiy in the crystal structure,
molecular disorder is the necessary consequence. In order to modellize the atomic density
distributions conectly in a way to obtain physically meaningful potentials, very accurate
Bragg intensities over a large sinO / ;, range are required. Xray experiments are generally more
restricted than neutron studies because of the sinO /;, dependence of the atomic scattering
factor f .
12.5 .1 Example of molecular disorder :
Almost free rotation of NH 3 groups in the crystal structure ofNi(NH3)612
As an example, related to the H/D problem, the dynamical disorder of the NH3 group in the
cubic high temperature phase of the metal hexamine halide Ni(NH3)6I2 (space group : Fm3m)
is presented . Tbc corresponding crystal structure is shown in Fig . 7 . With the NH3 tetrahedra
12 1 3
(3m symmetiy) on crystallographic sites of 4mm symmetiy it is obvious that they must be
orientationally disordered . At 19 .7 K, Ni(NH3) 612 undergoes a first order phase transition to a
probably ordered rhombohedral low temperature modification [4] .
rr
Nickel
~7 lodine
NN3 group with
hydrogen disorder
Fig . 7 .
High temperature structure of Ni(NH3 )6 12 The hexamine coordination is shown only
for the Ni atom at the origin .
Fig. 8 . Ni(NH 3 )612 : Proton density in a [001] section at z = 0 .23 ;
(a) and (b) experimental results at 295 K and 35 K,
12 14
(c) and (d) calculated densities at 295 K and 35 K.
Single ciystal neutron diffraction studies at 35 K and 295 K [5] revealed a planar proton
density distribution perpendicular to the fourfold axes (see Fig . 8) . Its four maxima are
directed towards the neighbouring iodines according to the influence of NH . . .I bonding . This
proton density can bc explained as a consequence of a coupled rotationaltranslational motion
of the ammine group .
12.6 Spin densities in magnetic molecular compounds
Molecular magnetic compounds are of great actual interest due to both, applicational
perspectives and fundamental research. The spin density distribution is an essential
information for the understanding of the magnetic properties of these materials ; it yields the
localisation of the magnetic electrons and give rise to the microscopic magnetic interactions .
Polarised neutron diffraction on single crystals is presentey the most powerful tool for
determining the spin densities in molecular compounds [6] . Results obtained from a data
treatment by the maximumentropy reconstruction method are presented for the purely
organic ferromagnet, ß4,4,5,5tetramethyl2 p(nitrophenyl)3oxido4,5
dihydroimidazolium 1oxyl (pNPNN) [7] .
References
1 . W. Reimers, E . Hellner, W. Treutmann, and G. Heger,
J. Phys . C : Solid State Phys . 15, 3597 (1982).
2 . A. Preisinger, K. Mereiter, O . Baumgartner, G. Heger, W . Mikenda, and H . Steidl,
Inorg. Chem. Acta 57,237 (1982) .
3 . R . J. Nelmes, W . F . Kuhs, C . J. Howard, J. E . Tibballs, and T . W . Ryan,
J. Phys . C : Solid State Phys . 18, L711 (1985).
4 . J . Eckert and W. Press, J. Chem. Phys . 73, 451 (1980) .
5 . P . Schiebel, A . Hoser, W . Prandl, G. Heger, and P. Schweiss,
J. Phys . l France 3, 987 (1993) .
6 . J. Schweizer, Physica B 234236, 772 (1997) .
7 . P . Schleger, A. PuigMolina, E. Ressouche, O . Rutty and J . Schweizer,
Acta Ciyst . A53, 426 (1997).
1215
Textbooks
G . E. Bacon, Neutron Diffraction, Clarendon Press, Oxford (1975) .
HERCULES : Neutron and Synchrotron Radiation for Condensed Matter Studies,
Vol . I and II (edited by J. Baruchel, J. L . Hodeau, M. S . Lehmann, J . R. Regnard and
C . Schlenker), Les Editions de Physique, Les Ulis & SpringerVerlag, Berlin (19931994) .
L. Dobrzynski and K . Blinowski, Neutrons and Solid State Physics,
Ellis Horwood Series in Physics and its Applications, New York (1994)
13
Inelastic Neutron Scattering
Phonons and Magnons
Markus Braden
13 . Inelastic neutron scattering : phonons and
magnons
II.
Markus Brader
Physikalisches Institut, Universität zu Köln,
Zülpicher Str . 77, D50937 Köln
bradenüph2.unikoeln .de
13 .1 Interaction and scattering law
13 .1 .1 Basic concepts of scattering experiments
Scattering experiments are performed with almost all types of radiation on varions
systems (solids, liquids, gases, atoms, nuclei, . . . ) . 'T'he radiation with well defined initial
properties ( wavevector 1 ; energy E) hits the sample, gets scattered and may be detected
again with well defined final properties (wavevector k' ; energy E') in the angular segment
r2dQ, the schematic picture of the scattering arrangement is drawn in figure 1 . Aim of
any scattering experiment is to obtain information on the states of the sample by use of
the knowledge of the interaction between the radiation (for example neutrons) and the
particles forming the sample . In this chapter we deal with the inelastic neutron scattering
in solids which is till today the most efficient way to study dispersion relations of lattice
vibrations and magnetic excitations .
The initial and final states of the neutron may be denoted by Qz and Q', those of the
sample by ~z and A' . (7 z is characterized by the wavevector k and the energy E = 21rLk2, (7'
respectively. 'The momentum transferred to the sample crystal, Q, and the energy transfer,
E = hw, have to fulfill the conservation laws, Q = 1  l' and ca = h( 27n, ) 2(k2  k'2). 'T'he
probability to observe a scattered neutron in the angular segment dQ and in the energy
interval dE' is described by the partial differential cross section which may be obtained
within the Bornapproximation, which is a perturbation theory of first order, i .e . one
considers the interaction between radiation and sample crystal to be small .
 (k 'lk)(m/2~)z ~  a ;,Q; pa;pa i
13 1
Figurel Schematical drawing of a general scattering experiment .
G dA'I f d'r exp(ilk'  r)V(r)exp(ik  r) > ~2
*s(w+E'E)
T'he cross section in equation (13 .1) is given by the sum of the transition matrix
elements between initial states aiAi and the final states (T'A' weighted by the probabilities
of the initial states .
In order to calculate the cross section and the observable intensity
distribution, one needs the interaction potential Ù (r) and detailed knowledge of the states
in the sample ~i .
In the inverse way one may use a measured intensity distribution in
order to characterize the sample states, for example the phonons .
This is the usual way of
the interpretation of any scattering experiment .
The sample states may be characterized
by specific parameters, for example the frequencies and the polarization patterns in case
of phonons, which with the aid of equation (13 .1) will be deduced from the experimental
intensity distribution .
13 .1 .2 Nuclear interaction  phonons
The nuclear interaction between the neutron and the core of the atoms is characterized
by an extension of 10 'À, which is extremely small in comparison to the wavelength of
thermal neutrons . Therefore, the scattering is isotrope and may be described by only one
parameter, the scattering length .
The interaction with the hole crystal is given by the
sum over the atoms
(13 tir (r) = 21 bjb(r  Rj )
.2),
where bj and Rj are the scattering length and the position of the jth atom . 'The
mixing of different isotopes at the same atom site in the crystallographic lattice yields a
further complication, rince different isotopes have different scattering lengths .
This means
132
(000)
Figure 2 Schematic drawing of the vectors determining the position of an atom in the crystal lattice .
that the interaction potential (13 .2)
does not show the full translation symmetry of the
crystal lattice .
The local variation of the scattering length Splits the differential cross
section into two contributions
d2a d2( d2~
(1,S2(1,E'  (dS2dE' ) `~ rz + (d52dE')zT' c °'L .
The coherent contribution is determined by the mean scattering length, whereas the
incoherent contribution is given by the root mean square deviation to the averaged scattering
length .
In order to calculate the differential cross section in (13 .1) it is
necessary to know the
states in the sample or at least to parameterize them . 'The sum over the states Az in
(13 .1) may be transformed to the correlation function, in which one has to introduce the
parameterized Eigenstates of the system .
In order to achieve this transformation in case
of the phonons we consider the vibrations of a crystal in harmonic approximation .
 Description of lattice drynarrrics irr harrrronic approxirrration A crystal consists of N
unit cells with ri atouts within each of theut, the equilibrium position of any atom is
given
by the position of the unit cell to which it belongs, 1,
and by the position of the atomic
site in the unit cell, d .
At a certain time the atout may be displaced from its equilibrium
position by u(l, d) .
The instantaneous position is hence given by Rl .d = l +d+u(l, d) (sec
figure 2) .
For simplification we consider first a lattice with only one atom in the unit cell, d = 0 ;
l describes then the equilibrium position of the atom . 'The interaction potential between
two atoms l and l', ~D (l, l'), may be expanded at the equilibrium position in teruts of
u(l)=u(l')=0 . The constant term does not give any contribution to the equations of
movement, it is relevant only for the total energy of the crystal structure .
Since at the
133
equilibrium position the atom is in rest, terms of first order are not allowed . In harmonic
approximation one assumes the expansion till the second order to be suficient . This
assumption is essential for the following analysis, since already the presence of third order
terms prohibits to solve the equations of moveurent in the general case .
In mort solids
anharmonic contributions to the potential are, however, small justifying the assumption .
If the anharmonic effects
have to be taken into consideration (for example close to the
melting of the crystal lattice), perturbation theory is the usual technique .
Using the definition
D,, s (l, l') = d2 ,D(l ' l')
(13 .4)
du, (1)du,s (1')
one obtains the equations of movement (a,,3 = x, y, z) to
T'he displacement of the atour l' in ,3direction yields a force on the atour l in adirection
of strength D,,s(1,l')uß(l'), D,, s (1,l') are therefore called the forceconstants . 'The real
problem in treating lattice dynamics consists in the large number of there equations, there
are 3N equations to be solved with N being of the order of 10 23 .
In order to avoid this
complexity one makes the Ansatz of plane waves :
the movements of all atoms are given
by the displacement in one unit Gell at time zero propagating in time and space as a plane
wave
exp(i u~(l) = e~M i / z
(1 l  w ot) (13 .6) .
Figure 3 shows the displacement pattern of a plane wave characterized by the wave
vector q, reflecting the propagation of the wave (planes perpendicular to (j are always
identically displaced), the vibration frequency wo
of each atour and the direction of the
oscillation given by the polarization vector c .
In the single atom lattice there are only
acoustic modes, they are called longitudinal (LA) if q is parallel to e and transversal (TA)
for q perpendicular to e .
The plane wave Ansatz (13 .6) for the equations of movement yields a system of three
equations for each qvalue
134
o
o
o
o
bo
ao
Lambda lattice parameter
Figure 3 Scheme of the displacernents in a transversal plane wave .
=1/.olr~_ D~(L, o)exp(igl)e 3 (13 .7) .
1,3
Here we use that the force constants depend only on the distance in real space (l  l')
and not on the particular values of l and l' . With (13 .7) one gets an easily solvable system ;
the original complexity of the problem is transferred to the number of these 3dimensional
probem .
For a complote solution of the crystal dynamics one would need to solve the
problem (13 .7) for Bach of the N10 23 allowed qvalues . In reality, however, one han to
analyze only a few different qvalues . In general it is sufficient to study only qvalues
within the firnt Brillouinzone .
M,e may define the dynamical matrix as
D~,~(q) = 1/~~D~,/~(l,o)e~p(Zql) (13 .8)
which allows to rewrite the equations (13 .7) in matrix form
w,e = D e (13 .9) .
The system (13 .9) is just a thesedimensional Eigenvalue problem .
For fixed q one han to determine the these Eigenvectors ej , j=1,2,3, together with
the these corresponding Eigenvalues, wj (q) . This may be achieved with the standard
numerical techniques . The dependence of the Eigenfrequencies on the wavevector, wj (q)
with j = l, 2, 3, is called the dispersion relation .
135
s
 ' f
N .mwn .I )oo K L .~um..un . .JOOK
11001 au.a~o . I I I l01 lJfOWn
a I
3 ~ I
. . [ .
F
Sr
I_r
I I
r I I 1 I 1 i
0 : 0+ Os I I I 0 0! 10
0 0 : 0+ On ot l0
Figure 4 Phonon dispersion of Al along the [100] and [011]directions (from reference [1]) .
The extension to a System with n Atoms in the primitive Gell can be easily donc, one
gets for each q an Eigenvalue problem in 3n dimensions .
The Eigenvectors have the
dimension ara and the dynamical matrix is 3ra * 3ra dimensional .
For each q
one finds
hence 3n Eigenmodes, therefore the complete phonon dispersion consists of 3n branches,
three of which have zero frequency for q > 0 . The latter branches are called acoustic
rince they are associated `vith the propagation of round .
The figure 4 shows the t ypical
presentation ùj against wavevector q for the phonon dispersion of aluminum .
The plane waves according to the Eigenfrequencies and to the Eigenvectors to each
of the allowed (1values form a.
complete set of fonctions for the displacements of the N
tunes n atours in the crystal .
Any distortion can be represented as a linear combination
of these plane waves . Obviously it is rather favorable to use this set for calculating the
differential cross section . However, for this purpose it is necessary to couvert the lattice
vibrations into quantum mechanics, the corresponding quasiparticle being the phonon .
A
onephonon protes is shown in the schematic figure 5 .
The momentum transfer Q = kk'
consists of the rum of a reciprocal lattice vector T and the wavevector q, which lies within
the firnt Brillouinzone .
Only q determines the wave vector of the contributing phonons,
however Q determines the differential cross section, i .e . the intensity .
The exact scattering may be deduced from the correlation fonction .
In the following
we only avant to discos the meaning of the different terms in the cross section
136
Tau
Figure 5
Scattering triangle corresponding to the observation of a phonon mode with wave vector q
at the reciprocallattice vector T.
d2a  (27)s
(dQdE' )  ( ~) 2vo
1 G j (q, Q) 1 2 (13 .10 .a)
~~~(s)
(13 .10 .b)
.(,rt,(wj«1) +1/2 +1/2) (13 .10 .c)
(13 .10 .(1),
with vo the volume of the reciprocal unit cell . Equation (13 .10) describing the intensity
of a onephonon measurement at specific Q closely resembles the elastic structure factor
of the Bragg reflection intensity, a part of expression (13 .10) is called dynamic structure
factor . 'The intensity is given by the sum over all reciprocal lattice and all wave vectors ;
however only the combination q+? = Q may contribute due to the 6function in (13 .10 .4) .
The second bfonction in (13 .10 .4) reflects the law of energy conservation, however, one
has to take into account that the scattering processes may lead to a creation as well as
to an annihilation of a single phonon, corresponding to the upper and the lower signs
respectively. There are two more general factors determining the intensity of the phonon
observation by neutron scattering . The term (13 .10b) indicates, independently of all
other terms, that the intensity is inversely proportional to the frequency of the mode .
High energy modes are always more difflcult to observe than the low lying ones . Since
neutron experiments suffer front the low flux of the existing sources, this effect frequently
prohibits the study of the high energy part of the phonon dispersion . 'T'he term (13 .10 .b)
137
esults from the quantum mechanics of a single harmonie oscillator :
the square of the
amplitude is proportional to W7 \4~ .
The terni (13 .10 .c) results from the Bosestatistics of the singulär mode with frequency
w j (q) , the occupation number is given by the Bosefunction :
n(w~(q))  exp( tLkl
(~) ~ ) 1
13 .11
ri,(wj (_q» tends for T > 0 towards zero, the phonons are frozen . For T > oc, n(wj(q»
approaches ( r kT"»,
i .e . the classical relation . The terni (13 .10 .c) indicates that the
Bosefunction is increased by +1 only in case of phonon creation . At low temperature
where n(wj(q)) is
close to zero, the phonon may be observed only in the creation mode,
the cross section for the annihilation process becomes vanishing since the phonon states
are no longer occupied . At finite temperature the Bosestatistics further simplifies the
observation of phonons with low frequencies .
The complex term in (13 .10 .a) is given by the dynamical structure factor :
C j (q, Q) = ~ bd  exp(  I1'd(Q) + z(2d d) * (Q e (q)) (13 .12),
d rri:d
where the sum is
extending to the atoms, numbered by the scalar d, in the primitive
cell .
They have the mass md scattering length bd and a three dimensional polarization
vector ed(q), the equilibrium position in the unit cell is given by dd .
Without the last
part equation (13 .12) corresponds to the elastic structure factor, in particular one finds
the same Debye M'aller factor exp(Wd(Q » .
'T'he whole term in the exponential function
determines whether the interference between atoms is constructive or destructive .
In the
dynamical structure factor there is
in addition to the elastic one the polarization term
(last parenthesis) ;
for instance only those atoms may contribute whose polarization vector,
possesses a component parallel to Q.
Since Q enters this term directly, the structure
factor increases `vith ~QI ; the intensity is proportional to Q2 . The interference and the
polarization term in (13 .12) cannot be separated in genoral, therefore one has to calculate
the structure factors precisely.
In addition to the interpretation of the frequency data the prediction of the intensity
is an important outcoming of model calculations .
Only with the help of these predictions
a neutron scattering experiment aiming at the lattice dynamics of a complex material can
13 8
e performed in an efficient manner .
Some easy examples may illustrate the significance of the terras in (13 .12) . Let us
consider a longitudinal acoustic mode polarized in the [100]direction ;
for this mode all
e d are parallel to [100] . 'T'he polarization term becomes maximum for Q=(h+~ 0 0) and
can be extracted from thé sum .
'The remaining interférence sum corresponds for small
~ to thé elastic structurefactor of (h00), 'T'he dynamic structure becomes hence strong
for strong Braggreflections .
thé strong Braggreflections .
In general acoustic phonons have to be measured close to
Since for optical modes thé atours may be displaced in
opposite directions, thé polarization term can change sign yielding a rather distinct sum
of thé interférence terra .
In a simple twoatomic structure thé optical mode has only a
weak dynamical structure factor close to thé strong Braggreflections (this argument is
no longer valid in case of négative scattering lengths) .
Why does inelastic neutron scattering play such a dominant role in thé study of lattice
dynamics? The central point is certainly due to similar masses of atours and thé neutron .
This yields thé possibility of elastic as well as that of inelastic scattering and renders
thé wavevectors of thermal neutrons comparable to thé wavevectors of thé phonons .
Inelastic neutron scattering allows to determine thé phonon dispersion over thé whole
Brillouin zone, whereas optical techniques (Raman and InfraRedscattering yields only
thé analvsis of modes at thé zone conter .
Recently there are serions efforts to perform lattice dynamical studies using synchrotron
radiation .
In case of thermal neutrons thé energies amount to 1100 meV and
correspond to thé typical phonon energies .
For comparison, CuK,radiation has an energy
of 8  l0'meV . In order to determine phonon frequencies, one needs a relative energy
resolution of 10 s  10  ', which may be achieved only by extreme expérimental effort .
The concomitant lors of intensity permits these measurements only at thé mort powerful
synchrotron sources, and even then thé measurements remain slow .
Me have seen that
thé onephonon process ,yields an intensity proportional to Q2, this may be used in case of
neutron scattering due to thé nuclear interaction .
In case of thé xrays thé large Qrange
is not at disposition since thé formfactor strongly reduces thé interaction .
In thé Gloser
future one may not expect, that inelastic xray scattering will supply results comparable
to neutron studies concerning thé eficiency .
The xray measurements, however, may become
valuable in cases where thé neutron scattering is hampered either by sample size or
139
y absorption .
13 .1 .3 Magnetic interaction  magnetic excitations
The neutron has a spin 1/2 which yields a coupling to the magnetic fields . The
interaction operator is given by
here i,z=1 .913 is the magnetic moment of the neutron, expressed in liN,
the nuclear
magneton, (~ the Paulispin operator and H the magnetic field induced by the electrons in
the sample .
H may arise from the velocity of the electrons as well as frora their magnetic
moment . In thé following we lirait thé discussion to thé latter contribution .
Furthermore we assume, that thé orbital moment has vanished . This assumption is
justified in case of quenching by crystal fields or for a halffilled shell (Mn 2 +, Fe i+, G(13 +) .
T'he Fouriercomponent of thé interaction potential is
_ 2 rr_ y,,c 2
V âDL
(~ rri jlIPez
(~ (13 .14)
with
here 'Yd
(Q) = ~( 1/2)YdFd(Q) 1~ SL(1, d)exp(iQ ' Rzd) (13 .15),
1 .d
is thé gyromagnetic factor, Fd(Q) thé formfactor of thé atour d and SL(l, d) _
Q x (Sjd x Q) with S(1d) boing thé spinoperator of thé atour .
There are two important différences between thé magnetic and thé nuclear interaction
of thé neutron with thé atour .
Due to thé extension of thé électron cloud, which causes
thé magnetic moment, thé interaction is nonlocal . Described by thé formfactor, F(Q),
thé interaction gradually decreases towards large Q . The detailed dependence of F(Q) is
determined by thé single atom .
Rare earths show, due to thé strong localization of thé
4felectrons, a less pronounced decrease when compared to thé transition metal ions with
more delocalized electrons .
In thé latter case thé decrease may be quite strong limiting
any measurement to thé firnt Brillouinzones .
The dependence of thé magnetic interaction
due to thé formfactor may be used to separate magnetic and nuclear contributions .
Furthermore,
thé magnetic interaction is mediated by vectoroperators .
Only those magnetic
13 10
1
r x z  w Z x E r A + L
6
5
_E a
3
F
3
2
00 0.2 0.4 0.6 0.8 0 0.2 0.4 0.4 0.2 0 0.8 0.6 0.4 0.2 0 0.1 0.2 0.3 0.4 0 .5
Reduced wave vector coordinate (ç)
Figure 6 Phonon dispersion of Ne along the three train symmetry directions (from Ref. [2]) .
moments may contribute to the interaction, which have a component perpendicular to
Q .
This yields the possibility to determine not only the size but also the direction of
magnetic moments .
13 .2 Analysis of lattice vibrations
13 .2 .1 Lattice dynamics in simple structures
For a simple crystal lattice one may determine the polarization patterns without detailed
model calculations .
The lattice dynamics of such a system may then be studied
experimentally without particular effort .
In figure 6 we show the phonon dispersion of Ne in the three main symmetry directions,
which according the common use are labeled 0, Y~ and A .
Ne crystallizes in a fcclattice
with only one atout in the primitive tell, therefore one expects only three acoustic branches
per qvalue .
One observes the three distinct branches only in the [xx0]direction, whereas
there are only single transverse branches along [x00] and [xxx] .
In the [x00]direction these
acoustic polarization patterns may be easily understood .
In the longitudinal mode atouts
are vibrating in [100]direction, i .e . parallel to the wave vector . The two transverse modes
are characterized by displacements in [010] or in [001]directions, i .e .
perpendicular to the
wavevector .
Since [100] represents a fourfold axis in the fcc lattice, the latter two modes
cannot be distinguished, they are degenerate . The saute situation is found along the
Figure 7 The plane in reciprocal space spaxmed by the (100) and (011) vectors for a fcclattice ; the
scattering triangle indicates the observation of Amodes .
[111]direction which is a threefold axis of the lattice .
'T'his behavior is a simple example
of the general relation between crystal symmetry and the phonon dispersion .
The crystal
symmetry yields constraints for the phonon modes which may be necessarily degenerate
at certain points or  like in the Nestructure  along a direction . In the case of more
complex structures it is essential to profit from the predictions of the symmetry analysis .
The [110]direction represents only a twofold axis since [110] and [001] are not identical,
as consequence the corresponding transverse acoustic branches are not equivalent .
In addition figure 6 shows that at X=(100)=(011) A and Ebranches are coinciding,
which may be explained due to the chape of the Brollouinzone .
Figure 7 presents the
plane of the reciprocal space spanned by (100) and (011) ;
one recognizes that starting
at the zonecenter, F, in the figure (133), in the [100]direction one will reach the zoneboundary
at (233)(100)=X . Similar, one will reach this point when starting at the
neighboring point (222) in [011]direction .
However, in this path one finds the border of
the Brillouinzone earlier and continues the last part on the zone boundary .
(100) and
(011) are equivalent points in reciprocal space ; they are connected by a reciprocal lattice
vector, (1 1 1) .
For the phonon branches we conclude that 0 and Ebranches have to
coincide . 'T'he symmetry further determines which branches coincide : for example the
longitudinal Ebrauch with the transversal Abrauch .
Again, similar considerations in
more complex systems may decisively contribute to the identification of the branches .
13 12
1s. 
1
tUMl
[cc01
~ 1 ~
10
517
if
0
0 0 .2 0 .4 0 .6 0 .8 1 .0 0 .8 0 .6 0 .4 0 .2 0 0 0 .2 0 .4
Reduced wave vector coordinate
(c)
Figure 8 Dispersion curves and crystal structure of F'eO (from reference [2]) .
Figure 7 further shows how to measure the Abranches .
One may observe the longitudinal
brauch in the (400)zone passing to (4+x 0 0) (the (400)zone has to be preferred to
(200) due to the langer value of Q2), whereas one may determine the transverse frequencies
in the (022)zone at (x 2 2) .
 NaClstructure  The NaCIstructure represents one of the mort simple possible
crystal structures with two atours per primitive tell .
It consists of two fcclattices shifted
against each other by (0 .5 0 .5 0 .5) . 'The entire crystal structure possesses fccsymmetry
too . Figure 8 shows the dispersion curves of FeO .
T'he six branches expected for the twoatomic structure are observed only in [xx0]
direction .
Like in case of the fcc Nelattice the transverse A and Abranches are doubly
degenerate . Also in other aspects, there is some resemblance with the Nephonon dispersion
; in both cases LAA and TAS branches coincide at the zone boundarv .
A more detailed discussion is needed in order to understand the optical modes at F .
The polarization pattern of an optical mode corresponds to an antiphase axial movement
of the ion pairs connected in [100], [010] or [001] direction . The three vibrations polarized
in the crystal directions should, however, be degenerate due to the cubic symmetry ;
one might expect only one optical frequency.
The optical vibration in the ionic lattice
possesses a polar character, i .e . there is a local polarization due to the opposite shifts
of cations and anions . For large wavelength, i .e . close to the zonetenter, the local
polarization adds to a macroscopic polarization only in case of the longitudinal mode .
1313
5
100s1 [OSl ] IOSSI [SSS
y i
4
0
r
1 .0 1.0 0
X W X E r
Reduced wave vector coordinate
(s)
0 .5
l
Figure 9 Phonon dispersion of NaCI (from reference [2]) .
This macroscopic polarization requires an additional energy, the longitudinal optic (LO)
mode is always higher in frequency than the trnaversal optic ('T'O) mode (note, that
there modes are only defined as the limit for q tending to zero .
The splitting between
LO and TOmode frequencies is called LydaneSachs'T'eller (LST) splitting and is related
by the LSTrelation to the dielectrical constant .
Polar mode frequencies may be easily
determined by InfraRed techniques ;
due to the form of the resolution ellipsoid neutron
scattering on this topic is frequently difficult . In metallic materials electric fields are
screened due to the free charge carriers at least for macroscopic distances .
As consequence
the LSTsplitting disappears .
The phonon dispersion may thon give information on the
efflciency of the metallic screening.
Figure 9 shows the phonon dispersion in NaCI, which is isostructural to FeO . Compared
to the latter one recognizes the perturbation of the curves arising mainly from the lower
optical frequencies . Within the Brillouinzone it is no longer possible to separate optical
and acoustic modes, the branches tend to cross each other but there is always a small gap
between branches of the came symmetry. 'This represents a general property : branches
of the same symmetry may not cross .
By mixing the polarization patterns it is always
possible to yield a gap reducing the total energy of the system . Whether this gap is small
or large depends on the similarity between the polarization patterns of the two branches .
1314
Similar branches may induce larger gaps, they are called to strougly interact .
13 .2 .2 Model calculations
The examples discussed above are characterized through their simplicity, which permits
to analyze the polarization patterns without detailed calculations .
one has to deal with systems of more than 10 atoms per primitive cell,
In actual topics
oue may identify
then the character of the phonon modes only with the aid of predictions of model
calculations .
As discussed above the lattice dynamics is described by the 3ndimensional Eigenvalue
problem with the dynamcal matrix
w 2e = De (13 .16)
D,a(d, (f ) =
1
1772~772~,)1/2
(D~,3 (Od,i' (f )CXP(i(Ii') (13 .17) .
(Od, l'(/') denote the force constants between the atoms d and d' in by l shifted cells .
The determination of the force constants represents the real problem in lattice dynamics,
in particular the question which constants are relevant .
Already by symmetry, the nine parameters per atompair are significantly reduced .
Furthermore, one may reduce the analysis to the cloner neighbors, as far as Do long range
force is involved .
'The next step consists in the development of potentials, from which one
may obtain the force constants for many pairs inducing only a few free parameters .
Frequently it is sufficient to consider axialsymmetric potentials with
V(r), i .e . the potential depends only on the distance between the two atoms . Such a
potential yields only two force constants, a
radial and a transversal one
a 2 V
(D x(ld, l'd') = a'To (13 .18),
r
(P1,(Id' 'd') = l l r
ar ~'TO (13 .19) .
In the mont simple model one may only introduce these radial and transverse force
constants for the close neighbors (BornvonKàrmàn Model) .
However, extending more
and more Shells will rapidly increase the number of parameters .
In particular the lattice
1315
dynamics of ionic compounds with the long range Coulombinteraction, tan only be poorly
described by such a model .
Even rohen parameterizing the Coulombpotential V (r)
x ~ by the charges,
Zd, Zd,, in order to deduce the respective force constants, the problem of the long range
persists . It is not possible to tut the rum at a certain distance, rince the rums (Io not
converge . The satisfying solution of this problem consists in the Ewaldmethod [1] .
The Coulombpotentials in an ionic crystal yields an attractive potential, which har
to be compensated by a repulsive one .
If the electron clouds of two ions of opposite
charge Start to overlap upon decrease of their distance, this repulsive potential will increase
rapidly. One may describe this interaction by a BornMayerpotential V(r) =
Bexp(rlro ), inducing only two parameters for one type of ionic pair, B and r o . Amongst
the varions extensions of this type of model, called "rigid ion", we mention only the Shell
model, rohere the polarizability of the ions is described by a Separation between an electron
cloud (the Shell) and the tores .
'There are many different ways to couple the tores
and the clouds by force constants .
In order to prepare an inelastic neutron scattering study on the lattice dynamics of
a complex material, even a simple and unadapted model may be helpful, as long as the
crystal structure and, therefore, the symmetry is correctly entered . By symmetry, degenerations
are fixed for certain points or even for unes in reciprocal space, and frequently the
structure factors follow some inelastic extinction rules .
In principle these predictions may
also be found by a careful analysis through group theory ; however, the use of a simple
model which does not need to describe the frequencies well is much less time demanding .
Some of these aspects have already been illustrated for the example of the NaCI structure
.
Concerning the dynamic structure factors one may add, that one will observe the
optical modes close to P best at the odd reciprocal lattice vectors (for example (333) )
independently of the forces involved .
13 .2 .3 Structural phase transitions and soft mode behavior
Structural phase transitions form still a topic of actual interest, where information
about the underlying microscopie mechanism may frequently be achieved only by inelastic
neutron scattering .
In figure 10 one finds the representation of a fictive structural phase transition in a
twodimensional crystal structure with two atoms in the primitive tell .
In the high sym
13 16
Figure 10 Schematic picture of a displacive phase transition occuring at the zone tenter and the
corresponding dispersion curve .
metry high temperature phase the black ion in the middle occupies a site with inversion
symmetry .
'This symmetry is broken at the phase transition due to the displacement of
the black ion .
The right part of figure 10 shows the corresponding dispersion curve, here
the polarization pattern of the Fmode corresponds to the static distortion belo,v
the
transition temperature, T, .
The phonon frequency of this mode softens upon approaching
the phase transition and is, therefore, called a "loftmode" .T'he structural instability,
however, tan be also seen in the dispersion quite above T, :
the frequency of the relevant
mode at P is lower than those of modes with qvalues in the Brillouinzone .
In addition to the phonon softening one expects a broadening of the line width in
frequency ; finally the width of the phonon mode may surpass its frequency . Such overdamped
modes may no longer be described in the harmonie approximation .
The best studied example for a zonetenter phase transition may be found in the
ferroelectric transition in perovskites, for example Pb'T'i0 3 see figure 11 . In the low
temperature phase the anions are deplaced against the cations, Pb, Ti, the corresponding
phonon frequency vanishes almost completely.
This polarization pattern has a strong
polar character and is connected to the dielectric constant through the LSTrelation . 'The
softening of the 'TO mode induces a divergence in the dielectric constant, which explains
the interest of the phenomena for technical applications .
A structural phase transition may also lead to an enlargement of the unit tell .
Here,
the equivalent atoms in neighboring tells are not displaced identically ;
a schematic picture
is given in figure 12, where neighboring black ions are shifting in opposite direction .
The
phonon mode associated with such a displacement pattern necessarily has a finite wave
1317
16
14
12
F.. . 10
ô 8
q
6
cr 4
G.
2
0
T
T>Tc
TTc
O O O O " O " O
8
8
" "
2 O O O i O O O
~ila
T>T .
0 q
Figure 12 Schetnatic pictiire of a displacive phase transition corresponding to a zoneboundary mode .
dynamics, which is analyzed almost exclusively by inelastic neutron scattering since the
largest effects are expected in the Brillouinzone .
The screening of the interatomic potentials through free charge carriers is determined
by the topology of the Fermisurface .
In particular there are singularities in the electronic
susceptibility when parts of the Fermisurface are parallel and may, hence, be connected
by a single nesting vector .
The susceptibility at this vector will be essentially increased
and may renormalize the phonon frequency of a mode just at this wave vector .
In most
cases this type of électron phonon coupling leads to a réduction of thé phonon frequency,
which shows up as a dip in thé dispersion curve, called a Kohnanomaly .
In particular thé
conventional superconductors, for example TaC in Figure 13, exhibit such effects .
'T'he
phonon dispersion of TaC shows pronounced dips, which are not observed in thé phonon
dispersion of normal metals .
The study and interpretation of similar anomalies in thé
highT, cuprates is subject of present research .
However, in this case thé aualysis gets
rather complicated due to thé large number of atoms in these systems .
13 .3 Magnetic excitations
13 .3 .1 Spin waves in a ferromagnet
Like thé crystal structure, magnetic order may be disturbed at finite temperature
with thé perturbation propagating through thé crystal .
Analogous to thé phonons, thé
quantisized excitations are called magnons .
The ground state of a ferromagnet results from thé interaction between spins of neighboring
atoms, which fa, ,ors a parallel alignment . The energy of a neighboring pair, S i , S j ,
depending on thé relative orientation of thé spins is
described within thé Heisenbergmodel
by c = JS z  S j , where J is thé Heisenberg exchange constant . For a chain of
13 19
21
[ooç 1 " 
19
18
17
16
"" 298 K
4
3
O
0 0.2 0.4 0 .6 0.8 1.0 0.8 0.6 0.4 0.2 0 0.1 0.2 0.3 0.4 0.3
Reduced wave vector coordinate (c)
Figure 13 Phonon dispersion of TaC, the dips, for example at (0 0 0 .7) andd at (0 .6 0 .6 0), indicate
modes renormalized throiigh the electron phonon coiipling, from reference [2] .
coupled spins the energy of the magnetic interaction amounts to
n,
U = 2J ~7 Sp  Sp+1 (13 .20) .
p=1
In the ground state all spins are parallel and Uo = 2NJS 2 ,
this corresponds to figure
14a . A possible excitation might consist in the flip of just one spin, like it is shown in
figure 14b . 'This perturbation yields a finite increase in energy of 8JS 2 . However, the temperature
dependence of several macroscopic properties like specific heat or magnetization
does not correspond to an exponential law, as it
has to be expected for a finite excitation
energy.
Spin waves (magnons) must have a much smaller energy than the single spin flip,
like phonons may have lower energy than an ionic vacancy for instance .
The distortion of the magnetic order corresponds to
a plane magnetic wave (with
propagation vector q and frequency w) and is drawn in Figure 14c .
Spins are precessing
around the direction of magnetic order (here z) with components
Sp  u  exp[i(p(ja  wt)] (13 .21),
1320
14 a15spinwave Magnon energy the , and reference drawing spins phonon precess of [5] adispersion simple corses 1a11111
ferromagnet curves (from reference in Fea) atground rooin [4]) state, temperature b) one lé'!~~~1'
spin and being two Qscans flipped at c)
41a11111
Figure
in
Schetnatic
:
.
.
Figure
constant
.
1321
n = v  cap[i(pga .  wt)] (13 .22),
where a, designates thé lattice constant and b is numbering thé spins .
Like in thé case of thé phonon dispersion one may deduce thé magnon relation .
In
case of a simple chain one yields
r~,w(q) = VS(1 cos(ga)) (13 .23),
which may be approximated for small q by hcw(q) = 2JS(ga) 2 , i .e . a quadratic relation .
In contrant an acoustic phonon dispersion is always linear in that qrange . Equation
(13 .23) may be extended to thé theredimensional case, in all cubic systems thé relation
hw(q) = 2JS(ga) 2 remains valid for small q .
Figure 15 shows thé magnon dispersion measured in Fe, from which one may obtain
thé exchange constant J ;
for comparison thé linear dispersion relation of thé LA branch
is added .
One may note, that in the case of Fe the magnon frequencies extend to higher
énergies than those of thé phonons .
Due to thé spécial form of thé résolution ellipsoid in
thé triple axis spectrometer, it is favorable to perform scann at constant energy revealing
both thé phonon and thé magnon, which exhibit approximately thé came intensities, see
right part of figure 15 .
Since magnons are bosons, their occupation is given by Bosestatistics like that of
thé phonons, équation (13 .11) .
Also for thé differential cross section one may deduce a
formula similar to équation (13 .10) valid for phonons
d2()
( )}
c~QdE'
(k'/k)  S  covst .  cap(2W(Q))F2(Q)(1 + Q2)
.
~Tq(n(w~) + 1/2 ± 1/2)  4(w + w j (q»  a(Q + q 1) (13 .24) .
One recognizes thé ternis for momentum and energy conservation as well as thé Bosefactor,
which is increased by one in case of magnon création .
Furthermore thé intensity is
modulated by thé same DebyeWaller factor as thé phonons . However, there is no terni
équivalent to thé dynamic structure factor, thé intensity is determined just by thé spin
S, thé form factor F(Q) and thé direction of thé momentum transfer .
1322
Ferromagnetic materials are still of considerable interest due to their enormous technical
potential in the context of data storage media .
Attempts to optiraize the technical
properties lead to binary or ternary compounds, where the complexity of the magnetic
order is considerably increased .
In all cases the study of the magnon dispersion given an
almost unique insight to the microscopic coupling terms .
13 .3 .2 Antiferromagnetic Excitations
Antiferromagnetic order results from a negative exchange constant J in U = 2J EP, S p 
SP+1 . The antiparallel alignment of neighboring spins however, leads to a
magnetic cell which is larger than the nuclear one . A classical example is given by the
antiferromagnetic order observed in MnO at 120 K (Shull et al . 1951) . Again one may
find excitations in an antiferromagnet, which have lower energy than the simple flip of a
single spin .
Again each spin deviates from the ordered position by a component given by
a plane wave .
'T'he calculation of the antiferromagnetic dispersion more closely resembles
that of the phonon case
4J S ) 2 (1  co .s 2 (q . a,))
w W , (q)  (
(q
MS Isira(q  a,)I (13 .25) .
In contrant to the ferromagnetically ordered structure and in close similarity to the
acoustic phonons, the frequency becomes linear in q for sufficiently small q . Figure 16
shows the magnon dispersion observed in RbMnF 3 .
In general both dispersion relations (13 .23) and (13 .25)
are not gaped, the magnon
energy vanishes for q approaching the zone conter, like in case of an acoustic phonon .
For
the acoustic phonon the zoneconter limit corresponds to an infinitely small translation of
the entire crystal which does not cost any energy, since no force constant is stretched .
In
case of the magnons the lirait corresponds to a rotation of the ordered moment, which in
the Heisenbergmodel does not involve any energy shift (the interaction depends only on
the relative orientation) .
However, in general this model is not sufficient, there are always
interactions faworing the orientation of a certain spin direction .
'These interactions yield
a finite gap in the excitation spectrum, however much smaller than the spin flip energy.
Antiferromagnetic materials have much less technical importance compared to ferromagnetism
.
However, antiferromagnetic corrélations in metallic systems are often essential
for thé understanding of thé electronic properties .
For instance thé physics of
hightempérature cuprate superconductors seems to be determined by thé closelyness of
1323
Y c
3
c
Cc
E
Figure 16 Magnon dispersion in RbMnF3 (from reference [4]) .
the antiferromagnetic order in the insulating parent compounds .
13 .3 .3 Crystal field excitations for rare earth ions
In the rare earth series one fieds unpaired electrons in the 4fshell, which are strongly
localized and therefore screened from the surrounding ions .
In consequence the total
momentum J remains a good quantum number .
For a free ion the the ground state
would be (2J + 1) times degenerate .
In a crystal this degeneraty is partially lifted due to
the  weak  Coulombfields of the surrounding ionic charges .
The transitions between
the single levels may be observed by inelastic neutron scattering .
(This is valid for the
crystal field splittings in transition metals too, but due to the larger overlap of the d
orbitals the excited levels in these compounds are usually to high in energy .)
earth ions are sufficiently diluted, interactions amongst them may be neglected .
If the rare
The level
frequencies show then no dispersion and may be studied with time of flight methods on a
polycristalline sample .
In figure 17 we show the observed spectrum compared to the crystal field scheme for
Pr13 3 . The levels of Pr 3+ with a J of 4 may split into not more than 9 levels . The local
symmetry of the site occupied by the ion in the lattice determines which levels may exist
with which multiplicity.
However, the symmetry cannot predict the sequence of the levels,
for this purpose one needs a quantitative information for the surrounding fields .
The single
levels are designated according to thé irreducible représentations of thé local symmetry
1324
; '
.
r,°'r,
Figure 17 Crystal field scheme and measured energy scans in PrB3 (T=1 .5 K), frorn reference [6] .
group by F i .
In close resemblance to equations (13 .10) and (13 .24) the differential cross
section arises from the sum of transition probabilities F i > F j ; these matrix elements
may be calculated within point charge models .
13.4 Conclusions
Inelastic neutron scattering is almost the unique technique to observe lattice vibrations
and magnetic excitations throughout the whole Brillouinzone .
The main part of our
knowledge on these topics has indeed been achieved by neutron studies .
Also the subjects of present interest, like highT, superconductors, heavy fermions,
quasicrystals,
C60 and compounds with colossal magnetoresistivity demand a detailed
analysis of their lattice dynamics as well as of their magnetism .
Frequently the materials
of current interest exhibit a large complexity ;
therefore their study requires a continuons
development of the experimental facilities as well as of the analysis methods .
References
1 N .W . Ashcroft and N.D . Mermin, Solid State Physics, HoltSaunders International
Editions, Philadelphia (1976) .
1325
.
.
2 H . Bilz and W . Kress, Phonon Dispersion Relations in Insulators, Springer Verlag,
Berlin Heidelberg NewYork (1979) .
3 M .T . Dove, Introduction to Lattice Dynamics, Cambridge University Press, Cambridge
(1993) .
4 C . Kittel, Einführung in die Festkörperphysik, R . Oldenbourg Verlag, München (1983) .
5 G . Shirane, V .J . Minkiewiecz and R . Nathans, Journal of Appl Physics 39, 3833
(1968) .
6 A . Furrer, Magnetic Neutron Scattering, World Scientific, Singapore (1995) .
further suggestions
P . Briiesch, Phonons : Theory and Experiments I, Il, III, Springer Verlag, Berlin Heidelberg
NewYork (1982) .
LandoltBörnstein Band 13, Metalle, Phononenzustände, Elektronenustände and Fermiflächen,
Springer Verlag, Berlin Heidelberg NewYork (1981) .
E Balcar and S .W. Lovesey, Theory of Magnetic Neutron and Photon Scattering, Oxford
Science Publications, Clarendon Press, Oxford (1989) .
G.L . Squires, Thermal Neutron Scattering, Cambridge University Press, Cambridge
(1978) .
14
Soft Matter :
Structure
Dietmar Schwahn
14 . Soft Matter : Structure
Dietmar Schwahn
14.1 . Introduction
The methods of small angle scattering (SAS) wich neutrons and Xrays are broadly used for
investigations ofmesoscopic structures in condensed materials . Whenever, atomic density or
chemical composition inhomogeneities of mesoscopic length scale exist in a sample, this
method can in principle be applied . SAS is a complimentary method to transmission electron
microscopy (TEM) ; TEM makes visible the microstructure in real space while the SAS
methods measure in reciprocal space and give quantitative data averaged over macroscopic
large volumes .
In this lecture the theoretical basis of small angle scattering with neutrons (SANS)
should be developed for the topic of the physics of polymers or, as it is said today, of "soft"
matter und should be clarified with simple experimental examples. Since the end of 1939 the
method of SAS was mainly developed by Guinier and Kratky and applied for questions in
metal physics . In one of Guinier's first experiments scattering from copper precipitates in
aluminum was correctly interpreted and the precipitates were identified as the origin of
hardening in socalled Duralumin . This type of precipitation are socalled GuinierPreston
zones ; they are still subject of active research. Today, neutron small angle scattering
technique is mainly used for soft matter; the main reason might be the relatively simple
possibilities of contrast variation using hydrogen and deuterium, which scatter neutrons quite
differently but do not change the chemistry ofthe polymer .
14.2 . Diffraction ofNeutrons at 3Dimensional Particles
In this part the basic equations of small angle scattering are discussed . For qualitatively
understanding in Figure 14 .1 two neutron pencils of rays are depicted in two spheres of
différent size. From this figure it becomes clear that diffraction from thé langer sphere occurs
into smaller angles and therefore smaller scattering vectors Q . The basic equation of small
angle scattering is given in Eq .(14 .1) .
dY (Q) 
1
L~ bi ez
V~,
dS2 
(14 .1)
141
with the macroscopic scattering crosssection dl/M in units of [cml ], the sample volume
V, the number N of atoms in the sample and the coherent scattering length b; ofthe atom i at
the position r i . One can consider the resultant diffraction pattern as a coherent superposition
of spherecal waves, emanating from single atoms with an amplitude determined by the
Fia .
14 .1 : Two pencils ofrays ofthe scatteringprobe in two particles of different size
coherent scattering length . In the region of small angle scattering the relation Q < 27c / a is
always fulfilled with the lattice constant a.
according to
e I
_>
length density p(r) =p and volume V . From Eq.(14 .2) one gets
Then the sum in Eq.(14 .1) can be approximated
Jd3rPUe
r
; QI
_
by an integral of the coherent scattering length density p(r) = b ; / S2 (atomic volume S2) and
the phase factor . In this approximation one get the basic relationshipfor SANS :
dl LQ)=
V
~Q_ z
d3r pr~e 
(14 .2)
In a ferst example we consider an homogeneous sample wich the constant coherent scattering
_d~ =F2 fd je'
M V ~ ~
3
L=(27c)s PZ g(Q)
V
Samples or apertures in front of the Sample are typically of cm size . Diffraction at those large
heterogeneities occurs within angles which are too Small to bc resolved ; such diffraction can
be approximated by a Delta fonction . Diffraction caused by the mean coherent scattering
142
length density of a sample against vacuum occurs in the 1/cm Q region and is usually
subtracted from the crosssection. So, one gets the expression for the crosssection according
to :
z
LLQ) = V
~,d,r (p(r) _ P)e'2' (14 .3)
This form of the scattering crosssection £i . is the starting equation for the analysis of
micellar structures, which we will not discuss in this lecture .
14.3 . Theory of Small Angle Scattering from linear Polymers
We now consider the main features of diffraction from linear polymer chains .
14.3 .1 Diffraction from a linear homo polymer
As a model of a linear chain one considers a polygon of z vectors r,, whose directions are
statistically independent. Such a polygon of a freely joint chain is depicted in Figure 14 .2 .
Figure 14.2 : Model ofafreely joint linear chain
Each vector r, represerts a moromer, which the chemical unit of a polymer of segment length
b . Such a chair can also be represented by another polygon with larger vectors r ; representing
several monomers . Both polygons correctly represent the global properties of the chain as the
endtoend vector R, which is evaluated from the sum of all vectors according to
143
The probability that a freely joint chain with z monomers talçes a conformation with the endtoend
vector R, is determined by the Gaussian distribution according to
3/2 2
W R,z 
3 ex  3R (14 .5)
(2Tczb2) pC 2zb 2 )
On the statistical average the mean endtoend distance is zero and its
is linear proportional to the number of monomers z .
=0 =R~=b 2 z
mean square deviation
The radius of gyration is given as R 2 = R2 /6 . A linear "real" chain is different from a freely
joint chain in so far as neighboring monomers are correlated. This effect is considered by the
parameter c z in Rg = c z b 2z/6 or expressed by the statistical segment length according to
a =bF and the radius of gyration Rg =a2 z / 6 or respectively the mean square endtoend
distance R,2, =62 z determined from scattering experiments . So, a statistical segment
length of polystyrene is determined as 6Ps = 6.8A. As in Figure 14 .2 a realistic chains can
therefore be represented by a polygon with vectors of segment length a .
The form factor of a linear chain measured in a SANS experiment is determined from the
sum of the phase factors from the monomers and an averaging over all possible chain
configurations according to
D
z
p(Q ) =
z2 Y,< e iQR i _ R i) >
(14 .6)
The meaning of the vectors R becomes clear from Figure 14 .2 . In a macroscopically large
sample the number of polymers is sufficiently large, in order to describe the polymer
conformation with the probability distribution of Eq .(14 .5) . The average value of the phase
factors between the positions i and j within the chain is calculated according to
< expiQR;j >= fd 3 R ;jw(R ij Ji  jl)exp(l2llij )= WJ(Q )
For the form factor one gets
Wij(Q) = exp(li jl 62
Q2) = Wa lljl .
144
2
P(Q) = 1 ~exp(Ii  j'6 Q2 ) (14 .7)
z ;;
and alter some calculation one gets the well known Debye formula
with x = R g
2 Q 2 .
PDebye(Db) (Q) 2[x  1 + exp(x) ] (14 .8)
x
In Figure14 .3 the form factor according to Debye's formula has been plotted.
0.8
a
0.6
0.4
0.2
0.0
0 2 4 6 8 10
x = (RgQ)2
Figure 14.3 : Debyeformfactor ofa linear chain
The Symbol beside Eq .(14 .6) represents the form factor of a linear chain determined
exclusively by intramolecular phase factors . Such symbols should help to make transparent
the meaning of scattering laws ofmore complex polymers .
There are expressions for the form factor in Eq.(14 .6) being approximately valid in the
regions of small and large scattering vector if compared with the inverse size of the polymer ;
they have a much simpler form and can easily be used for the analysis of the scattering data.
So in the region of small Q, e.g . Q« 1/Rg one finds
PDb 13 Rg Q2 or the Zimm approximation : Ppb 1 + 3Rg Q2 (14.9)
as depicted in Figure 14 .4a. From this plot one gets the radius ofgyration and the scattering in
forward direction according to Eq .(14 .9), delivering the polymer molar volume and volume
145
2.5
2.0
0.0 0.5 1 .0 1 .5 2.0 2.5 3.0
Figure 14 .4a : Socalled Zimm representation : Within the Zimm approximation the plot of 1/P
versus QZ gives a straight for the Debye form factor. The slope of the straight line is
proportional to R g .
0.5
Kratkyauftragung
0.0 0 2 4 6 8 10
RQ
Figure 14 .4b : "Kratky plot" of Debye's form factor :At large Q the representation of
Qz . p(Q) versus Q gives a constant value.
14 6
fraction. In the region of large Q one gets the expression for Q»1/Rg
PDb 2/(QR g ) Z (14 .10)
and according to the representation in Figure14 .4b a power law or scaling law with a slope of
2 . The scaling law in Eq.(14 .10) shows a socalled fractal dimensionality D=2 .
14.3 .2 . Polymer melts
We now consider a melt consisting of n linear polymers within a sample volume VS . The
polymers are of the saure type and consist of z monomers wich the coherent scattering length
b . In the Sample there are in total N = n  z monomers . The scattering cross section is derived
from Eq . (14 .1) and averaged over all conformations according to
___t<
d~ ~~Q_
dÇ2 Vs Vs ;;
~QÉj
Z>=b2Y (14 .11)
Now, Eq .(14 .11) can be splitted into an intramolecular and intermolecular interference terras
P(Q) und W(Q) according to
_dY __b z
A2 Vs ny < e'Q > +n(n1)y< e'Qr' >
~~ ?i
Z2 P(Q)
~W(Q)
and
~(Q)  V
Nz [ P(Q) +nW (Q)~
A
with the coherent scattering length density p = b/S2, molar volume V, the Avogadro number
NA and the molar volume S2 of the monomers . The conesponding symbol for inter molecular
interference is the following
H
147
Equations (14 .12) and (14 .13) are determined by infra und intermolecular interferences as
also made visible by the accompanying symbol.
14 .3 .3 . Babinet Principal
Incompressible melts show no thermal density fluctuations and therefore no diffraction can
occur in such a single type polymer melt . The scattering cross section must be zero and
following Eq. (14 .13) one therefore gets the following relationship
P(Q)= nW(Q)
b
H
representing the Babinet principal .
14 .3 .4. Melt of deuferated and protonated polymers with chemically identical monomers
ofsame segment length .
We now discuss a blend of chemically identical polymers whose components are either
protonated or deuferated . For further theoretical consideration we introduce an occupation
operator a ; with the following meaning
1 b ; =b p
0 b ; = b
The operator is 6 ; =1 and 6 ; =0, ifthe monomer at the position i is deuterated and protonated,
respectively . The coherent scattering length of a monomer at the position i is then described
as
b i =a; (b, bH)+bH=6;'Ob+b, (14 .16)
This expression inserted into Eq .(14 .1) gives
and fmally
N
aL 1 7QP' N iQr 2
d22(Q)V
s a=1 t=1 _
=s(Q)
148
with the partial structure factor SDD . The symbol for SDD bas the following form
D
D
and describes thé intra and intermolecular interférences between thé deuterated monomers .
Quite generally, thé scattering cross section can be described as a sum of thépartial structure
factors according to
with the conesponding symbols
dS2 (Q)= V LbDSDD +2b DbHSDH +bHSHH J (14 .19)
s
D D H D H H
D
In case of an incompressible melt thé partial structure factors are related according to
SDD  SHH
SDH
and thus one gets in correspondence wich Eq .(14 .18)
z
U2 (Q) = Ab
Vs SDD' (14 .21)
The defmition of thé occupation operators in Eq.(14.15) implicitly contains thé condition of
incompressibility, as no free volume is included. The partial structure factor ofthé deuterated
monomers is given
SDD =I)nZ Z P(Q)+q) 2 n 2 ZZ W(Q) (14 .22)
with volume fraction d) of thé polymer component D. Because of thé Babinet principal one
has z P(Q) =  nW and one gets
(14 .20)
149
`l
~(Q) ,"o (D(1d)VP(Q)
dn NA  ~
(14 .23)
with the structure factor
S (Q) = ~D (1 ~D )V P°b (Q) .
(14 .24)
So, the variation of contrast of chemically identical polymers enables the experimental
determination ofthe form factor of a single chain in a melt of chemically identical polymers .
In Figure 14 .5 an experimental example is shown for a polystyrene melt.
Figurel4j : Structure factor of a 50% mixture of polystyrene in double logarithmic
representation . Thepower law behavior at large is described by statistical chain
14 .4 . HD Polymer blend in solution
Next we derive the scattering law of an isotopic polymer blend in solution .
introduce occupation operators with the meaning
a (r ; )=
1 b ; =b °
10 b ; =b oderb
1 b ; = b
0 b ; = b ° oder b
Again we
(14 .25)
1440
and which lead to the scattering cross section
dE _ 1 N
d~( Q ) Y~b V
DaD(rn)+bHaH
(rn)+b0(1aD(rn)_  6H(rn)))e'Q'~ >
s 1
which after some calculation leads to the form
z
according to.
The partial structure factors are given as :
(bD  bo ~TD(rr)+(bx  bo)6x(Ei)+ b, o, e iQr; 2 > (14.26)
0
and, fmally, to a sum of partial structure factors weighted with conesponding contrast factors
d~(Q)=V [4bDS DD +24bD4b .S DH +4bHS 1 (14.27)
5
D(H) D(H)
D D
SDD = (PnZ ZP(Q)+ (1) Zn2 Z Z W(Q) (14.28)
SHH =(1 ~D )nZZP(Q)+
~D Zn2ZZW(Q) (14.29)
H
S De = (D(1  (D~2Z2 W(Q) (14.30)
H D
and fmally one delivers the following scattering law
dl(Q)= V
~bDbH) Z q)(1d)nZ Z P(Q)+(br oiy b [ o)Z nZ Z P(Q)+n 2 Z Z W(Q) ] } (14.31)
5
For this systems the Babinet principal is not valid as it contains polymers and solvent
molecules . If one matches the scattering length of the solvents and the averaged one of the
polymers (broiy =d)bD +( 1 ~)bH) according to broiy =b o (,,zero" contrast), the second term
in Eq .(14 .31) does not contribute to the scattering and, consequently, one again determines
the form factor of a single chain according to
(Q) = c 1)(11) VP(Q)K (14.32)
ddY
144 1
with c the volume fraction of polymers in solution and the contrast factor K . This again is a
demonstration of the possibilities of contrast variation with neutrons allowing to measure the
form factor P(Q) of a polymer chain in solution .
14 .5 Scattering from a Block Copolymer
Figure 14 .6 :
Presentation ofa Diblock Copolymer
We now derive the scattering law of a linear polymer, consisting of the two
blocks A" and
B" of different polymers and which are
symmetric with respect to the
number of the
monomers z = 2z D = 2z H .
The scattering cross section is given as
_dl __ 1 Ab2SDD
dn Vs
(14 .33)
with the relationship SDD = SHH = SDH because of assuming an
incompressible melt.
The
various partial structure factors are given as :
r 1 2 7Z ,2
z
SDD =n PDD +n2~2 WDD (14 .34)
(2,
)
2
z \2 2 z
II
DH PDH +n
nC2/ ~2j
,WDH (14 .35)
SI,
=nCzJ 2
2 2
P,, +n2(ZJ 2
WH (14 .36)
The symbolic representation of the structure factor of diblock copolymers has the form
144 2
For the intramolecular and intermolecular terms of interference one has PDD = PHH and
WT = WDD = WAH = W,, .
the total chain is given as
Because of z ZPT = 2 (z / 2)Z PDD + 2 (z / 2)Z PDH the form factor of
2PT = PDD +PDH (14 .37)
which wich nWT =PT (Babinet principal) fmally leads to thé partial structure factor
z
[PDD  PT1
(14 .38)
and thé scattering cross section
dl(Q)=K 4
[PDD (Q) PT (Q)1' (14 .39)
described as thé différence of thé intramolecular form factor of a single block ( PDD ; PDH )
and
thé total chain (PT ).
These form factors of a symmetrical diblock copolymer are plotted in
Figure14 .7. An interférence peak is observed whose position is according to Q * R g =1 .9
related to thé radius of gyration and Q* therefore has to be observed at 1 .9 . 10 Z A  ' . The
observation of an interférence peak in diblock copolymers becomes plausible from thé
consideration, that composition fluctuations of thé blocks A and B can only occur on thé
length scale of thé polymer . As an experimental example we show thé structure factor of a
melt .
0 .8
0 .4
Diblockcopolymer
0 .20
0 .15
0 .4
xg100A
[/ 1
0 .8
â 0 .10
â
0 .00
0 .00 0 .02 0 .04 0.06 0.08 0 .10 0.00 0 .02 0 .04 0 .06 0.08 0.10
Q[A
0 .05
Q[,A ']
Figure 14.7 : Form factor ofa symmetrical diblock copolymer
1443
3 .0
ô 2 .5
U
2 .0
O
1 .5
a
1 .0
0 .5
PEPPDMS
T=170°C;P=1365 bar
0 .0 0 2 4 6 8 10
Q [102X1]
Figure 14 .8 :
Structurfactor ofa PEPPDMS diblock copolymer
14 .6 . Binary Melt with different Polymers
The structure factor of an ideal binary melt is evaluated within the "random phase"
approximation (RPA) according to
\'_ 1 1
S D , (Q/
(14 .40)
~VDPDb(Q)+(11»VHPDb(Q)
The inverse structure factor is obtained from the sum of the inverse form factors of both
ideal" chains weighted with their molar volumes and volume fractions . Eq . (14 .40)
corresponds to an ideal solution of two components with mixing energy being zero and
therefore no phase transition phenomena . Those ideal solution are usually not found in reality ;
as demonstrated in Figure14.9 even isotopic mixtures of chemically identical polymers show
phase decomposition at low temperatures because of a small but finite mixing interaction
energy . For polymer blends such interaction is described by the FlolyHuggins (FH)
parameter
rh  rcr .
The FHparameter bas the meaning of a
free enthalpy of mixing with the enthapy and
entropie terras hh
and F'6 , respectively . In the RPA approximation the interaction parameter
added accordingto
S' (Q) = S o ' (Q) 2F (14 .42)
1444
500
450
400
U
0
;, 350
42,
300
s~.
250
200
dPs/ps
VN 1 .42106cni /mo
  
Binodal
Spinodal
150
0.0 0.2 0.4 0.6 0.8 0.0 0.5 1.0 1 .5 2.0 2.5
Composition
1 [l0~mol/cmb]
Figure 14 .9 : Phase diagram and FloryHuggins interaction parameter ofan isotopic dPS/PS
blend
the structure factor of an ideal mixture . For small Q Eq. (14 .42) can be approximated in Zimm
approximation according to
S' (Q)= S'(0)+AQ2 (14 .43)
wich the inverse structure factor S '(0) = 2[FS  F] at Q=0 and the FHparameter at the
spinodal temperature, 2F, = + , being inversely proportional to both chain
VD
(1 1»Vx
molar volumes and being related to the translatorial entropy of mixing . In experimental
reality one tries to measure at sufficiently small Q in order to be able to use Eq .(14 .43) for
analysis of the scattering data . As shown in Figure 14 .9, the spinodal temperature represents
the phase boundaiy between the metastable und unstable twophase regions and the unstable
region touches the stable onephase region at the critical point .
phase at high temperatures the FHparameter is
In the single homogeneous
smaller than F, = 2 / V in accordance with
the Gibbs condition of stability of a positive S(0) ; S(0) represents a susceptibility which
according to the fluctuationdissipation theorem is related with the free enthalpy of mixing
AG according to
7 2 (AG/RT)
aq) 2
(14 .44)
In case of F > F, the System decomposes with the mechanism of spinodal decomposition in
two macroscopically large phases which one polymer component dominating . The free
enthalpy of mixing of polymer blends was originally formulated within the
approximation by Flory and Huggins, it gives the saure result as the randomphase
mean field
1445
6
Û
ô 4
3 .0
2 .5
; 0 1 .5
0 .0
0 .0 0 .3 0 .6 0 .9 1 .2 1 .5 2 .32 2 .33 2 .34 2 .35 2 .36
Qz [10
4 X
2 ]
1/T [10'/I,]
Figure 14.10a : Structurefactor S Q) in Zimm representation ofa critical mixture dPS/PVME
polymer blend at various temperatures.
Figurel4.10b : S '(0) plotted versus IIT. The solid lines describe the critical behavior ofthe
thermal composition fluctuations. Near the critical temperature one observes deviationsfrom
the mean field behavior. The spinodal and critical temperatures are determined frorn the
extrapolation S  '(0) =0; S  '(0) =0 means an infinite susceptibily.
approximation being a mean field approximation as well . According to RPA the slope A in
E«14 .43) is related to the square of the radius of gyration of both chains assumed as being
undisturbed .
Next we discuss an experimental example of a binary blend of a deuterated polystyrene (d
PS) und polyvinylmethylether (PVME) . This mixture shows the specialty being miscible at
low temperatures and decomposes in two macroscopic phases at high temperatures .
reasons are a prefen ed interaction between PS und PVME (Fh < 0) and an increase of the
total free volume during decomposition (n < 0 ) . The free volume is related with the entropy
F. and in case of F, > F c becomes dominant and the driving force for the process of
decomposition at high temperatures .
0 .5
The
The SANS experiments were exclusively performed
within the homogeneous one phase region . In Figure 14.10 S(Q) is plotted in Zimm
representation (a) and l/S(0) versus 1/T in (b) . One clearly realizes the increasing scattering at
higher temperatures (the inverse S(Q) is of course decreasing), from which one can conclude
to stronger thermal composition fluctuations . The inverse susceptibility is linearly
proportional to 1/T, it is zero at the spinodal respectively at the critical point, and its slope
directly gives Fh . The observed linear shape of S '(0) with 1/T is representative for the
144 6
scaling behavior of the susceptibility within the universality class of mean field
approximation (the corresponding critical exponent is y =1) .
This experiment follows the mean field approximation quite well and can be sufficiently
well interpreted with the theoretical approach presented here . The reason is the relatively
large molar volume of several 10' cm' /mol, which allows observations of deviation from the
mean field approximation only very near (about 1K) the critical temperature, when the
thermal composition fluctuations are sufficiently large.
References
Text books :
[1] A. Guinier und G . Fournet, Small angle scattering ofXrays . Wiley, New York
(1956)
[2] A. Guinier, Chapter 10 in Xray diffraction . W.H. Freeman & Company, San
Francisco (1963)
[3] O. Glatter and O . Kratky (ed .), Small angle scattering. Academic Press (1982)
[4] J.S . Higgins and H.C . Benoit, Polymers and neutron scattering . Clarendon
Press, Oxford (1994)
Review articles :
[5] P.G. de Gennes, Scaling concepts inpolymerphysics. Comell University Press,
New York (1979)
[6] K. Binder, Advances in Polymer Science 112, 181 (1994)
[7] F .S . Bates, G.H. Fredrickson, Ann. Rev . Phys. Chem . 41, 525 (1990)
[8] G. Wignall : Neutron Scattering in Encyclopedia of Polymer Sciences and
Engineering 10 (1987) 112
[9] Dietmar Schwahn and Kell Mortensen: Thermal Composition Fluctuations in
Polymer Blends Studied with Small Angle Neutron Scattering, Chapter 8 in
Scattering in Polymeric and Colloidal Systems, eds . W . Brown and K .
Mortensen, Gordon and Breach Publishers (2000)
Articles :
[10] D. Schwahn, K . Mortensen, H. YeeMadeira, Phys . Rev . Lett . 58, 1544 (l987)
1447
[11] D . Schwahn, K . Mortensen, T. Springer, H. YeeMadeira, R. Thomas J . Chem .
Phys . 87, 6078 (1987)
[12] D . Schwahn, S . Janßen, T . Springer, J. Chem. Phys . 97, 8775 (1992)
[13] D . Schwahn, G . Meier, K . Mortensen and S . Janßen, J . Phys.11(France) 4, 837
(1994)
[14] D . Schwahn, H. Frielinghaus, K . Mortensen, and K. Almdal, Phys . Rev . Lett.
77, 3153 (1996) ;
[15] H . Frielinghaus, D . Schwahn, K . Mortensen, K. Almdal, T. Springer,
Macromolecules 29, 3263 (1996)
[16] L . Leibler, Macromolecules 13, 1602 (1980)
15
Polymer Dynamics
Dieter Richter
15 . Polymer Dynamics
D. Richter
15.1 Introduction
In our every day life plastics or polymers play a very important role . Polymeric materials are
used, because they are durable, cheaply to produce, easily to process and because they exhibit
very versatile and favorable mechanical properties, e .g . depending on temperature or time the
same polymer may be viscose, rubber elastic, very tough with high impact strength or even
brittle . In the simplest case polymers are long linear chain molecules, build from one
repeating unit, the monomer ; such polymers are called linear homopolymers .
Since in gerreral rotational isomers may be easily formed at each bond of the chain backbone,
long chain polymers possess a very large number of irrternal degrees of freedora which
contribute importantly to the entropic part of the molecules free energy . At length scales
somewhat larger than the size of the monomer, the detailed chemical structure of the chain
building blocks ceases to be of importance and very general properties determined by the
statistical mechanics of the chains prevail, e .g . the conformational entropy follows from the
number of possible arrangements of a chain sequence in space . According to the central lirait
theorem the most probable arrangement is that of a Gaussian coil, e .g . the polymer chain
performs a rarrdom walk in space . If pieces of the chain are now stretched an errtropic force
arises and acts on these stretched segments endeavouring to restore them to the most probable
contorted state . Such forces are the basis ofrubber elasticity .
This lecture aims to identify general principles of chain motion on a molecular scale which
underlie the macroscopic mechanical properties, and presents concepts and experimental
results on these motional mechanisms in space and time . Thereby, we restrict ourselves to
melts ofhoraopolymers .
Neutron scattering with its space time sensitivity on a molecular and atomic scale unravels the
details of the molecular motions in question . Commencing at the scale of the single bond,
where movements take place at a pace as in normal liquids, quasielastic neutron scattering
(QENS) provides insight into local relaxation processes . At longer length scales first the
entropy driven Rouse motion and at even larger distances the effect of entanglement
151
constraints due to the mutual interpenetration ofchains comes into the observation range. The
most powerful technique suitable for these investigations, the neutron spin echo spectroscopy
(NSE) operates in the time domain and uncovers a time range from about 2ps to 200ns and
accesses momentum transfers between 0.0lÂ 1 and 3A 1 . The second important high
resolution technique is neutron backscattering providing an energy resolution of about 1 ~ueV
and covering a Qrange 0.1
is the KohlrauschWilliamWatts relaxation time and ß < 1 the stretching exponent .
in good approximation follows a VogelFulcher temperature dependence .
(T) ~~ exp
A
T To
(15 .2)
The temperature offset in the denominator of the exponent leads to a divergence of i
To, a temperature below Tg which, however, may never be reached in equilibrium.
15
Boson peak
10
rast
5
~s~av
0,
0
0
a
3 4 5 6 7
1000K/T
Figure 15 .1 : Relaxation landscape of PB . u and ßsio, correspond to the classical relaxation
processes and are treated here .
The dielectric ßrelaxation is considered to be a result of a partial reorientation of the
molecular dipoles in the substance .
It is interpreted as a local activated process, where the
dipole hops between two positions separated by an activation energy E .
The relaxation time
follows an Arrhenius behaviour
153
(15 .3)
T ß ( E)=T ô exp
E
k,T
 (E )21
g ( E)  exp  EO (15 .4)
due to the disorder in the material the activation energies E are distributed around an average
value Eo . For the distribution function in general a Gaussian is assumed .
Empirically it is found that the width a(T) decreases with increasing temperature . Though
such processes have been investigated well by spectroscopic techniques, their molecular
origin is still unclear . Here QENS with its ability to provide space time resolution on the
proper scales contributes to a further exploration of the molecular mechanisms behind these
relaxations .
15 .2 .1 Dynamic structure factors
We commence with the derivation of the dynamic structure factor for the ßprocess which we
consider as a hopping process between two adjacent sites . For such a process the self
conelation function has been derived in the lecture on quasielastic scattering, it is given by a
sum of two contributions .
sm (Qd)
1+
Qd
+ 2
Cl
s
QQd)J
expC
T2E)J
(15 .5)
Sel
Sine?
Here d is the distance between the two sites and T(E) is the jump time conesponding to an
activation energy E . The complete scattering function is obtained in averaging Eq .[15 .5] with
the barrier distribution function g(E) obtained e .g . by dielectric spectroscopy. The Q
dependence of the two contributions to Eq .[15 .5] is displayed in Fig .15 .2 as a function of
Q(d = 1.5A) . From the oscillation of bottr contributions with Q the jump distance may be
obtained . The associated time scale may be found from the time decay ofthe inelastic part .
154
Figure 15 .2 :
Elastic and inelastic contribution to the incoherent scattering function for jump
motion between two site . The Figure assumes a jump distance of 1.5Â .
The associated pair conelation function is more difficult to obtain, since now we have to deal
with a change of configurations of atoms rather than with single atom jumps . The conceptual
différence between the pair and the self correlation fonction for jump processes may bc
visualized most easily considering rotational jumps . Let us regard e.g . the 120° rotational
jumps of a methyl group around its symmetry axis. An incoherent study would reveal the
atomic jumps ofthe associated hydrogens. The pair correlation function reflects the change of
atomic configurations before and after the jump . Since a 120° jump does not change the
configuration, a coherent scattering experiment would not reveal anything .
Back to the pair conelation fonction for the ßprocess, where we will introduce a simple
approximation . We know that for t = 0 the pair conelation function is reflected by the static
structure factor S(Q) . Therefore for t = 0 the corresponding pair conelation fonction for the ß
process must reveal SQ . We now assume that the inelastic scattering is related to
uncorrelated jumps of thé différent atoms . Then all interférences for thé inelastic process are
destructive and thé inelastic foret factor should be idenfcal to that of thé self conelation
fonction. For thé normalized dynamic structure factor for thé ßprocess we arrive at
S(Q,t) ß  S(Q) Slnel (Q) + Sinel ( Q ) e 2t/ti(E)\
S l (Q)  (Q) S« )
g (E)
(15 .6)
155
This incoherent approximation does not reveal e .g . symmetry related cancellations, but
displays a major feature of the corresponding dynamic structure factor, namely the relative
suppression of the inelastic contributions from local jump processes at the maximum of the
structure factor . Fig .15 .3 displays the situation for polybutadiene . There a ßprocess
corresponding to a jump length of d = 1 .5Â has been found . The corresponding inelastic
dynamic structure factor is strongly reduced at the position of the flrst peak, while it
contributes strongly at higher Q. Fig .15 .3 suggests a Q selectivity for thé différent relaxation
processes : at thé structure factor maximum local jump processes should not contribute and thé
relaxation due to flow should dominate . On thé other hand at larger Q, in particular in thé
minimum ofthé structure factor, thé secondary relaxation should reveal itself.
0 .5
0
Figure 15 .3 : Static structure factor S(Q) and normalized inelastic contribution S" to
S(Q)
S(Q,ca)IS(Q) for PB .
We now assume that thé a and thé ßrelaxation are statistically independent. Then, in real
space thé joint correlation function is given by a convolution of thé corresponding functions
for both separated processes . In Qspace this convolution becomes a product and we may
write thé total scattering function as a product of thé structure factor due to thé a and ß
processes .
156
S (Q, t) = Sa (Q, t) S ß (Q, t) / S (Q)
S (Q)
(15 .7)
The approximation behind Eq .[15 .7] is called Vinyard approximation and approximates the
proper pair correlation fonction by its self counter part . The self correlation fonction for a
diffusive process relates directly to the mean square displacement .
2
Sse(f (Q,t) = exp 12
(r2
(t)"
(15 .8)
where (r 2(t» is the mean square displacement of the flowing particle . According to
Eq .[15 .1] this should be described by a stretched exponential with the consequence
(r2 (t)> =D tß
and
=QZ1aD, lp
(15 .9)
the combination of Eq .[15 .8] and [15 .9] invokes sublinear diffusion of the polymer segments
as the underlying reason for the stretched exponential behaviour . Its signature is a power law
dependence ofthe KohlrauschWilliamWatts relaxation times T.,,, with an exponent 2/ß .
15.2 .2 Experimental results
15.2 .2 .1 Self correlation function
We commence with the secondaiy relaxation taking polyisobutylene as an example. Fig . 15 .4
presents the relaxation map of PIB . The solid line corresponds to the dielectric ßrelaxation,
the dashed line named S represerrts NMR results interpreted as a methyl group rotation. y and
y' are theoretically predicted relaxation mechanisms . In the dynamic regime, where the (Xrelaxation
is too slow to contribute, neutron backscattering has been employed, in order to
unravel details of the ßprocess in this polymer. Fig .15 .5 presents as an example a spectrom
taken at T = 270K and Q = 1 .7Â1 . The spectrum is characterized by a narrow peak, which
nearly coincides with the instrumental resolution function (dashed line) and a broad foot
revealing the relaxational behaviour. Such a spectral shape is typical for broad distributions of
relaxation times, where only a part of it is resolved in the spectrum .
157
10
an
0 2
0
Figure 15.4 : Relaxation map for PIB .
Y marks the atrace, " relates to
dielectric relaxation experiments on
the firelaxation, " results from
QENSexperiments .
3 4 5 6 7 8
1000 / T(K)
210'
â
Figure 15 .5 : Backscattering spectrum
from PIB at 270K at a Qvalue
Q = 1 .7A. The dashed line gives the
resolution function, while the solid
line displays the fit with the model
(sec text) .
0 10
5 0 5 10
E( ~teV)
w
0 .9
0 .8
N
a 0 .7
0 .6
Figure 15 .6 : EISF for PIB (1 : 250K,
" : 270K) . Solid lines : EISF for
methylgroup rotation, dashed lines :
fit result for a jump distance
d = 2.7A.
0 .5
0 0.5 1 1 .5 2
Q (À 1 )
158
Fig .15 .6 displays the elastic intensity observed for PIB as a function of Q . The data were
corrected for multiple scattering and fitted with Eq .[15 .5] . This elastic incoherent structure
factor (EISF) (see lecture Quasielastic Scattering) reveals a jump distance d = 2.7A . For
comparison the solid lines display the prediction for methyl group rotation, which was
invoked by NMR spectroscopy . Obviously the neutron data point into the direction ofa larger
motional amplitude .
The squares in Fig . 15 .4 display the neutron results for the /3 time scale . Within a factor of 2
they agree with the dielectric spectroscopy results . Since the underlying process has an
amplitude of 2.7A and is also dielectrically active, it cannot be understood as due to a
methylgroup rotation alone . A possible interpretation is a combined backbone and methyl
motion which is also supported by simulation results .
We now turn to the arelaxation and ask, whether the sub linear diffusion argument is
supported by quasielastic neutron scattering. Fig. 15 .7 displays KohlrauschWilliamWatts
relaxation rates obtained for four different polymers, polyvinylether (PVE) at 340K,
polyisobutylene (PIB) at 365K, polybutadiene (PB) at 280K and polyisoprene (PI) at 340K.
PVE
40K
u
0.2 0 .4 0.6 0 .8 1 pI
340K
Figure 15 .7 : (zrWW)f for 4 different polymers as a function of Q. The solid lines display a
Q' power law .
159
In order to test Eq .[15 .9] the relaxation rates have been exponentiated with the exponent /3,
obtained from the stretching of the relaxation fonctions in these polymers in dielectric
spectroscopy . According to Eq.[15 .9], z,6 should bc proportional to Q"' . The solid lines in
Fig .15 .7 display this power law relation . As may be seen, in all cases within experimental
error the experimental relaxation times again obtained by backscattering spectroscopy follow
the predicted power law behaviour . Thus, the experimental evidence supports a sub linear
diffusion process as underlying the arelaxation . We remark that this result is in disagreement
wich assertions that the stretchnd exponential relaxation fonction of the aprocess originates
from heterogeneous motional processes, where polymer segments in different parts of the
sample would relax at different relaxation rates .
15 .2 .3 Pair correlation function
The dynamic pair correlation fonction for polymer relaxation has been studied thoroughly on
polybutadiene as a fonction of temperature and momentum transfer . Fig . 15 .8 gives a synopsis
of these results . The dynamic data presented have been taken at the positions of the first and
second peaks in the static structure factor of this polymer . As may be seen from the middle
part of Fig .15 .8 the first peak of the static structure factor moves strongly with temperature .
This peak originates from interchain correlations, where weak v . d. Waals interactions lead to
thermal expansion. The second peak relates mainly to intrachain correlations as may be seen
from the temperature independence of its position indicative for covalent bonds . The
temperature dependent relaxation spectra were rescaled in their time dependence wich the
characteristic time for viscosity relaxation z, (actually the time dependent monomeric friction
coefficient was used, see next paragraph) . By this procedure the time correlation functions at
the first peak assemble to a master culve, showing that the dynamics at the interchain distance
follows the saine relaxational behaviour as the macroscopic flow . On the other hand as
evidenced by the lower part of Fig. 15 .8 at the second structure peak, such a scaling does not
reassemble the data points to a master curve . Obviously the dynamics at the second peak at
higher Q follows different dynamics .
15 10
C
0.8
d 0.6
ô,
0.4
0.2
o ILl1 I I I . Y
104 103 10_ 2 101 101 lo 1
t/T
ô
0 .8
C~ 0 .4
0
0 .2
0
d 1 d I e l d LULll J i 2
1012 10 10 108 106 104 102 10o
t/T
11
Figure 15 .8 : NSE spectra from PB taken at the first and second structure factor peak. The
time is rescaled with the temperature dependence from flow relaxation . Center :
S(Q) for different temperatures .
Fig .15 .9 displays the temperature dependence ofthe corresponding relaxation rates .
While the
data at the first peak nicely agree with the temperature dependence of the arelaxation, as
already evidenced by the scaling, the relaxation rates taken at the second peak follow an
Arrhenius temperature dependence with a same activation energy as that of the corresponding
dielectric /process .
il
12
3 3.5 4 4.5 5 5 .5 6
1000 / T(K)
Figure 15 .9 : Relaxation rates at the first and second structure factor peak of PB in an
Arrhenius representation . Solid lines : a and ßtraces for this polymers .
An evaluation of the structure factor following Eq.
[15 .6] and [15 .7] reveals a jump distance
for the fiprocess of d  1.5A . It also shows that the assumption of statistically independent a
and relaxations is supported by the temperature and momentum transfer dependent spectra .
15 .3 Entropy driven dynamies  the Rouse regime
As outlined in the introduction, the conformational entropy of a chain acts as a resource for
restoring forces for chain conformations, deviating from thermal equilibrium .
In this Chapter
we deal with these entropy driven dynamics in terms of the Rouse model and present NSE
results on the spacetime evolution of the Rouse relaxation and fmally discuss recent
molecular dynamic simulations which have been performed in parallel to NSE experiments,
in order to explore the limits of the Rouse picture.
15 12
15.3 .1 Entropie forces  the Rouse model
As the simplest model for chair relaxation, the Rouse model considers a Gaussian chair in a
heat bath. The building blocks of such a Gaussian chair are segments consisting of several
monomers, so that their end to end distance follows a Gaussian distribution. Their
conformations are described by vectors ami , = r,  r,+1 along the chair. Thereby r is the
position vector of the segment "n" . The chair is described by a succession of freely
connected segments of length f . We are interested in the motion ofthese segments on a length
scale
f < r < R e, where R e"2 = n P Z is the end to end distance ofthe chair. The motion is described by
a Langevin equation
~o dn =V
"F (rn) + J n(t) ,
where ;o is the monomerc friction coefficient . For the stochastic force f(t) we have
(fn(t»=0 and (fna(t)fmß( 0» =2kBT a, and /3 denote the
Cartesian components of r . F(r,d is the free energy of the polymer chair . The force terni in
Eq .[15 .10] is dominated by the conformational entropy of the chair
S=k,~n W({rn })
where W (lLnl) is the probability for a chair conformation lrn} of a Gaussian chair of n
segments .
3/2
expp
{1177 }
j 3 (Li
2 Ë Z
With the boundary conditions offorce free ends Eq .[15 .10] is readily solved by cosine Fourier
transformation, resulting in a spectrum of normal modes . These solutions are similar to e.g .
the transverse vibrational modes of a linear chair except that relaxational motions are
involved instead of periodic vibrations . The dispersion ofthe relaxation rates 11r is qua dratic
in the number ofknots p along the chair.
1513
1 3kBT ~ z 2 72 2 p2
a = f2 N2 P =WN2P p 0 =aR
where rR is the Rouse time  the longest time in the relaxations spectrum  and W is the
elementary Rouse rate . The mode conelation function for the Rouse modes is obtained as
(xp (t) ~
N~ z
xq
R
(0» =Saßspe 6,zpz
exp (tlrp ) (15 .13)
(xo xô (0» = Saß
N t
0
Thereby xp is the acomponent of the number p normal mode and xô is the centre of mass
coordinate .
In order to study Brownian motion, the segment conelation functions in the real
space 0 nn, (t) =
«
n,
(t)  n ( 0»Zl
are required. They are obtained by retransformation ofthe
normal coordinates leading to
4r,2,,(t) =6DRt+Inml
Ë2
4N~Z N 1 r pz m ~
+ z z cos
Z p=, P ~ N
p R t~~
in Eq.[15 .14] we use the tact that the mean square displacement of the centre of mass
provides the diffusion constant. For the special case of the self conelation function (n  m)
Ar,,, (t) reveals the mean square displacement of a polymer segment. We obtain
3kTt 11/2
In contrast to normal diffusion Ar,2, does not grow linearly, but wich the square route oftime .
For the translational diffusion coefficient DR =kBT/N;o is obtained. DR is inversely
proportional to the number of friction performing segments .
15 14
By means of neutron scattering two different correlation functions may be accessed . In the
case of coherent scattering, all partial waves emanating from different scattering centres are
capable of interference  the Fourier transform of the pair correlation function of a single
chain is measured . In contrast incoherent scattering, where the interferences from partial
waves of different scatterers are destructive, measures the self conelation function . The self
correlation function leads directly to the mean square displacement of the diffusiog segments .
In Gaussian approximation for t < ZR we have
~ 2
kBT e 4 \v2
C 12L"o
in the case of coherent scattering, which observes the pair correlation function, interferences
from scattering waves emanating for various segments complicate the scattering function .
With Eq.[15 .14] we obtain
S(Q, t) =1exp [ Q 2 DRt] 1 exp {1Inml Q2~2
N 6
2 R2 Q 2 1
7 2 p2
for small Q (QRE < 1) the second and third terms are negligible and S(Q t)
centre ofmass diffusion of the chain .
describes the
S(Q,t)=N exp (DRt) (15 .18)
For QRE > 1 and t < ZR the internal relaxations dominate . Converting the sums in Eq .[15 .17]
to integrals and aller some algebra de Gennes has derived an expression for the dynamic
structure factor.
1 515
S (Q,t) = 12 fdu exp ~ u_ (S2Rt) vz h )1
(u (nRt)vz
Q Y 0
(15 .19)
h(y) =  i A cos(xy) (1exp( x2»
0
We observe that in spite of the complicated functional form S(Q t),
function, only depends on one variable, the Rouse variable .
like the self correlation
(~ t) v2  Qz 3kRT f Z t 
R
6 N ;0 6
YVt (15 .20)
Since there is no length scale in the problem, for différent momentum transfers the dynamic
structure factors are predicted to collapse to one master cuive, if they are represented as a
function ofthe Rouse variable .
15 .3 .2 Neutron spin echo results
The self correlation function of a Rouse chain was first obseved on polydimethylsiloxane
(PDMS) . Since a straight forward study of the incoherent scattering by NSE is vey difficult 
due to spin flip scattering a severe loss of polarization occurs leading to vey weak signals 
the measurements of the self correlation fonction were performed on high molecular weight
deuterated PDMS chains which contained short protonated labels at random positions . In such
a sanple the scattering essentially originates from the contrast between the protonated
sequence and a deuterated environnent and therefore is coherent. On the other hand the
sequences are randonly distributed, so that there is no constructive interference of partial
waves arising from différent sequences . Under these conditions the scattering experiments
measures the self correlation fonction .
In Fig .15 .10 the corresponding NSE spectra are plotted against the scaling variable of the
Rouse model . The results for the different momentum transfers follow a common straight
line . In Gaussian approximation for the case of the self correlation function the scattering
function directly measures the mean square segment displacement, which according to
Eq .[15 .15] obeys a square root law in time . This behaviour may be directly read off fron
Fig .15 .10 .
15 16
The pair correlation function arising from the segment motion within one given chain is
observed, if some protonated chains are dissolved in a deuterated matrix. Fig .15 .11 displays
the observed spectra from polyethylethylene (90% dPEE, 10% hPEE) at a molecular weight
of Mw = 20.000 . The solid lines give the prediction of the dynamic structure factor of
Eq .[15 .19 ] . Obviously veiy good agreement is achieved.
a 0.2
0 2 4 6 8 10
Q 202F
Figure 15.10 : Self correlation for a PDMS melt T = 100C . The data at different momentum
transfers are plotted us the scaling variable ofthe Rouse model (6  Ë) .
0.8
PEE Homopolymer, T=473K
0 .05
0 .08
0 .10
0 .121
0 .2 
Rouse
0. ~87
Q/A i
0 f
0 10
t/ns
Figure 15 .11 : Single chain structure factor from a PEE melt at 473K . The solid lines
represent a joint fit with the Rouse model .
1
20
15 1 7
We now use these data, in order to investigate the scaling prediction inherent in Eq.[15 .19 ] .
Fig .15 .12 presents a plot of the data of Fig .15 .11, now as a function of the Rouse scaling
variable (Eq.[15 .20]) .
10 1 20
2 (W' 4 t) 2
0
Figure 15 .12 :
Single chain structure factor from PEE melts as a function ofthe Rouse scaling
variable .
The data follow with satisfying precision the scaling prediction. The Small deviations are
related to the translational diffusion of the chairs . This becomes evident from Fig .15 .13,
where the obtained relaxation rates I(Q) are plotted versus Q in a double logarithmic fashion .
Q/A1
Figure 15 .13 : Relaxation rates from PEE melts vs . Q for two different temperatures.
1518
The dashed line gives the Rouse prediction r cc W C4Q 4 . While at larger momentum transfers
the experimental results follow very well this prediction, towards lower Q, a systematic
relative increase of the relaxation rate is observed. Including the diffusion, we have
D+Q 2W f4
6
the solid lines in Fig .15 .13 represents the prediction of Eq .[15 .21 ] . Perfect agreement is
obtained.
15.3 .3 Computer simulation
In order to learn about the limits of the Rouse model, recently a detailed quantitative
comparison of molecular dynamics (MD) computer simulations on a 100 Catom
polyethylene chain (PE) with NSE experiments on PE chains of similar molecular weight bas
been perfor